#------------------------------------------------------------------------------
#$Date: 2017-02-07 17:13:06 +0200 (Tue, 07 Feb 2017) $
#$Revision: 191892 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103545.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103545
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.5 La3 Nb0.5 O14'
_chemical_formula_weight         1070.65
_chemical_name_systematic        ?
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   8.014
_cell_length_b                   8.014
_cell_length_c                   5.046
_cell_measurement_temperature    293(2)
_cell_volume                     280.7
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         9.9E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.597
_diffrn_measured_fraction_theta_max 0.597
_diffrn_radiation_source         synchrotron
_diffrn_radiation_wavelength     0.54920
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0533
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            456
_diffrn_reflns_theta_full        25.52
_diffrn_reflns_theta_max         25.52
_diffrn_reflns_theta_min         2.27
_exptl_absorpt_coefficient_mu    14.382
_exptl_crystal_density_diffrn    6.335
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             474
_refine_diff_density_max         1.478
_refine_diff_density_min         -1.754
_refine_diff_density_rms         0.426
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.09(9)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.973
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     38
_refine_ls_number_reflns         456
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.973
_refine_ls_R_factor_all          0.0412
_refine_ls_R_factor_gt           0.0409
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1111
_refine_ls_wR_factor_ref         0.1122
_reflns_number_gt                454
_reflns_number_total             456
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-9.9d3.cif
_cod_data_source_block           9.9d3
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

Changing (with the help of Perl) all _diffrn_radiation_source values in
the files that were reportedly colected on the HASYLAB D3 beamline
(Hamburg) from 'fine-focus sealed tube' to synchrotron.

The command was:

perl -i -ne \
    "s/'fine-focus sealed tube'/synchrotron/; \
    print unless /_diffrn_radiation_type|_diffrn_radiation_monochromator/" \
    *d3*.cif \
    11.57split.cif \
    21.85split.cif \
    22.85split.cif

Saulius Gra\<zulis
;
_cod_original_formula_sum        'Ga5.50 La3 Nb0.50 O14'
_cod_database_code               2103545
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La -0.43207(11) 0.0000 0.0000 0.0114(3) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0131(6) Uani 0.50 6 d SP
Ga2 Ga -0.6667 -0.3333 -0.5250(5) 0.0092(4) Uani 1 3 d S
Ga3 Ga -0.7672(2) 0.0000 -0.5000 0.0111(4) Uani 1 2 d S
Nb Nb 0.0000 0.0000 0.0000 0.0131(6) Uani 0.50 6 d SP
O1 O -0.3333 0.3333 0.171(3) 0.012(2) Uani 1 3 d S
O3 O -0.2196(13) -0.0719(18) -0.240(3) 0.039(4) Uani 1 1 d .
O2 O -0.695(2) -0.1488(18) 0.309(3) 0.049(5) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.9700 1.5670 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -0.8490 2.7800 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2490 1.0300 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 66.6(6) 6 .
O3 La O2 106.7(6) 6 .
O3 La O2 139.9(4) . .
O3 La O2 139.9(4) 6 6
O3 La O2 106.7(6) . 6
O2 La O2 102.0(7) . 6
O3 La O1 79.4(3) 6 .
O3 La O1 123.0(3) . .
O2 La O1 92.1(4) . .
O2 La O1 72.1(5) 6 .
O3 La O1 123.0(3) 6 2_455
O3 La O1 79.4(3) . 2_455
O2 La O1 72.1(5) . 2_455
O2 La O1 92.1(4) 6 2_455
O1 La O1 155.13(7) . 2_455
O3 La O2 64.3(4) 6 4_445
O3 La O2 79.2(5) . 4_445
O2 La O2 63.6(5) . 4_445
O2 La O2 155.7(2) 6 4_445
O1 La O2 125.2(4) . 4_445
O1 La O2 65.4(4) 2_455 4_445
O3 La O2 79.2(5) 6 2_565
O3 La O2 64.3(4) . 2_565
O2 La O2 155.7(2) . 2_565
O2 La O2 63.6(5) 6 2_565
O1 La O2 65.4(4) . 2_565
O1 La O2 125.2(4) 2_455 2_565
O2 La O2 136.5(4) 4_445 2_565
O3 La Ga2 85.3(4) 6 1_556
O3 La Ga2 110.6(4) . 1_556
O2 La Ga2 31.1(3) . 1_556
O2 La Ga2 130.8(3) 6 1_556
O1 La Ga2 110.5(3) . 1_556
O1 La Ga2 65.2(4) 2_455 1_556
O2 La Ga2 32.5(2) 4_445 1_556
O2 La Ga2 164.5(2) 2_565 1_556
O3 La Ga2 110.6(4) 6 2_564
O3 La Ga2 85.3(4) . 2_564
O2 La Ga2 130.8(3) . 2_564
O2 La Ga2 31.1(3) 6 2_564
O1 La Ga2 65.2(4) . 2_564
O1 La Ga2 110.5(3) 2_455 2_564
O2 La Ga2 164.5(2) 4_445 2_564
O2 La Ga2 32.5(2) 2_565 2_564
Ga2 La Ga2 161.44(3) 1_556 2_564
O3 La Ga1 33.3(3) 6 .
O3 La Ga1 33.3(3) . .
O2 La Ga1 129.0(4) . .
O2 La Ga1 129.0(4) 6 .
O1 La Ga1 102.44(3) . .
O1 La Ga1 102.43(3) 2_455 .
O2 La Ga1 68.2(2) 4_445 .
O2 La Ga1 68.2(2) 2_565 .
Ga2 La Ga1 99.281(15) 1_556 .
Ga2 La Ga1 99.282(15) 2_564 .
O3 La Nb 33.3(3) 6 .
O3 La Nb 33.3(3) . .
O2 La Nb 129.0(4) . .
O2 La Nb 129.0(4) 6 .
O1 La Nb 102.44(3) . .
O1 La Nb 102.43(3) 2_455 .
O2 La Nb 68.2(2) 4_445 .
O2 La Nb 68.2(2) 2_565 .
Ga2 La Nb 99.281(15) 1_556 .
Ga2 La Nb 99.282(15) 2_564 .
Ga1 La Nb 0.0 . .
O3 Ga1 O3 107.2(9) 2 .
O3 Ga1 O3 83.3(6) 2 3
O3 Ga1 O3 86.2(6) . 3
O3 Ga1 O3 86.2(6) 2 5
O3 Ga1 O3 162.2(7) . 5
O3 Ga1 O3 107.2(9) 3 5
O3 Ga1 O3 86.2(6) 2 6
O3 Ga1 O3 83.3(6) . 6
O3 Ga1 O3 162.2(7) 3 6
O3 Ga1 O3 86.2(6) 5 6
O3 Ga1 O3 162.2(7) 2 4
O3 Ga1 O3 86.2(6) . 4
O3 Ga1 O3 86.2(6) 3 4
O3 Ga1 O3 83.3(6) 5 4
O3 Ga1 O3 107.2(9) 6 4
O3 Ga1 La 41.6(3) 2 2
O3 Ga1 La 98.9(3) . 2
O3 Ga1 La 41.6(3) 3 2
O3 Ga1 La 98.9(3) 5 2
O3 Ga1 La 126.4(5) 6 2
O3 Ga1 La 126.4(5) 4 2
O3 Ga1 La 126.4(5) 2 4
O3 Ga1 La 126.4(5) . 4
O3 Ga1 La 98.9(3) 3 4
O3 Ga1 La 41.6(3) 5 4
O3 Ga1 La 98.9(3) 6 4
O3 Ga1 La 41.6(3) 4 4
La Ga1 La 120.0 2 4
O3 Ga1 La 98.9(3) 2 .
O3 Ga1 La 41.6(3) . .
O3 Ga1 La 126.4(5) 3 .
O3 Ga1 La 126.4(5) 5 .
O3 Ga1 La 41.6(3) 6 .
O3 Ga1 La 98.9(3) 4 .
La Ga1 La 120.0 2 .
La Ga1 La 120.0 4 .
O3 Ga1 O2 51.4(4) 2 1_655
O3 Ga1 O2 146.3(4) . 1_655
O3 Ga1 O2 67.2(5) 3 1_655
O3 Ga1 O2 51.5(4) 5 1_655
O3 Ga1 O2 116.2(5) 6 1_655
O3 Ga1 O2 111.1(4) 4 1_655
La Ga1 O2 47.4(3) 2 1_655
La Ga1 O2 79.9(2) 4 1_655
La Ga1 O2 148.41(17) . 1_655
O3 Ga1 O2 67.2(5) 2 5_445
O3 Ga1 O2 51.5(4) . 5_445
O3 Ga1 O2 51.4(4) 3 5_445
O3 Ga1 O2 146.3(4) 5 5_445
O3 Ga1 O2 111.1(4) 6 5_445
O3 Ga1 O2 116.2(5) 4 5_445
La Ga1 O2 47.4(3) 2 5_445
La Ga1 O2 148.41(17) 4 5_445
La Ga1 O2 79.9(2) . 5_445
O2 Ga1 O2 94.8(5) 1_655 5_445
O3 Ga1 O2 51.5(4) 2 4_445
O3 Ga1 O2 67.2(5) . 4_445
O3 Ga1 O2 111.1(4) 3 4_445
O3 Ga1 O2 116.2(5) 5 4_445
O3 Ga1 O2 51.4(4) 6 4_445
O3 Ga1 O2 146.3(4) 4 4_445
La Ga1 O2 79.9(2) 2 4_445
La Ga1 O2 148.40(17) 4 4_445
La Ga1 O2 47.4(3) . 4_445
O2 Ga1 O2 102.4(3) 1_655 4_445
O2 Ga1 O2 63.2(3) 5_445 4_445
O1 Ga2 O2 117.6(5) 2_455 3_454
O1 Ga2 O2 117.6(5) 2_455 4_444
O2 Ga2 O2 100.3(6) 3_454 4_444
O1 Ga2 O2 117.6(5) 2_455 1_554
O2 Ga2 O2 100.3(6) 3_454 1_554
O2 Ga2 O2 100.3(6) 4_444 1_554
O1 Ga2 O1 179.999(4) 2_455 2_454
O2 Ga2 O1 62.4(5) 3_454 2_454
O2 Ga2 O1 62.4(5) 4_444 2_454
O2 Ga2 O1 62.4(5) 1_554 2_454
O1 Ga2 La 135.24(3) 2_455 4_444
O2 Ga2 La 56.9(6) 3_454 4_444
O2 Ga2 La 43.3(3) 4_444 4_444
O2 Ga2 La 106.6(5) 1_554 4_444
O1 Ga2 La 44.76(3) 2_454 4_444
O1 Ga2 La 135.25(3) 2_455 2_454
O2 Ga2 La 43.3(3) 3_454 2_454
O2 Ga2 La 106.6(5) 4_444 2_454
O2 Ga2 La 56.9(6) 1_554 2_454
O1 Ga2 La 44.76(3) 2_454 2_454
La Ga2 La 75.14(4) 4_444 2_454
O1 Ga2 La 135.24(3) 2_455 1_554
O2 Ga2 La 106.6(5) 3_454 1_554
O2 Ga2 La 56.9(6) 4_444 1_554
O2 Ga2 La 43.3(3) 1_554 1_554
O1 Ga2 La 44.76(3) 2_454 1_554
La Ga2 La 75.14(4) 4_444 1_554
La Ga2 La 75.14(4) 2_454 1_554
O1 Ga2 O3 65.2(3) 2_455 4_445
O2 Ga2 O3 59.1(4) 3_454 4_445
O2 Ga2 O3 102.4(7) 4_444 4_445
O2 Ga2 O3 151.7(5) 1_554 4_445
O1 Ga2 O3 114.8(3) 2_454 4_445
La Ga2 O3 79.4(3) 4_444 4_445
La Ga2 O3 100.02(16) 2_454 4_445
La Ga2 O3 154.5(3) 1_554 4_445
O1 Ga2 O3 65.2(3) 2_455 .
O2 Ga2 O3 151.7(5) 3_454 .
O2 Ga2 O3 59.1(4) 4_444 .
O2 Ga2 O3 102.4(7) 1_554 .
O1 Ga2 O3 114.8(3) 2_454 .
La Ga2 O3 100.02(16) 4_444 .
La Ga2 O3 154.5(3) 2_454 .
La Ga2 O3 79.4(3) 1_554 .
O3 Ga2 O3 103.7(3) 4_445 .
O1 Ga2 O3 65.2(3) 2_455 3_455
O2 Ga2 O3 102.4(7) 3_454 3_455
O2 Ga2 O3 151.7(5) 4_444 3_455
O2 Ga2 O3 59.1(4) 1_554 3_455
O1 Ga2 O3 114.8(3) 2_454 3_455
La Ga2 O3 154.5(3) 4_444 3_455
La Ga2 O3 79.4(3) 2_454 3_455
La Ga2 O3 100.01(16) 1_554 3_455
O3 Ga2 O3 103.7(3) 4_445 3_455
O3 Ga2 O3 103.7(3) . 3_455
O1 Ga2 La 41.90(3) 2_455 4_445
O2 Ga2 La 98.0(3) 3_454 4_445
O2 Ga2 La 88.1(6) 4_444 4_445
O2 Ga2 La 158.2(6) 1_554 4_445
O1 Ga2 La 138.10(3) 2_454 4_445
La Ga2 La 93.347(5) 4_444 4_445
La Ga2 La 139.788(5) 2_454 4_445
La Ga2 La 139.788(5) 1_554 4_445
O3 Ga2 La 39.78(17) 4_445 4_445
O3 Ga2 La 64.6(3) . 4_445
O3 Ga2 La 105.2(2) 3_455 4_445
O3 Ga3 O3 134.5(8) 3_455 5_454
O3 Ga3 O2 108.1(5) 3_455 1_554
O3 Ga3 O2 100.6(7) 5_454 1_554
O3 Ga3 O2 100.6(7) 3_455 6
O3 Ga3 O2 108.0(5) 5_454 6
O2 Ga3 O2 100.6(13) 1_554 6
O3 Ga3 O3 78.4(7) 3_455 2_454
O3 Ga3 O3 74.2(6) 5_454 2_454
O2 Ga3 O3 77.5(7) 1_554 2_454
O2 Ga3 O3 177.4(5) 6 2_454
O3 Ga3 O3 74.2(6) 3_455 4_455
O3 Ga3 O3 78.4(7) 5_454 4_455
O2 Ga3 O3 177.4(5) 1_554 4_455
O2 Ga3 O3 77.5(7) 6 4_455
O3 Ga3 O3 104.3(4) 2_454 4_455
O3 Ga3 Nb 35.5(3) 3_455 1_455
O3 Ga3 Nb 110.8(5) 5_454 1_455
O2 Ga3 Nb 143.3(3) 1_554 1_455
O2 Ga3 Nb 87.6(6) 6 1_455
O3 Ga3 Nb 92.9(2) 2_454 1_455
O3 Ga3 Nb 38.8(3) 4_455 1_455
O3 Ga3 Nb 110.8(5) 3_455 1_454
O3 Ga3 Nb 35.5(3) 5_454 1_454
O2 Ga3 Nb 87.6(6) 1_554 1_454
O2 Ga3 Nb 143.3(3) 6 1_454
O3 Ga3 Nb 38.8(3) 2_454 1_454
O3 Ga3 Nb 92.9(2) 4_455 1_454
Nb Ga3 Nb 107.03(5) 1_455 1_454
O3 Ga3 O1 160.0(6) 3_455 1_554
O3 Ga3 O1 61.6(4) 5_454 1_554
O2 Ga3 O1 74.7(4) 1_554 1_554
O2 Ga3 O1 59.7(5) 6 1_554
O3 Ga3 O1 121.1(4) 2_454 1_554
O3 Ga3 O1 102.7(3) 4_455 1_554
Nb Ga3 O1 137.07(18) 1_455 1_554
Nb Ga3 O1 89.0(2) 1_454 1_554
O3 Ga3 O1 61.6(4) 3_455 2_455
O3 Ga3 O1 160.0(6) 5_454 2_455
O2 Ga3 O1 59.7(5) 1_554 2_455
O2 Ga3 O1 74.7(4) 6 2_455
O3 Ga3 O1 102.7(3) 2_454 2_455
O3 Ga3 O1 121.1(4) 4_455 2_455
Nb Ga3 O1 89.0(2) 1_455 2_455
Nb Ga3 O1 137.07(18) 1_454 2_455
O1 Ga3 O1 106.13(19) 1_554 2_455
O3 Ga3 O3 45.7(3) 3_455 1_455
O3 Ga3 O3 89.2(7) 5_454 1_455
O2 Ga3 O3 134.6(6) 1_554 1_455
O2 Ga3 O3 118.4(7) 6 1_455
O3 Ga3 O3 62.6(4) 2_454 1_455
O3 Ga3 O3 47.9(2) 4_455 1_455
Nb Ga3 O3 32.9(2) 1_455 1_455
Nb Ga3 O3 75.1(2) 1_454 1_455
O1 Ga3 O3 144.3(2) 1_554 1_455
O1 Ga3 O3 107.2(3) 2_455 1_455
O3 Ga3 O3 89.2(7) 3_455 6_454
O3 Ga3 O3 45.7(3) 5_454 6_454
O2 Ga3 O3 118.4(7) 1_554 6_454
O2 Ga3 O3 134.6(6) 6 6_454
O3 Ga3 O3 47.9(2) 2_454 6_454
O3 Ga3 O3 62.6(4) 4_455 6_454
Nb Ga3 O3 75.1(2) 1_455 6_454
Nb Ga3 O3 32.9(2) 1_454 6_454
O1 Ga3 O3 107.2(3) 1_554 6_454
O1 Ga3 O3 144.3(2) 2_455 6_454
O3 Ga3 O3 45.7(5) 1_455 6_454
O3 Nb O3 107.2(9) 2 .
O3 Nb O3 83.3(6) 2 3
O3 Nb O3 86.2(6) . 3
O3 Nb O3 86.2(6) 2 5
O3 Nb O3 162.2(7) . 5
O3 Nb O3 107.2(9) 3 5
O3 Nb O3 86.2(6) 2 6
O3 Nb O3 83.3(6) . 6
O3 Nb O3 162.2(7) 3 6
O3 Nb O3 86.2(6) 5 6
O3 Nb O3 162.2(7) 2 4
O3 Nb O3 86.2(6) . 4
O3 Nb O3 86.2(6) 3 4
O3 Nb O3 83.3(6) 5 4
O3 Nb O3 107.2(9) 6 4
O3 Nb Ga3 54.2(5) 2 1_656
O3 Nb Ga3 159.8(5) . 1_656
O3 Nb Ga3 98.1(4) 3 1_656
O3 Nb Ga3 32.2(3) 5 1_656
O3 Nb Ga3 87.2(4) 6 1_656
O3 Nb Ga3 113.7(3) 4 1_656
O3 Nb Ga3 32.2(3) 2 4_446
O3 Nb Ga3 98.1(4) . 4_446
O3 Nb Ga3 113.7(3) 3 4_446
O3 Nb Ga3 87.2(4) 5 4_446
O3 Nb Ga3 54.2(5) 6 4_446
O3 Nb Ga3 159.8(5) 4 4_446
Ga3 Nb Ga3 61.99(4) 1_656 4_446
O3 Nb Ga3 98.1(4) 2 4_445
O3 Nb Ga3 32.2(3) . 4_445
O3 Nb Ga3 54.2(5) 3 4_445
O3 Nb Ga3 159.8(5) 5 4_445
O3 Nb Ga3 113.7(3) 6 4_445
O3 Nb Ga3 87.2(4) 4 4_445
Ga3 Nb Ga3 145.41(2) 1_656 4_445
Ga3 Nb Ga3 107.03(5) 4_446 4_445
O3 Nb Ga3 113.7(3) 2 1_655
O3 Nb Ga3 87.2(4) . 1_655
O3 Nb Ga3 32.2(3) 3 1_655
O3 Nb Ga3 98.1(4) 5 1_655
O3 Nb Ga3 159.8(5) 6 1_655
O3 Nb Ga3 54.2(5) 4 1_655
Ga3 Nb Ga3 107.03(5) 1_656 1_655
Ga3 Nb Ga3 145.41(2) 4_446 1_655
Ga3 Nb Ga3 61.99(4) 4_445 1_655
O3 Nb Ga3 87.2(4) 2 2_565
O3 Nb Ga3 113.7(3) . 2_565
O3 Nb Ga3 159.8(5) 3 2_565
O3 Nb Ga3 54.2(5) 5 2_565
O3 Nb Ga3 32.2(3) 6 2_565
O3 Nb Ga3 98.1(4) 4 2_565
Ga3 Nb Ga3 61.99(4) 1_656 2_565
Ga3 Nb Ga3 61.99(4) 4_446 2_565
Ga3 Nb Ga3 145.41(2) 4_445 2_565
Ga3 Nb Ga3 145.41(2) 1_655 2_565
O3 Nb Ga3 159.8(5) 2 2_564
O3 Nb Ga3 54.2(5) . 2_564
O3 Nb Ga3 87.2(4) 3 2_564
O3 Nb Ga3 113.7(3) 5 2_564
O3 Nb Ga3 98.1(4) 6 2_564
O3 Nb Ga3 32.2(3) 4 2_564
Ga3 Nb Ga3 145.41(2) 1_656 2_564
Ga3 Nb Ga3 145.41(2) 4_446 2_564
Ga3 Nb Ga3 61.99(4) 4_445 2_564
Ga3 Nb Ga3 61.99(4) 1_655 2_564
Ga3 Nb Ga3 107.03(5) 2_565 2_564
Ga2 O1 La 109.9(4) 2_565 .
Ga2 O1 La 109.9(4) 2_565 2_565
La O1 La 109.0(4) . 2_565
Ga2 O1 La 109.9(4) 2_565 4_455
La O1 La 109.0(4) . 4_455
La O1 La 109.0(4) 2_565 4_455
Ga2 O1 O2 146.4(3) 2_565 2_565
La O1 O2 62.3(4) . 2_565
La O1 O2 52.0(4) 2_565 2_565
La O1 O2 103.2(6) 4_455 2_565
Ga2 O1 O2 146.4(3) 2_565 6
La O1 O2 52.0(4) . 6
La O1 O2 103.2(6) 2_565 6
La O1 O2 62.3(4) 4_455 6
O2 O1 O2 57.2(5) 2_565 6
Ga2 O1 O2 146.4(3) 2_565 5_455
La O1 O2 103.2(6) . 5_455
La O1 O2 62.3(4) 2_565 5_455
La O1 O2 52.0(4) 4_455 5_455
O2 O1 O2 57.2(5) 2_565 5_455
O2 O1 O2 57.2(5) 6 5_455
Ga2 O1 O2 31.4(3) 2_565 2_566
La O1 O2 96.9(3) . 2_566
La O1 O2 88.7(4) 2_565 2_566
La O1 O2 140.7(5) 4_455 2_566
O2 O1 O2 115.0(3) 2_565 2_566
O2 O1 O2 148.77(13) 6 2_566
O2 O1 O2 148.77(13) 5_455 2_566
Ga2 O1 O2 31.4(3) 2_565 6_556
La O1 O2 88.7(4) . 6_556
La O1 O2 140.7(5) 2_565 6_556
La O1 O2 96.9(3) 4_455 6_556
O2 O1 O2 148.77(13) 2_565 6_556
O2 O1 O2 115.0(3) 6 6_556
O2 O1 O2 148.77(13) 5_455 6_556
O2 O1 O2 53.7(5) 2_566 6_556
Ga2 O1 O2 31.4(3) 2_565 5_456
La O1 O2 140.7(5) . 5_456
La O1 O2 96.9(3) 2_565 5_456
La O1 O2 88.7(4) 4_455 5_456
O2 O1 O2 148.77(13) 2_565 5_456
O2 O1 O2 148.77(13) 6 5_456
O2 O1 O2 115.0(3) 5_455 5_456
O2 O1 O2 53.7(5) 2_566 5_456
O2 O1 O2 53.7(5) 6_556 5_456
Ga2 O1 O3 83.6(4) 2_565 6
La O1 O3 48.27(17) . 6
La O1 O3 81.8(3) 2_565 6
La O1 O3 157.2(4) 4_455 6
O2 O1 O3 67.0(5) 2_565 6
O2 O1 O3 96.1(4) 6 6
O2 O1 O3 124.1(5) 5_455 6
O2 O1 O3 56.6(3) 2_566 6
O2 O1 O3 85.4(5) 6_556 6
O2 O1 O3 110.3(5) 5_456 6
Ga2 O1 O3 83.6(4) 2_565 5_455
La O1 O3 81.8(3) . 5_455
La O1 O3 157.2(4) 2_565 5_455
La O1 O3 48.27(18) 4_455 5_455
O2 O1 O3 124.1(5) 2_565 5_455
O2 O1 O3 67.0(5) 6 5_455
O2 O1 O3 96.1(4) 5_455 5_455
O2 O1 O3 110.3(5) 2_566 5_455
O2 O1 O3 56.6(3) 6_556 5_455
O2 O1 O3 85.4(5) 5_456 5_455
O3 O1 O3 118.79(15) 6 5_455
Ga2 O1 O3 83.6(4) 2_565 2_565
La O1 O3 157.2(4) . 2_565
La O1 O3 48.27(17) 2_565 2_565
La O1 O3 81.8(3) 4_455 2_565
O2 O1 O3 96.1(4) 2_565 2_565
O2 O1 O3 124.1(5) 6 2_565
O2 O1 O3 67.0(5) 5_455 2_565
O2 O1 O3 85.4(5) 2_566 2_565
O2 O1 O3 110.3(5) 6_556 2_565
O2 O1 O3 56.6(3) 5_456 2_565
O3 O1 O3 118.79(15) 6 2_565
O3 O1 O3 118.79(15) 5_455 2_565
Ga2 O1 Ga2 179.997(1) 2_565 2_564
La O1 Ga2 70.1(4) . 2_564
La O1 Ga2 70.1(4) 2_565 2_564
La O1 Ga2 70.1(4) 4_455 2_564
O2 O1 Ga2 33.6(3) 2_565 2_564
O2 O1 Ga2 33.6(3) 6 2_564
O2 O1 Ga2 33.6(3) 5_455 2_564
O2 O1 Ga2 148.6(3) 2_566 2_564
O2 O1 Ga2 148.6(3) 6_556 2_564
O2 O1 Ga2 148.6(3) 5_456 2_564
O3 O1 Ga2 96.4(4) 6 2_564
O3 O1 Ga2 96.4(4) 5_455 2_564
O3 O1 Ga2 96.4(4) 2_565 2_564
Ga2 O1 O2 78.7(4) 2_565 3_565
La O1 O2 94.4(2) . 3_565
La O1 O2 42.57(19) 2_565 3_565
La O1 O2 149.3(2) 4_455 3_565
O2 O1 O2 69.9(4) 2_565 3_565
O2 O1 O2 125.8(4) 6 3_565
O2 O1 O2 104.4(5) 5_455 3_565
O2 O1 O2 49.8(5) 2_566 3_565
O2 O1 O2 103.3(4) 6_556 3_565
O2 O1 O2 85.0(3) 5_456 3_565
O3 O1 O2 49.1(3) 6 3_565
O3 O1 O2 159.5(5) 5_455 3_565
O3 O1 O2 69.7(3) 2_565 3_565
Ga2 O1 O2 101.3(4) 2_564 3_565
Ga2 O1 O2 78.7(4) 2_565 .
La O1 O2 42.57(19) . .
La O1 O2 149.3(2) 2_565 .
La O1 O2 94.4(3) 4_455 .
O2 O1 O2 104.4(5) 2_565 .
O2 O1 O2 69.9(4) 6 .
O2 O1 O2 125.8(4) 5_455 .
O2 O1 O2 85.0(3) 2_566 .
O2 O1 O2 49.8(5) 6_556 .
O2 O1 O2 103.3(4) 5_456 .
O3 O1 O2 69.7(3) 6 .
O3 O1 O2 49.1(3) 5_455 .
O3 O1 O2 159.5(5) 2_565 .
Ga2 O1 O2 101.3(4) 2_564 .
O2 O1 O2 116.3(2) 3_565 .
Ga2 O1 O2 78.7(4) 2_565 4_455
La O1 O2 149.3(2) . 4_455
La O1 O2 94.4(3) 2_565 4_455
La O1 O2 42.57(19) 4_455 4_455
O2 O1 O2 125.8(4) 2_565 4_455
O2 O1 O2 104.4(5) 6 4_455
O2 O1 O2 69.9(4) 5_455 4_455
O2 O1 O2 103.3(4) 2_566 4_455
O2 O1 O2 85.0(3) 6_556 4_455
O2 O1 O2 49.8(5) 5_456 4_455
O3 O1 O2 159.5(5) 6 4_455
O3 O1 O2 69.7(3) 5_455 4_455
O3 O1 O2 49.1(3) 2_565 4_455
Ga2 O1 O2 101.3(4) 2_564 4_455
O2 O1 O2 116.3(2) 3_565 4_455
O2 O1 O2 116.3(2) . 4_455
Ga2 O1 Ga3 62.2(2) 2_565 2_565
La O1 Ga3 78.11(9) . 2_565
La O1 Ga3 72.19(9) 2_565 2_565
La O1 Ga3 171.3(5) 4_455 2_565
O2 O1 Ga3 84.4(2) 2_565 2_565
O2 O1 Ga3 126.1(4) 6 2_565
O2 O1 Ga3 132.4(4) 5_455 2_565
O2 O1 Ga3 31.0(2) 2_566 2_565
O2 O1 Ga3 78.0(4) 6_556 2_565
O2 O1 Ga3 82.6(5) 5_456 2_565
O3 O1 Ga3 30.4(2) 6 2_565
O3 O1 Ga3 130.4(4) 5_455 2_565
O3 O1 Ga3 93.4(3) 2_565 2_565
Ga2 O1 Ga3 117.8(2) 2_564 2_565
O2 O1 Ga3 29.92(17) 3_565 2_565
O2 O1 Ga3 87.7(3) . 2_565
O2 O1 Ga3 129.3(4) 4_455 2_565
Ga2 O1 Ga3 62.2(2) 2_565 1_556
La O1 Ga3 72.19(9) . 1_556
La O1 Ga3 171.3(5) 2_565 1_556
La O1 Ga3 78.11(9) 4_455 1_556
O2 O1 Ga3 132.4(4) 2_565 1_556
O2 O1 Ga3 84.4(2) 6 1_556
O2 O1 Ga3 126.1(4) 5_455 1_556
O2 O1 Ga3 82.6(5) 2_566 1_556
O2 O1 Ga3 31.0(2) 6_556 1_556
O2 O1 Ga3 78.0(4) 5_456 1_556
O3 O1 Ga3 93.4(3) 6 1_556
O3 O1 Ga3 30.4(2) 5_455 1_556
O3 O1 Ga3 130.4(4) 2_565 1_556
Ga2 O1 Ga3 117.8(2) 2_564 1_556
O2 O1 Ga3 129.3(4) 3_565 1_556
O2 O1 Ga3 29.92(16) . 1_556
O2 O1 Ga3 87.7(3) 4_455 1_556
Ga3 O1 Ga3 100.0(3) 2_565 1_556
Ga2 O1 Ga3 62.2(2) 2_565 4_456
La O1 Ga3 171.3(5) . 4_456
La O1 Ga3 78.11(9) 2_565 4_456
La O1 Ga3 72.19(9) 4_455 4_456
O2 O1 Ga3 126.1(4) 2_565 4_456
O2 O1 Ga3 132.4(4) 6 4_456
O2 O1 Ga3 84.4(2) 5_455 4_456
O2 O1 Ga3 78.0(4) 2_566 4_456
O2 O1 Ga3 82.6(5) 6_556 4_456
O2 O1 Ga3 31.0(2) 5_456 4_456
O3 O1 Ga3 130.4(4) 6 4_456
O3 O1 Ga3 93.4(3) 5_455 4_456
O3 O1 Ga3 30.4(2) 2_565 4_456
Ga2 O1 Ga3 117.8(2) 2_564 4_456
O2 O1 Ga3 87.7(3) 3_565 4_456
O2 O1 Ga3 129.3(4) . 4_456
O2 O1 Ga3 29.92(17) 4_455 4_456
Ga3 O1 Ga3 100.0(3) 2_565 4_456
Ga3 O1 Ga3 100.0(3) 1_556 4_456
Ga2 O1 O3 118.7(3) 2_565 .
La O1 O3 27.58(18) . .
La O1 O3 81.6(3) 2_565 .
La O1 O3 122.8(5) 4_455 .
O2 O1 O3 39.9(4) 2_565 .
O2 O1 O3 60.6(4) 6 .
O2 O1 O3 93.3(5) 5_455 .
O2 O1 O3 93.6(3) 2_566 .
O2 O1 O3 108.9(4) 6_556 .
O2 O1 O3 147.3(5) 5_456 .
O3 O1 O3 37.0(4) 6 .
O3 O1 O3 108.5(4) 5_455 .
O3 O1 O3 129.8(4) 2_565 .
Ga2 O1 O3 61.3(3) 2_564 .
O2 O1 O3 71.8(3) 3_565 .
O2 O1 O3 68.9(2) . .
O2 O1 O3 162.5(6) 4_455 .
Ga3 O1 O3 65.75(17) 2_565 .
Ga3 O1 O3 98.84(18) 1_556 .
Ga3 O1 O3 158.15(13) 4_456 .
Ga2 O1 O3 118.7(3) 2_565 4_455
La O1 O3 81.6(3) . 4_455
La O1 O3 122.8(5) 2_565 4_455
La O1 O3 27.58(18) 4_455 4_455
O2 O1 O3 93.3(5) 2_565 4_455
O2 O1 O3 39.9(4) 6 4_455
O2 O1 O3 60.6(4) 5_455 4_455
O2 O1 O3 147.3(5) 2_566 4_455
O2 O1 O3 93.6(3) 6_556 4_455
O2 O1 O3 108.8(4) 5_456 4_455
O3 O1 O3 129.8(4) 6 4_455
O3 O1 O3 37.0(4) 5_455 4_455
O3 O1 O3 108.5(4) 2_565 4_455
Ga2 O1 O3 61.3(3) 2_564 4_455
O2 O1 O3 162.5(6) 3_565 4_455
O2 O1 O3 71.8(3) . 4_455
O2 O1 O3 68.9(2) 4_455 4_455
Ga3 O1 O3 158.15(13) 2_565 4_455
Ga3 O1 O3 65.75(17) 1_556 4_455
Ga3 O1 O3 98.84(18) 4_456 4_455
O3 O1 O3 98.9(4) . 4_455
Ga2 O1 O3 118.7(3) 2_565 3_565
La O1 O3 122.8(5) . 3_565
La O1 O3 27.58(18) 2_565 3_565
La O1 O3 81.6(3) 4_455 3_565
O2 O1 O3 60.6(4) 2_565 3_565
O2 O1 O3 93.3(5) 6 3_565
O2 O1 O3 39.9(4) 5_455 3_565
O2 O1 O3 108.8(4) 2_566 3_565
O2 O1 O3 147.3(5) 6_556 3_565
O2 O1 O3 93.6(3) 5_456 3_565
O3 O1 O3 108.5(4) 6 3_565
O3 O1 O3 129.8(4) 5_455 3_565
O3 O1 O3 37.0(4) 2_565 3_565
Ga2 O1 O3 61.3(3) 2_564 3_565
O2 O1 O3 68.9(2) 3_565 3_565
O2 O1 O3 162.5(6) . 3_565
O2 O1 O3 71.8(3) 4_455 3_565
Ga3 O1 O3 98.84(18) 2_565 3_565
Ga3 O1 O3 158.15(13) 1_556 3_565
Ga3 O1 O3 65.75(17) 4_456 3_565
O3 O1 O3 98.9(4) . 3_565
O3 O1 O3 98.9(4) 4_455 3_565
Ga2 O1 Ga3 137.04(14) 2_565 2_564
La O1 Ga3 58.0(2) . 2_564
La O1 Ga3 52.6(2) 2_565 2_564
La O1 Ga3 112.9(5) 4_455 2_564
O2 O1 Ga3 10.0(3) 2_565 2_564
O2 O1 Ga3 63.0(4) 6 2_564
O2 O1 Ga3 67.1(3) 5_455 2_564
O2 O1 Ga3 105.7(2) 2_566 2_564
O2 O1 Ga3 140.4(3) 6_556 2_564
O2 O1 Ga3 146.3(3) 5_456 2_564
O3 O1 Ga3 57.1(3) 6 2_564
O3 O1 Ga3 128.4(4) 5_455 2_564
O3 O1 Ga3 99.5(3) 2_565 2_564
Ga2 O1 Ga3 42.96(14) 2_564 2_564
O2 O1 Ga3 63.0(3) 3_565 2_564
O2 O1 Ga3 100.5(2) . 2_564
O2 O1 Ga3 134.6(4) 4_455 2_564
Ga3 O1 Ga3 74.83(10) 2_565 2_564
Ga3 O1 Ga3 129.99(15) 1_556 2_564
Ga3 O1 Ga3 129.99(15) 4_456 2_564
O3 O1 Ga3 32.9(2) . 2_564
O3 O1 Ga3 101.0(4) 4_455 2_564
O3 O1 Ga3 66.1(2) 3_565 2_564
Ga2 O1 Ga3 137.04(14) 2_565 .
La O1 Ga3 52.6(2) . .
La O1 Ga3 112.9(5) 2_565 .
La O1 Ga3 58.0(2) 4_455 .
O2 O1 Ga3 67.1(3) 2_565 .
O2 O1 Ga3 10.0(3) 6 .
O2 O1 Ga3 63.0(4) 5_455 .
O2 O1 Ga3 146.3(3) 2_566 .
O2 O1 Ga3 105.7(2) 6_556 .
O2 O1 Ga3 140.4(3) 5_456 .
O3 O1 Ga3 99.5(3) 6 .
O3 O1 Ga3 57.1(3) 5_455 .
O3 O1 Ga3 128.4(4) 2_565 .
Ga2 O1 Ga3 42.96(14) 2_564 .
O2 O1 Ga3 134.6(4) 3_565 .
O2 O1 Ga3 63.0(3) . .
O2 O1 Ga3 100.5(2) 4_455 .
Ga3 O1 Ga3 129.99(15) 2_565 .
Ga3 O1 Ga3 74.83(10) 1_556 .
Ga3 O1 Ga3 129.99(15) 4_456 .
O3 O1 Ga3 66.1(2) . .
O3 O1 Ga3 32.9(2) 4_455 .
O3 O1 Ga3 101.0(4) 3_565 .
Ga3 O1 Ga3 72.3(2) 2_564 .
Ga2 O1 Ga3 137.04(14) 2_565 4_455
La O1 Ga3 112.9(5) . 4_455
La O1 Ga3 58.0(2) 2_565 4_455
La O1 Ga3 52.6(2) 4_455 4_455
O2 O1 Ga3 63.0(4) 2_565 4_455
O2 O1 Ga3 67.0(3) 6 4_455
O2 O1 Ga3 10.0(3) 5_455 4_455
O2 O1 Ga3 140.4(3) 2_566 4_455
O2 O1 Ga3 146.3(3) 6_556 4_455
O2 O1 Ga3 105.7(2) 5_456 4_455
O3 O1 Ga3 128.4(4) 6 4_455
O3 O1 Ga3 99.5(3) 5_455 4_455
O3 O1 Ga3 57.1(3) 2_565 4_455
Ga2 O1 Ga3 42.96(14) 2_564 4_455
O2 O1 Ga3 100.5(2) 3_565 4_455
O2 O1 Ga3 134.6(4) . 4_455
O2 O1 Ga3 63.0(3) 4_455 4_455
Ga3 O1 Ga3 129.99(15) 2_565 4_455
Ga3 O1 Ga3 129.99(15) 1_556 4_455
Ga3 O1 Ga3 74.83(10) 4_456 4_455
O3 O1 Ga3 101.0(4) . 4_455
O3 O1 Ga3 66.1(2) 4_455 4_455
O3 O1 Ga3 32.9(2) 3_565 4_455
Ga3 O1 Ga3 72.3(2) 2_564 4_455
Ga3 O1 Ga3 72.3(2) . 4_455
Ga2 O1 Nb 100.6(2) 2_565 .
La O1 Nb 45.93(4) . .
La O1 Nb 70.80(9) 2_565 .
La O1 Nb 146.8(5) 4_455 .
O2 O1 Nb 49.2(3) 2_565 .
O2 O1 Nb 85.1(4) 6 .
O2 O1 Nb 106.3(4) 5_455 .
O2 O1 Nb 71.57(18) 2_566 .
O2 O1 Nb 102.7(3) 6_556 .
O2 O1 Nb 124.4(4) 5_456 .
O3 O1 Nb 17.8(3) 6 .
O3 O1 Nb 126.1(2) 5_455 .
O3 O1 Nb 115.1(2) 2_565 .
Ga2 O1 Nb 79.4(2) 2_564 .
O2 O1 Nb 48.8(3) 3_565 .
O2 O1 Nb 78.75(16) . .
O2 O1 Nb 164.14(19) 4_455 .
Ga3 O1 Nb 41.81(3) 2_565 .
Ga3 O1 Nb 106.13(8) 1_556 .
Ga3 O1 Nb 136.36(16) 4_456 .
O3 O1 Nb 24.72(15) . .
O3 O1 Nb 123.6(3) 4_455 .
O3 O1 Nb 95.28(19) 3_565 .
Ga3 O1 Nb 39.29(7) 2_564 .
Ga3 O1 Nb 90.82(19) . .
Ga3 O1 Nb 111.0(3) 4_455 .
Ga2 O1 Ga1 100.6(2) 2_565 .
La O1 Ga1 45.93(4) . .
La O1 Ga1 70.80(9) 2_565 .
La O1 Ga1 146.8(5) 4_455 .
O2 O1 Ga1 49.2(3) 2_565 .
O2 O1 Ga1 85.1(4) 6 .
O2 O1 Ga1 106.3(4) 5_455 .
O2 O1 Ga1 71.57(18) 2_566 .
O2 O1 Ga1 102.7(3) 6_556 .
O2 O1 Ga1 124.4(4) 5_456 .
O3 O1 Ga1 17.8(3) 6 .
O3 O1 Ga1 126.1(2) 5_455 .
O3 O1 Ga1 115.1(2) 2_565 .
Ga2 O1 Ga1 79.4(2) 2_564 .
O2 O1 Ga1 48.8(3) 3_565 .
O2 O1 Ga1 78.75(16) . .
O2 O1 Ga1 164.14(19) 4_455 .
Ga3 O1 Ga1 41.81(3) 2_565 .
Ga3 O1 Ga1 106.13(8) 1_556 .
Ga3 O1 Ga1 136.36(16) 4_456 .
O3 O1 Ga1 24.72(15) . .
O3 O1 Ga1 123.6(3) 4_455 .
O3 O1 Ga1 95.28(19) 3_565 .
Ga3 O1 Ga1 39.29(7) 2_564 .
Ga3 O1 Ga1 90.82(19) . .
Ga3 O1 Ga1 111.0(3) 4_455 .
Nb O1 Ga1 0.0 . .
Ga2 O1 Nb 100.6(2) 2_565 1_455
La O1 Nb 70.80(9) . 1_455
La O1 Nb 146.8(5) 2_565 1_455
La O1 Nb 45.93(4) 4_455 1_455
O2 O1 Nb 106.3(4) 2_565 1_455
O2 O1 Nb 49.2(3) 6 1_455
O2 O1 Nb 85.1(4) 5_455 1_455
O2 O1 Nb 124.4(4) 2_566 1_455
O2 O1 Nb 71.57(18) 6_556 1_455
O2 O1 Nb 102.7(3) 5_456 1_455
O3 O1 Nb 115.1(2) 6 1_455
O3 O1 Nb 17.8(3) 5_455 1_455
O3 O1 Nb 126.1(2) 2_565 1_455
Ga2 O1 Nb 79.4(2) 2_564 1_455
O2 O1 Nb 164.14(19) 3_565 1_455
O2 O1 Nb 48.8(3) . 1_455
O2 O1 Nb 78.75(16) 4_455 1_455
Ga3 O1 Nb 136.36(16) 2_565 1_455
Ga3 O1 Nb 41.81(3) 1_556 1_455
Ga3 O1 Nb 106.13(8) 4_456 1_455
O3 O1 Nb 95.28(19) . 1_455
O3 O1 Nb 24.72(15) 4_455 1_455
O3 O1 Nb 123.6(3) 3_565 1_455
Ga3 O1 Nb 111.0(3) 2_564 1_455
Ga3 O1 Nb 39.29(7) . 1_455
Ga3 O1 Nb 90.82(19) 4_455 1_455
Nb O1 Nb 116.72(12) . 1_455
Ga1 O1 Nb 116.72(12) . 1_455
Ga2 O1 Ga1 100.6(2) 2_565 1_455
La O1 Ga1 70.80(9) . 1_455
La O1 Ga1 146.8(5) 2_565 1_455
La O1 Ga1 45.93(4) 4_455 1_455
O2 O1 Ga1 106.3(4) 2_565 1_455
O2 O1 Ga1 49.2(3) 6 1_455
O2 O1 Ga1 85.1(4) 5_455 1_455
O2 O1 Ga1 124.4(4) 2_566 1_455
O2 O1 Ga1 71.57(18) 6_556 1_455
O2 O1 Ga1 102.7(3) 5_456 1_455
O3 O1 Ga1 115.1(2) 6 1_455
O3 O1 Ga1 17.8(3) 5_455 1_455
O3 O1 Ga1 126.1(2) 2_565 1_455
Ga2 O1 Ga1 79.4(2) 2_564 1_455
O2 O1 Ga1 164.14(19) 3_565 1_455
O2 O1 Ga1 48.8(3) . 1_455
O2 O1 Ga1 78.75(16) 4_455 1_455
Ga3 O1 Ga1 136.36(16) 2_565 1_455
Ga3 O1 Ga1 41.81(3) 1_556 1_455
Ga3 O1 Ga1 106.13(8) 4_456 1_455
O3 O1 Ga1 95.28(19) . 1_455
O3 O1 Ga1 24.72(15) 4_455 1_455
O3 O1 Ga1 123.6(3) 3_565 1_455
Ga3 O1 Ga1 111.0(3) 2_564 1_455
Ga3 O1 Ga1 39.29(7) . 1_455
Ga3 O1 Ga1 90.82(19) 4_455 1_455
Nb O1 Ga1 116.72(12) . 1_455
Ga1 O1 Ga1 116.72(12) . 1_455
Nb O1 Ga1 0.0 1_455 1_455
Ga2 O1 Ga1 100.6(2) 2_565 1_565
La O1 Ga1 146.8(5) . 1_565
La O1 Ga1 45.93(4) 2_565 1_565
La O1 Ga1 70.80(9) 4_455 1_565
O2 O1 Ga1 85.1(4) 2_565 1_565
O2 O1 Ga1 106.3(4) 6 1_565
O2 O1 Ga1 49.2(3) 5_455 1_565
O2 O1 Ga1 102.7(3) 2_566 1_565
O2 O1 Ga1 124.4(4) 6_556 1_565
O2 O1 Ga1 71.57(18) 5_456 1_565
O3 O1 Ga1 126.1(2) 6 1_565
O3 O1 Ga1 115.1(2) 5_455 1_565
O3 O1 Ga1 17.8(3) 2_565 1_565
Ga2 O1 Ga1 79.4(2) 2_564 1_565
O2 O1 Ga1 78.75(16) 3_565 1_565
O2 O1 Ga1 164.14(19) . 1_565
O2 O1 Ga1 48.8(3) 4_455 1_565
Ga3 O1 Ga1 106.13(8) 2_565 1_565
Ga3 O1 Ga1 136.36(16) 1_556 1_565
Ga3 O1 Ga1 41.81(4) 4_456 1_565
O3 O1 Ga1 123.6(3) . 1_565
O3 O1 Ga1 95.28(19) 4_455 1_565
O3 O1 Ga1 24.72(15) 3_565 1_565
Ga3 O1 Ga1 90.82(19) 2_564 1_565
Ga3 O1 Ga1 111.0(3) . 1_565
Ga3 O1 Ga1 39.29(7) 4_455 1_565
Nb O1 Ga1 116.72(12) . 1_565
Ga1 O1 Ga1 116.72(12) . 1_565
Nb O1 Ga1 116.72(12) 1_455 1_565
Ga1 O1 Ga1 116.72(12) 1_455 1_565
Ga2 O1 Nb 100.6(2) 2_565 1_565
La O1 Nb 146.8(5) . 1_565
La O1 Nb 45.93(4) 2_565 1_565
La O1 Nb 70.80(9) 4_455 1_565
O2 O1 Nb 85.1(4) 2_565 1_565
O2 O1 Nb 106.3(4) 6 1_565
O2 O1 Nb 49.2(3) 5_455 1_565
O2 O1 Nb 102.7(3) 2_566 1_565
O2 O1 Nb 124.4(4) 6_556 1_565
O2 O1 Nb 71.57(18) 5_456 1_565
O3 O1 Nb 126.1(2) 6 1_565
O3 O1 Nb 115.1(2) 5_455 1_565
O3 O1 Nb 17.8(3) 2_565 1_565
Ga2 O1 Nb 79.4(2) 2_564 1_565
O2 O1 Nb 78.75(16) 3_565 1_565
O2 O1 Nb 164.14(19) . 1_565
O2 O1 Nb 48.8(3) 4_455 1_565
Ga3 O1 Nb 106.13(8) 2_565 1_565
Ga3 O1 Nb 136.36(16) 1_556 1_565
Ga3 O1 Nb 41.81(4) 4_456 1_565
O3 O1 Nb 123.6(3) . 1_565
O3 O1 Nb 95.28(19) 4_455 1_565
O3 O1 Nb 24.72(15) 3_565 1_565
Ga3 O1 Nb 90.82(19) 2_564 1_565
Ga3 O1 Nb 111.0(3) . 1_565
Ga3 O1 Nb 39.29(7) 4_455 1_565
Nb O1 Nb 116.72(12) . 1_565
Ga1 O1 Nb 116.72(12) . 1_565
Nb O1 Nb 116.72(12) 1_455 1_565
Ga1 O1 Nb 116.72(12) 1_455 1_565
Ga1 O1 Nb 0.0 1_565 1_565
Ga2 O1 O2 81.6(3) 2_565 4_445
La O1 O2 29.1(2) . 4_445
La O1 O2 114.84(14) 2_565 4_445
La O1 O2 127.13(14) 4_455 4_445
O2 O1 O2 82.8(5) 2_565 4_445
O2 O1 O2 79.8(3) 6 4_445
O2 O1 O2 131.9(4) 5_455 4_445
O2 O1 O2 69.0(3) 2_566 4_445
O2 O1 O2 66.0(5) 6_556 4_445
O2 O1 O2 113.0(4) 5_456 4_445
O3 O1 O2 34.4(3) 6 4_445
O3 O1 O2 84.5(2) 5_455 4_445
O3 O1 O2 150.7(4) 2_565 4_445
Ga2 O1 O2 98.4(3) 2_564 4_445
O2 O1 O2 82.6(3) 3_565 4_445
O2 O1 O2 35.5(3) . 4_445
O2 O1 O2 149.0(5) 4_455 4_445
Ga3 O1 O2 57.36(13) 2_565 4_445
Ga3 O1 O2 61.88(15) 1_556 4_445
Ga3 O1 O2 143.7(4) 4_456 4_445
O3 O1 O2 42.9(3) . 4_445
O3 O1 O2 100.79(19) 4_455 4_445
O3 O1 O2 139.2(3) 3_565 4_445
Ga3 O1 O2 75.17(18) 2_564 4_445
Ga3 O1 O2 78.26(16) . 4_445
Ga3 O1 O2 141.3(4) 4_455 4_445
Nb O1 O2 44.29(14) . 4_445
Ga1 O1 O2 44.29(14) . 4_445
Nb O1 O2 81.63(11) 1_455 4_445
Ga1 O1 O2 81.63(11) 1_455 4_445
Ga1 O1 O2 160.37(12) 1_565 4_445
Nb O1 O2 160.37(12) 1_565 4_445
Ga2 O1 O2 81.6(3) 2_565 1_665
La O1 O2 127.13(14) . 1_665
La O1 O2 29.1(2) 2_565 1_665
La O1 O2 114.84(14) 4_455 1_665
O2 O1 O2 79.8(3) 2_565 1_665
O2 O1 O2 131.9(4) 6 1_665
O2 O1 O2 82.8(5) 5_455 1_665
O2 O1 O2 66.0(5) 2_566 1_665
O2 O1 O2 113.0(4) 6_556 1_665
O2 O1 O2 69.0(3) 5_456 1_665
O3 O1 O2 84.5(2) 6 1_665
O3 O1 O2 150.7(4) 5_455 1_665
O3 O1 O2 34.4(3) 2_565 1_665
Ga2 O1 O2 98.4(3) 2_564 1_665
O2 O1 O2 35.5(3) 3_565 1_665
O2 O1 O2 149.0(5) . 1_665
O2 O1 O2 82.6(3) 4_455 1_665
Ga3 O1 O2 61.88(15) 2_565 1_665
Ga3 O1 O2 143.7(4) 1_556 1_665
Ga3 O1 O2 57.36(13) 4_456 1_665
O3 O1 O2 100.79(19) . 1_665
O3 O1 O2 139.2(3) 4_455 1_665
O3 O1 O2 42.9(3) 3_565 1_665
Ga3 O1 O2 78.26(16) 2_564 1_665
Ga3 O1 O2 141.3(4) . 1_665
Ga3 O1 O2 75.17(18) 4_455 1_665
Nb O1 O2 81.63(11) . 1_665
Ga1 O1 O2 81.63(11) . 1_665
Nb O1 O2 160.37(12) 1_455 1_665
Ga1 O1 O2 160.37(12) 1_455 1_665
Ga1 O1 O2 44.29(14) 1_565 1_665
Nb O1 O2 44.29(14) 1_565 1_665
O2 O1 O2 117.90(13) 4_445 1_665
Ga2 O1 O2 81.6(3) 2_565 3_465
La O1 O2 114.84(14) . 3_465
La O1 O2 127.13(14) 2_565 3_465
La O1 O2 29.1(2) 4_455 3_465
O2 O1 O2 131.9(4) 2_565 3_465
O2 O1 O2 82.8(5) 6 3_465
O2 O1 O2 79.8(3) 5_455 3_465
O2 O1 O2 113.0(4) 2_566 3_465
O2 O1 O2 69.0(3) 6_556 3_465
O2 O1 O2 66.0(5) 5_456 3_465
O3 O1 O2 150.7(4) 6 3_465
O3 O1 O2 34.4(3) 5_455 3_465
O3 O1 O2 84.5(2) 2_565 3_465
Ga2 O1 O2 98.4(3) 2_564 3_465
O2 O1 O2 149.0(5) 3_565 3_465
O2 O1 O2 82.6(3) . 3_465
O2 O1 O2 35.5(3) 4_455 3_465
Ga3 O1 O2 143.7(4) 2_565 3_465
Ga3 O1 O2 57.36(13) 1_556 3_465
Ga3 O1 O2 61.88(15) 4_456 3_465
O3 O1 O2 139.2(3) . 3_465
O3 O1 O2 42.9(3) 4_455 3_465
O3 O1 O2 100.79(19) 3_565 3_465
Ga3 O1 O2 141.3(4) 2_564 3_465
Ga3 O1 O2 75.17(18) . 3_465
Ga3 O1 O2 78.26(16) 4_455 3_465
Nb O1 O2 160.37(12) . 3_465
Ga1 O1 O2 160.37(12) . 3_465
Nb O1 O2 44.29(14) 1_455 3_465
Ga1 O1 O2 44.29(14) 1_455 3_465
Ga1 O1 O2 81.62(11) 1_565 3_465
Nb O1 O2 81.62(11) 1_565 3_465
O2 O1 O2 117.90(12) 4_445 3_465
O2 O1 O2 117.90(12) 1_665 3_465
Ga2 O1 O3 51.8(2) 2_565 1_556
La O1 O3 64.1(2) . 1_556
La O1 O3 103.1(2) 2_565 1_556
La O1 O3 147.4(3) 4_455 1_556
O2 O1 O3 100.7(3) 2_565 1_556
O2 O1 O3 115.6(3) 6 1_556
O2 O1 O3 157.8(4) 5_455 1_556
O2 O1 O3 33.2(3) 2_566 1_556
O2 O1 O3 52.8(3) 6_556 1_556
O2 O1 O3 82.0(4) 5_456 1_556
O3 O1 O3 33.7(4) 6 1_556
O3 O1 O3 99.7(3) 5_455 1_556
O3 O1 O3 117.3(4) 2_565 1_556
Ga2 O1 O3 128.2(2) 2_564 1_556
O2 O1 O3 61.0(2) 3_565 1_556
O2 O1 O3 58.2(3) . 1_556
O2 O1 O3 130.5(5) 4_455 1_556
Ga3 O1 O3 31.06(15) 2_565 1_556
Ga3 O1 O3 69.5(2) 1_556 1_556
Ga3 O1 O3 110.1(4) 4_456 1_556
O3 O1 O3 66.83(19) . 1_556
O3 O1 O3 129.90(12) 4_455 1_556
O3 O1 O3 129.90(12) 3_565 1_556
Ga3 O1 O3 90.81(13) 2_564 1_556
Ga3 O1 O3 113.81(12) . 1_556
Ga3 O1 O3 159.80(19) 4_455 1_556
Nb O1 O3 51.52(13) . 1_556
Ga1 O1 O3 51.52(13) . 1_556
Nb O1 O3 105.92(17) 1_455 1_556
Ga1 O1 O3 105.92(17) 1_455 1_556
Ga1 O1 O3 133.4(2) 1_565 1_556
Nb O1 O3 133.4(2) 1_565 1_556
O2 O1 O3 35.9(2) 4_445 1_556
O2 O1 O3 90.8(2) 1_665 1_556
O2 O1 O3 121.6(3) 3_465 1_556
Ga2 O1 O3 51.8(2) 2_565 3_566
La O1 O3 147.4(3) . 3_566
La O1 O3 64.1(2) 2_565 3_566
La O1 O3 103.1(2) 4_455 3_566
O2 O1 O3 115.6(3) 2_565 3_566
O2 O1 O3 157.7(4) 6 3_566
O2 O1 O3 100.7(3) 5_455 3_566
O2 O1 O3 52.8(3) 2_566 3_566
O2 O1 O3 82.0(4) 6_556 3_566
O2 O1 O3 33.2(3) 5_456 3_566
O3 O1 O3 99.7(3) 6 3_566
O3 O1 O3 117.3(4) 5_455 3_566
O3 O1 O3 33.7(4) 2_565 3_566
Ga2 O1 O3 128.2(2) 2_564 3_566
O2 O1 O3 58.2(3) 3_565 3_566
O2 O1 O3 130.5(5) . 3_566
O2 O1 O3 61.0(2) 4_455 3_566
Ga3 O1 O3 69.5(2) 2_565 3_566
Ga3 O1 O3 110.1(4) 1_556 3_566
Ga3 O1 O3 31.06(15) 4_456 3_566
O3 O1 O3 129.90(12) . 3_566
O3 O1 O3 129.90(12) 4_455 3_566
O3 O1 O3 66.83(19) 3_565 3_566
Ga3 O1 O3 113.81(12) 2_564 3_566
Ga3 O1 O3 159.80(19) . 3_566
Ga3 O1 O3 90.81(13) 4_455 3_566
Nb O1 O3 105.92(17) . 3_566
Ga1 O1 O3 105.92(17) . 3_566
Nb O1 O3 133.4(2) 1_455 3_566
Ga1 O1 O3 133.4(2) 1_455 3_566
Ga1 O1 O3 51.52(14) 1_565 3_566
Nb O1 O3 51.52(14) 1_565 3_566
O2 O1 O3 121.6(3) 4_445 3_566
O2 O1 O3 35.9(2) 1_665 3_566
O2 O1 O3 90.8(2) 3_465 3_566
O3 O1 O3 85.8(3) 1_556 3_566
Ga2 O1 O3 51.8(2) 2_565 4_456
La O1 O3 103.1(2) . 4_456
La O1 O3 147.4(3) 2_565 4_456
La O1 O3 64.1(2) 4_455 4_456
O2 O1 O3 157.8(4) 2_565 4_456
O2 O1 O3 100.7(3) 6 4_456
O2 O1 O3 115.6(3) 5_455 4_456
O2 O1 O3 82.0(4) 2_566 4_456
O2 O1 O3 33.2(3) 6_556 4_456
O2 O1 O3 52.8(3) 5_456 4_456
O3 O1 O3 117.3(4) 6 4_456
O3 O1 O3 33.7(4) 5_455 4_456
O3 O1 O3 99.7(3) 2_565 4_456
Ga2 O1 O3 128.2(2) 2_564 4_456
O2 O1 O3 130.5(5) 3_565 4_456
O2 O1 O3 61.0(2) . 4_456
O2 O1 O3 58.2(3) 4_455 4_456
Ga3 O1 O3 110.1(4) 2_565 4_456
Ga3 O1 O3 31.06(15) 1_556 4_456
Ga3 O1 O3 69.5(2) 4_456 4_456
O3 O1 O3 129.90(12) . 4_456
O3 O1 O3 66.83(19) 4_455 4_456
O3 O1 O3 129.90(12) 3_565 4_456
Ga3 O1 O3 159.80(19) 2_564 4_456
Ga3 O1 O3 90.81(13) . 4_456
Ga3 O1 O3 113.81(12) 4_455 4_456
Nb O1 O3 133.4(2) . 4_456
Ga1 O1 O3 133.4(2) . 4_456
Nb O1 O3 51.52(14) 1_455 4_456
Ga1 O1 O3 51.52(14) 1_455 4_456
Ga1 O1 O3 105.92(17) 1_565 4_456
Nb O1 O3 105.92(17) 1_565 4_456
O2 O1 O3 90.8(2) 4_445 4_456
O2 O1 O3 121.6(3) 1_665 4_456
O2 O1 O3 35.9(2) 3_465 4_456
O3 O1 O3 85.8(3) 1_556 4_456
O3 O1 O3 85.8(3) 3_566 4_456
Ga2 O1 La 29.60(10) 2_565 1_556
La O1 La 80.3(3) . 1_556
La O1 La 121.9(3) 2_565 1_556
La O1 La 121.9(3) 4_455 1_556
O2 O1 La 129.0(3) 2_565 1_556
O2 O1 La 123.4(2) 6 1_556
O2 O1 La 173.6(3) 5_455 1_556
O2 O1 La 33.8(4) 2_566 1_556
O2 O1 La 25.0(3) 6_556 1_556
O2 O1 La 60.8(3) 5_456 1_556
O3 O1 La 62.2(3) 6 1_556
O3 O1 La 79.0(3) 5_455 1_556
O3 O1 La 111.6(5) 2_565 1_556
Ga2 O1 La 150.40(10) 2_564 1_556
O2 O1 La 80.5(3) 3_565 1_556
O2 O1 La 53.7(3) . 1_556
O2 O1 La 104.3(4) 4_455 1_556
Ga3 O1 La 53.34(18) 2_565 1_556
Ga3 O1 La 49.49(17) 1_556 1_556
Ga3 O1 La 91.7(3) 4_456 1_556
O3 O1 La 92.2(3) . 1_556
O3 O1 La 115.2(2) 4_455 1_556
O3 O1 La 142.0(3) 3_565 1_556
Ga3 O1 La 119.25(5) 2_564 1_556
Ga3 O1 La 116.63(5) . 1_556
Ga3 O1 La 166.4(2) 4_455 1_556
Nb O1 La 80.01(12) . 1_556
Ga1 O1 La 80.01(12) . 1_556
Nb O1 La 91.10(14) 1_455 1_556
Ga1 O1 La 91.10(14) 1_455 1_556
Ga1 O1 La 129.2(3) 1_565 1_556
Nb O1 La 129.2(3) 1_565 1_556
O2 O1 La 52.2(2) 4_445 1_556
O2 O1 La 99.4(3) 1_665 1_556
O2 O1 La 93.9(3) 3_465 1_556
O3 O1 La 28.65(15) 1_556 1_556
O3 O1 La 78.2(3) 3_566 1_556
O3 O1 La 58.1(2) 4_456 1_556
Ga2 O1 La 29.60(10) 2_565 2_566
La O1 La 121.9(3) . 2_566
La O1 La 80.3(3) 2_565 2_566
La O1 La 121.9(3) 4_455 2_566
O2 O1 La 123.4(2) 2_565 2_566
O2 O1 La 173.6(3) 6 2_566
O2 O1 La 129.0(3) 5_455 2_566
O2 O1 La 25.0(3) 2_566 2_566
O2 O1 La 60.8(3) 6_556 2_566
O2 O1 La 33.8(4) 5_456 2_566
O3 O1 La 79.0(3) 6 2_566
O3 O1 La 111.6(5) 5_455 2_566
O3 O1 La 62.2(3) 2_565 2_566
Ga2 O1 La 150.40(10) 2_564 2_566
O2 O1 La 53.7(3) 3_565 2_566
O2 O1 La 104.3(4) . 2_566
O2 O1 La 80.5(3) 4_455 2_566
Ga3 O1 La 49.49(17) 2_565 2_566
Ga3 O1 La 91.7(3) 1_556 2_566
Ga3 O1 La 53.34(18) 4_456 2_566
O3 O1 La 115.2(2) . 2_566
O3 O1 La 142.0(4) 4_455 2_566
O3 O1 La 92.2(3) 3_565 2_566
Ga3 O1 La 116.63(5) 2_564 2_566
Ga3 O1 La 166.4(2) . 2_566
Ga3 O1 La 119.25(5) 4_455 2_566
Nb O1 La 91.10(14) . 2_566
Ga1 O1 La 91.10(14) . 2_566
Nb O1 La 129.2(3) 1_455 2_566
Ga1 O1 La 129.2(3) 1_455 2_566
Ga1 O1 La 80.01(12) 1_565 2_566
Nb O1 La 80.01(12) 1_565 2_566
O2 O1 La 93.9(3) 4_445 2_566
O2 O1 La 52.2(2) 1_665 2_566
O2 O1 La 99.4(3) 3_465 2_566
O3 O1 La 58.1(2) 1_556 2_566
O3 O1 La 28.65(15) 3_566 2_566
O3 O1 La 78.2(3) 4_456 2_566
La O1 La 50.65(16) 1_556 2_566
Ga2 O1 La 29.60(10) 2_565 4_456
La O1 La 121.9(3) . 4_456
La O1 La 121.9(3) 2_565 4_456
La O1 La 80.3(3) 4_455 4_456
O2 O1 La 173.6(3) 2_565 4_456
O2 O1 La 129.0(3) 6 4_456
O2 O1 La 123.4(2) 5_455 4_456
O2 O1 La 60.8(3) 2_566 4_456
O2 O1 La 33.8(4) 6_556 4_456
O2 O1 La 25.0(3) 5_456 4_456
O3 O1 La 111.6(5) 6 4_456
O3 O1 La 62.2(3) 5_455 4_456
O3 O1 La 79.0(3) 2_565 4_456
Ga2 O1 La 150.40(10) 2_564 4_456
O2 O1 La 104.3(4) 3_565 4_456
O2 O1 La 80.5(3) . 4_456
O2 O1 La 53.7(3) 4_455 4_456
Ga3 O1 La 91.7(3) 2_565 4_456
Ga3 O1 La 53.34(18) 1_556 4_456
Ga3 O1 La 49.49(17) 4_456 4_456
O3 O1 La 142.0(4) . 4_456
O3 O1 La 92.2(3) 4_455 4_456
O3 O1 La 115.2(2) 3_565 4_456
Ga3 O1 La 166.4(2) 2_564 4_456
Ga3 O1 La 119.25(5) . 4_456
Ga3 O1 La 116.63(5) 4_455 4_456
Nb O1 La 129.2(3) . 4_456
Ga1 O1 La 129.2(3) . 4_456
Nb O1 La 80.01(12) 1_455 4_456
Ga1 O1 La 80.01(12) 1_455 4_456
Ga1 O1 La 91.10(14) 1_565 4_456
Nb O1 La 91.10(14) 1_565 4_456
O2 O1 La 99.4(3) 4_445 4_456
O2 O1 La 93.9(3) 1_665 4_456
O2 O1 La 52.2(2) 3_465 4_456
O3 O1 La 78.2(3) 1_556 4_456
O3 O1 La 58.1(2) 3_566 4_456
O3 O1 La 28.65(15) 4_456 4_456
La O1 La 50.65(16) 1_556 4_456
La O1 La 50.65(16) 2_566 4_456
Ga2 O1 O3 115.3(2) 2_565 4
La O1 O3 60.91(18) . 4
La O1 O3 49.48(16) 2_565 4
La O1 O3 134.3(6) 4_455 4
O2 O1 O3 31.2(3) 2_565 4
O2 O1 O3 82.5(5) 6 4
O2 O1 O3 85.3(4) 5_455 4
O2 O1 O3 83.9(2) 2_566 4
O2 O1 O3 125.2(4) 6_556 4
O2 O1 O3 128.6(4) 5_456 4
O3 O1 O3 40.0(4) 6 4
O3 O1 O3 141.7(3) 5_455 4
O3 O1 O3 97.0(2) 2_565 4
Ga2 O1 O3 64.7(2) 2_564 4
O2 O1 O3 43.6(4) 3_565 4
O2 O1 O3 99.9(2) . 4
O2 O1 O3 143.4(3) 4_455 4
Ga3 O1 O3 53.13(15) 2_565 4
Ga3 O1 O3 128.89(11) 1_556 4
Ga3 O1 O3 124.73(11) 4_456 4
O3 O1 O3 33.5(2) . 4
O3 O1 O3 121.9(5) 4_455 4
O3 O1 O3 72.0(3) 3_565 4
Ga3 O1 O3 21.83(15) 2_564 4
Ga3 O1 O3 91.0(3) . 4
Ga3 O1 O3 88.4(3) 4_455 4
Nb O1 O3 23.73(12) . 4
Ga1 O1 O3 23.73(12) . 4
Nb O1 O3 126.8(3) 1_455 4
Ga1 O1 O3 126.8(3) 1_455 4
Ga1 O1 O3 94.70(17) 1_565 4
Nb O1 O3 94.70(17) 1_565 4
O2 O1 O3 67.24(18) 4_445 4
O2 O1 O3 67.52(16) 1_665 4
O2 O1 O3 163.1(4) 3_465 4
O3 O1 O3 72.58(13) 1_556 4
O3 O1 O3 99.8(2) 3_566 4
O3 O1 O3 157.1(3) 4_456 4
La O1 O3 101.10(18) 1_556 4
La O1 O3 96.12(17) 2_566 4
La O1 O3 144.6(3) 4_456 4
Ga2 O1 O3 115.3(2) 2_565 3_455
La O1 O3 49.48(16) . 3_455
La O1 O3 134.3(6) 2_565 3_455
La O1 O3 60.91(18) 4_455 3_455
O2 O1 O3 85.3(4) 2_565 3_455
O2 O1 O3 31.2(3) 6 3_455
O2 O1 O3 82.5(5) 5_455 3_455
O2 O1 O3 128.6(4) 2_566 3_455
O2 O1 O3 83.9(2) 6_556 3_455
O2 O1 O3 125.2(4) 5_456 3_455
O3 O1 O3 97.0(2) 6 3_455
O3 O1 O3 40.0(4) 5_455 3_455
O3 O1 O3 141.7(3) 2_565 3_455
Ga2 O1 O3 64.7(2) 2_564 3_455
O2 O1 O3 143.4(3) 3_565 3_455
O2 O1 O3 43.6(4) . 3_455
O2 O1 O3 99.9(2) 4_455 3_455
Ga3 O1 O3 124.73(11) 2_565 3_455
Ga3 O1 O3 53.13(15) 1_556 3_455
Ga3 O1 O3 128.89(11) 4_456 3_455
O3 O1 O3 72.0(3) . 3_455
O3 O1 O3 33.5(2) 4_455 3_455
O3 O1 O3 121.9(5) 3_565 3_455
Ga3 O1 O3 88.4(3) 2_564 3_455
Ga3 O1 O3 21.83(15) . 3_455
Ga3 O1 O3 91.0(3) 4_455 3_455
Nb O1 O3 94.70(17) . 3_455
Ga1 O1 O3 94.70(17) . 3_455
Nb O1 O3 23.73(12) 1_455 3_455
Ga1 O1 O3 23.73(12) 1_455 3_455
Ga1 O1 O3 126.8(3) 1_565 3_455
Nb O1 O3 126.8(3) 1_565 3_455
O2 O1 O3 67.52(16) 4_445 3_455
O2 O1 O3 163.1(4) 1_665 3_455
O2 O1 O3 67.24(18) 3_465 3_455
O3 O1 O3 99.8(2) 1_556 3_455
O3 O1 O3 157.1(3) 3_566 3_455
O3 O1 O3 72.58(14) 4_456 3_455
La O1 O3 96.12(17) 1_556 3_455
La O1 O3 144.6(3) 2_566 3_455
La O1 O3 101.10(18) 4_456 3_455
O3 O1 O3 103.1(3) 4 3_455
Ga2 O1 O3 115.3(2) 2_565 1_565
La O1 O3 134.4(6) . 1_565
La O1 O3 60.91(18) 2_565 1_565
La O1 O3 49.47(16) 4_455 1_565
O2 O1 O3 82.5(5) 2_565 1_565
O2 O1 O3 85.3(4) 6 1_565
O2 O1 O3 31.2(3) 5_455 1_565
O2 O1 O3 125.2(4) 2_566 1_565
O2 O1 O3 128.6(4) 6_556 1_565
O2 O1 O3 83.9(2) 5_456 1_565
O3 O1 O3 141.7(3) 6 1_565
O3 O1 O3 97.0(2) 5_455 1_565
O3 O1 O3 40.0(4) 2_565 1_565
Ga2 O1 O3 64.7(2) 2_564 1_565
O2 O1 O3 99.9(2) 3_565 1_565
O2 O1 O3 143.4(3) . 1_565
O2 O1 O3 43.6(4) 4_455 1_565
Ga3 O1 O3 128.89(11) 2_565 1_565
Ga3 O1 O3 124.73(11) 1_556 1_565
Ga3 O1 O3 53.13(15) 4_456 1_565
O3 O1 O3 121.9(5) . 1_565
O3 O1 O3 72.0(3) 4_455 1_565
O3 O1 O3 33.5(2) 3_565 1_565
Ga3 O1 O3 91.0(3) 2_564 1_565
Ga3 O1 O3 88.4(3) . 1_565
Ga3 O1 O3 21.83(15) 4_455 1_565
Nb O1 O3 126.8(3) . 1_565
Ga1 O1 O3 126.8(3) . 1_565
Nb O1 O3 94.70(17) 1_455 1_565
Ga1 O1 O3 94.70(17) 1_455 1_565
Ga1 O1 O3 23.73(12) 1_565 1_565
Nb O1 O3 23.73(12) 1_565 1_565
O2 O1 O3 163.1(4) 4_445 1_565
O2 O1 O3 67.24(18) 1_665 1_565
O2 O1 O3 67.52(16) 3_465 1_565
O3 O1 O3 157.1(3) 1_556 1_565
O3 O1 O3 72.58(13) 3_566 1_565
O3 O1 O3 99.80(19) 4_456 1_565
La O1 O3 144.6(3) 1_556 1_565
La O1 O3 101.10(18) 2_566 1_565
La O1 O3 96.12(17) 4_456 1_565
O3 O1 O3 103.1(3) 4 1_565
O3 O1 O3 103.1(3) 3_455 1_565
Ga2 O1 Ga2 71.64(18) 2_565 1_566
La O1 Ga2 135.94(2) . 1_566
La O1 Ga2 111.38(3) 2_565 1_566
La O1 Ga2 40.43(16) 4_455 1_566
O2 O1 Ga2 138.2(5) 2_565 1_566
O2 O1 Ga2 101.4(4) 6 1_566
O2 O1 Ga2 81.0(2) 5_455 1_566
O2 O1 Ga2 100.8(4) 2_566 1_566
O2 O1 Ga2 70.7(4) 6_556 1_566
O2 O1 Ga2 48.4(3) 5_456 1_566
O3 O1 Ga2 154.7(5) 6 1_566
O3 O1 Ga2 54.3(3) 5_455 1_566
O3 O1 Ga2 64.9(2) 2_565 1_566
Ga2 O1 Ga2 108.35(18) 2_564 1_566
O2 O1 Ga2 127.5(4) 3_565 1_566
O2 O1 Ga2 99.3(2) . 1_566
O2 O1 Ga2 17.1(3) 4_455 1_566
Ga3 O1 Ga2 130.9(4) 2_565 1_566
Ga3 O1 Ga2 70.57(12) 1_556 1_566
Ga3 O1 Ga2 40.27(6) 4_456 1_566
O3 O1 Ga2 160.6(2) . 1_566
O3 O1 Ga2 62.1(2) 4_455 1_566
O3 O1 Ga2 88.71(13) 3_565 1_566
Ga3 O1 Ga2 148.0(3) 2_564 1_566
Ga3 O1 Ga2 95.01(9) . 1_566
Ga3 O1 Ga2 75.86(6) 4_455 1_566
Nb O1 Ga2 172.2(4) . 1_566
Ga1 O1 Ga2 172.2(4) . 1_566
Nb O1 Ga2 65.87(2) 1_455 1_566
Ga1 O1 Ga2 65.87(2) 1_455 1_566
Ga1 O1 Ga2 65.87(2) 1_565 1_566
Nb O1 Ga2 65.87(2) 1_565 1_566
O2 O1 Ga2 132.1(2) 4_445 1_566
O2 O1 Ga2 96.92(15) 1_665 1_566
O2 O1 Ga2 21.64(15) 3_465 1_566
O3 O1 Ga2 121.0(4) 1_556 1_566
O3 O1 Ga2 69.50(17) 3_566 1_566
O3 O1 Ga2 41.51(14) 4_456 1_566
La O1 Ga2 92.7(2) 1_556 1_566
La O1 Ga2 82.0(2) 2_566 1_566
La O1 Ga2 43.10(9) 4_456 1_566
O3 O1 Ga2 160.54(17) 4 1_566
O3 O1 Ga2 88.85(11) 3_455 1_566
O3 O1 Ga2 58.73(13) 1_565 1_566
Ga2 O1 Ga2 71.65(18) 2_565 1_556
La O1 Ga2 40.43(16) . 1_556
La O1 Ga2 135.94(2) 2_565 1_556
La O1 Ga2 111.38(4) 4_455 1_556
O2 O1 Ga2 101.4(4) 2_565 1_556
O2 O1 Ga2 81.0(2) 6 1_556
O2 O1 Ga2 138.2(5) 5_455 1_556
O2 O1 Ga2 70.7(4) 2_566 1_556
O2 O1 Ga2 48.4(3) 6_556 1_556
O2 O1 Ga2 100.8(4) 5_456 1_556
O3 O1 Ga2 54.3(3) 6 1_556
O3 O1 Ga2 64.9(2) 5_455 1_556
O3 O1 Ga2 154.7(5) 2_565 1_556
Ga2 O1 Ga2 108.36(18) 2_564 1_556
O2 O1 Ga2 99.3(2) 3_565 1_556
O2 O1 Ga2 17.1(3) . 1_556
O2 O1 Ga2 127.5(4) 4_455 1_556
Ga3 O1 Ga2 70.57(12) 2_565 1_556
Ga3 O1 Ga2 40.27(6) 1_556 1_556
Ga3 O1 Ga2 130.9(4) 4_456 1_556
O3 O1 Ga2 62.1(2) . 1_556
O3 O1 Ga2 88.71(13) 4_455 1_556
O3 O1 Ga2 160.6(2) 3_565 1_556
Ga3 O1 Ga2 95.01(9) 2_564 1_556
Ga3 O1 Ga2 75.86(6) . 1_556
Ga3 O1 Ga2 148.0(3) 4_455 1_556
Nb O1 Ga2 65.87(2) . 1_556
Ga1 O1 Ga2 65.87(2) . 1_556
Nb O1 Ga2 65.87(2) 1_455 1_556
Ga1 O1 Ga2 65.87(2) 1_455 1_556
Ga1 O1 Ga2 172.2(4) 1_565 1_556
Nb O1 Ga2 172.2(4) 1_565 1_556
O2 O1 Ga2 21.64(15) 4_445 1_556
O2 O1 Ga2 132.1(2) 1_665 1_556
O2 O1 Ga2 96.92(15) 3_465 1_556
O3 O1 Ga2 41.51(14) 1_556 1_556
O3 O1 Ga2 121.0(4) 3_566 1_556
O3 O1 Ga2 69.50(17) 4_456 1_556
La O1 Ga2 43.10(9) 1_556 1_556
La O1 Ga2 92.7(2) 2_566 1_556
La O1 Ga2 82.0(2) 4_456 1_556
O3 O1 Ga2 88.85(11) 4 1_556
O3 O1 Ga2 58.73(13) 3_455 1_556
O3 O1 Ga2 160.54(17) 1_565 1_556
Ga2 O1 Ga2 110.56(17) 1_566 1_556
Ga2 O1 Ga2 71.65(18) 2_565 1_666
La O1 Ga2 111.38(4) . 1_666
La O1 Ga2 40.43(16) 2_565 1_666
La O1 Ga2 135.94(2) 4_455 1_666
O2 O1 Ga2 81.0(2) 2_565 1_666
O2 O1 Ga2 138.2(5) 6 1_666
O2 O1 Ga2 101.4(4) 5_455 1_666
O2 O1 Ga2 48.4(3) 2_566 1_666
O2 O1 Ga2 100.8(4) 6_556 1_666
O2 O1 Ga2 70.7(4) 5_456 1_666
O3 O1 Ga2 64.9(2) 6 1_666
O3 O1 Ga2 154.7(5) 5_455 1_666
O3 O1 Ga2 54.3(3) 2_565 1_666
Ga2 O1 Ga2 108.36(18) 2_564 1_666
O2 O1 Ga2 17.1(3) 3_565 1_666
O2 O1 Ga2 127.5(4) . 1_666
O2 O1 Ga2 99.3(2) 4_455 1_666
Ga3 O1 Ga2 40.27(6) 2_565 1_666
Ga3 O1 Ga2 130.9(4) 1_556 1_666
Ga3 O1 Ga2 70.57(12) 4_456 1_666
O3 O1 Ga2 88.71(13) . 1_666
O3 O1 Ga2 160.6(2) 4_455 1_666
O3 O1 Ga2 62.1(2) 3_565 1_666
Ga3 O1 Ga2 75.86(6) 2_564 1_666
Ga3 O1 Ga2 148.0(3) . 1_666
Ga3 O1 Ga2 95.01(9) 4_455 1_666
Nb O1 Ga2 65.87(2) . 1_666
Ga1 O1 Ga2 65.87(2) . 1_666
Nb O1 Ga2 172.2(4) 1_455 1_666
Ga1 O1 Ga2 172.2(4) 1_455 1_666
Ga1 O1 Ga2 65.87(2) 1_565 1_666
Nb O1 Ga2 65.87(2) 1_565 1_666
O2 O1 Ga2 96.92(15) 4_445 1_666
O2 O1 Ga2 21.64(15) 1_665 1_666
O2 O1 Ga2 132.1(2) 3_465 1_666
O3 O1 Ga2 69.50(17) 1_556 1_666
O3 O1 Ga2 41.51(14) 3_566 1_666
O3 O1 Ga2 121.0(4) 4_456 1_666
La O1 Ga2 82.0(2) 1_556 1_666
La O1 Ga2 43.10(9) 2_566 1_666
La O1 Ga2 92.7(2) 4_456 1_666
O3 O1 Ga2 58.73(13) 4 1_666
O3 O1 Ga2 160.54(17) 3_455 1_666
O3 O1 Ga2 88.85(11) 1_565 1_666
Ga2 O1 Ga2 110.56(17) 1_566 1_666
Ga2 O1 Ga2 110.56(17) 1_556 1_666
Ga2 O1 O1 110.4(4) 2_565 2_465
La O1 O1 119.0(4) . 2_465
La O1 O1 97.8(3) 2_565 2_465
La O1 O1 12.44(3) 4_455 2_465
O2 O1 O1 100.7(6) 2_565 2_465
O2 O1 O1 69.2(4) 6 2_465
O2 O1 O1 45.2(3) 5_455 2_465
O2 O1 O1 138.4(5) 2_566 2_465
O2 O1 O1 103.7(4) 6_556 2_465
O2 O1 O1 84.7(4) 5_456 2_465
O3 O1 O1 164.9(6) 6 2_465
O3 O1 O1 59.78(18) 5_455 2_465
O3 O1 O1 69.7(3) 2_565 2_465
Ga2 O1 O1 69.6(4) 2_564 2_465
O2 O1 O1 136.97(19) 3_565 2_465
O2 O1 O1 106.8(2) . 2_465
O2 O1 O1 35.5(2) 4_455 2_465
Ga3 O1 O1 162.7(3) 2_565 2_465
Ga3 O1 O1 88.81(9) 1_556 2_465
Ga3 O1 O1 63.53(10) 4_456 2_465
O3 O1 O1 127.9(6) . 2_465
O3 O1 O1 38.91(18) 4_455 2_465
O3 O1 O1 70.2(3) 3_565 2_465
Ga3 O1 O1 110.8(5) 2_564 2_465
Ga3 O1 O1 66.6(3) . 2_465
Ga3 O1 O1 43.6(2) 4_455 2_465
Nb O1 O1 149.0(6) . 2_465
Ga1 O1 O1 149.0(6) . 2_465
Nb O1 O1 58.36(6) 1_455 2_465
Ga1 O1 O1 58.36(6) 1_455 2_465
Ga1 O1 O1 58.36(6) 1_565 2_465
Nb O1 O1 58.36(6) 1_565 2_465
O2 O1 O1 139.37(18) 4_445 2_465
O2 O1 O1 102.44(13) 1_665 2_465
O2 O1 O1 34.8(2) 3_465 2_465
O3 O1 O1 156.4(4) 1_556 2_465
O3 O1 O1 93.6(2) 3_566 2_465
O3 O1 O1 70.6(2) 4_456 2_465
La O1 O1 128.4(4) 1_556 2_465
La O1 O1 115.9(3) 2_566 2_465
La O1 O1 81.5(3) 4_456 2_465
O3 O1 O1 130.5(5) 4 2_465
O3 O1 O1 72.4(2) 3_455 2_465
O3 O1 O1 37.39(14) 1_565 2_465
Ga2 O1 O1 38.79(18) 1_566 2_465
Ga2 O1 O1 123.686(17) 1_556 2_465
Ga2 O1 O1 123.686(17) 1_666 2_465
Ga2 O1 O1 110.4(4) 2_565 2_455
La O1 O1 12.44(3) . 2_455
La O1 O1 119.0(4) 2_565 2_455
La O1 O1 97.8(3) 4_455 2_455
O2 O1 O1 69.2(4) 2_565 2_455
O2 O1 O1 45.2(3) 6 2_455
O2 O1 O1 100.7(6) 5_455 2_455
O2 O1 O1 103.7(4) 2_566 2_455
O2 O1 O1 84.7(4) 6_556 2_455
O2 O1 O1 138.4(5) 5_456 2_455
O3 O1 O1 59.78(18) 6 2_455
O3 O1 O1 69.7(3) 5_455 2_455
O3 O1 O1 164.9(6) 2_565 2_455
Ga2 O1 O1 69.6(4) 2_564 2_455
O2 O1 O1 106.8(2) 3_565 2_455
O2 O1 O1 35.5(2) . 2_455
O2 O1 O1 136.97(19) 4_455 2_455
Ga3 O1 O1 88.81(9) 2_565 2_455
Ga3 O1 O1 63.53(10) 1_556 2_455
Ga3 O1 O1 162.7(3) 4_456 2_455
O3 O1 O1 38.91(18) . 2_455
O3 O1 O1 70.2(3) 4_455 2_455
O3 O1 O1 127.9(6) 3_565 2_455
Ga3 O1 O1 66.6(3) 2_564 2_455
Ga3 O1 O1 43.6(2) . 2_455
Ga3 O1 O1 110.8(5) 4_455 2_455
Nb O1 O1 58.36(6) . 2_455
Ga1 O1 O1 58.36(6) . 2_455
Nb O1 O1 58.36(6) 1_455 2_455
Ga1 O1 O1 58.36(6) 1_455 2_455
Ga1 O1 O1 149.0(6) 1_565 2_455
Nb O1 O1 149.0(6) 1_565 2_455
O2 O1 O1 34.8(2) 4_445 2_455
O2 O1 O1 139.37(18) 1_665 2_455
O2 O1 O1 102.44(14) 3_465 2_455
O3 O1 O1 70.6(2) 1_556 2_455
O3 O1 O1 156.4(4) 3_566 2_455
O3 O1 O1 93.6(2) 4_456 2_455
La O1 O1 81.5(3) 1_556 2_455
La O1 O1 128.4(4) 2_566 2_455
La O1 O1 115.9(3) 4_456 2_455
O3 O1 O1 72.4(2) 4 2_455
O3 O1 O1 37.39(14) 3_455 2_455
O3 O1 O1 130.5(5) 1_565 2_455
Ga2 O1 O1 123.686(18) 1_566 2_455
Ga2 O1 O1 38.79(18) 1_556 2_455
Ga2 O1 O1 123.685(17) 1_666 2_455
O1 O1 O1 108.5(4) 2_465 2_455
Ga2 O1 O1 110.4(4) 2_565 2_565
La O1 O1 97.8(3) . 2_565
La O1 O1 12.44(3) 2_565 2_565
La O1 O1 119.0(4) 4_455 2_565
O2 O1 O1 45.2(3) 2_565 2_565
O2 O1 O1 100.7(6) 6 2_565
O2 O1 O1 69.2(4) 5_455 2_565
O2 O1 O1 84.7(4) 2_566 2_565
O2 O1 O1 138.4(5) 6_556 2_565
O2 O1 O1 103.7(4) 5_456 2_565
O3 O1 O1 69.7(3) 6 2_565
O3 O1 O1 164.9(6) 5_455 2_565
O3 O1 O1 59.78(18) 2_565 2_565
Ga2 O1 O1 69.6(4) 2_564 2_565
O2 O1 O1 35.5(2) 3_565 2_565
O2 O1 O1 136.97(19) . 2_565
O2 O1 O1 106.8(2) 4_455 2_565
Ga3 O1 O1 63.53(10) 2_565 2_565
Ga3 O1 O1 162.7(3) 1_556 2_565
Ga3 O1 O1 88.81(9) 4_456 2_565
O3 O1 O1 70.2(3) . 2_565
O3 O1 O1 127.9(6) 4_455 2_565
O3 O1 O1 38.91(18) 3_565 2_565
Ga3 O1 O1 43.6(2) 2_564 2_565
Ga3 O1 O1 110.8(5) . 2_565
Ga3 O1 O1 66.6(3) 4_455 2_565
Nb O1 O1 58.36(6) . 2_565
Ga1 O1 O1 58.36(6) . 2_565
Nb O1 O1 149.0(6) 1_455 2_565
Ga1 O1 O1 149.0(6) 1_455 2_565
Ga1 O1 O1 58.36(6) 1_565 2_565
Nb O1 O1 58.36(6) 1_565 2_565
O2 O1 O1 102.44(13) 4_445 2_565
O2 O1 O1 34.8(2) 1_665 2_565
O2 O1 O1 139.37(18) 3_465 2_565
O3 O1 O1 93.6(2) 1_556 2_565
O3 O1 O1 70.6(2) 3_566 2_565
O3 O1 O1 156.4(4) 4_456 2_565
La O1 O1 115.9(3) 1_556 2_565
La O1 O1 81.5(3) 2_566 2_565
La O1 O1 128.4(4) 4_456 2_565
O3 O1 O1 37.39(14) 4 2_565
O3 O1 O1 130.5(5) 3_455 2_565
O3 O1 O1 72.4(2) 1_565 2_565
Ga2 O1 O1 123.686(17) 1_566 2_565
Ga2 O1 O1 123.685(17) 1_556 2_565
Ga2 O1 O1 38.79(18) 1_666 2_565
O1 O1 O1 108.5(4) 2_465 2_565
O1 O1 O1 108.5(4) 2_455 2_565
Ga2 O1 O1 180.0 2_565 1_554
La O1 O1 70.1(4) . 1_554
La O1 O1 70.1(4) 2_565 1_554
La O1 O1 70.1(4) 4_455 1_554
O2 O1 O1 33.6(3) 2_565 1_554
O2 O1 O1 33.6(3) 6 1_554
O2 O1 O1 33.6(3) 5_455 1_554
O2 O1 O1 148.6(3) 2_566 1_554
O2 O1 O1 148.6(3) 6_556 1_554
O2 O1 O1 148.6(3) 5_456 1_554
O3 O1 O1 96.4(4) 6 1_554
O3 O1 O1 96.4(4) 5_455 1_554
O3 O1 O1 96.4(4) 2_565 1_554
Ga2 O1 O1 0.0 2_564 1_554
O2 O1 O1 101.3(4) 3_565 1_554
O2 O1 O1 101.3(4) . 1_554
O2 O1 O1 101.3(4) 4_455 1_554
Ga3 O1 O1 117.8(2) 2_565 1_554
Ga3 O1 O1 117.8(2) 1_556 1_554
Ga3 O1 O1 117.8(2) 4_456 1_554
O3 O1 O1 61.3(3) . 1_554
O3 O1 O1 61.3(3) 4_455 1_554
O3 O1 O1 61.3(3) 3_565 1_554
Ga3 O1 O1 42.96(14) 2_564 1_554
Ga3 O1 O1 42.96(14) . 1_554
Ga3 O1 O1 42.96(14) 4_455 1_554
Nb O1 O1 79.4(2) . 1_554
Ga1 O1 O1 79.4(2) . 1_554
Nb O1 O1 79.4(2) 1_455 1_554
Ga1 O1 O1 79.4(2) 1_455 1_554
Ga1 O1 O1 79.4(2) 1_565 1_554
Nb O1 O1 79.4(2) 1_565 1_554
O2 O1 O1 98.4(3) 4_445 1_554
O2 O1 O1 98.4(3) 1_665 1_554
O2 O1 O1 98.4(3) 3_465 1_554
O3 O1 O1 128.2(2) 1_556 1_554
O3 O1 O1 128.2(2) 3_566 1_554
O3 O1 O1 128.2(2) 4_456 1_554
La O1 O1 150.40(10) 1_556 1_554
La O1 O1 150.40(10) 2_566 1_554
La O1 O1 150.40(10) 4_456 1_554
O3 O1 O1 64.7(2) 4 1_554
O3 O1 O1 64.7(2) 3_455 1_554
O3 O1 O1 64.7(2) 1_565 1_554
Ga2 O1 O1 108.35(18) 1_566 1_554
Ga2 O1 O1 108.36(18) 1_556 1_554
Ga2 O1 O1 108.36(18) 1_666 1_554
O1 O1 O1 69.6(4) 2_465 1_554
O1 O1 O1 69.6(4) 2_455 1_554
O1 O1 O1 69.6(4) 2_565 1_554
Ga2 O1 O1 0.001(1) 2_565 1_556
La O1 O1 109.9(4) . 1_556
La O1 O1 109.9(4) 2_565 1_556
La O1 O1 109.9(4) 4_455 1_556
O2 O1 O1 146.4(3) 2_565 1_556
O2 O1 O1 146.4(3) 6 1_556
O2 O1 O1 146.4(3) 5_455 1_556
O2 O1 O1 31.4(3) 2_566 1_556
O2 O1 O1 31.4(3) 6_556 1_556
O2 O1 O1 31.4(3) 5_456 1_556
O3 O1 O1 83.6(4) 6 1_556
O3 O1 O1 83.6(4) 5_455 1_556
O3 O1 O1 83.6(4) 2_565 1_556
Ga2 O1 O1 180.0 2_564 1_556
O2 O1 O1 78.7(4) 3_565 1_556
O2 O1 O1 78.7(4) . 1_556
O2 O1 O1 78.7(4) 4_455 1_556
Ga3 O1 O1 62.2(2) 2_565 1_556
Ga3 O1 O1 62.2(2) 1_556 1_556
Ga3 O1 O1 62.2(2) 4_456 1_556
O3 O1 O1 118.7(3) . 1_556
O3 O1 O1 118.7(3) 4_455 1_556
O3 O1 O1 118.7(3) 3_565 1_556
Ga3 O1 O1 137.04(14) 2_564 1_556
Ga3 O1 O1 137.04(14) . 1_556
Ga3 O1 O1 137.04(14) 4_455 1_556
Nb O1 O1 100.6(2) . 1_556
Ga1 O1 O1 100.6(2) . 1_556
Nb O1 O1 100.6(2) 1_455 1_556
Ga1 O1 O1 100.6(2) 1_455 1_556
Ga1 O1 O1 100.6(2) 1_565 1_556
Nb O1 O1 100.6(2) 1_565 1_556
O2 O1 O1 81.6(3) 4_445 1_556
O2 O1 O1 81.6(3) 1_665 1_556
O2 O1 O1 81.6(3) 3_465 1_556
O3 O1 O1 51.8(2) 1_556 1_556
O3 O1 O1 51.8(2) 3_566 1_556
O3 O1 O1 51.8(2) 4_456 1_556
La O1 O1 29.60(10) 1_556 1_556
La O1 O1 29.60(10) 2_566 1_556
La O1 O1 29.60(10) 4_456 1_556
O3 O1 O1 115.3(2) 4 1_556
O3 O1 O1 115.3(2) 3_455 1_556
O3 O1 O1 115.3(2) 1_565 1_556
Ga2 O1 O1 71.64(18) 1_566 1_556
Ga2 O1 O1 71.65(18) 1_556 1_556
Ga2 O1 O1 71.64(18) 1_666 1_556
O1 O1 O1 110.4(4) 2_465 1_556
O1 O1 O1 110.4(4) 2_455 1_556
O1 O1 O1 110.4(4) 2_565 1_556
O1 O1 O1 179.999(2) 1_554 1_556
Ga2 O1 Ga3 71.59(17) 2_565 4_446
La O1 Ga3 45.41(15) . 4_446
La O1 Ga3 100.87(5) 2_565 4_446
La O1 Ga3 146.77(3) 4_455 4_446
O2 O1 Ga3 83.8(3) 2_565 4_446
O2 O1 Ga3 97.4(3) 6 4_446
O2 O1 Ga3 140.3(4) 5_455 4_446
O2 O1 Ga3 51.7(2) 2_566 4_446
O2 O1 Ga3 66.6(3) 6_556 4_446
O2 O1 Ga3 102.0(4) 5_456 4_446
O3 O1 Ga3 20.0(3) 6 4_446
O3 O1 Ga3 100.8(2) 5_455 4_446
O3 O1 Ga3 130.4(3) 2_565 4_446
Ga2 O1 Ga3 108.42(17) 2_564 4_446
O2 O1 Ga3 63.71(17) 3_565 4_446
O2 O1 Ga3 52.7(2) . 4_446
O2 O1 Ga3 149.7(5) 4_455 4_446
Ga3 O1 Ga3 37.07(6) 2_565 4_446
Ga3 O1 Ga3 73.67(13) 1_556 4_446
Ga3 O1 Ga3 129.6(4) 4_456 4_446
O3 O1 Ga3 47.3(2) . 4_446
O3 O1 Ga3 121.10(14) 4_455 4_446
O3 O1 Ga3 128.10(15) 3_565 4_446
Ga3 O1 Ga3 74.33(5) 2_564 4_446
Ga3 O1 Ga3 97.36(8) . 4_446
Ga3 O1 Ga3 146.7(3) 4_455 4_446
Nb O1 Ga3 36.18(3) . 4_446
Ga1 O1 Ga3 36.18(3) . 4_446
Nb O1 Ga3 100.85(4) 1_455 4_446
Ga1 O1 Ga3 100.85(4) 1_455 4_446
Ga1 O1 Ga3 142.42(8) 1_565 4_446
Nb O1 Ga3 142.42(8) 1_565 4_446
O2 O1 Ga3 20.35(12) 4_445 4_446
O2 O1 Ga3 98.33(17) 1_665 4_446
O2 O1 Ga3 130.8(2) 3_465 4_446
O3 O1 Ga3 20.05(13) 1_556 4_446
O3 O1 Ga3 102.8(3) 3_566 4_446
O3 O1 Ga3 97.6(2) 4_456 4_446
La O1 Ga3 45.57(8) 1_556 4_446
La O1 Ga3 76.57(17) 2_566 4_446
La O1 Ga3 96.2(2) 4_456 4_446
O3 O1 Ga3 59.56(12) 4 4_446
O3 O1 Ga3 87.87(11) 3_455 4_446
O3 O1 Ga3 161.60(17) 1_565 4_446
Ga2 O1 Ga3 137.4(3) 1_566 4_446
Ga2 O1 Ga3 36.03(4) 1_556 4_446
Ga2 O1 Ga3 76.97(9) 1_666 4_446
O1 O1 Ga3 159.21(4) 2_465 4_446
O1 O1 Ga3 53.84(13) 2_455 4_446
O1 O1 Ga3 89.20(6) 2_565 4_446
O1 O1 Ga3 108.42(17) 1_554 4_446
O1 O1 Ga3 71.58(17) 1_556 4_446
Ga2 O1 Ga3 71.58(17) 2_565 1_666
La O1 Ga3 146.77(3) . 1_666
La O1 Ga3 45.41(15) 2_565 1_666
La O1 Ga3 100.87(5) 4_455 1_666
O2 O1 Ga3 97.4(3) 2_565 1_666
O2 O1 Ga3 140.3(4) 6 1_666
O2 O1 Ga3 83.8(3) 5_455 1_666
O2 O1 Ga3 66.6(3) 2_566 1_666
O2 O1 Ga3 102.0(4) 6_556 1_666
O2 O1 Ga3 51.7(2) 5_456 1_666
O3 O1 Ga3 100.8(2) 6 1_666
O3 O1 Ga3 130.4(3) 5_455 1_666
O3 O1 Ga3 20.0(3) 2_565 1_666
Ga2 O1 Ga3 108.42(17) 2_564 1_666
O2 O1 Ga3 52.7(2) 3_565 1_666
O2 O1 Ga3 149.7(5) . 1_666
O2 O1 Ga3 63.71(18) 4_455 1_666
Ga3 O1 Ga3 73.67(13) 2_565 1_666
Ga3 O1 Ga3 129.6(4) 1_556 1_666
Ga3 O1 Ga3 37.06(6) 4_456 1_666
O3 O1 Ga3 121.10(14) . 1_666
O3 O1 Ga3 128.10(15) 4_455 1_666
O3 O1 Ga3 47.3(2) 3_565 1_666
Ga3 O1 Ga3 97.36(8) 2_564 1_666
Ga3 O1 Ga3 146.7(3) . 1_666
Ga3 O1 Ga3 74.33(5) 4_455 1_666
Nb O1 Ga3 100.85(4) . 1_666
Ga1 O1 Ga3 100.85(4) . 1_666
Nb O1 Ga3 142.42(8) 1_455 1_666
Ga1 O1 Ga3 142.42(8) 1_455 1_666
Ga1 O1 Ga3 36.18(3) 1_565 1_666
Nb O1 Ga3 36.18(3) 1_565 1_666
O2 O1 Ga3 130.8(2) 4_445 1_666
O2 O1 Ga3 20.35(12) 1_665 1_666
O2 O1 Ga3 98.33(17) 3_465 1_666
O3 O1 Ga3 97.6(2) 1_556 1_666
O3 O1 Ga3 20.05(13) 3_566 1_666
O3 O1 Ga3 102.8(3) 4_456 1_666
La O1 Ga3 96.2(2) 1_556 1_666
La O1 Ga3 45.56(8) 2_566 1_666
La O1 Ga3 76.57(17) 4_456 1_666
O3 O1 Ga3 87.87(11) 4 1_666
O3 O1 Ga3 161.60(17) 3_455 1_666
O3 O1 Ga3 59.56(12) 1_565 1_666
Ga2 O1 Ga3 76.97(9) 1_566 1_666
Ga2 O1 Ga3 137.4(3) 1_556 1_666
Ga2 O1 Ga3 36.03(4) 1_666 1_666
O1 O1 Ga3 89.20(6) 2_465 1_666
O1 O1 Ga3 159.21(4) 2_455 1_666
O1 O1 Ga3 53.85(13) 2_565 1_666
O1 O1 Ga3 108.42(17) 1_554 1_666
O1 O1 Ga3 71.58(17) 1_556 1_666
Ga3 O1 Ga3 110.51(16) 4_446 1_666
Ga2 O1 Ga3 71.58(17) 2_565 2_465
La O1 Ga3 100.87(5) . 2_465
La O1 Ga3 146.77(3) 2_565 2_465
La O1 Ga3 45.41(15) 4_455 2_465
O2 O1 Ga3 140.3(4) 2_565 2_465
O2 O1 Ga3 83.8(3) 6 2_465
O2 O1 Ga3 97.4(3) 5_455 2_465
O2 O1 Ga3 102.0(4) 2_566 2_465
O2 O1 Ga3 51.7(2) 6_556 2_465
O2 O1 Ga3 66.6(3) 5_456 2_465
O3 O1 Ga3 130.4(3) 6 2_465
O3 O1 Ga3 20.0(3) 5_455 2_465
O3 O1 Ga3 100.8(2) 2_565 2_465
Ga2 O1 Ga3 108.42(17) 2_564 2_465
O2 O1 Ga3 149.7(5) 3_565 2_465
O2 O1 Ga3 63.71(18) . 2_465
O2 O1 Ga3 52.7(2) 4_455 2_465
Ga3 O1 Ga3 129.6(4) 2_565 2_465
Ga3 O1 Ga3 37.06(6) 1_556 2_465
Ga3 O1 Ga3 73.67(13) 4_456 2_465
O3 O1 Ga3 128.10(15) . 2_465
O3 O1 Ga3 47.3(2) 4_455 2_465
O3 O1 Ga3 121.10(14) 3_565 2_465
Ga3 O1 Ga3 146.7(3) 2_564 2_465
Ga3 O1 Ga3 74.33(5) . 2_465
Ga3 O1 Ga3 97.36(8) 4_455 2_465
Nb O1 Ga3 142.42(8) . 2_465
Ga1 O1 Ga3 142.42(8) . 2_465
Nb O1 Ga3 36.18(3) 1_455 2_465
Ga1 O1 Ga3 36.18(3) 1_455 2_465
Ga1 O1 Ga3 100.85(4) 1_565 2_465
Nb O1 Ga3 100.85(4) 1_565 2_465
O2 O1 Ga3 98.33(17) 4_445 2_465
O2 O1 Ga3 130.8(2) 1_665 2_465
O2 O1 Ga3 20.35(12) 3_465 2_465
O3 O1 Ga3 102.8(3) 1_556 2_465
O3 O1 Ga3 97.6(2) 3_566 2_465
O3 O1 Ga3 20.05(13) 4_456 2_465
La O1 Ga3 76.57(17) 1_556 2_465
La O1 Ga3 96.2(2) 2_566 2_465
La O1 Ga3 45.57(8) 4_456 2_465
O3 O1 Ga3 161.60(17) 4 2_465
O3 O1 Ga3 59.56(12) 3_455 2_465
O3 O1 Ga3 87.87(11) 1_565 2_465
Ga2 O1 Ga3 36.03(4) 1_566 2_465
Ga2 O1 Ga3 76.97(9) 1_556 2_465
Ga2 O1 Ga3 137.4(3) 1_666 2_465
O1 O1 Ga3 53.85(13) 2_465 2_465
O1 O1 Ga3 89.20(6) 2_455 2_465
O1 O1 Ga3 159.21(4) 2_565 2_465
O1 O1 Ga3 108.42(17) 1_554 2_465
O1 O1 Ga3 71.58(17) 1_556 2_465
Ga3 O1 Ga3 110.51(16) 4_446 2_465
Ga3 O1 Ga3 110.51(16) 1_666 2_465
Ga2 O1 O3 86.3(2) 2_565 5
La O1 O3 65.98(13) . 5
La O1 O3 60.94(10) 2_565 5
La O1 O3 163.6(5) 4_455 5
O2 O1 O3 60.4(3) 2_565 5
O2 O1 O3 105.7(4) 6 5
O2 O1 O3 112.7(4) 5_455 5
O2 O1 O3 55.1(3) 2_566 5
O2 O1 O3 98.6(4) 6_556 5
O2 O1 O3 104.9(4) 5_456 5
O3 O1 O3 21.7(3) 6 5
O3 O1 O3 140.4(3) 5_455 5
O3 O1 O3 97.9(3) 2_565 5
Ga2 O1 O3 93.7(2) 2_564 5
O2 O1 O3 28.6(3) 3_565 5
O2 O1 O3 91.4(2) . 5
O2 O1 O3 144.7(3) 4_455 5
Ga3 O1 O3 24.09(18) 2_565 5
Ga3 O1 O3 113.3(2) 1_556 5
Ga3 O1 O3 115.3(2) 4_456 5
O3 O1 O3 46.0(3) . 5
O3 O1 O3 144.9(3) 4_455 5
O3 O1 O3 88.3(2) 3_565 5
Ga3 O1 O3 50.78(17) 2_564 5
Ga3 O1 O3 112.0(2) . 5
Ga3 O1 O3 113.6(2) 4_455 5
Nb O1 O3 21.41(16) . 5
Ga1 O1 O3 21.41(16) . 5
Nb O1 O3 135.87(12) 1_455 5
Ga1 O1 O3 135.87(12) 1_455 5
Ga1 O1 O3 104.41(10) 1_565 5
Nb O1 O3 104.41(10) 1_565 5
O2 O1 O3 56.07(14) 4_445 5
O2 O1 O3 63.52(15) 1_665 5
O2 O1 O3 167.3(4) 3_465 5
O3 O1 O3 46.3(2) 1_556 5
O3 O1 O3 84.6(2) 3_566 5
O3 O1 O3 131.7(3) 4_456 5
La O1 O3 73.62(18) 1_556 5
La O1 O3 71.13(19) 2_566 5
La O1 O3 115.8(3) 4_456 5
O3 O1 O3 29.2(3) 4 5
O3 O1 O3 115.40(15) 3_455 5
O3 O1 O3 121.81(13) 1_565 5
Ga2 O1 O3 152.9(3) 1_566 5
Ga2 O1 O3 75.56(11) 1_556 5
Ga2 O1 O3 45.41(13) 1_666 5
O1 O1 O3 157.1(4) 2_465 5
O1 O1 O3 78.27(13) 2_455 5
O1 O1 O3 49.45(11) 2_565 5
O1 O1 O3 93.7(2) 1_554 5
O1 O1 O3 86.3(2) 1_556 5
Ga3 O1 O3 39.93(10) 4_446 5
Ga3 O1 O3 81.26(13) 1_666 5
Ga3 O1 O3 149.0(3) 2_465 5
Ga2 O1 O3 86.3(2) 2_565 2_455
La O1 O3 60.94(10) . 2_455
La O1 O3 163.6(5) 2_565 2_455
La O1 O3 65.98(13) 4_455 2_455
O2 O1 O3 112.7(4) 2_565 2_455
O2 O1 O3 60.4(3) 6 2_455
O2 O1 O3 105.7(4) 5_455 2_455
O2 O1 O3 104.9(4) 2_566 2_455
O2 O1 O3 55.1(3) 6_556 2_455
O2 O1 O3 98.6(4) 5_456 2_455
O3 O1 O3 97.9(3) 6 2_455
O3 O1 O3 21.7(3) 5_455 2_455
O3 O1 O3 140.4(3) 2_565 2_455
Ga2 O1 O3 93.7(2) 2_564 2_455
O2 O1 O3 144.7(3) 3_565 2_455
O2 O1 O3 28.6(3) . 2_455
O2 O1 O3 91.4(2) 4_455 2_455
Ga3 O1 O3 115.3(2) 2_565 2_455
Ga3 O1 O3 24.09(18) 1_556 2_455
Ga3 O1 O3 113.3(2) 4_456 2_455
O3 O1 O3 88.3(2) . 2_455
O3 O1 O3 46.0(3) 4_455 2_455
O3 O1 O3 144.9(3) 3_565 2_455
Ga3 O1 O3 113.6(2) 2_564 2_455
Ga3 O1 O3 50.78(17) . 2_455
Ga3 O1 O3 112.0(2) 4_455 2_455
Nb O1 O3 104.41(10) . 2_455
Ga1 O1 O3 104.41(10) . 2_455
Nb O1 O3 21.41(16) 1_455 2_455
Ga1 O1 O3 21.41(16) 1_455 2_455
Ga1 O1 O3 135.87(12) 1_565 2_455
Nb O1 O3 135.87(12) 1_565 2_455
O2 O1 O3 63.52(15) 4_445 2_455
O2 O1 O3 167.3(4) 1_665 2_455
O2 O1 O3 56.07(14) 3_465 2_455
O3 O1 O3 84.6(2) 1_556 2_455
O3 O1 O3 131.7(3) 3_566 2_455
O3 O1 O3 46.3(2) 4_456 2_455
La O1 O3 71.14(19) 1_556 2_455
La O1 O3 115.8(3) 2_566 2_455
La O1 O3 73.62(18) 4_456 2_455
O3 O1 O3 121.81(14) 4 2_455
O3 O1 O3 29.2(3) 3_455 2_455
O3 O1 O3 115.40(15) 1_565 2_455
Ga2 O1 O3 75.56(11) 1_566 2_455
Ga2 O1 O3 45.41(13) 1_556 2_455
Ga2 O1 O3 152.9(3) 1_666 2_455
O1 O1 O3 78.27(13) 2_465 2_455
O1 O1 O3 49.45(11) 2_455 2_455
O1 O1 O3 157.1(4) 2_565 2_455
O1 O1 O3 93.7(2) 1_554 2_455
O1 O1 O3 86.3(2) 1_556 2_455
Ga3 O1 O3 81.26(13) 4_446 2_455
Ga3 O1 O3 149.0(3) 1_666 2_455
Ga3 O1 O3 39.93(10) 2_465 2_455
O3 O1 O3 119.58(5) 5 2_455
Ga2 O1 O3 86.3(2) 2_565 6_565
La O1 O3 163.6(5) . 6_565
La O1 O3 65.98(13) 2_565 6_565
La O1 O3 60.94(10) 4_455 6_565
O2 O1 O3 105.7(4) 2_565 6_565
O2 O1 O3 112.7(4) 6 6_565
O2 O1 O3 60.4(3) 5_455 6_565
O2 O1 O3 98.6(4) 2_566 6_565
O2 O1 O3 104.9(4) 6_556 6_565
O2 O1 O3 55.1(3) 5_456 6_565
O3 O1 O3 140.4(3) 6 6_565
O3 O1 O3 97.9(3) 5_455 6_565
O3 O1 O3 21.7(3) 2_565 6_565
Ga2 O1 O3 93.7(2) 2_564 6_565
O2 O1 O3 91.4(2) 3_565 6_565
O2 O1 O3 144.7(3) . 6_565
O2 O1 O3 28.6(3) 4_455 6_565
Ga3 O1 O3 113.3(2) 2_565 6_565
Ga3 O1 O3 115.3(2) 1_556 6_565
Ga3 O1 O3 24.09(18) 4_456 6_565
O3 O1 O3 144.9(3) . 6_565
O3 O1 O3 88.3(2) 4_455 6_565
O3 O1 O3 46.0(3) 3_565 6_565
Ga3 O1 O3 112.0(2) 2_564 6_565
Ga3 O1 O3 113.6(2) . 6_565
Ga3 O1 O3 50.78(17) 4_455 6_565
Nb O1 O3 135.87(12) . 6_565
Ga1 O1 O3 135.87(12) . 6_565
Nb O1 O3 104.41(10) 1_455 6_565
Ga1 O1 O3 104.41(10) 1_455 6_565
Ga1 O1 O3 21.41(16) 1_565 6_565
Nb O1 O3 21.41(16) 1_565 6_565
O2 O1 O3 167.3(4) 4_445 6_565
O2 O1 O3 56.07(14) 1_665 6_565
O2 O1 O3 63.52(15) 3_465 6_565
O3 O1 O3 131.7(3) 1_556 6_565
O3 O1 O3 46.3(2) 3_566 6_565
O3 O1 O3 84.6(2) 4_456 6_565
La O1 O3 115.8(3) 1_556 6_565
La O1 O3 73.62(18) 2_566 6_565
La O1 O3 71.13(19) 4_456 6_565
O3 O1 O3 115.40(15) 4 6_565
O3 O1 O3 121.81(13) 3_455 6_565
O3 O1 O3 29.2(3) 1_565 6_565
Ga2 O1 O3 45.41(13) 1_566 6_565
Ga2 O1 O3 152.9(3) 1_556 6_565
Ga2 O1 O3 75.56(11) 1_666 6_565
O1 O1 O3 49.45(12) 2_465 6_565
O1 O1 O3 157.1(4) 2_455 6_565
O1 O1 O3 78.27(13) 2_565 6_565
O1 O1 O3 93.7(2) 1_554 6_565
O1 O1 O3 86.3(2) 1_556 6_565
Ga3 O1 O3 149.0(3) 4_446 6_565
Ga3 O1 O3 39.93(10) 1_666 6_565
Ga3 O1 O3 81.26(13) 2_465 6_565
O3 O1 O3 119.58(5) 5 6_565
O3 O1 O3 119.58(5) 2_455 6_565
Ga2 O1 O3 55.8(3) 2_565 4_556
La O1 O3 83.10(19) . 4_556
La O1 O3 74.3(2) 2_565 4_556
La O1 O3 164.7(5) 4_455 4_556
O2 O1 O3 90.6(3) 2_565 4_556
O2 O1 O3 132.3(4) 6 4_556
O2 O1 O3 136.0(4) 5_455 4_556
O2 O1 O3 24.5(3) 2_566 4_556
O2 O1 O3 73.4(4) 6_556 4_556
O2 O1 O3 76.0(5) 5_456 4_556
O3 O1 O3 36.3(3) 6 4_556
O3 O1 O3 127.8(4) 5_455 4_556
O3 O1 O3 90.4(3) 2_565 4_556
Ga2 O1 O3 124.2(3) 2_564 4_556
O2 O1 O3 31.8(2) 3_565 4_556
O2 O1 O3 88.4(4) . 4_556
O2 O1 O3 123.3(4) 4_455 4_556
Ga3 O1 O3 6.70(19) 2_565 4_556
Ga3 O1 O3 97.5(3) 1_556 4_556
Ga3 O1 O3 94.4(3) 4_456 4_556
O3 O1 O3 72.20(14) . 4_556
O3 O1 O3 160.1(2) 4_455 4_556
O3 O1 O3 100.0(2) 3_565 4_556
Ga3 O1 O3 81.24(19) 2_564 4_556
Ga3 O1 O3 135.49(17) . 4_556
Ga3 O1 O3 132.24(15) 4_455 4_556
Nb O1 O3 48.45(18) . 4_556
Ga1 O1 O3 48.45(18) . 4_556
Nb O1 O3 136.3(2) 1_455 4_556
Ga1 O1 O3 136.3(2) 1_455 4_556
Ga1 O1 O3 104.44(14) 1_565 4_556
Nb O1 O3 104.44(14) 1_565 4_556
O2 O1 O3 60.43(18) 4_445 4_556
O2 O1 O3 60.70(18) 1_665 4_556
O2 O1 O3 137.4(4) 3_465 4_556
O3 O1 O3 30.4(2) 1_556 4_556
O3 O1 O3 64.4(3) 3_566 4_556
O3 O1 O3 104.7(4) 4_456 4_556
La O1 O3 49.3(2) 1_556 4_556
La O1 O3 43.1(2) 2_566 4_556
La O1 O3 85.3(3) 4_456 4_556
O3 O1 O3 59.46(13) 4 4_556
O3 O1 O3 127.88(7) 3_455 4_556
O3 O1 O3 127.88(7) 1_565 4_556
Ga2 O1 O3 124.3(4) 1_566 4_556
Ga2 O1 O3 71.44(16) 1_556 4_556
Ga2 O1 O3 39.19(11) 1_666 4_556
O1 O1 O3 157.9(4) 2_465 4_556
O1 O1 O3 93.23(19) 2_455 4_556
O1 O1 O3 66.8(2) 2_565 4_556
O1 O1 O3 124.2(3) 1_554 4_556
O1 O1 O3 55.8(3) 1_556 4_556
Ga3 O1 O3 40.13(12) 4_446 4_556
Ga3 O1 O3 70.42(15) 1_666 4_556
Ga3 O1 O3 124.6(4) 2_465 4_556
O3 O1 O3 30.6(4) 5 4_556
O3 O1 O3 114.86(19) 2_455 4_556
O3 O1 O3 109.30(18) 6_565 4_556
Ga2 O1 O3 55.8(3) 2_565 3_456
La O1 O3 74.3(2) . 3_456
La O1 O3 164.7(5) 2_565 3_456
La O1 O3 83.10(19) 4_455 3_456
O2 O1 O3 136.0(4) 2_565 3_456
O2 O1 O3 90.6(3) 6 3_456
O2 O1 O3 132.3(4) 5_455 3_456
O2 O1 O3 76.0(5) 2_566 3_456
O2 O1 O3 24.5(3) 6_556 3_456
O2 O1 O3 73.4(4) 5_456 3_456
O3 O1 O3 90.4(3) 6 3_456
O3 O1 O3 36.3(3) 5_455 3_456
O3 O1 O3 127.8(4) 2_565 3_456
Ga2 O1 O3 124.2(3) 2_564 3_456
O2 O1 O3 123.3(4) 3_565 3_456
O2 O1 O3 31.8(2) . 3_456
O2 O1 O3 88.4(4) 4_455 3_456
Ga3 O1 O3 94.4(3) 2_565 3_456
Ga3 O1 O3 6.70(19) 1_556 3_456
Ga3 O1 O3 97.5(3) 4_456 3_456
O3 O1 O3 100.0(2) . 3_456
O3 O1 O3 72.20(14) 4_455 3_456
O3 O1 O3 160.1(2) 3_565 3_456
Ga3 O1 O3 132.24(15) 2_564 3_456
Ga3 O1 O3 81.24(19) . 3_456
Ga3 O1 O3 135.49(17) 4_455 3_456
Nb O1 O3 104.44(14) . 3_456
Ga1 O1 O3 104.44(14) . 3_456
Nb O1 O3 48.45(18) 1_455 3_456
Ga1 O1 O3 48.45(18) 1_455 3_456
Ga1 O1 O3 136.3(2) 1_565 3_456
Nb O1 O3 136.3(2) 1_565 3_456
O2 O1 O3 60.70(18) 4_445 3_456
O2 O1 O3 137.4(4) 1_665 3_456
O2 O1 O3 60.43(18) 3_465 3_456
O3 O1 O3 64.4(3) 1_556 3_456
O3 O1 O3 104.7(4) 3_566 3_456
O3 O1 O3 30.4(2) 4_456 3_456
La O1 O3 43.1(2) 1_556 3_456
La O1 O3 85.3(3) 2_566 3_456
La O1 O3 49.3(2) 4_456 3_456
O3 O1 O3 127.88(7) 4 3_456
O3 O1 O3 59.46(13) 3_455 3_456
O3 O1 O3 127.88(7) 1_565 3_456
Ga2 O1 O3 71.44(16) 1_566 3_456
Ga2 O1 O3 39.19(11) 1_556 3_456
Ga2 O1 O3 124.3(4) 1_666 3_456
O1 O1 O3 93.23(19) 2_465 3_456
O1 O1 O3 66.8(2) 2_455 3_456
O1 O1 O3 157.9(4) 2_565 3_456
O1 O1 O3 124.2(3) 1_554 3_456
O1 O1 O3 55.8(3) 1_556 3_456
Ga3 O1 O3 70.43(15) 4_446 3_456
Ga3 O1 O3 124.6(4) 1_666 3_456
Ga3 O1 O3 40.13(12) 2_465 3_456
O3 O1 O3 109.30(18) 5 3_456
O3 O1 O3 30.6(4) 2_455 3_456
O3 O1 O3 114.86(19) 6_565 3_456
O3 O1 O3 91.5(4) 4_556 3_456
Ga2 O1 O3 55.8(3) 2_565 1_566
La O1 O3 164.7(5) . 1_566
La O1 O3 83.09(19) 2_565 1_566
La O1 O3 74.3(2) 4_455 1_566
O2 O1 O3 132.3(4) 2_565 1_566
O2 O1 O3 136.0(4) 6 1_566
O2 O1 O3 90.6(3) 5_455 1_566
O2 O1 O3 73.4(4) 2_566 1_566
O2 O1 O3 76.0(5) 6_556 1_566
O2 O1 O3 24.5(3) 5_456 1_566
O3 O1 O3 127.8(4) 6 1_566
O3 O1 O3 90.4(3) 5_455 1_566
O3 O1 O3 36.3(3) 2_565 1_566
Ga2 O1 O3 124.2(3) 2_564 1_566
O2 O1 O3 88.4(4) 3_565 1_566
O2 O1 O3 123.3(4) . 1_566
O2 O1 O3 31.8(2) 4_455 1_566
Ga3 O1 O3 97.5(3) 2_565 1_566
Ga3 O1 O3 94.4(3) 1_556 1_566
Ga3 O1 O3 6.70(19) 4_456 1_566
O3 O1 O3 160.1(2) . 1_566
O3 O1 O3 100.0(2) 4_455 1_566
O3 O1 O3 72.20(14) 3_565 1_566
Ga3 O1 O3 135.49(17) 2_564 1_566
Ga3 O1 O3 132.24(15) . 1_566
Ga3 O1 O3 81.24(19) 4_455 1_566
Nb O1 O3 136.3(2) . 1_566
Ga1 O1 O3 136.3(2) . 1_566
Nb O1 O3 104.44(14) 1_455 1_566
Ga1 O1 O3 104.44(14) 1_455 1_566
Ga1 O1 O3 48.45(18) 1_565 1_566
Nb O1 O3 48.45(18) 1_565 1_566
O2 O1 O3 137.4(4) 4_445 1_566
O2 O1 O3 60.43(18) 1_665 1_566
O2 O1 O3 60.70(18) 3_465 1_566
O3 O1 O3 104.7(4) 1_556 1_566
O3 O1 O3 30.4(2) 3_566 1_566
O3 O1 O3 64.4(3) 4_456 1_566
La O1 O3 85.3(3) 1_556 1_566
La O1 O3 49.3(2) 2_566 1_566
La O1 O3 43.1(2) 4_456 1_566
O3 O1 O3 127.88(7) 4 1_566
O3 O1 O3 127.88(7) 3_455 1_566
O3 O1 O3 59.46(13) 1_565 1_566
Ga2 O1 O3 39.19(11) 1_566 1_566
Ga2 O1 O3 124.3(4) 1_556 1_566
Ga2 O1 O3 71.44(16) 1_666 1_566
O1 O1 O3 66.8(2) 2_465 1_566
O1 O1 O3 157.9(4) 2_455 1_566
O1 O1 O3 93.23(19) 2_565 1_566
O1 O1 O3 124.2(3) 1_554 1_566
O1 O1 O3 55.8(3) 1_556 1_566
Ga3 O1 O3 124.6(4) 4_446 1_566
Ga3 O1 O3 40.13(12) 1_666 1_566
Ga3 O1 O3 70.42(15) 2_465 1_566
O3 O1 O3 114.86(18) 5 1_566
O3 O1 O3 109.30(18) 2_455 1_566
O3 O1 O3 30.6(4) 6_565 1_566
O3 O1 O3 91.5(4) 4_556 1_566
O3 O1 O3 91.5(4) 3_456 1_566
Ga2 O1 O2 141.31(15) 2_565 1_554
La O1 O2 38.9(3) . 1_554
La O1 O2 103.9(4) 2_565 1_554
La O1 O2 74.9(3) 4_455 1_554
O2 O1 O2 53.4(2) 2_565 1_554
O2 O1 O2 13.3(3) 6 1_554
O2 O1 O2 67.5(4) 5_455 1_554
O2 O1 O2 135.8(2) 2_566 1_554
O2 O1 O2 111.2(3) 6_556 1_554
O2 O1 O2 156.8(2) 5_456 1_554
O3 O1 O2 83.1(3) 6 1_554
O3 O1 O2 71.5(4) 5_455 1_554
O3 O1 O2 134.2(5) 2_565 1_554
Ga2 O1 O2 38.69(14) 2_564 1_554
O2 O1 O2 117.4(3) 3_565 1_554
O2 O1 O2 62.6(3) . 1_554
O2 O1 O2 117.4(3) 4_455 1_554
Ga3 O1 O2 113.3(2) 2_565 1_554
Ga3 O1 O2 82.51(18) 1_556 1_554
Ga3 O1 O2 145.7(3) 4_456 1_554
O3 O1 O2 48.4(2) . 1_554
O3 O1 O2 50.7(3) 4_455 1_554
O3 O1 O2 100.0(4) 3_565 1_554
Ga3 O1 O2 56.9(2) 2_564 1_554
Ga3 O1 O2 17.83(14) . 1_554
Ga3 O1 O2 77.6(2) 4_455 1_554
Nb O1 O2 73.13(19) . 1_554
Ga1 O1 O2 73.13(19) . 1_554
Nb O1 O2 54.13(17) 1_455 1_554
Ga1 O1 O2 54.13(17) 1_455 1_554
Ga1 O1 O2 116.6(3) 1_565 1_554
Nb O1 O2 116.6(3) 1_565 1_554
O2 O1 O2 67.26(17) 4_445 1_554
O2 O1 O2 132.7(3) 1_665 1_554
O2 O1 O2 92.9(3) 3_465 1_554
O3 O1 O2 102.89(17) 1_556 1_554
O3 O1 O2 166.8(3) 3_566 1_554
O3 O1 O2 104.49(18) 4_456 1_554
La O1 O2 114.19(11) 1_556 1_554
La O1 O2 160.80(14) 2_566 1_554
La O1 O2 133.00(12) 4_456 1_554
O3 O1 O2 73.9(3) 4 1_554
O3 O1 O2 31.9(2) 3_455 1_554
O3 O1 O2 97.2(3) 1_565 1_554
Ga2 O1 O2 112.83(18) 1_566 1_554
Ga2 O1 O2 71.09(14) 1_556 1_554
Ga2 O1 O2 132.3(2) 1_666 1_554
O1 O1 O2 82.4(3) 2_465 1_554
O1 O1 O2 33.4(3) 2_455 1_554
O1 O1 O2 98.6(4) 2_565 1_554
O1 O1 O2 38.69(14) 1_554 1_554
O1 O1 O2 141.31(15) 1_556 1_554
Ga3 O1 O2 84.23(14) 4_446 1_554
Ga3 O1 O2 146.8(3) 1_666 1_554
Ga3 O1 O2 90.21(15) 2_465 1_554
O3 O1 O2 94.3(2) 5 1_554
O3 O1 O2 59.9(2) 2_455 1_554
O3 O1 O2 125.4(3) 6_565 1_554
O3 O1 O2 119.4(2) 4_556 1_554
O3 O1 O2 88.1(2) 3_456 1_554
O3 O1 O2 149.1(2) 1_566 1_554
Ga2 O1 O2 141.31(15) 2_565 3_564
La O1 O2 74.9(3) . 3_564
La O1 O2 38.9(3) 2_565 3_564
La O1 O2 103.9(4) 4_455 3_564
O2 O1 O2 13.3(3) 2_565 3_564
O2 O1 O2 67.5(4) 6 3_564
O2 O1 O2 53.4(2) 5_455 3_564
O2 O1 O2 111.2(3) 2_566 3_564
O2 O1 O2 156.8(2) 6_556 3_564
O2 O1 O2 135.8(2) 5_456 3_564
O3 O1 O2 71.5(4) 6 3_564
O3 O1 O2 134.2(5) 5_455 3_564
O3 O1 O2 83.1(3) 2_565 3_564
Ga2 O1 O2 38.69(14) 2_564 3_564
O2 O1 O2 62.6(3) 3_565 3_564
O2 O1 O2 117.4(3) . 3_564
O2 O1 O2 117.4(3) 4_455 3_564
Ga3 O1 O2 82.51(18) 2_565 3_564
Ga3 O1 O2 145.7(3) 1_556 3_564
Ga3 O1 O2 113.3(2) 4_456 3_564
O3 O1 O2 50.7(3) . 3_564
O3 O1 O2 100.0(4) 4_455 3_564
O3 O1 O2 48.4(2) 3_565 3_564
Ga3 O1 O2 17.83(14) 2_564 3_564
Ga3 O1 O2 77.6(2) . 3_564
Ga3 O1 O2 56.9(2) 4_455 3_564
Nb O1 O2 54.13(17) . 3_564
Ga1 O1 O2 54.13(17) . 3_564
Nb O1 O2 116.6(3) 1_455 3_564
Ga1 O1 O2 116.6(3) 1_455 3_564
Ga1 O1 O2 73.13(19) 1_565 3_564
Nb O1 O2 73.13(19) 1_565 3_564
O2 O1 O2 92.9(3) 4_445 3_564
O2 O1 O2 67.26(17) 1_665 3_564
O2 O1 O2 132.7(3) 3_465 3_564
O3 O1 O2 104.49(18) 1_556 3_564
O3 O1 O2 102.89(17) 3_566 3_564
O3 O1 O2 166.8(3) 4_456 3_564
La O1 O2 133.01(12) 1_556 3_564
La O1 O2 114.19(11) 2_566 3_564
La O1 O2 160.80(14) 4_456 3_564
O3 O1 O2 31.9(2) 4 3_564
O3 O1 O2 97.2(3) 3_455 3_564
O3 O1 O2 73.9(3) 1_565 3_564
Ga2 O1 O2 132.3(2) 1_566 3_564
Ga2 O1 O2 112.83(18) 1_556 3_564
Ga2 O1 O2 71.09(14) 1_666 3_564
O1 O1 O2 98.6(4) 2_465 3_564
O1 O1 O2 82.4(3) 2_455 3_564
O1 O1 O2 33.4(3) 2_565 3_564
O1 O1 O2 38.69(14) 1_554 3_564
O1 O1 O2 141.31(14) 1_556 3_564
Ga3 O1 O2 90.21(15) 4_446 3_564
Ga3 O1 O2 84.23(14) 1_666 3_564
Ga3 O1 O2 146.8(3) 2_465 3_564
O3 O1 O2 59.9(2) 5 3_564
O3 O1 O2 125.4(3) 2_455 3_564
O3 O1 O2 94.3(2) 6_565 3_564
O3 O1 O2 88.1(2) 4_556 3_564
O3 O1 O2 149.1(2) 3_456 3_564
O3 O1 O2 119.4(2) 1_566 3_564
O2 O1 O2 65.5(2) 1_554 3_564
Ga2 O1 O2 141.31(14) 2_565 4_454
La O1 O2 103.9(4) . 4_454
La O1 O2 74.9(3) 2_565 4_454
La O1 O2 38.9(3) 4_455 4_454
O2 O1 O2 67.5(4) 2_565 4_454
O2 O1 O2 53.4(2) 6 4_454
O2 O1 O2 13.3(3) 5_455 4_454
O2 O1 O2 156.8(2) 2_566 4_454
O2 O1 O2 135.8(2) 6_556 4_454
O2 O1 O2 111.2(3) 5_456 4_454
O3 O1 O2 134.2(5) 6 4_454
O3 O1 O2 83.1(3) 5_455 4_454
O3 O1 O2 71.5(4) 2_565 4_454
Ga2 O1 O2 38.69(14) 2_564 4_454
O2 O1 O2 117.4(3) 3_565 4_454
O2 O1 O2 117.4(3) . 4_454
O2 O1 O2 62.6(3) 4_455 4_454
Ga3 O1 O2 145.7(3) 2_565 4_454
Ga3 O1 O2 113.3(2) 1_556 4_454
Ga3 O1 O2 82.51(18) 4_456 4_454
O3 O1 O2 100.0(4) . 4_454
O3 O1 O2 48.4(2) 4_455 4_454
O3 O1 O2 50.7(3) 3_565 4_454
Ga3 O1 O2 77.6(2) 2_564 4_454
Ga3 O1 O2 56.9(2) . 4_454
Ga3 O1 O2 17.83(14) 4_455 4_454
Nb O1 O2 116.6(3) . 4_454
Ga1 O1 O2 116.6(3) . 4_454
Nb O1 O2 73.13(19) 1_455 4_454
Ga1 O1 O2 73.13(19) 1_455 4_454
Ga1 O1 O2 54.13(17) 1_565 4_454
Nb O1 O2 54.13(17) 1_565 4_454
O2 O1 O2 132.7(3) 4_445 4_454
O2 O1 O2 92.9(3) 1_665 4_454
O2 O1 O2 67.26(17) 3_465 4_454
O3 O1 O2 166.8(3) 1_556 4_454
O3 O1 O2 104.49(18) 3_566 4_454
O3 O1 O2 102.89(17) 4_456 4_454
La O1 O2 160.80(14) 1_556 4_454
La O1 O2 133.00(12) 2_566 4_454
La O1 O2 114.19(10) 4_456 4_454
O3 O1 O2 97.2(3) 4 4_454
O3 O1 O2 73.9(3) 3_455 4_454
O3 O1 O2 31.9(2) 1_565 4_454
Ga2 O1 O2 71.09(14) 1_566 4_454
Ga2 O1 O2 132.3(2) 1_556 4_454
Ga2 O1 O2 112.83(18) 1_666 4_454
O1 O1 O2 33.4(3) 2_465 4_454
O1 O1 O2 98.6(4) 2_455 4_454
O1 O1 O2 82.4(3) 2_565 4_454
O1 O1 O2 38.69(14) 1_554 4_454
O1 O1 O2 141.31(14) 1_556 4_454
Ga3 O1 O2 146.8(3) 4_446 4_454
Ga3 O1 O2 90.21(15) 1_666 4_454
Ga3 O1 O2 84.23(14) 2_465 4_454
O3 O1 O2 125.4(3) 5 4_454
O3 O1 O2 94.3(2) 2_455 4_454
O3 O1 O2 59.9(2) 6_565 4_454
O3 O1 O2 149.1(2) 4_556 4_454
O3 O1 O2 119.4(2) 3_456 4_454
O3 O1 O2 88.1(2) 1_566 4_454
O2 O1 O2 65.5(2) 1_554 4_454
O2 O1 O2 65.5(2) 3_564 4_454
Ga2 O1 O3 146.43(15) 2_565 6_554
La O1 O3 47.5(3) . 6_554
La O1 O3 67.4(3) 2_565 6_554
La O1 O3 102.0(4) 4_455 6_554
O2 O1 O3 15.6(3) 2_565 6_554
O2 O1 O3 46.7(4) 6 6_554
O2 O1 O3 64.3(4) 5_455 6_554
O2 O1 O3 117.2(2) 2_566 6_554
O2 O1 O3 135.9(4) 6_556 6_554
O2 O1 O3 163.1(3) 5_456 6_554
O3 O1 O3 62.8(3) 6 6_554
O3 O1 O3 111.5(4) 5_455 6_554
O3 O1 O3 111.5(4) 2_565 6_554
Ga2 O1 O3 33.57(15) 2_564 6_554
O2 O1 O3 79.1(3) 3_565 6_554
O2 O1 O3 89.0(3) . 6_554
O2 O1 O3 134.1(5) 4_455 6_554
Ga3 O1 O3 86.42(18) 2_565 6_554
Ga3 O1 O3 116.7(2) 1_556 6_554
Ga3 O1 O3 141.1(3) 4_456 6_554
O3 O1 O3 29.1(4) . 6_554
O3 O1 O3 85.8(3) 4_455 6_554
O3 O1 O3 75.3(3) 3_565 6_554
Ga3 O1 O3 16.84(11) 2_564 6_554
Ga3 O1 O3 55.77(19) . 6_554
Ga3 O1 O3 72.0(2) 4_455 6_554
Nb O1 O3 46.09(17) . 6_554
Ga1 O1 O3 46.09(17) . 6_554
Nb O1 O3 94.1(2) 1_455 6_554
Ga1 O1 O3 94.1(2) 1_455 6_554
Ga1 O1 O3 99.4(3) 1_565 6_554
Nb O1 O3 99.4(3) 1_565 6_554
O2 O1 O3 70.8(2) 4_445 6_554
O2 O1 O3 94.5(2) 1_665 6_554
O2 O1 O3 128.0(3) 3_465 6_554
O3 O1 O3 95.2(3) 1_556 6_554
O3 O1 O3 130.3(2) 3_566 6_554
O3 O1 O3 143.9(2) 4_456 6_554
La O1 O3 121.26(15) 1_556 6_554
La O1 O3 132.19(9) 2_566 6_554
La O1 O3 169.41(16) 4_456 6_554
O3 O1 O3 36.1(2) 4 6_554
O3 O1 O3 71.7(3) 3_455 6_554
O3 O1 O3 93.1(3) 1_565 6_554
Ga2 O1 O3 141.7(3) 1_566 6_554
Ga2 O1 O3 87.53(19) 1_556 6_554
Ga2 O1 O3 92.61(14) 1_666 6_554
O1 O1 O3 103.0(5) 2_465 6_554
O1 O1 O3 53.7(3) 2_455 6_554
O1 O1 O3 59.7(3) 2_565 6_554
O1 O1 O3 33.57(15) 1_554 6_554
O1 O1 O3 146.43(15) 1_556 6_554
Ga3 O1 O3 76.11(17) 4_446 6_554
Ga3 O1 O3 112.76(17) 1_666 6_554
Ga3 O1 O3 130.0(2) 2_465 6_554
O3 O1 O3 62.69(15) 5 6_554
O3 O1 O3 97.7(2) 2_455 6_554
O3 O1 O3 119.1(4) 6_565 6_554
O3 O1 O3 93.1(3) 4_556 6_554
O3 O1 O3 120.4(3) 3_456 6_554
O3 O1 O3 147.53(18) 1_566 6_554
O2 O1 O3 40.05(18) 1_554 6_554
O2 O1 O3 28.95(18) 3_564 6_554
O2 O1 O3 71.9(2) 4_454 6_554
Ga2 O1 O3 146.43(16) 2_565 5_454
La O1 O3 67.4(3) . 5_454
La O1 O3 102.0(4) 2_565 5_454
La O1 O3 47.5(3) 4_455 5_454
O2 O1 O3 64.3(4) 2_565 5_454
O2 O1 O3 15.6(3) 6 5_454
O2 O1 O3 46.7(4) 5_455 5_454
O2 O1 O3 163.1(3) 2_566 5_454
O2 O1 O3 117.2(2) 6_556 5_454
O2 O1 O3 135.9(4) 5_456 5_454
O3 O1 O3 111.5(4) 6 5_454
O3 O1 O3 62.8(3) 5_455 5_454
O3 O1 O3 111.5(4) 2_565 5_454
Ga2 O1 O3 33.57(15) 2_564 5_454
O2 O1 O3 134.1(5) 3_565 5_454
O2 O1 O3 79.1(3) . 5_454
O2 O1 O3 89.0(3) 4_455 5_454
Ga3 O1 O3 141.1(3) 2_565 5_454
Ga3 O1 O3 86.42(18) 1_556 5_454
Ga3 O1 O3 116.7(2) 4_456 5_454
O3 O1 O3 75.3(3) . 5_454
O3 O1 O3 29.1(4) 4_455 5_454
O3 O1 O3 85.8(3) 3_565 5_454
Ga3 O1 O3 72.0(2) 2_564 5_454
Ga3 O1 O3 16.84(11) . 5_454
Ga3 O1 O3 55.77(19) 4_455 5_454
Nb O1 O3 99.4(3) . 5_454
Ga1 O1 O3 99.4(3) . 5_454
Nb O1 O3 46.09(17) 1_455 5_454
Ga1 O1 O3 46.09(17) 1_455 5_454
Ga1 O1 O3 94.1(2) 1_565 5_454
Nb O1 O3 94.1(2) 1_565 5_454
O2 O1 O3 94.5(2) 4_445 5_454
O2 O1 O3 128.0(3) 1_665 5_454
O2 O1 O3 70.8(2) 3_465 5_454
O3 O1 O3 130.3(2) 1_556 5_454
O3 O1 O3 143.9(2) 3_566 5_454
O3 O1 O3 95.2(3) 4_456 5_454
La O1 O3 132.19(9) 1_556 5_454
La O1 O3 169.41(16) 2_566 5_454
La O1 O3 121.26(15) 4_456 5_454
O3 O1 O3 93.1(3) 4 5_454
O3 O1 O3 36.1(2) 3_455 5_454
O3 O1 O3 71.7(3) 1_565 5_454
Ga2 O1 O3 87.5(2) 1_566 5_454
Ga2 O1 O3 92.61(14) 1_556 5_454
Ga2 O1 O3 141.7(3) 1_666 5_454
O1 O1 O3 53.7(3) 2_465 5_454
O1 O1 O3 59.7(3) 2_455 5_454
O1 O1 O3 103.0(5) 2_565 5_454
O1 O1 O3 33.57(15) 1_554 5_454
O1 O1 O3 146.43(16) 1_556 5_454
Ga3 O1 O3 112.76(17) 4_446 5_454
Ga3 O1 O3 130.0(2) 1_666 5_454
Ga3 O1 O3 76.11(17) 2_465 5_454
O3 O1 O3 119.1(4) 5 5_454
O3 O1 O3 62.69(15) 2_455 5_454
O3 O1 O3 97.7(2) 6_565 5_454
O3 O1 O3 147.53(18) 4_556 5_454
O3 O1 O3 93.1(3) 3_456 5_454
O3 O1 O3 120.4(3) 1_566 5_454
O2 O1 O3 28.95(18) 1_554 5_454
O2 O1 O3 71.9(2) 3_564 5_454
O2 O1 O3 40.05(18) 4_454 5_454
O3 O1 O3 57.2(3) 6_554 5_454
Ga2 O1 O3 146.43(16) 2_565 2_564
La O1 O3 102.0(4) . 2_564
La O1 O3 47.5(3) 2_565 2_564
La O1 O3 67.4(3) 4_455 2_564
O2 O1 O3 46.7(4) 2_565 2_564
O2 O1 O3 64.3(4) 6 2_564
O2 O1 O3 15.6(3) 5_455 2_564
O2 O1 O3 135.9(4) 2_566 2_564
O2 O1 O3 163.1(3) 6_556 2_564
O2 O1 O3 117.2(2) 5_456 2_564
O3 O1 O3 111.5(4) 6 2_564
O3 O1 O3 111.5(4) 5_455 2_564
O3 O1 O3 62.8(3) 2_565 2_564
Ga2 O1 O3 33.57(15) 2_564 2_564
O2 O1 O3 89.0(3) 3_565 2_564
O2 O1 O3 134.1(5) . 2_564
O2 O1 O3 79.1(3) 4_455 2_564
Ga3 O1 O3 116.7(2) 2_565 2_564
Ga3 O1 O3 141.1(3) 1_556 2_564
Ga3 O1 O3 86.42(18) 4_456 2_564
O3 O1 O3 85.8(3) . 2_564
O3 O1 O3 75.3(3) 4_455 2_564
O3 O1 O3 29.1(4) 3_565 2_564
Ga3 O1 O3 55.77(19) 2_564 2_564
Ga3 O1 O3 72.0(2) . 2_564
Ga3 O1 O3 16.84(11) 4_455 2_564
Nb O1 O3 94.1(2) . 2_564
Ga1 O1 O3 94.1(2) . 2_564
Nb O1 O3 99.4(3) 1_455 2_564
Ga1 O1 O3 99.4(3) 1_455 2_564
Ga1 O1 O3 46.09(17) 1_565 2_564
Nb O1 O3 46.09(17) 1_565 2_564
O2 O1 O3 128.0(3) 4_445 2_564
O2 O1 O3 70.8(2) 1_665 2_564
O2 O1 O3 94.5(2) 3_465 2_564
O3 O1 O3 143.9(2) 1_556 2_564
O3 O1 O3 95.2(3) 3_566 2_564
O3 O1 O3 130.3(2) 4_456 2_564
La O1 O3 169.41(16) 1_556 2_564
La O1 O3 121.26(15) 2_566 2_564
La O1 O3 132.19(9) 4_456 2_564
O3 O1 O3 71.7(3) 4 2_564
O3 O1 O3 93.1(3) 3_455 2_564
O3 O1 O3 36.1(2) 1_565 2_564
Ga2 O1 O3 92.61(14) 1_566 2_564
Ga2 O1 O3 141.7(3) 1_556 2_564
Ga2 O1 O3 87.5(2) 1_666 2_564
O1 O1 O3 59.7(3) 2_465 2_564
O1 O1 O3 103.0(5) 2_455 2_564
O1 O1 O3 53.7(3) 2_565 2_564
O1 O1 O3 33.57(15) 1_554 2_564
O1 O1 O3 146.43(15) 1_556 2_564
Ga3 O1 O3 130.0(2) 4_446 2_564
Ga3 O1 O3 76.11(17) 1_666 2_564
Ga3 O1 O3 112.76(17) 2_465 2_564
O3 O1 O3 97.7(2) 5 2_564
O3 O1 O3 119.1(4) 2_455 2_564
O3 O1 O3 62.69(15) 6_565 2_564
O3 O1 O3 120.4(3) 4_556 2_564
O3 O1 O3 147.53(18) 3_456 2_564
O3 O1 O3 93.1(3) 1_566 2_564
O2 O1 O3 71.9(2) 1_554 2_564
O2 O1 O3 40.05(18) 3_564 2_564
O2 O1 O3 28.95(18) 4_454 2_564
O3 O1 O3 57.2(3) 6_554 2_564
O3 O1 O3 57.2(3) 5_454 2_564
Ga2 O1 O1 54.3(3) 2_565 2_466
La O1 O1 136.2(2) . 2_466
La O1 O1 114.77(15) 2_565 2_466
La O1 O1 57.01(8) 4_455 2_466
O2 O1 O1 154.1(5) 2_565 2_466
O2 O1 O1 115.5(4) 6 2_466
O2 O1 O1 97.3(2) 5_455 2_466
O2 O1 O1 83.8(5) 2_566 2_466
O2 O1 O1 56.6(4) 6_556 2_466
O2 O1 O1 33.3(4) 5_456 2_466
O3 O1 O1 137.6(6) 6 2_466
O3 O1 O1 57.7(3) 5_455 2_466
O3 O1 O1 66.5(2) 2_565 2_466
Ga2 O1 O1 125.7(3) 2_564 2_466
O2 O1 O1 117.4(5) 3_565 2_466
O2 O1 O1 94.4(3) . 2_466
O2 O1 O1 28.4(3) 4_455 2_466
Ga3 O1 O1 114.5(5) 2_565 2_466
Ga3 O1 O1 64.47(19) 1_556 2_466
Ga3 O1 O1 36.94(10) 4_456 2_466
O3 O1 O1 163.3(3) . 2_466
O3 O1 O1 75.6(2) 4_455 2_466
O3 O1 O1 97.54(14) 3_565 2_466
Ga3 O1 O1 162.9(3) 2_564 2_466
Ga3 O1 O1 107.72(12) . 2_466
Ga3 O1 O1 91.18(12) 4_455 2_466
Nb O1 O1 154.9(5) . 2_466
Ga1 O1 O1 154.9(5) . 2_466
Nb O1 O1 72.994(11) 1_455 2_466
Ga1 O1 O1 72.994(11) 1_455 2_466
Ga1 O1 O1 72.994(11) 1_565 2_466
Nb O1 O1 72.994(11) 1_565 2_466
O2 O1 O1 121.9(4) 4_445 2_466
O2 O1 O1 93.3(2) 1_665 2_466
O2 O1 O1 32.71(19) 3_465 2_466
O3 O1 O1 104.3(4) 1_556 2_466
O3 O1 O1 60.4(2) 3_566 2_466
O3 O1 O1 33.41(17) 4_456 2_466
La O1 O1 76.6(3) 1_556 2_466
La O1 O1 67.0(3) 2_566 2_466
La O1 O1 26.15(17) 4_456 2_466
O3 O1 O1 160.2(3) 4 2_466
O3 O1 O1 96.71(12) 3_455 2_466
O3 O1 O1 71.93(14) 1_565 2_466
Ga2 O1 O1 17.32(9) 1_566 2_466
Ga2 O1 O1 101.6(3) 1_556 2_466
Ga2 O1 O1 101.6(3) 1_666 2_466
O1 O1 O1 56.11(9) 2_465 2_466
O1 O1 O1 125.75(17) 2_455 2_466
O1 O1 O1 125.75(18) 2_565 2_466
O1 O1 O1 125.7(3) 1_554 2_466
O1 O1 O1 54.3(3) 1_556 2_466
Ga3 O1 O1 122.0(4) 4_446 2_466
Ga3 O1 O1 73.02(14) 1_666 2_466
Ga3 O1 O1 37.70(2) 2_465 2_466
O3 O1 O1 137.8(4) 5 2_466
O3 O1 O1 76.48(13) 2_455 2_466
O3 O1 O1 51.60(16) 6_565 2_466
O3 O1 O1 107.8(5) 4_556 2_466
O3 O1 O1 63.3(2) 3_456 2_466
O3 O1 O1 32.91(14) 1_566 2_466
O2 O1 O1 125.2(2) 1_554 2_466
O2 O1 O1 145.2(2) 3_564 2_466
O2 O1 O1 88.1(2) 4_454 2_466
O3 O1 O1 158.9(4) 6_554 2_466
O3 O1 O1 103.0(2) 5_454 2_466
O3 O1 O1 107.48(19) 2_564 2_466
Ga2 O1 O1 54.3(3) 2_565 2_456
La O1 O1 57.01(8) . 2_456
La O1 O1 136.2(2) 2_565 2_456
La O1 O1 114.77(14) 4_455 2_456
O2 O1 O1 115.5(4) 2_565 2_456
O2 O1 O1 97.3(2) 6 2_456
O2 O1 O1 154.1(5) 5_455 2_456
O2 O1 O1 56.6(4) 2_566 2_456
O2 O1 O1 33.3(4) 6_556 2_456
O2 O1 O1 83.8(5) 5_456 2_456
O3 O1 O1 57.7(3) 6 2_456
O3 O1 O1 66.5(2) 5_455 2_456
O3 O1 O1 137.6(6) 2_565 2_456
Ga2 O1 O1 125.7(3) 2_564 2_456
O2 O1 O1 94.4(3) 3_565 2_456
O2 O1 O1 28.4(3) . 2_456
O2 O1 O1 117.4(5) 4_455 2_456
Ga3 O1 O1 64.47(19) 2_565 2_456
Ga3 O1 O1 36.94(10) 1_556 2_456
Ga3 O1 O1 114.5(5) 4_456 2_456
O3 O1 O1 75.6(2) . 2_456
O3 O1 O1 97.54(14) 4_455 2_456
O3 O1 O1 163.3(3) 3_565 2_456
Ga3 O1 O1 107.72(12) 2_564 2_456
Ga3 O1 O1 91.18(12) . 2_456
Ga3 O1 O1 162.9(3) 4_455 2_456
Nb O1 O1 72.994(11) . 2_456
Ga1 O1 O1 72.994(11) . 2_456
Nb O1 O1 72.995(11) 1_455 2_456
Ga1 O1 O1 72.995(11) 1_455 2_456
Ga1 O1 O1 154.9(5) 1_565 2_456
Nb O1 O1 154.9(5) 1_565 2_456
O2 O1 O1 32.71(19) 4_445 2_456
O2 O1 O1 121.9(4) 1_665 2_456
O2 O1 O1 93.3(2) 3_465 2_456
O3 O1 O1 33.41(16) 1_556 2_456
O3 O1 O1 104.3(4) 3_566 2_456
O3 O1 O1 60.4(2) 4_456 2_456
La O1 O1 26.15(17) 1_556 2_456
La O1 O1 76.6(3) 2_566 2_456
La O1 O1 67.0(3) 4_456 2_456
O3 O1 O1 96.71(12) 4 2_456
O3 O1 O1 71.93(14) 3_455 2_456
O3 O1 O1 160.2(3) 1_565 2_456
Ga2 O1 O1 101.6(3) 1_566 2_456
Ga2 O1 O1 17.32(9) 1_556 2_456
Ga2 O1 O1 101.6(3) 1_666 2_456
O1 O1 O1 125.75(18) 2_465 2_456
O1 O1 O1 56.11(9) 2_455 2_456
O1 O1 O1 125.75(18) 2_565 2_456
O1 O1 O1 125.7(3) 1_554 2_456
O1 O1 O1 54.3(3) 1_556 2_456
Ga3 O1 O1 37.70(2) 4_446 2_456
Ga3 O1 O1 122.0(4) 1_666 2_456
Ga3 O1 O1 73.02(14) 2_465 2_456
O3 O1 O1 76.48(13) 5 2_456
O3 O1 O1 51.60(16) 2_455 2_456
O3 O1 O1 137.8(4) 6_565 2_456
O3 O1 O1 63.3(2) 4_556 2_456
O3 O1 O1 32.91(14) 3_456 2_456
O3 O1 O1 107.8(5) 1_566 2_456
O2 O1 O1 88.1(2) 1_554 2_456
O2 O1 O1 125.2(2) 3_564 2_456
O2 O1 O1 145.2(2) 4_454 2_456
O3 O1 O1 103.0(2) 6_554 2_456
O3 O1 O1 107.48(19) 5_454 2_456
O3 O1 O1 158.9(4) 2_564 2_456
O1 O1 O1 89.4(4) 2_466 2_456
Ga2 O1 O1 54.3(3) 2_565 2_566
La O1 O1 114.77(15) . 2_566
La O1 O1 57.01(8) 2_565 2_566
La O1 O1 136.2(2) 4_455 2_566
O2 O1 O1 97.3(2) 2_565 2_566
O2 O1 O1 154.1(5) 6 2_566
O2 O1 O1 115.5(4) 5_455 2_566
O2 O1 O1 33.3(4) 2_566 2_566
O2 O1 O1 83.8(5) 6_556 2_566
O2 O1 O1 56.6(4) 5_456 2_566
O3 O1 O1 66.5(2) 6 2_566
O3 O1 O1 137.6(6) 5_455 2_566
O3 O1 O1 57.7(3) 2_565 2_566
Ga2 O1 O1 125.7(3) 2_564 2_566
O2 O1 O1 28.4(3) 3_565 2_566
O2 O1 O1 117.4(5) . 2_566
O2 O1 O1 94.4(3) 4_455 2_566
Ga3 O1 O1 36.93(10) 2_565 2_566
Ga3 O1 O1 114.5(5) 1_556 2_566
Ga3 O1 O1 64.47(19) 4_456 2_566
O3 O1 O1 97.54(14) . 2_566
O3 O1 O1 163.3(3) 4_455 2_566
O3 O1 O1 75.6(2) 3_565 2_566
Ga3 O1 O1 91.18(12) 2_564 2_566
Ga3 O1 O1 162.9(3) . 2_566
Ga3 O1 O1 107.72(12) 4_455 2_566
Nb O1 O1 72.994(11) . 2_566
Ga1 O1 O1 72.994(11) . 2_566
Nb O1 O1 154.9(5) 1_455 2_566
Ga1 O1 O1 154.9(5) 1_455 2_566
Ga1 O1 O1 72.994(11) 1_565 2_566
Nb O1 O1 72.994(11) 1_565 2_566
O2 O1 O1 93.3(2) 4_445 2_566
O2 O1 O1 32.71(19) 1_665 2_566
O2 O1 O1 121.9(4) 3_465 2_566
O3 O1 O1 60.4(2) 1_556 2_566
O3 O1 O1 33.41(16) 3_566 2_566
O3 O1 O1 104.3(4) 4_456 2_566
La O1 O1 67.0(3) 1_556 2_566
La O1 O1 26.15(17) 2_566 2_566
La O1 O1 76.6(3) 4_456 2_566
O3 O1 O1 71.93(14) 4 2_566
O3 O1 O1 160.2(3) 3_455 2_566
O3 O1 O1 96.71(12) 1_565 2_566
Ga2 O1 O1 101.6(3) 1_566 2_566
Ga2 O1 O1 101.6(3) 1_556 2_566
Ga2 O1 O1 17.32(9) 1_666 2_566
O1 O1 O1 125.75(18) 2_465 2_566
O1 O1 O1 125.75(18) 2_455 2_566
O1 O1 O1 56.11(9) 2_565 2_566
O1 O1 O1 125.7(3) 1_554 2_566
O1 O1 O1 54.3(3) 1_556 2_566
Ga3 O1 O1 73.02(14) 4_446 2_566
Ga3 O1 O1 37.70(2) 1_666 2_566
Ga3 O1 O1 122.0(4) 2_465 2_566
O3 O1 O1 51.60(16) 5 2_566
O3 O1 O1 137.8(4) 2_455 2_566
O3 O1 O1 76.48(13) 6_565 2_566
O3 O1 O1 32.91(14) 4_556 2_566
O3 O1 O1 107.8(5) 3_456 2_566
O3 O1 O1 63.3(2) 1_566 2_566
O2 O1 O1 145.2(2) 1_554 2_566
O2 O1 O1 88.1(2) 3_564 2_566
O2 O1 O1 125.2(2) 4_454 2_566
O3 O1 O1 107.48(19) 6_554 2_566
O3 O1 O1 158.9(4) 5_454 2_566
O3 O1 O1 103.0(2) 2_564 2_566
O1 O1 O1 89.4(4) 2_466 2_566
O1 O1 O1 89.4(4) 2_456 2_566
Ga2 O1 O3 86.6(2) 2_565 2
La O1 O3 41.63(18) . 2
La O1 O3 86.41(11) 2_565 2
La O1 O3 150.6(3) 4_455 2
O2 O1 O3 66.2(4) 2_565 2
O2 O1 O3 90.3(4) 6 2
O2 O1 O3 123.3(4) 5_455 2
O2 O1 O3 61.3(2) 2_566 2
O2 O1 O3 84.7(4) 6_556 2
O2 O1 O3 114.8(4) 5_456 2
O3 O1 O3 6.7(3) 6 2
O3 O1 O3 113.3(3) 5_455 2
O3 O1 O3 125.3(4) 2_565 2
Ga2 O1 O3 93.4(2) 2_564 2
O2 O1 O3 55.6(2) 3_565 2
O2 O1 O3 64.3(2) . 2
O2 O1 O3 164.6(5) 4_455 2
Ga3 O1 O3 36.76(16) 2_565 2
Ga3 O1 O3 89.38(14) 1_556 2
Ga3 O1 O3 136.7(3) 4_456 2
O3 O1 O3 32.7(4) . 2
O3 O1 O3 123.17(15) 4_455 2
O3 O1 O3 112.40(13) 3_565 2
Ga3 O1 O3 56.52(13) 2_564 2
Ga3 O1 O3 93.28(19) . 2
Ga3 O1 O3 128.8(3) 4_455 2
Nb O1 O3 18.19(11) . 2
Ga1 O1 O3 18.19(11) . 2
Nb O1 O3 108.64(13) 1_455 2
Ga1 O1 O3 108.64(13) 1_455 2
Ga1 O1 O3 131.56(12) 1_565 2
Nb O1 O3 131.56(12) 1_565 2
O2 O1 O3 28.81(17) 4_445 2
O2 O1 O3 90.94(18) 1_665 2
O2 O1 O3 146.5(2) 3_465 2
O3 O1 O3 35.2(3) 1_556 2
O3 O1 O3 106.17(17) 3_566 2
O3 O1 O3 115.31(19) 4_456 2
La O1 O3 62.89(15) 1_556 2
La O1 O3 84.5(2) 2_566 2
La O1 O3 113.3(3) 4_456 2
O3 O1 O3 41.8(2) 4 2
O3 O1 O3 90.3(2) 3_455 2
O3 O1 O3 144.8(2) 1_565 2
Ga2 O1 O3 155.4(3) 1_566 2
Ga2 O1 O3 49.55(10) 1_556 2
Ga2 O1 O3 71.53(14) 1_666 2
O1 O1 O3 159.6(4) 2_465 2
O1 O1 O3 53.06(16) 2_455 2
O1 O1 O3 74.15(10) 2_565 2
O1 O1 O3 93.4(2) 1_554 2
O1 O1 O3 86.6(2) 1_556 2
Ga3 O1 O3 18.04(11) 4_446 2
Ga3 O1 O3 107.48(16) 1_666 2
Ga3 O1 O3 126.40(17) 2_465 2
O3 O1 O3 27.64(14) 5 2
O3 O1 O3 92.07(14) 2_455 2
O3 O1 O3 146.93(17) 6_565 2
O3 O1 O3 42.3(3) 4_556 2
O3 O1 O3 87.0(2) 3_456 2
O3 O1 O3 133.7(3) 1_566 2
O2 O1 O3 77.2(2) 1_554 2
O2 O1 O3 72.17(19) 3_564 2
O2 O1 O3 132.0(3) 4_454 2
O3 O1 O3 60.08(12) 6_554 2
O3 O1 O3 105.9(3) 5_454 2
O3 O1 O3 112.0(2) 2_564 2
O1 O1 O3 139.4(4) 2_466 2
O1 O1 O3 54.96(10) 2_456 2
O1 O1 O3 73.14(16) 2_566 2
Ga2 O1 O3 86.6(2) 2_565 6_455
La O1 O3 86.41(11) . 6_455
La O1 O3 150.6(3) 2_565 6_455
La O1 O3 41.63(18) 4_455 6_455
O2 O1 O3 123.3(4) 2_565 6_455
O2 O1 O3 66.2(4) 6 6_455
O2 O1 O3 90.3(4) 5_455 6_455
O2 O1 O3 114.8(4) 2_566 6_455
O2 O1 O3 61.3(2) 6_556 6_455
O2 O1 O3 84.7(4) 5_456 6_455
O3 O1 O3 125.3(4) 6 6_455
O3 O1 O3 6.7(3) 5_455 6_455
O3 O1 O3 113.3(3) 2_565 6_455
Ga2 O1 O3 93.4(2) 2_564 6_455
O2 O1 O3 164.6(5) 3_565 6_455
O2 O1 O3 55.5(2) . 6_455
O2 O1 O3 64.3(2) 4_455 6_455
Ga3 O1 O3 136.7(3) 2_565 6_455
Ga3 O1 O3 36.75(16) 1_556 6_455
Ga3 O1 O3 89.38(14) 4_456 6_455
O3 O1 O3 112.40(13) . 6_455
O3 O1 O3 32.7(4) 4_455 6_455
O3 O1 O3 123.17(15) 3_565 6_455
Ga3 O1 O3 128.8(3) 2_564 6_455
Ga3 O1 O3 56.52(13) . 6_455
Ga3 O1 O3 93.28(19) 4_455 6_455
Nb O1 O3 131.57(12) . 6_455
Ga1 O1 O3 131.57(12) . 6_455
Nb O1 O3 18.19(11) 1_455 6_455
Ga1 O1 O3 18.19(11) 1_455 6_455
Ga1 O1 O3 108.64(13) 1_565 6_455
Nb O1 O3 108.64(13) 1_565 6_455
O2 O1 O3 90.94(18) 4_445 6_455
O2 O1 O3 146.5(2) 1_665 6_455
O2 O1 O3 28.81(17) 3_465 6_455
O3 O1 O3 106.17(17) 1_556 6_455
O3 O1 O3 115.30(19) 3_566 6_455
O3 O1 O3 35.2(3) 4_456 6_455
La O1 O3 84.5(2) 1_556 6_455
La O1 O3 113.3(3) 2_566 6_455
La O1 O3 62.89(15) 4_456 6_455
O3 O1 O3 144.8(2) 4 6_455
O3 O1 O3 41.8(2) 3_455 6_455
O3 O1 O3 90.3(2) 1_565 6_455
Ga2 O1 O3 49.55(10) 1_566 6_455
Ga2 O1 O3 71.53(14) 1_556 6_455
Ga2 O1 O3 155.4(3) 1_666 6_455
O1 O1 O3 53.06(16) 2_465 6_455
O1 O1 O3 74.15(10) 2_455 6_455
O1 O1 O3 159.6(4) 2_565 6_455
O1 O1 O3 93.4(2) 1_554 6_455
O1 O1 O3 86.6(2) 1_556 6_455
Ga3 O1 O3 107.48(16) 4_446 6_455
Ga3 O1 O3 126.40(16) 1_666 6_455
Ga3 O1 O3 18.04(11) 2_465 6_455
O3 O1 O3 146.93(17) 5 6_455
O3 O1 O3 27.64(14) 2_455 6_455
O3 O1 O3 92.07(13) 6_565 6_455
O3 O1 O3 133.7(3) 4_556 6_455
O3 O1 O3 42.3(3) 3_456 6_455
O3 O1 O3 87.00(19) 1_566 6_455
O2 O1 O3 72.17(19) 1_554 6_455
O2 O1 O3 132.0(3) 3_564 6_455
O2 O1 O3 77.2(2) 4_454 6_455
O3 O1 O3 112.0(2) 6_554 6_455
O3 O1 O3 60.08(12) 5_454 6_455
O3 O1 O3 105.9(3) 2_564 6_455
O1 O1 O3 54.96(10) 2_466 6_455
O1 O1 O3 73.14(16) 2_456 6_455
O1 O1 O3 139.4(4) 2_566 6_455
O3 O1 O3 119.64(4) 2 6_455
Ga2 O1 O3 86.6(2) 2_565 5_565
La O1 O3 150.6(3) . 5_565
La O1 O3 41.63(18) 2_565 5_565
La O1 O3 86.41(11) 4_455 5_565
O2 O1 O3 90.3(4) 2_565 5_565
O2 O1 O3 123.3(4) 6 5_565
O2 O1 O3 66.2(4) 5_455 5_565
O2 O1 O3 84.7(4) 2_566 5_565
O2 O1 O3 114.8(4) 6_556 5_565
O2 O1 O3 61.3(2) 5_456 5_565
O3 O1 O3 113.3(3) 6 5_565
O3 O1 O3 125.3(4) 5_455 5_565
O3 O1 O3 6.7(3) 2_565 5_565
Ga2 O1 O3 93.4(2) 2_564 5_565
O2 O1 O3 64.3(2) 3_565 5_565
O2 O1 O3 164.6(5) . 5_565
O2 O1 O3 55.5(2) 4_455 5_565
Ga3 O1 O3 89.38(14) 2_565 5_565
Ga3 O1 O3 136.7(3) 1_556 5_565
Ga3 O1 O3 36.75(16) 4_456 5_565
O3 O1 O3 123.17(15) . 5_565
O3 O1 O3 112.39(13) 4_455 5_565
O3 O1 O3 32.7(4) 3_565 5_565
Ga3 O1 O3 93.28(19) 2_564 5_565
Ga3 O1 O3 128.8(3) . 5_565
Ga3 O1 O3 56.52(13) 4_455 5_565
Nb O1 O3 108.64(13) . 5_565
Ga1 O1 O3 108.64(13) . 5_565
Nb O1 O3 131.56(12) 1_455 5_565
Ga1 O1 O3 131.56(12) 1_455 5_565
Ga1 O1 O3 18.19(11) 1_565 5_565
Nb O1 O3 18.19(11) 1_565 5_565
O2 O1 O3 146.5(2) 4_445 5_565
O2 O1 O3 28.81(17) 1_665 5_565
O2 O1 O3 90.94(18) 3_465 5_565
O3 O1 O3 115.30(19) 1_556 5_565
O3 O1 O3 35.2(3) 3_566 5_565
O3 O1 O3 106.17(17) 4_456 5_565
La O1 O3 113.3(3) 1_556 5_565
La O1 O3 62.89(15) 2_566 5_565
La O1 O3 84.5(2) 4_456 5_565
O3 O1 O3 90.3(2) 4 5_565
O3 O1 O3 144.8(2) 3_455 5_565
O3 O1 O3 41.8(2) 1_565 5_565
Ga2 O1 O3 71.53(14) 1_566 5_565
Ga2 O1 O3 155.4(3) 1_556 5_565
Ga2 O1 O3 49.55(10) 1_666 5_565
O1 O1 O3 74.15(10) 2_465 5_565
O1 O1 O3 159.6(4) 2_455 5_565
O1 O1 O3 53.06(16) 2_565 5_565
O1 O1 O3 93.4(2) 1_554 5_565
O1 O1 O3 86.6(2) 1_556 5_565
Ga3 O1 O3 126.40(17) 4_446 5_565
Ga3 O1 O3 18.04(11) 1_666 5_565
Ga3 O1 O3 107.48(16) 2_465 5_565
O3 O1 O3 92.07(14) 5 5_565
O3 O1 O3 146.93(17) 2_455 5_565
O3 O1 O3 27.64(14) 6_565 5_565
O3 O1 O3 87.00(19) 4_556 5_565
O3 O1 O3 133.7(3) 3_456 5_565
O3 O1 O3 42.3(3) 1_566 5_565
O2 O1 O3 132.0(3) 1_554 5_565
O2 O1 O3 77.2(2) 3_564 5_565
O2 O1 O3 72.17(19) 4_454 5_565
O3 O1 O3 105.9(3) 6_554 5_565
O3 O1 O3 112.0(2) 5_454 5_565
O3 O1 O3 60.08(12) 2_564 5_565
O1 O1 O3 73.14(16) 2_466 5_565
O1 O1 O3 139.4(4) 2_456 5_565
O1 O1 O3 54.96(10) 2_566 5_565
O3 O1 O3 119.64(4) 2 5_565
O3 O1 O3 119.64(4) 6_455 5_565
Ga2 O1 La 98.48(16) 2_565 2_455
La O1 La 37.02(3) . 2_455
La O1 La 143.3(4) 2_565 2_455
La O1 La 81.11(9) 4_455 2_455
O2 O1 La 91.6(3) 2_565 2_455
O2 O1 La 49.2(2) 6 2_455
O2 O1 La 104.8(4) 5_455 2_455
O2 O1 La 105.6(4) 2_566 2_455
O2 O1 La 68.0(3) 6_556 2_455
O2 O1 La 118.9(3) 5_456 2_455
O3 O1 La 78.8(2) 6 2_455
O3 O1 La 44.8(3) 5_455 2_455
O3 O1 La 162.4(2) 2_565 2_455
Ga2 O1 La 81.52(16) 2_564 2_455
O2 O1 La 127.8(2) 3_565 2_455
O2 O1 La 21.0(3) . 2_455
O2 O1 La 114.02(18) 4_455 2_455
Ga3 O1 La 103.11(7) 2_565 2_455
Ga3 O1 La 40.93(6) 1_556 2_455
Ga3 O1 La 137.31(16) 4_456 2_455
O3 O1 La 64.25(15) . 2_455
O3 O1 La 55.16(13) 4_455 2_455
O3 O1 La 142.5(4) 3_565 2_455
Ga3 O1 La 90.79(15) 2_564 2_455
Ga3 O1 La 42.02(3) . 2_455
Ga3 O1 La 113.9(2) 4_455 2_455
Nb O1 La 81.82(5) . 2_455
Ga1 O1 La 81.82(5) . 2_455
Nb O1 La 36.34(2) 1_455 2_455
Ga1 O1 La 36.34(2) 1_455 2_455
Ga1 O1 La 150.1(2) 1_565 2_455
Nb O1 La 150.1(2) 1_565 2_455
O2 O1 La 46.03(11) 4_445 2_455
O2 O1 La 163.16(11) 1_665 2_455
O2 O1 La 78.57(12) 3_465 2_455
O3 O1 La 76.42(13) 1_556 2_455
O3 O1 La 150.0(3) 3_566 2_455
O3 O1 La 69.05(13) 4_456 2_455
La O1 La 74.65(8) 1_556 2_455
La O1 La 125.2(2) 2_566 2_455
La O1 La 94.22(12) 4_456 2_455
O3 O1 La 97.77(16) 4 2_455
O3 O1 La 23.46(12) 3_455 2_455
O3 O1 La 126.4(2) 1_565 2_455
Ga2 O1 La 99.08(3) 1_566 2_455
Ga2 O1 La 35.27(2) 1_556 2_455
Ga2 O1 La 142.94(9) 1_666 2_455
O1 O1 La 93.35(12) 2_465 2_455
O1 O1 La 25.39(7) 2_455 2_455
O1 O1 La 133.7(3) 2_565 2_455
O1 O1 La 81.52(16) 1_554 2_455
O1 O1 La 98.48(16) 1_556 2_455
Ga3 O1 La 66.10(2) 4_446 2_455
Ga3 O1 La 170.0(3) 1_666 2_455
Ga3 O1 La 63.90(2) 2_465 2_455
O3 O1 La 99.65(11) 5 2_455
O3 O1 La 24.06(10) 2_455 2_455
O3 O1 La 140.74(11) 6_565 2_455
O3 O1 La 105.32(13) 4_556 2_455
O3 O1 La 45.66(17) 3_456 2_455
O3 O1 La 133.1(2) 1_566 2_455
O2 O1 La 43.22(13) 1_554 2_455
O2 O1 La 104.9(2) 3_564 2_455
O2 O1 La 97.2(2) 4_454 2_455
O3 O1 La 76.09(19) 6_554 2_455
O3 O1 La 58.21(12) 5_454 2_455
O3 O1 La 113.5(3) 2_564 2_455
O1 O1 La 100.45(8) 2_466 2_455
O1 O1 La 49.27(9) 2_456 2_455
O1 O1 La 136.8(2) 2_566 2_455
O3 O1 La 72.29(13) 2 2_455
O3 O1 La 49.79(11) 6_455 2_455
O3 O1 La 167.49(17) 5_565 2_455
Ga2 O1 La 98.48(16) 2_565 4
La O1 La 81.12(9) . 4
La O1 La 37.03(3) 2_565 4
La O1 La 143.3(4) 4_455 4
O2 O1 La 49.2(2) 2_565 4
O2 O1 La 104.8(4) 6 4
O2 O1 La 91.6(3) 5_455 4
O2 O1 La 68.0(3) 2_566 4
O2 O1 La 118.9(3) 6_556 4
O2 O1 La 105.6(4) 5_456 4
O3 O1 La 44.8(3) 6 4
O3 O1 La 162.4(2) 5_455 4
O3 O1 La 78.8(2) 2_565 4
Ga2 O1 La 81.52(16) 2_564 4
O2 O1 La 21.0(3) 3_565 4
O2 O1 La 114.02(18) . 4
O2 O1 La 127.8(2) 4_455 4
Ga3 O1 La 40.93(6) 2_565 4
Ga3 O1 La 137.31(16) 1_556 4
Ga3 O1 La 103.11(6) 4_456 4
O3 O1 La 55.16(13) . 4
O3 O1 La 142.5(4) 4_455 4
O3 O1 La 64.25(15) 3_565 4
Ga3 O1 La 42.02(3) 2_564 4
Ga3 O1 La 113.9(2) . 4
Ga3 O1 La 90.79(15) 4_455 4
Nb O1 La 36.34(2) . 4
Ga1 O1 La 36.34(2) . 4
Nb O1 La 150.1(2) 1_455 4
Ga1 O1 La 150.1(2) 1_455 4
Ga1 O1 La 81.82(5) 1_565 4
Nb O1 La 81.82(5) 1_565 4
O2 O1 La 78.57(12) 4_445 4
O2 O1 La 46.03(11) 1_665 4
O2 O1 La 163.16(11) 3_465 4
O3 O1 La 69.05(13) 1_556 4
O3 O1 La 76.42(13) 3_566 4
O3 O1 La 150.0(3) 4_456 4
La O1 La 94.22(12) 1_556 4
La O1 La 74.65(8) 2_566 4
La O1 La 125.2(2) 4_456 4
O3 O1 La 23.46(12) 4 4
O3 O1 La 126.4(2) 3_455 4
O3 O1 La 97.77(16) 1_565 4
Ga2 O1 La 142.94(9) 1_566 4
Ga2 O1 La 99.08(3) 1_556 4
Ga2 O1 La 35.27(2) 1_666 4
O1 O1 La 133.7(3) 2_465 4
O1 O1 La 93.35(12) 2_455 4
O1 O1 La 25.39(7) 2_565 4
O1 O1 La 81.52(16) 1_554 4
O1 O1 La 98.48(16) 1_556 4
Ga3 O1 La 63.90(2) 4_446 4
Ga3 O1 La 66.10(2) 1_666 4
Ga3 O1 La 170.0(3) 2_465 4
O3 O1 La 24.06(10) 5 4
O3 O1 La 140.75(11) 2_455 4
O3 O1 La 99.64(11) 6_565 4
O3 O1 La 45.66(17) 4_556 4
O3 O1 La 133.1(2) 3_456 4
O3 O1 La 105.32(13) 1_566 4
O2 O1 La 97.2(2) 1_554 4
O2 O1 La 43.22(13) 3_564 4
O2 O1 La 104.9(2) 4_454 4
O3 O1 La 58.22(12) 6_554 4
O3 O1 La 113.5(3) 5_454 4
O3 O1 La 76.09(19) 2_564 4
O1 O1 La 136.8(2) 2_466 4
O1 O1 La 100.45(8) 2_456 4
O1 O1 La 49.27(9) 2_566 4
O3 O1 La 49.79(11) 2 4
O3 O1 La 167.49(17) 6_455 4
O3 O1 La 72.29(13) 5_565 4
La O1 La 117.86(8) 2_455 4
Ga2 O1 La 98.48(16) 2_565 1_565
La O1 La 143.3(4) . 1_565
La O1 La 81.11(9) 2_565 1_565
La O1 La 37.02(3) 4_455 1_565
O2 O1 La 104.8(4) 2_565 1_565
O2 O1 La 91.6(3) 6 1_565
O2 O1 La 49.2(2) 5_455 1_565
O2 O1 La 118.9(3) 2_566 1_565
O2 O1 La 105.6(4) 6_556 1_565
O2 O1 La 68.0(3) 5_456 1_565
O3 O1 La 162.4(2) 6 1_565
O3 O1 La 78.8(2) 5_455 1_565
O3 O1 La 44.8(3) 2_565 1_565
Ga2 O1 La 81.52(16) 2_564 1_565
O2 O1 La 114.02(18) 3_565 1_565
O2 O1 La 127.8(2) . 1_565
O2 O1 La 21.0(3) 4_455 1_565
Ga3 O1 La 137.31(16) 2_565 1_565
Ga3 O1 La 103.11(6) 1_556 1_565
Ga3 O1 La 40.93(6) 4_456 1_565
O3 O1 La 142.5(4) . 1_565
O3 O1 La 64.25(15) 4_455 1_565
O3 O1 La 55.16(13) 3_565 1_565
Ga3 O1 La 113.9(2) 2_564 1_565
Ga3 O1 La 90.79(15) . 1_565
Ga3 O1 La 42.02(3) 4_455 1_565
Nb O1 La 150.1(2) . 1_565
Ga1 O1 La 150.1(2) . 1_565
Nb O1 La 81.82(5) 1_455 1_565
Ga1 O1 La 81.82(5) 1_455 1_565
Ga1 O1 La 36.34(2) 1_565 1_565
Nb O1 La 36.34(2) 1_565 1_565
O2 O1 La 163.16(11) 4_445 1_565
O2 O1 La 78.57(12) 1_665 1_565
O2 O1 La 46.03(11) 3_465 1_565
O3 O1 La 150.0(3) 1_556 1_565
O3 O1 La 69.05(13) 3_566 1_565
O3 O1 La 76.42(13) 4_456 1_565
La O1 La 125.2(2) 1_556 1_565
La O1 La 94.22(12) 2_566 1_565
La O1 La 74.65(8) 4_456 1_565
O3 O1 La 126.4(2) 4 1_565
O3 O1 La 97.77(16) 3_455 1_565
O3 O1 La 23.46(12) 1_565 1_565
Ga2 O1 La 35.27(2) 1_566 1_565
Ga2 O1 La 142.94(9) 1_556 1_565
Ga2 O1 La 99.08(3) 1_666 1_565
O1 O1 La 25.39(7) 2_465 1_565
O1 O1 La 133.7(3) 2_455 1_565
O1 O1 La 93.35(12) 2_565 1_565
O1 O1 La 81.52(16) 1_554 1_565
O1 O1 La 98.48(16) 1_556 1_565
Ga3 O1 La 170.0(3) 4_446 1_565
Ga3 O1 La 63.90(2) 1_666 1_565
Ga3 O1 La 66.10(2) 2_465 1_565
O3 O1 La 140.74(11) 5 1_565
O3 O1 La 99.64(11) 2_455 1_565
O3 O1 La 24.06(10) 6_565 1_565
O3 O1 La 133.1(2) 4_556 1_565
O3 O1 La 105.32(13) 3_456 1_565
O3 O1 La 45.66(17) 1_566 1_565
O2 O1 La 104.9(2) 1_554 1_565
O2 O1 La 97.2(2) 3_564 1_565
O2 O1 La 43.22(13) 4_454 1_565
O3 O1 La 113.5(3) 6_554 1_565
O3 O1 La 76.09(19) 5_454 1_565
O3 O1 La 58.21(12) 2_564 1_565
O1 O1 La 49.27(9) 2_466 1_565
O1 O1 La 136.8(2) 2_456 1_565
O1 O1 La 100.45(8) 2_566 1_565
O3 O1 La 167.49(17) 2 1_565
O3 O1 La 72.29(13) 6_455 1_565
O3 O1 La 49.79(11) 5_565 1_565
La O1 La 117.86(8) 2_455 1_565
La O1 La 117.86(8) 4 1_565
Ga2 O1 O2 83.5(2) 2_565 3_455
La O1 O2 32.4(3) . 3_455
La O1 O2 138.1(2) 2_565 3_455
La O1 O2 102.43(13) 4_455 3_455
O2 O1 O2 94.7(5) 2_565 3_455
O2 O1 O2 67.9(3) 6 3_455
O2 O1 O2 125.1(4) 5_455 3_455
O2 O1 O2 83.8(4) 2_566 3_455
O2 O1 O2 57.4(5) 6_556 3_455
O2 O1 O2 111.0(4) 5_456 3_455
O3 O1 O2 59.8(3) 6 3_455
O3 O1 O2 59.3(3) 5_455 3_455
O3 O1 O2 167.2(5) 2_565 3_455
Ga2 O1 O2 96.5(2) 2_564 3_455
O2 O1 O2 107.8(3) 3_565 3_455
O2 O1 O2 11.3(3) . 3_455
O2 O1 O2 127.4(4) 4_455 3_455
Ga3 O1 O2 80.87(13) 2_565 3_455
Ga3 O1 O2 40.96(19) 1_556 3_455
Ga3 O1 O2 139.1(4) 4_456 3_455
O3 O1 O2 58.0(3) . 3_455
O3 O1 O2 77.67(17) 4_455 3_455
O3 O1 O2 155.0(4) 3_565 3_455
Ga3 O1 O2 90.0(2) 2_564 3_455
Ga3 O1 O2 62.69(11) . 3_455
Ga3 O1 O2 134.9(3) 4_455 3_455
Nb O1 O2 67.72(17) . 3_455
Ga1 O1 O2 67.72(17) . 3_455
Nb O1 O2 56.54(12) 1_455 3_455
Ga1 O1 O2 56.54(12) 1_455 3_455
Ga1 O1 O2 172.9(2) 1_565 3_455
Nb O1 O2 172.9(2) 1_565 3_455
O2 O1 O2 25.49(17) 4_445 3_455
O2 O1 O2 142.6(2) 1_665 3_455
O2 O1 O2 93.35(19) 3_465 3_455
O3 O1 O2 53.59(16) 1_556 3_455
O3 O1 O2 134.0(3) 3_566 3_455
O3 O1 O2 72.0(3) 4_456 3_455
La O1 O2 55.82(14) 1_556 3_455
La O1 O2 105.8(2) 2_566 3_455
La O1 O2 89.7(2) 4_456 3_455
O3 O1 O2 88.7(2) 4 3_455
O3 O1 O2 46.22(16) 3_455 3_455
O3 O1 O2 149.2(2) 1_565 3_455
Ga2 O1 O2 110.5(2) 1_566 3_455
Ga2 O1 O2 13.18(12) 1_556 3_455
Ga2 O1 O2 121.12(17) 1_666 3_455
O1 O1 O2 114.86(14) 2_465 3_455
O1 O1 O2 27.5(3) 2_455 3_455
O1 O1 O2 125.8(2) 2_565 3_455
O1 O1 O2 96.5(2) 1_554 3_455
O1 O1 O2 83.5(2) 1_556 3_455
Ga3 O1 O2 44.35(13) 4_446 3_455
Ga3 O1 O2 150.5(3) 1_666 3_455
Ga3 O1 O2 74.82(19) 2_465 3_455
O3 O1 O2 81.51(17) 5 3_455
O3 O1 O2 38.07(18) 2_455 3_455
O3 O1 O2 155.9(3) 6_565 3_455
O3 O1 O2 82.63(16) 4_556 3_455
O3 O1 O2 42.2(2) 3_456 3_455
O3 O1 O2 132.8(3) 1_566 3_455
O2 O1 O2 58.46(12) 1_554 3_455
O2 O1 O2 107.3(3) 3_564 3_455
O2 O1 O2 119.3(2) 4_454 3_455
O3 O1 O2 79.7(2) 6_554 3_455
O3 O1 O2 79.46(16) 5_454 3_455
O3 O1 O2 130.0(3) 2_564 3_455
O1 O1 O2 105.3(3) 2_466 3_455
O1 O1 O2 29.70(19) 2_456 3_455
O1 O1 O2 114.0(2) 2_566 3_455
O3 O1 O2 54.0(2) 2 3_455
O3 O1 O2 65.6(2) 6_455 3_455
O3 O1 O2 168.5(3) 5_565 3_455
La O1 O2 22.86(10) 2_455 3_455
La O1 O2 103.41(16) 4 3_455
La O1 O2 137.68(14) 1_565 3_455
Ga2 O1 O2 83.5(2) 2_565 4
La O1 O2 102.43(12) . 4
La O1 O2 32.4(3) 2_565 4
La O1 O2 138.1(2) 4_455 4
O2 O1 O2 67.9(3) 2_565 4
O2 O1 O2 125.1(4) 6 4
O2 O1 O2 94.7(5) 5_455 4
O2 O1 O2 57.4(5) 2_566 4
O2 O1 O2 111.0(4) 6_556 4
O2 O1 O2 83.8(4) 5_456 4
O3 O1 O2 59.3(3) 6 4
O3 O1 O2 167.2(5) 5_455 4
O3 O1 O2 59.8(3) 2_565 4
Ga2 O1 O2 96.5(2) 2_564 4
O2 O1 O2 11.3(3) 3_565 4
O2 O1 O2 127.4(4) . 4
O2 O1 O2 107.8(3) 4_455 4
Ga3 O1 O2 40.96(19) 2_565 4
Ga3 O1 O2 139.1(4) 1_556 4
Ga3 O1 O2 80.87(13) 4_456 4
O3 O1 O2 77.67(17) . 4
O3 O1 O2 155.0(4) 4_455 4
O3 O1 O2 58.0(3) 3_565 4
Ga3 O1 O2 62.69(11) 2_564 4
Ga3 O1 O2 134.9(3) . 4
Ga3 O1 O2 90.0(2) 4_455 4
Nb O1 O2 56.54(12) . 4
Ga1 O1 O2 56.54(12) . 4
Nb O1 O2 172.9(2) 1_455 4
Ga1 O1 O2 172.9(2) 1_455 4
Ga1 O1 O2 67.72(17) 1_565 4
Nb O1 O2 67.72(17) 1_565 4
O2 O1 O2 93.35(19) 4_445 4
O2 O1 O2 25.49(16) 1_665 4
O2 O1 O2 142.6(2) 3_465 4
O3 O1 O2 72.0(3) 1_556 4
O3 O1 O2 53.59(16) 3_566 4
O3 O1 O2 134.0(3) 4_456 4
La O1 O2 89.7(2) 1_556 4
La O1 O2 55.82(14) 2_566 4
La O1 O2 105.8(2) 4_456 4
O3 O1 O2 46.22(15) 4 4
O3 O1 O2 149.2(2) 3_455 4
O3 O1 O2 88.7(2) 1_565 4
Ga2 O1 O2 121.12(17) 1_566 4
Ga2 O1 O2 110.5(2) 1_556 4
Ga2 O1 O2 13.18(12) 1_666 4
O1 O1 O2 125.8(2) 2_465 4
O1 O1 O2 114.86(14) 2_455 4
O1 O1 O2 27.5(3) 2_565 4
O1 O1 O2 96.5(2) 1_554 4
O1 O1 O2 83.5(2) 1_556 4
Ga3 O1 O2 74.82(19) 4_446 4
Ga3 O1 O2 44.35(13) 1_666 4
Ga3 O1 O2 150.5(3) 2_465 4
O3 O1 O2 38.07(18) 5 4
O3 O1 O2 155.9(3) 2_455 4
O3 O1 O2 81.51(17) 6_565 4
O3 O1 O2 42.2(2) 4_556 4
O3 O1 O2 132.8(3) 3_456 4
O3 O1 O2 82.63(16) 1_566 4
O2 O1 O2 119.3(2) 1_554 4
O2 O1 O2 58.46(12) 3_564 4
O2 O1 O2 107.3(3) 4_454 4
O3 O1 O2 79.46(16) 6_554 4
O3 O1 O2 130.0(3) 5_454 4
O3 O1 O2 79.7(2) 2_564 4
O1 O1 O2 114.0(2) 2_466 4
O1 O1 O2 105.3(3) 2_456 4
O1 O1 O2 29.70(19) 2_566 4
O3 O1 O2 65.6(2) 2 4
O3 O1 O2 168.5(3) 6_455 4
O3 O1 O2 54.0(2) 5_565 4
La O1 O2 137.68(14) 2_455 4
La O1 O2 22.86(10) 4 4
La O1 O2 103.41(16) 1_565 4
O2 O1 O2 118.75(8) 3_455 4
Ga2 O1 O2 83.5(2) 2_565 1_565
La O1 O2 138.1(2) . 1_565
La O1 O2 102.43(13) 2_565 1_565
La O1 O2 32.4(3) 4_455 1_565
O2 O1 O2 125.1(4) 2_565 1_565
O2 O1 O2 94.7(5) 6 1_565
O2 O1 O2 67.9(3) 5_455 1_565
O2 O1 O2 111.0(4) 2_566 1_565
O2 O1 O2 83.8(4) 6_556 1_565
O2 O1 O2 57.4(5) 5_456 1_565
O3 O1 O2 167.2(5) 6 1_565
O3 O1 O2 59.8(3) 5_455 1_565
O3 O1 O2 59.3(3) 2_565 1_565
Ga2 O1 O2 96.5(2) 2_564 1_565
O2 O1 O2 127.4(4) 3_565 1_565
O2 O1 O2 107.8(3) . 1_565
O2 O1 O2 11.3(3) 4_455 1_565
Ga3 O1 O2 139.1(4) 2_565 1_565
Ga3 O1 O2 80.87(13) 1_556 1_565
Ga3 O1 O2 40.96(19) 4_456 1_565
O3 O1 O2 155.0(4) . 1_565
O3 O1 O2 58.0(3) 4_455 1_565
O3 O1 O2 77.67(17) 3_565 1_565
Ga3 O1 O2 134.9(3) 2_564 1_565
Ga3 O1 O2 90.0(2) . 1_565
Ga3 O1 O2 62.69(11) 4_455 1_565
Nb O1 O2 172.9(2) . 1_565
Ga1 O1 O2 172.9(2) . 1_565
Nb O1 O2 67.72(17) 1_455 1_565
Ga1 O1 O2 67.72(17) 1_455 1_565
Ga1 O1 O2 56.54(12) 1_565 1_565
Nb O1 O2 56.54(12) 1_565 1_565
O2 O1 O2 142.6(2) 4_445 1_565
O2 O1 O2 93.35(19) 1_665 1_565
O2 O1 O2 25.48(17) 3_465 1_565
O3 O1 O2 134.0(3) 1_556 1_565
O3 O1 O2 72.0(3) 3_566 1_565
O3 O1 O2 53.59(16) 4_456 1_565
La O1 O2 105.8(2) 1_556 1_565
La O1 O2 89.7(2) 2_566 1_565
La O1 O2 55.82(14) 4_456 1_565
O3 O1 O2 149.2(2) 4 1_565
O3 O1 O2 88.7(2) 3_455 1_565
O3 O1 O2 46.22(15) 1_565 1_565
Ga2 O1 O2 13.18(12) 1_566 1_565
Ga2 O1 O2 121.12(17) 1_556 1_565
Ga2 O1 O2 110.5(2) 1_666 1_565
O1 O1 O2 27.5(3) 2_465 1_565
O1 O1 O2 125.8(2) 2_455 1_565
O1 O1 O2 114.86(13) 2_565 1_565
O1 O1 O2 96.5(2) 1_554 1_565
O1 O1 O2 83.5(2) 1_556 1_565
Ga3 O1 O2 150.5(3) 4_446 1_565
Ga3 O1 O2 74.82(19) 1_666 1_565
Ga3 O1 O2 44.35(13) 2_465 1_565
O3 O1 O2 155.9(3) 5 1_565
O3 O1 O2 81.51(17) 2_455 1_565
O3 O1 O2 38.07(18) 6_565 1_565
O3 O1 O2 132.8(3) 4_556 1_565
O3 O1 O2 82.63(16) 3_456 1_565
O3 O1 O2 42.2(2) 1_566 1_565
O2 O1 O2 107.3(3) 1_554 1_565
O2 O1 O2 119.3(2) 3_564 1_565
O2 O1 O2 58.46(12) 4_454 1_565
O3 O1 O2 130.0(3) 6_554 1_565
O3 O1 O2 79.7(2) 5_454 1_565
O3 O1 O2 79.46(16) 2_564 1_565
O1 O1 O2 29.70(19) 2_466 1_565
O1 O1 O2 114.0(2) 2_456 1_565
O1 O1 O2 105.3(3) 2_566 1_565
O3 O1 O2 168.5(3) 2 1_565
O3 O1 O2 54.0(2) 6_455 1_565
O3 O1 O2 65.6(2) 5_565 1_565
La O1 O2 103.41(16) 2_455 1_565
La O1 O2 137.68(14) 4 1_565
La O1 O2 22.86(10) 1_565 1_565
O2 O1 O2 118.75(8) 3_455 1_565
O2 O1 O2 118.75(8) 4 1_565
Ga2 O1 O3 30.03(12) 2_565 6_556
La O1 O3 86.6(3) . 6_556
La O1 O3 101.8(3) 2_565 6_556
La O1 O3 137.8(4) 4_455 6_556
O2 O1 O3 118.6(3) 2_565 6_556
O2 O1 O3 136.8(3) 6 6_556
O2 O1 O3 163.2(4) 5_455 6_556
O2 O1 O3 14.5(4) 2_566 6_556
O2 O1 O3 43.0(3) 6_556 6_556
O2 O1 O3 58.9(4) 5_456 6_556
O3 O1 O3 53.6(3) 6 6_556
O3 O1 O3 98.8(4) 5_455 6_556
O3 O1 O3 98.8(4) 2_565 6_556
Ga2 O1 O3 149.97(12) 2_564 6_556
O2 O1 O3 60.7(3) 3_565 6_556
O2 O1 O3 70.5(4) . 6_556
O2 O1 O3 108.2(4) 4_455 6_556
Ga3 O1 O3 35.7(2) 2_565 6_556
Ga3 O1 O3 69.6(2) 1_556 6_556
Ga3 O1 O3 87.1(3) 4_456 6_556
O3 O1 O3 89.2(3) . 6_556
O3 O1 O3 135.3(2) 4_455 6_556
O3 O1 O3 123.3(4) 3_565 6_556
Ga3 O1 O3 108.61(12) 2_564 6_556
Ga3 O1 O3 132.55(12) . 6_556
Ga3 O1 O3 154.86(17) 4_455 6_556
Nb O1 O3 70.66(16) . 6_556
Ga1 O1 O3 70.66(16) . 6_556
Nb O1 O3 111.2(2) 1_455 6_556
Ga1 O1 O3 111.2(2) 1_455 6_556
Ga1 O1 O3 116.4(2) 1_565 6_556
Nb O1 O3 116.4(2) 1_565 6_556
O2 O1 O3 57.7(2) 4_445 6_556
O2 O1 O3 80.4(3) 1_665 6_556
O2 O1 O3 108.7(3) 3_465 6_556
O3 O1 O3 23.2(2) 1_556 6_556
O3 O1 O3 65.4(3) 3_566 6_556
O3 O1 O3 74.4(2) 4_456 6_556
La O1 O3 20.14(12) 1_556 6_556
La O1 O3 36.81(15) 2_566 6_556
La O1 O3 58.75(19) 4_456 6_556
O3 O1 O3 87.7(3) 4 6_556
O3 O1 O3 114.1(2) 3_455 6_556
O3 O1 O3 137.9(3) 1_565 6_556
Ga2 O1 O3 101.5(3) 1_566 6_556
Ga2 O1 O3 56.69(16) 1_556 6_556
Ga2 O1 O3 62.04(19) 1_666 6_556
O1 O1 O3 140.3(4) 2_465 6_556
O1 O1 O3 91.7(3) 2_455 6_556
O1 O1 O3 96.2(3) 2_565 6_556
O1 O1 O3 149.97(12) 1_554 6_556
O1 O1 O3 30.03(12) 1_556 6_556
Ga3 O1 O3 43.19(13) 4_446 6_556
Ga3 O1 O3 80.7(2) 1_666 6_556
Ga3 O1 O3 94.0(2) 2_465 6_556
O3 O1 O3 58.63(16) 5 6_556
O3 O1 O3 91.0(3) 2_455 6_556
O3 O1 O3 109.6(3) 6_565 6_556
O3 O1 O3 30.6(3) 4_556 6_556
O3 O1 O3 63.1(2) 3_456 6_556
O3 O1 O3 81.6(3) 1_566 6_556
O2 O1 O3 124.86(15) 1_554 6_556
O2 O1 O3 118.19(15) 3_564 6_556
O2 O1 O3 169.5(2) 4_454 6_556
O3 O1 O3 116.40(16) 6_554 6_556
O3 O1 O3 149.29(8) 5_454 6_556
O3 O1 O3 149.29(8) 2_564 6_556
O1 O1 O3 84.2(4) 2_466 6_556
O1 O1 O3 42.1(2) 2_456 6_556
O1 O1 O3 47.7(3) 2_566 6_556
O3 O1 O3 56.72(16) 2 6_556
O3 O1 O3 104.0(3) 6_455 6_556
O3 O1 O3 98.7(2) 5_565 6_556
La O1 O3 91.23(15) 2_455 6_556
La O1 O3 76.24(15) 4 6_556
La O1 O3 126.8(2) 1_565 6_556
O2 O1 O3 69.86(18) 3_455 6_556
O2 O1 O3 69.6(2) 4 6_556
O2 O1 O3 113.6(3) 1_565 6_556
Ga3 O3 Nb 112.4(5) 4_445 .
Ga3 O3 Ga1 112.4(5) 4_445 .
Nb O3 Ga1 0.0 . .
Ga3 O3 La 138.4(5) 4_445 .
Nb O3 La 105.1(5) . .
Ga1 O3 La 105.1(5) . .
Ga3 O3 Ga3 94.3(6) 4_445 2_564
Nb O3 Ga3 87.0(4) . 2_564
Ga1 O3 Ga3 87.0(4) . 2_564
La O3 Ga3 105.4(5) . 2_564
Ga3 O3 O3 155.2(9) 4_445 6
Nb O3 O3 48.4(3) . 6
Ga1 O3 O3 48.4(3) . 6
La O3 O3 56.7(3) . 6
Ga3 O3 O3 99.2(6) 2_564 6
Ga3 O3 O3 65.6(5) 4_445 3
Nb O3 O3 46.9(3) . 3
Ga1 O3 O3 46.9(3) . 3
La O3 O3 149.4(3) . 3
Ga3 O3 O3 87.4(3) 2_564 3
O3 O3 O3 94.28(8) 6 3
Ga3 O3 O3 105.5(3) 4_445 4
Nb O3 O3 46.9(3) . 4
Ga1 O3 O3 46.9(3) . 4
La O3 O3 113.2(6) . 4
Ga3 O3 O3 40.2(3) 2_564 4
O3 O3 O3 73.3(6) 6 4
O3 O3 O3 60.000(1) 3 4
Ga3 O3 O2 125.9(8) 4_445 2_565
Nb O3 O2 95.2(5) . 2_565
Ga1 O3 O2 95.2(5) . 2_565
La O3 O2 65.6(4) . 2_565
Ga3 O3 O2 39.8(4) 2_564 2_565
O3 O3 O2 76.1(6) 6 2_565
O3 O3 O2 120.8(6) 3 2_565
O3 O3 O2 61.3(6) 4 2_565
Ga3 O3 O3 62.6(5) 4_445 6_554
Nb O3 O3 119.0(6) . 6_554
Ga1 O3 O3 119.0(6) . 6_554
La O3 O3 113.6(5) . 6_554
Ga3 O3 O3 39.0(4) 2_564 6_554
O3 O3 O3 136.8(10) 6 6_554
O3 O3 O3 93.98(10) 3 6_554
O3 O3 O3 74.5(4) 4 6_554
O2 O3 O3 63.4(5) 2_565 6_554
Ga3 O3 O2 40.1(4) 4_445 5_445
Nb O3 O2 95.2(6) . 5_445
Ga1 O3 O2 95.2(6) . 5_445
La O3 O2 120.9(6) . 5_445
Ga3 O3 O2 131.0(5) 2_564 5_445
O3 O3 O2 118.4(9) 6 5_445
O3 O3 O2 61.3(6) 3 5_445
O3 O3 O2 120.7(6) 4 5_445
O2 O3 O2 165.5(8) 2_565 5_445
O3 O3 O2 102.7(6) 6_554 5_445
Ga3 O3 O2 36.3(3) 4_445 4_444
Nb O3 O2 148.5(5) . 4_444
Ga1 O3 O2 148.5(5) . 4_444
La O3 O2 103.9(4) . 4_444
Ga3 O3 O2 97.1(7) 2_564 4_444
O3 O3 O2 157.4(7) 6 4_444
O3 O3 O2 101.9(5) 3 4_444
O3 O3 O2 128.5(4) 4 4_444
O2 O3 O2 107.9(6) 2_565 4_444
O3 O3 O2 58.1(6) 6_554 4_444
O2 O3 O2 58.8(8) 5_445 4_444
Ga3 O3 O1 87.9(4) 4_445 2_455
Nb O3 O1 133.0(8) . 2_455
Ga1 O3 O1 133.0(8) . 2_455
La O3 O1 52.4(3) . 2_455
Ga3 O3 O1 135.1(5) 2_564 2_455
O3 O3 O1 96.8(6) 6 2_455
O3 O3 O1 132.8(7) 3 2_455
O3 O3 O1 165.4(6) 4 2_455
O2 O3 O1 106.4(4) 2_565 2_455
O3 O3 O1 108.0(4) 6_554 2_455
O2 O3 O1 73.2(4) 5_445 2_455
O2 O3 O1 60.7(5) 4_444 2_455
Ga3 O3 O3 100.8(5) 4_445 2
Nb O3 O3 36.4(5) . 2
Ga1 O3 O3 36.4(5) . 2
La O3 O3 98.5(6) . 2
Ga3 O3 O3 122.9(2) 2_564 2
O3 O3 O3 54.4(6) 6 2
O3 O3 O3 52.2(4) 3 2
O3 O3 O3 82.7(3) 4 2
O2 O3 O3 125.8(5) 2_565 2
O3 O3 O3 145.9(3) 6_554 2
O2 O3 O3 67.7(5) 5_445 2
O2 O3 O3 126.2(5) 4_444 2
O1 O3 O3 100.4(4) 2_455 2
Ga3 O3 O2 112.8(7) 4_445 4_445
Nb O3 O2 79.9(6) . 4_445
Ga1 O3 O2 79.9(6) . 4_445
La O3 O2 56.3(4) . 4_445
Ga3 O3 O2 152.7(4) 2_564 4_445
O3 O3 O2 54.5(6) 6 4_445
O3 O3 O2 100.5(5) 3 4_445
O3 O3 O2 123.4(3) 4 4_445
O2 O3 O2 117.4(5) 2_565 4_445
O3 O3 O2 161.1(4) 6_554 4_445
O2 O3 O2 74.4(5) 5_445 4_445
O2 O3 O2 106.5(6) 4_444 4_445
O1 O3 O2 53.2(4) 2_455 4_445
O3 O3 O2 50.9(4) 2 4_445
Ga3 O3 O3 22.7(4) 4_445 2_554
Nb O3 O3 99.4(4) . 2_554
Ga1 O3 O3 99.4(4) . 2_554
La O3 O3 155.5(7) . 2_554
Ga3 O3 O3 74.7(4) 2_564 2_554
O3 O3 O3 147.8(4) 6 2_554
O3 O3 O3 54.4(6) 3 2_554
O3 O3 O3 83.1(3) 4 2_554
O2 O3 O3 111.6(6) 2_565 2_554
O3 O3 O3 51.1(5) 6_554 2_554
O2 O3 O3 56.7(3) 5_445 2_554
O2 O3 O3 52.6(4) 4_444 2_554
O1 O3 O3 109.9(4) 2_455 2_554
O3 O3 O3 101.8(6) 2 2_554
O2 O3 O3 130.9(5) 4_445 2_554
Ga3 O3 Ga2 65.7(3) 4_445 .
Nb O3 Ga2 160.6(7) . .
Ga1 O3 Ga2 160.6(7) . .
La O3 Ga2 72.9(2) . .
Ga3 O3 Ga2 112.2(5) 2_564 .
O3 O3 Ga2 126.1(4) 6 .
O3 O3 Ga2 128.4(5) 3 .
O3 O3 Ga2 152.1(5) 4 .
O2 O3 Ga2 101.1(4) 2_565 .
O3 O3 Ga2 78.2(3) 6_554 .
O2 O3 Ga2 70.8(5) 5_445 .
O2 O3 Ga2 31.8(2) 4_444 .
O1 O3 Ga2 31.1(3) 2_455 .
O3 O3 Ga2 124.2(3) 2 .
O2 O3 Ga2 83.3(3) 4_445 .
O3 O3 Ga2 84.3(4) 2_554 .
Ga3 O3 Ga3 63.0(3) 4_445 1_655
Nb O3 Ga3 59.9(2) . 1_655
Ga1 O3 Ga3 59.9(2) . 1_655
La O3 Ga3 157.8(4) . 1_655
Ga3 O3 Ga3 60.2(2) 2_564 1_655
O3 O3 Ga3 106.4(2) 6 1_655
O3 O3 Ga3 28.73(16) 3 1_655
O3 O3 Ga3 44.6(3) 4 1_655
O2 O3 Ga3 97.8(4) 2_565 1_655
O3 O3 Ga3 67.2(3) 6_554 1_655
O2 O3 Ga3 78.9(4) 5_445 1_655
O2 O3 Ga3 95.1(4) 4_444 1_655
O1 O3 Ga3 149.8(4) 2_455 1_655
O3 O3 Ga3 78.8(3) 2 1_655
O2 O3 Ga3 128.8(5) 4_445 1_655
O3 O3 Ga3 42.7(2) 2_554 1_655
Ga2 O3 Ga3 126.9(3) . 1_655
Ga3 O3 La 74.3(4) 4_445 4_445
Nb O3 La 101.3(6) . 4_445
Ga1 O3 La 101.3(6) . 4_445
La O3 La 81.3(4) . 4_445
Ga3 O3 La 167.8(5) 2_564 4_445
O3 O3 La 93.0(8) 6 4_445
O3 O3 La 91.8(5) 3 4_445
O3 O3 La 146.6(5) 4 4_445
O2 O3 La 145.9(4) 2_565 4_445
O3 O3 La 129.0(5) 6_554 4_445
O2 O3 La 40.0(3) 5_445 4_445
O2 O3 La 71.1(5) 4_444 4_445
O1 O3 La 42.04(19) 2_455 4_445
O3 O3 La 64.9(2) 2 4_445
O2 O3 La 39.2(3) 4_445 4_445
O3 O3 La 95.0(2) 2_554 4_445
Ga2 O3 La 59.33(18) . 4_445
Ga3 O3 La 116.3(3) 1_655 4_445
Ga3 O3 O2 116.9(6) 4_445 6
Nb O3 O2 129.5(4) . 6
Ga1 O3 O2 129.5(4) . 6
La O3 O2 36.9(3) . 6
Ga3 O3 O2 79.3(4) 2_564 6
O3 O3 O2 86.1(4) 6 6
O3 O3 O2 166.6(6) 3 6
O3 O3 O2 107.6(6) 4 6
O2 O3 O2 46.3(4) 2_565 6
O3 O3 O2 76.9(4) 6_554 6
O2 O3 O2 129.9(6) 5_445 6
O2 O3 O2 81.8(3) 4_444 6
O1 O3 O2 60.2(2) 2_455 6
O3 O3 O2 135.2(6) 2 6
O2 O3 O2 90.6(4) 4_445 6
O3 O3 O2 122.5(7) 2_554 6
Ga2 O3 O2 59.9(2) . 6
Ga3 O3 O2 138.9(5) 1_655 6
La O3 O2 101.6(3) 4_445 6
Ga3 O3 O3 119.5(4) 4_445 5
Nb O3 O3 8.9(3) . 5
Ga1 O3 O3 8.9(3) . 5
La O3 O3 99.8(5) . 5
Ga3 O3 O3 81.5(3) 2_564 5
O3 O3 O3 43.6(3) 6 5
O3 O3 O3 53.9(5) 3 5
O3 O3 O3 42.1(3) 4 5
O2 O3 O3 86.6(3) 2_565 5
O3 O3 O3 116.2(5) 6_554 5
O2 O3 O3 104.0(5) 5_445 5
O2 O3 O3 155.8(4) 4_444 5
O1 O3 O3 134.9(7) 2_455 5
O3 O3 O3 43.3(3) 2 5
O2 O3 O3 82.3(5) 4_445 5
O3 O3 O3 104.4(3) 2_554 5
Ga2 O3 O3 165.6(7) . 5
Ga3 O3 O3 63.0(3) 1_655 5
La O3 O3 107.8(4) 4_445 5
O2 O3 O3 121.3(3) 6 5
Ga3 O3 Ga3 118.3(6) 4_445 4_446
Nb O3 Ga3 52.2(4) . 4_446
Ga1 O3 Ga3 52.2(4) . 4_446
La O3 Ga3 72.1(4) . 4_446
Ga3 O3 Ga3 134.1(4) 2_564 4_446
O3 O3 Ga3 39.7(5) 6 4_446
O3 O3 Ga3 79.1(2) 3 4_446
O3 O3 Ga3 97.07(13) 4 4_446
O2 O3 Ga3 115.4(4) 2_565 4_446
O3 O3 Ga3 171.1(3) 6_554 4_446
O2 O3 Ga3 78.9(5) 5_445 4_446
O2 O3 Ga3 128.4(6) 4_444 4_446
O1 O3 Ga3 80.9(4) 2_455 4_446
O3 O3 Ga3 26.8(3) 2 4_446
O2 O3 Ga3 27.8(2) 4_445 4_446
O3 O3 Ga3 126.0(6) 2_554 4_446
Ga2 O3 Ga3 110.4(4) . 4_446
Ga3 O3 Ga3 104.9(3) 1_655 4_446
La O3 Ga3 57.4(2) 4_445 4_446
O2 O3 Ga3 108.9(3) 6 4_446
O3 O3 Ga3 55.1(3) 5 4_446
Ga3 O3 Ga2 114.3(6) 4_445 2_564
Nb O3 Ga2 118.8(4) . 2_564
Ga1 O3 Ga2 118.8(4) . 2_564
La O3 Ga2 58.0(3) . 2_564
Ga3 O3 Ga2 52.6(3) 2_564 2_564
O3 O3 Ga2 90.4(5) 6 2_564
O3 O3 Ga2 139.9(5) 3 2_564
O3 O3 Ga2 83.6(5) 4 2_564
O2 O3 Ga2 24.0(2) 2_565 2_564
O3 O3 Ga2 57.9(3) 6_554 2_564
O2 O3 Ga2 145.6(6) 5_445 2_564
O2 O3 Ga2 87.3(5) 4_444 2_564
O1 O3 Ga2 85.8(2) 2_455 2_564
O3 O3 Ga2 144.6(5) 2 2_564
O2 O3 Ga2 114.2(3) 4_445 2_564
O3 O3 Ga2 108.8(6) 2_554 2_564
Ga2 O3 Ga2 77.1(2) . 2_564
Ga3 O3 Ga2 112.5(4) 1_655 2_564
La O3 Ga2 127.8(2) 4_445 2_564
O2 O3 Ga2 26.77(18) 6 2_564
O3 O3 Ga2 109.99(14) 5 2_564
Ga3 O3 Ga2 124.9(3) 4_446 2_564
Ga3 O3 O3 64.1(5) 4_445 5_554
Nb O3 O3 79.3(3) . 5_554
Ga1 O3 O3 79.3(3) . 5_554
La O3 O3 143.2(4) . 5_554
Ga3 O3 O3 37.8(2) 2_564 5_554
O3 O3 O3 117.3(4) 6 5_554
O3 O3 O3 55.3(3) 3 5_554
O3 O3 O3 44.2(4) 4 5_554
O2 O3 O3 77.6(4) 2_565 5_554
O3 O3 O3 41.9(3) 6_554 5_554
O2 O3 O3 94.5(4) 5_445 5_554
O2 O3 O3 85.0(6) 4_444 5_554
O1 O3 O3 145.2(6) 2_455 5_554
O3 O3 O3 104.7(3) 2 5_554
O2 O3 O3 155.4(5) 4_445 5_554
O3 O3 O3 41.6(3) 2_554 5_554
Ga2 O3 O3 114.2(5) . 5_554
Ga3 O3 O3 26.68(18) 1_655 5_554
La O3 O3 134.54(19) 4_445 5_554
O2 O3 O3 112.8(4) 6 5_554
O3 O3 O3 79.2(3) 5 5_554
Ga3 O3 O3 129.6(4) 4_446 5_554
Ga2 O3 O3 87.4(3) 2_564 5_554
Ga3 O3 Ga1 45.1(4) 4_445 1_554
Nb O3 Ga1 105.8(4) . 1_554
Ga1 O3 Ga1 105.8(4) . 1_554
La O3 Ga1 137.9(6) . 1_554
Ga3 O3 Ga1 49.2(2) 2_564 1_554
O3 O3 Ga1 144.2(6) 6 1_554
O3 O3 Ga1 71.03(11) 3 1_554
O3 O3 Ga1 71.03(11) 4 1_554
O2 O3 Ga1 83.8(5) 2_565 1_554
O3 O3 Ga1 24.59(19) 6_554 1_554
O2 O3 Ga1 83.8(3) 5_445 1_554
O2 O3 Ga1 57.5(4) 4_444 1_554
O1 O3 Ga1 117.4(4) 2_455 1_554
O3 O3 Ga1 123.2(4) 2 1_554
O2 O3 Ga1 157.9(4) 4_445 1_554
O3 O3 Ga1 28.0(3) 2_554 1_554
Ga2 O3 Ga1 86.4(3) . 1_554
Ga3 O3 Ga1 47.12(16) 1_655 1_554
La O3 Ga1 119.2(2) 4_445 1_554
O2 O3 Ga1 101.1(4) 6 1_554
O3 O3 Ga1 106.7(4) 5 1_554
Ga3 O3 Ga1 149.9(3) 4_446 1_554
Ga2 O3 Ga1 82.2(3) 2_564 1_554
O3 O3 Ga1 27.9(3) 5_554 1_554
Ga3 O3 Nb 45.1(4) 4_445 1_554
Nb O3 Nb 105.8(4) . 1_554
Ga1 O3 Nb 105.8(4) . 1_554
La O3 Nb 137.9(6) . 1_554
Ga3 O3 Nb 49.2(2) 2_564 1_554
O3 O3 Nb 144.2(6) 6 1_554
O3 O3 Nb 71.03(11) 3 1_554
O3 O3 Nb 71.03(11) 4 1_554
O2 O3 Nb 83.8(5) 2_565 1_554
O3 O3 Nb 24.59(19) 6_554 1_554
O2 O3 Nb 83.8(3) 5_445 1_554
O2 O3 Nb 57.5(4) 4_444 1_554
O1 O3 Nb 117.4(4) 2_455 1_554
O3 O3 Nb 123.2(4) 2 1_554
O2 O3 Nb 157.9(4) 4_445 1_554
O3 O3 Nb 28.0(3) 2_554 1_554
Ga2 O3 Nb 86.4(3) . 1_554
Ga3 O3 Nb 47.12(16) 1_655 1_554
La O3 Nb 119.2(2) 4_445 1_554
O2 O3 Nb 101.1(4) 6 1_554
O3 O3 Nb 106.7(4) 5 1_554
Ga3 O3 Nb 149.9(3) 4_446 1_554
Ga2 O3 Nb 82.2(3) 2_564 1_554
O3 O3 Nb 27.9(3) 5_554 1_554
Ga1 O3 Nb 0.0 1_554 1_554
Ga3 O3 O2 77.1(4) 4_445 1_554
Nb O3 O2 170.3(4) . 1_554
Ga1 O3 O2 170.3(4) . 1_554
La O3 O2 66.8(3) . 1_554
Ga3 O3 O2 90.1(4) 2_564 1_554
O3 O3 O2 123.2(2) 6 1_554
O3 O3 O2 142.3(3) 3 1_554
O3 O3 O2 130.1(5) 4 1_554
O2 O3 O2 76.8(3) 2_565 1_554
O3 O3 O2 62.6(3) 6_554 1_554
O2 O3 O2 93.7(4) 5_445 1_554
O2 O3 O2 41.1(4) 4_444 1_554
O1 O3 O2 46.7(3) 2_455 1_554
O3 O3 O2 146.8(3) 2 1_554
O2 O3 O2 98.8(3) 4_445 1_554
O3 O3 O2 88.7(6) 2_554 1_554
Ga2 O3 O2 24.83(18) . 1_554
Ga3 O3 O2 126.0(4) 1_655 1_554
La O3 O2 83.1(2) 4_445 1_554
O2 O3 O2 40.8(4) 6 1_554
O3 O3 O2 161.8(2) 5 1_554
Ga3 O3 O2 126.2(3) 4_446 1_554
Ga2 O3 O2 52.9(2) 2_564 1_554
O3 O3 O2 103.9(5) 5_554 1_554
Ga1 O3 O2 79.0(3) 1_554 1_554
Nb O3 O2 79.0(3) 1_554 1_554
Ga3 O3 La 67.5(4) 4_445 2
Nb O3 La 53.8(3) . 2
Ga1 O3 La 53.8(3) . 2
La O3 La 127.6(6) . 2
Ga3 O3 La 118.5(3) 2_564 2
O3 O3 La 87.8(5) 6 2
O3 O3 La 31.1(3) 3 2
O3 O3 La 86.8(4) 4 2
O2 O3 La 147.2(4) 2_565 2
O3 O3 La 118.4(3) 6_554 2
O2 O3 La 41.4(5) 5_445 2
O2 O3 La 98.0(4) 4_444 2
O1 O3 La 103.8(4) 2_455 2
O3 O3 La 33.8(2) 2 2
O2 O3 La 72.0(4) 4_445 2
O3 O3 La 69.0(4) 2_554 2
Ga2 O3 La 111.5(3) . 2
Ga3 O3 La 59.23(15) 1_655 2
La O3 La 61.8(2) 4_445 2
O2 O3 La 161.9(4) 6 2
O3 O3 La 62.68(13) 5 2
Ga3 O3 La 57.2(2) 4_446 2
Ga2 O3 La 170.4(3) 2_564 2
O3 O3 La 85.07(17) 5_554 2
Ga1 O3 La 93.83(18) 1_554 2
Nb O3 La 93.83(18) 1_554 2
O2 O3 La 135.1(3) 1_554 2
Ga3 O3 O1 158.0(6) 4_445 .
Nb O3 O1 88.8(3) . .
Ga1 O3 O1 88.8(3) . .
La O3 O1 29.42(15) . .
Ga3 O3 O1 80.3(3) 2_564 .
O3 O3 O1 46.2(3) 6 .
O3 O3 O1 134.7(4) 3 .
O3 O3 O1 84.1(5) 4 .
O2 O3 O1 41.7(4) 2_565 .
O3 O3 O1 102.6(5) 6_554 .
O2 O3 O1 148.5(5) 5_445 .
O2 O3 O1 122.7(4) 4_444 .
O1 O3 O1 81.3(2) 2_455 .
O3 O3 O1 100.0(5) 2 .
O2 O3 O1 75.6(3) 4_445 .
O3 O3 O1 153.1(7) 2_554 .
Ga2 O3 O1 96.4(2) . .
Ga3 O3 O1 128.7(3) 1_655 .
La O3 O1 108.6(3) 4_445 .
O2 O3 O1 41.2(3) 6 .
O3 O3 O1 81.1(3) 5 .
Ga3 O3 O1 79.1(3) 4_446 .
Ga2 O3 O1 46.1(2) 2_564 .
O3 O3 O1 116.9(2) 5_554 .
Ga1 O3 O1 125.1(4) 1_554 .
Nb O3 O1 125.1(4) 1_554 .
O2 O3 O1 81.6(3) 1_554 .
La O3 O1 133.7(4) 2 .
Ga3 O3 Ga3 153.3(5) 4_445 2_565
Nb O3 Ga3 41.6(2) . 2_565
Ga1 O3 Ga3 41.6(2) . 2_565
La O3 Ga3 64.1(3) . 2_565
Ga3 O3 Ga3 90.7(3) 2_564 2_565
O3 O3 Ga3 10.1(3) 6 2_565
O3 O3 Ga3 88.5(2) 3 2_565
O3 O3 Ga3 63.3(3) 4 2_565
O2 O3 Ga3 72.1(3) 2_565 2_565
O3 O3 Ga3 129.3(6) 6_554 2_565
O2 O3 Ga3 122.1(6) 5_445 2_565
O2 O3 Ga3 167.2(4) 4_444 2_565
O1 O3 Ga3 106.7(4) 2_455 2_565
O3 O3 Ga3 55.2(3) 2 2_565
O2 O3 Ga3 63.7(3) 4_445 2_565
O3 O3 Ga3 139.9(4) 2_554 2_565
Ga2 O3 Ga3 135.4(3) . 2_565
Ga3 O3 Ga3 97.5(2) 1_655 2_565
La O3 Ga3 101.4(4) 4_445 2_565
O2 O3 Ga3 89.8(3) 6 2_565
O3 O3 Ga3 35.6(3) 5 2_565
Ga3 O3 Ga3 45.78(16) 4_446 2_565
Ga2 O3 Ga3 89.5(2) 2_564 2_565
O3 O3 Ga3 107.3(3) 5_554 2_565
Ga1 O3 Ga3 134.2(3) 1_554 2_565
Nb O3 Ga3 134.2(3) 1_554 2_565
O2 O3 Ga3 129.2(3) 1_554 2_565
La O3 Ga3 87.0(3) 2 2_565
O1 O3 Ga3 48.7(2) . 2_565
Ga3 O3 La 64.3(4) 4_445 1_554
Nb O3 La 148.7(6) . 1_554
Ga1 O3 La 148.7(6) . 1_554
La O3 La 92.4(4) . 1_554
Ga3 O3 La 63.1(3) 2_564 1_554
O3 O3 La 140.5(5) 6 1_554
O3 O3 La 118.11(12) 3 1_554
O3 O3 La 102.5(3) 4 1_554
O2 O3 La 68.2(4) 2_565 1_554
O3 O3 La 30.11(16) 6_554 1_554
O2 O3 La 97.9(5) 5_445 1_554
O2 O3 La 40.1(5) 4_444 1_554
O1 O3 La 78.1(3) 2_455 1_554
O3 O3 La 165.0(4) 2 1_554
O2 O3 La 131.1(3) 4_445 1_554
O3 O3 La 65.4(5) 2_554 1_554
Ga2 O3 La 49.69(19) . 1_554
Ga3 O3 La 94.9(3) 1_655 1_554
La O3 La 107.0(2) 4_445 1_554
O2 O3 La 57.1(3) 6 1_554
O3 O3 La 144.5(5) 5 1_554
Ga3 O3 La 158.7(3) 4_446 1_554
Ga2 O3 La 50.39(18) 2_564 1_554
O3 O3 La 71.4(4) 5_554 1_554
Ga1 O3 La 48.05(18) 1_554 1_554
Nb O3 La 48.05(18) 1_554 1_554
O2 O3 La 32.56(19) 1_554 1_554
La O3 La 131.7(2) 2 1_554
O1 O3 La 94.6(3) . 1_554
Ga3 O3 La 139.7(3) 2_565 1_554
Ga3 O3 O2 94.5(7) 4_445 3_564
Nb O3 O2 87.9(4) . 3_564
Ga1 O3 O2 87.9(4) . 3_564
La O3 O2 104.5(5) . 3_564
Ga3 O3 O2 1.1(2) 2_564 3_564
O3 O3 O2 99.4(6) 6 3_564
O3 O3 O2 88.5(4) 3 3_564
O3 O3 O2 41.2(3) 4 3_564
O2 O3 O2 39.1(6) 2_565 3_564
O3 O3 O2 38.6(4) 6_554 3_564
O2 O3 O2 131.6(5) 5_445 3_564
O2 O3 O2 96.7(7) 4_444 3_564
O1 O3 O2 134.0(5) 2_455 3_564
O3 O3 O2 123.9(2) 2 3_564
O2 O3 O2 152.6(4) 4_445 3_564
O3 O3 O2 75.1(4) 2_554 3_564
Ga2 O3 O2 111.4(4) . 3_564
Ga3 O3 O2 61.2(3) 1_655 3_564
La O3 O2 167.6(4) 4_445 3_564
O2 O3 O2 78.3(4) 6 3_564
O3 O3 O2 82.3(3) 5 3_564
Ga3 O3 O2 134.7(3) 4_446 3_564
Ga2 O3 O2 51.5(3) 2_564 3_564
O3 O3 O2 38.6(3) 5_554 3_564
Ga1 O3 O2 49.4(3) 1_554 3_564
Nb O3 O2 49.4(3) 1_554 3_564
O2 O3 O2 89.1(4) 1_554 3_564
La O3 O2 119.5(3) 2 3_564
O1 O3 O2 79.7(4) . 3_564
Ga3 O3 O2 91.0(3) 2_565 3_564
La O3 O2 62.3(3) 1_554 3_564
Ga3 O3 O2 127.3(5) 4_445 .
Nb O3 O2 103.6(6) . .
Ga1 O3 O2 103.6(6) . .
La O3 O2 20.2(2) . .
Ga3 O3 O2 125.5(3) 2_564 .
O3 O3 O2 58.4(4) 6 .
O3 O3 O2 137.8(4) 3 .
O3 O3 O2 127.1(4) 4 .
O2 O3 O2 85.7(3) 2_565 .
O3 O3 O2 128.1(3) 6_554 .
O2 O3 O2 101.5(4) 5_445 .
O2 O3 O2 99.3(3) 4_444 .
O1 O3 O2 40.0(4) 2_455 .
O3 O3 O2 85.9(5) 2 .
O2 O3 O2 38.1(3) 4_445 .
O3 O3 O2 149.7(3) 2_554 .
Ga2 O3 O2 67.7(3) . .
Ga3 O3 O2 163.3(5) 1_655 .
La O3 O2 61.6(2) 4_445 .
O2 O3 O2 52.6(4) 6 .
O3 O3 O2 101.1(6) 5 .
Ga3 O3 O2 59.3(3) 4_446 .
Ga2 O3 O2 76.73(19) 2_564 .
O3 O3 O2 163.3(2) 5_554 .
Ga1 O3 O2 149.5(4) 1_554 .
Nb O3 O2 149.5(4) 1_554 .
O2 O3 O2 70.7(2) 1_554 .
La O3 O2 110.1(4) 2 .
O1 O3 O2 47.5(2) . .
Ga3 O3 O2 67.9(3) 2_565 .
La O3 O2 101.5(3) 1_554 .
O2 O3 O2 124.7(4) 3_564 .
Ga3 O3 Ga2 31.9(4) 4_445 2_554
Nb O3 Ga2 98.6(4) . 2_554
Ga1 O3 Ga2 98.6(4) . 2_554
La O3 Ga2 126.4(4) . 2_554
Ga3 O3 Ga2 123.5(4) 2_564 2_554
O3 O3 Ga2 126.0(8) 6 2_554
O3 O3 Ga2 60.3(5) 3 2_554
O3 O3 Ga2 118.0(4) 4 2_554
O2 O3 Ga2 157.7(5) 2_565 2_554
O3 O3 Ga2 94.5(4) 6_554 2_554
O2 O3 Ga2 8.2(3) 5_445 2_554
O2 O3 Ga2 53.3(4) 4_444 2_554
O1 O3 Ga2 76.4(2) 2_455 2_554
O3 O3 Ga2 74.0(2) 2 2_554
O2 O3 Ga2 82.4(4) 4_445 2_554
O3 O3 Ga2 48.81(18) 2_554 2_554
Ga2 O3 Ga2 69.46(18) . 2_554
Ga3 O3 Ga2 74.43(16) 1_655 2_554
La O3 Ga2 46.90(13) 4_445 2_554
O2 O3 Ga2 129.4(3) 6 2_554
O3 O3 Ga2 107.39(13) 5 2_554
Ga3 O3 Ga2 86.9(3) 4_446 2_554
Ga2 O3 Ga2 140.6(3) 2_564 2_554
O3 O3 Ga2 87.8(2) 5_554 2_554
Ga1 O3 Ga2 75.63(16) 1_554 2_554
Nb O3 Ga2 75.63(16) 1_554 2_554
O2 O3 Ga2 90.7(3) 1_554 2_554
La O3 Ga2 45.06(12) 2 2_554
O1 O3 Ga2 155.3(4) . 2_554
Ga3 O3 Ga2 129.1(4) 2_565 2_554
La O3 Ga2 91.3(2) 1_554 2_554
O2 O3 Ga2 123.9(4) 3_564 2_554
O2 O3 Ga2 107.8(3) . 2_554
Ga3 O3 La 145.8(7) 4_445 2_565
Nb O3 La 74.3(3) . 2_565
Ga1 O3 La 74.3(3) . 2_565
La O3 La 61.7(2) . 2_565
Ga3 O3 La 51.74(19) 2_564 2_565
O3 O3 La 53.0(5) 6 2_565
O3 O3 La 110.8(4) 3 2_565
O3 O3 La 53.1(5) 4 2_565
O2 O3 La 24.1(3) 2_565 2_565
O3 O3 La 84.5(5) 6_554 2_565
O2 O3 La 169.3(6) 5_445 2_565
O2 O3 La 131.8(6) 4_444 2_565
O1 O3 La 112.5(3) 2_455 2_565
O3 O3 La 101.9(4) 2 2_565
O2 O3 La 101.4(3) 4_445 2_565
O3 O3 La 126.0(4) 2_554 2_565
Ga2 O3 La 118.9(3) . 2_565
Ga3 O3 La 97.0(2) 1_655 2_565
La O3 La 139.0(3) 4_445 2_565
O2 O3 La 59.2(2) 6 2_565
O3 O3 La 65.39(15) 5 2_565
Ga3 O3 La 92.7(2) 4_446 2_565
Ga2 O3 La 45.08(13) 2_564 2_565
O3 O3 La 85.53(15) 5_554 2_565
Ga1 O3 La 100.8(3) 1_554 2_565
Nb O3 La 100.8(3) 1_554 2_565
O2 O3 La 96.7(3) 1_554 2_565
La O3 La 128.1(2) 2 2_565
O1 O3 La 32.36(10) . 2_565
Ga3 O3 La 48.17(10) 2_565 2_565
La O3 La 92.3(3) 1_554 2_565
O2 O3 La 51.5(3) 3_564 2_565
O2 O3 La 79.6(2) . 2_565
Ga2 O3 La 171.0(2) 2_554 2_565
Ga3 O3 O2 149.6(5) 4_445 3_565
Nb O3 O2 45.6(3) . 3_565
Ga1 O3 O2 45.6(3) . 3_565
La O3 O2 71.7(3) . 3_565
Ga3 O3 O2 67.5(3) 2_564 3_565
O3 O3 O2 32.0(5) 6 3_565
O3 O3 O2 88.6(4) 3 3_565
O3 O3 O2 44.9(4) 4 3_565
O2 O3 O2 53.4(4) 2_565 3_565
O3 O3 O2 106.1(6) 6_554 3_565
O2 O3 O2 139.4(6) 5_445 3_565
O2 O3 O2 161.3(7) 4_444 3_565
O1 O3 O2 122.3(5) 2_455 3_565
O3 O3 O2 72.4(3) 2 3_565
O2 O3 O2 86.4(4) 4_445 3_565
O3 O3 O2 127.8(3) 2_554 3_565
Ga2 O3 O2 142.9(3) . 3_565
Ga3 O3 O2 86.6(3) 1_655 3_565
La O3 O2 124.6(4) 4_445 3_565
O2 O3 O2 84.7(3) 6 3_565
O3 O3 O2 36.9(3) 5 3_565
Ga3 O3 O2 68.5(2) 4_446 3_565
Ga2 O3 O2 74.9(2) 2_564 3_565
O3 O3 O2 88.4(3) 5_554 3_565
Ga1 O3 O2 113.1(4) 1_554 3_565
Nb O3 O2 113.1(4) 1_554 3_565
O2 O3 O2 124.9(4) 1_554 3_565
La O3 O2 98.9(3) 2 3_565
O1 O3 O2 46.5(3) . 3_565
Ga3 O3 O2 23.23(17) 2_565 3_565
La O3 O2 121.2(4) 1_554 3_565
O2 O3 O2 67.8(2) 3_564 3_565
O2 O3 O2 82.5(5) . 3_565
Ga2 O3 O2 144.0(3) 2_554 3_565
La O3 O2 29.88(15) 2_565 3_565
Ga3 O3 Ga2 118.2(5) 4_445 1_556
Nb O3 Ga2 91.7(5) . 1_556
Ga1 O3 Ga2 91.7(5) . 1_556
La O3 Ga2 41.5(3) . 1_556
Ga3 O3 Ga2 145.0(3) 2_564 1_556
O3 O3 Ga2 56.3(5) 6 1_556
O3 O3 Ga2 116.6(4) 3 1_556
O3 O3 Ga2 129.56(17) 4 1_556
O2 O3 Ga2 105.7(4) 2_565 1_556
O3 O3 Ga2 147.39(16) 6_554 1_556
O2 O3 Ga2 84.0(4) 5_445 1_556
O2 O3 Ga2 101.9(5) 4_444 1_556
O1 O3 Ga2 42.8(3) 2_455 1_556
O3 O3 Ga2 66.3(3) 2 1_556
O2 O3 Ga2 16.1(2) 4_445 1_556
O3 O3 Ga2 139.7(3) 2_554 1_556
Ga2 O3 Ga2 73.9(2) . 1_556
Ga3 O3 Ga2 144.8(4) 1_655 1_556
La O3 Ga2 44.76(16) 4_445 1_556
O2 O3 Ga2 74.6(2) 6 1_556
O3 O3 Ga2 92.3(5) 5 1_556
Ga3 O3 Ga2 41.14(15) 4_446 1_556
Ga2 O3 Ga2 99.00(18) 2_564 1_556
O3 O3 Ga2 170.7(5) 5_554 1_556
Ga1 O3 Ga2 159.4(2) 1_554 1_556
Nb O3 Ga2 159.4(2) 1_554 1_556
O2 O3 Ga2 85.3(2) 1_554 1_556
La O3 Ga2 87.8(3) 2 1_556
O1 O3 Ga2 64.7(2) . 1_556
Ga3 O3 Ga2 66.4(2) 2_565 1_556
La O3 Ga2 117.86(19) 1_554 1_556
O2 O3 Ga2 144.4(4) 3_564 1_556
O2 O3 Ga2 22.31(16) . 1_556
Ga2 O3 Ga2 91.4(3) 2_554 1_556
La O3 Ga2 94.27(19) 2_565 1_556
O2 O3 Ga2 86.9(3) 3_565 1_556
Ga3 O3 O2 82.2(3) 4_445 6_655
Nb O3 O2 42.1(3) . 6_655
Ga1 O3 O2 42.1(3) . 6_655
La O3 O2 139.4(4) . 6_655
Ga3 O3 O2 59.8(2) 2_564 6_655
O3 O3 O2 86.9(3) 6 6_655
O3 O3 O2 30.3(3) 3 6_655
O3 O3 O2 30.2(4) 4 6_655
O2 O3 O2 90.5(3) 2_565 6_655
O3 O3 O2 79.5(3) 6_554 6_655
O2 O3 O2 90.5(3) 5_445 6_655
O2 O3 O2 114.9(3) 4_444 6_655
O1 O3 O2 163.1(4) 2_455 6_655
O3 O3 O2 68.3(3) 2 6_655
O2 O3 O2 118.8(4) 4_445 6_655
O3 O3 O2 62.5(3) 2_554 6_655
Ga2 O3 O2 146.7(4) . 6_655
Ga3 O3 O2 19.8(2) 1_655 6_655
La O3 O2 121.5(3) 4_445 6_655
O2 O3 O2 136.7(4) 6 6_655
O3 O3 O2 43.9(4) 5 6_655
Ga3 O3 O2 91.8(3) 4_446 6_655
Ga2 O3 O2 110.7(3) 2_564 6_655
O3 O3 O2 38.0(3) 5_554 6_655
Ga1 O3 O2 63.8(2) 1_554 6_655
Nb O3 O2 63.8(2) 1_554 6_655
O2 O3 O2 141.9(4) 1_554 6_655
La O3 O2 59.76(18) 2 6_655
O1 O3 O2 112.4(3) . 6_655
Ga3 O3 O2 77.8(3) 2_565 6_655
La O3 O2 109.3(3) 1_554 6_655
O2 O3 O2 60.8(3) 3_564 6_655
O2 O3 O2 145.0(3) . 6_655
Ga2 O3 O2 88.1(2) 2_554 6_655
La O3 O2 82.9(3) 2_565 6_655
O2 O3 O2 67.7(5) 3_565 6_655
Ga2 O3 O2 132.8(4) 1_556 6_655
Ga3 O3 O1 93.9(6) 4_445 1_554
Nb O3 O1 128.7(5) . 1_554
Ga1 O3 O1 128.7(5) . 1_554
La O3 O1 75.6(4) . 1_554
Ga3 O3 O1 46.2(2) 2_564 1_554
O3 O3 O1 110.4(6) 6 1_554
O3 O3 O1 129.1(4) 3 1_554
O3 O3 O1 84.7(4) 4 1_554
O2 O3 O1 36.9(3) 2_565 1_554
O3 O3 O1 38.3(3) 6_554 1_554
O2 O3 O1 129.4(5) 5_445 1_554
O2 O3 O1 71.0(5) 4_444 1_554
O1 O3 O1 88.9(3) 2_455 1_554
O3 O3 O1 162.7(3) 2 1_554
O2 O3 O1 130.2(3) 4_445 1_554
O3 O3 O1 88.5(6) 2_554 1_554
Ga2 O3 O1 70.2(3) . 1_554
Ga3 O3 O1 100.4(4) 1_655 1_554
La O3 O1 128.7(2) 4_445 1_554
O2 O3 O1 39.7(3) 6 1_554
O3 O3 O1 120.8(2) 5 1_554
Ga3 O3 O1 145.5(3) 4_446 1_554
Ga2 O3 O1 20.74(17) 2_564 1_554
O3 O3 O1 73.8(3) 5_554 1_554
Ga1 O3 O1 62.9(3) 1_554 1_554
Nb O3 O1 62.9(3) 1_554 1_554
O2 O3 O1 45.7(2) 1_554 1_554
La O3 O1 156.7(4) 2 1_554
O1 O3 O1 66.83(19) . 1_554
Ga3 O3 O1 108.3(3) 2_565 1_554
La O3 O1 31.50(18) 1_554 1_554
O2 O3 O1 45.1(2) 3_564 1_554
O2 O3 O1 92.3(2) . 1_554
Ga2 O3 O1 122.7(3) 2_554 1_554
La O3 O1 60.9(2) 2_565 1_554
O2 O3 O1 90.3(3) 3_565 1_554
Ga2 O3 O1 114.2(2) 1_556 1_554
O2 O3 O1 105.4(3) 6_655 1_554
Ga3 O3 O1 72.2(5) 4_445 1_545
Nb O3 O1 74.1(5) . 1_545
Ga1 O3 O1 74.1(5) . 1_545
La O3 O1 102.4(5) . 1_545
Ga3 O3 O1 149.7(3) 2_564 1_545
O3 O3 O1 86.0(8) 6 1_545
O3 O3 O1 62.3(4) 3 1_545
O3 O3 O1 116.1(4) 4 1_545
O2 O3 O1 161.9(5) 2_565 1_545
O3 O3 O1 134.6(5) 6_554 1_545
O2 O3 O1 32.5(4) 5_445 1_545
O2 O3 O1 87.7(5) 4_444 1_545
O1 O3 O1 72.9(3) 2_455 1_545
O3 O3 O1 39.53(19) 2 1_545
O2 O3 O1 47.1(3) 4_445 1_545
O3 O3 O1 85.0(4) 2_554 1_545
Ga2 O3 O1 87.3(3) . 1_545
Ga3 O3 O1 89.6(2) 1_655 1_545
La O3 O1 30.95(12) 4_445 1_545
O2 O3 O1 131.0(3) 6 1_545
O3 O3 O1 82.1(3) 5 1_545
Ga3 O3 O1 46.5(3) 4_446 1_545
Ga2 O3 O1 157.7(3) 2_564 1_545
O3 O3 O1 113.73(16) 5_554 1_545
Ga1 O3 O1 113.0(3) 1_554 1_545
Nb O3 O1 113.0(3) 1_554 1_545
O2 O3 O1 112.1(3) 1_554 1_545
La O3 O1 31.41(11) 2 1_545
O1 O3 O1 121.9(5) . 1_545
Ga3 O3 O1 90.6(4) 2_565 1_545
La O3 O1 127.8(3) 1_554 1_545
O2 O3 O1 150.7(3) 3_564 1_545
O2 O3 O1 82.7(3) . 1_545
Ga2 O3 O1 40.5(2) 2_554 1_545
La O3 O1 138.7(4) 2_565 1_545
O2 O3 O1 111.0(4) 3_565 1_545
Ga2 O3 O1 60.9(2) 1_556 1_545
O2 O3 O1 91.0(2) 6_655 1_545
O1 O3 O1 157.1(3) 1_554 1_545
Ga3 O3 La 115.2(4) 4_445 4
Nb O3 La 34.7(3) . 4
Ga1 O3 La 34.7(3) . 4
La O3 La 105.8(3) . 4
Ga3 O3 La 52.83(17) 2_564 4
O3 O3 La 59.9(3) 6 4
O3 O3 La 59.9(3) 3 4
O3 O3 La 14.36(17) 4 4
O2 O3 La 65.4(3) 2_565 4
O3 O3 La 88.7(4) 6_554 4
O2 O3 La 120.6(5) 5_445 4
O2 O3 La 142.4(6) 4_444 4
O1 O3 La 156.2(4) 2_455 4
O3 O3 La 71.1(2) 2 4
O2 O3 La 109.0(4) 4_445 4
O3 O3 La 93.78(15) 2_554 4
Ga2 O3 La 164.7(5) . 4
Ga3 O3 La 52.27(12) 1_655 4
La O3 La 136.0(4) 4_445 4
O2 O3 La 109.5(3) 6 4
O3 O3 La 28.67(17) 5 4
Ga3 O3 La 83.0(2) 4_446 4
Ga2 O3 La 89.2(2) 2_564 4
O3 O3 La 57.4(2) 5_554 4
Ga1 O3 La 84.9(2) 1_554 4
Nb O3 La 84.9(2) 1_554 4
O2 O3 La 140.2(4) 1_554 4
La O3 La 81.75(16) 2 4
O1 O3 La 78.48(16) . 4
Ga3 O3 La 49.88(10) 2_565 4
La O3 La 115.8(3) 1_554 4
O2 O3 La 53.66(18) 3_564 4
O2 O3 La 116.3(4) . 4
Ga2 O3 La 120.15(19) 2_554 4
La O3 La 50.91(11) 2_565 4
O2 O3 La 34.3(2) 3_565 4
Ga2 O3 La 115.7(3) 1_556 4
O2 O3 La 34.0(2) 6_655 4
O1 O3 La 94.6(2) 1_554 4
O1 O3 La 107.7(3) 1_545 4
Ga3 O3 Ga3 98.8(4) 4_445 .
Nb O3 Ga3 148.8(4) . .
Ga1 O3 Ga3 148.8(4) . .
La O3 Ga3 46.7(2) . .
Ga3 O3 Ga3 88.8(3) 2_564 .
O3 O3 Ga3 102.11(15) 6 .
O3 O3 Ga3 163.57(19) 3 .
O3 O3 Ga3 123.7(6) 4 .
O2 O3 Ga3 63.2(3) 2_565 .
O3 O3 Ga3 73.28(19) 6_554 .
O2 O3 Ga3 110.6(5) 5_445 .
O2 O3 Ga3 62.7(3) 4_444 .
O1 O3 Ga3 46.76(19) 2_455 .
O3 O3 Ga3 140.8(4) 2 .
O2 O3 Ga3 90.1(3) 4_445 .
O3 O3 Ga3 109.2(6) 2_554 .
Ga2 O3 Ga3 40.02(11) . .
Ga3 O3 Ga3 140.4(4) 1_655 .
La O3 Ga3 88.57(17) 4_445 .
O2 O3 Ga3 20.1(2) 6 .
O3 O3 Ga3 141.0(2) 5 .
Ga3 O3 Ga3 114.5(2) 4_446 .
Ga2 O3 Ga3 40.11(10) 2_564 .
O3 O3 Ga3 114.4(4) 5_554 .
Ga1 O3 Ga3 94.5(3) 1_554 .
Nb O3 Ga3 94.5(3) 1_554 .
O2 O3 Ga3 21.73(17) 1_554 .
La O3 Ga3 149.4(3) 2 .
O1 O3 Ga3 60.00(18) . .
Ga3 O3 Ga3 107.55(18) 2_565 .
La O3 Ga3 46.60(12) 1_554 .
O2 O3 Ga3 87.7(3) 3_564 .
O2 O3 Ga3 55.4(2) . .
Ga2 O3 Ga3 109.44(19) 2_554 .
La O3 Ga3 78.91(17) 2_565 .
O2 O3 Ga3 104.7(3) 3_565 .
Ga2 O3 Ga3 74.52(13) 1_556 .
O2 O3 Ga3 148.4(4) 6_655 .
O1 O3 Ga3 43.10(12) 1_554 .
O1 O3 Ga3 119.5(2) 1_545 .
La O3 Ga3 128.3(3) 4 .
Ga3 O3 Ga3 113.8(4) 4_445 1_656
Nb O3 Ga3 12.5(3) . 1_656
Ga1 O3 Ga3 12.5(3) . 1_656
La O3 Ga3 99.0(4) . 1_656
Ga3 O3 Ga3 99.2(3) 2_564 1_656
O3 O3 Ga3 43.7(2) 6 1_656
O3 O3 Ga3 50.87(16) 3 1_656
O3 O3 Ga3 59.20(13) 4 1_656
O2 O3 Ga3 102.9(3) 2_565 1_656
O3 O3 Ga3 131.2(3) 6_554 1_656
O2 O3 Ga3 89.2(5) 5_445 1_656
O2 O3 Ga3 147.1(5) 4_444 1_656
O1 O3 Ga3 120.7(5) 2_455 1_656
O3 O3 Ga3 25.15(18) 2 1_656
O2 O3 Ga3 67.7(3) 4_445 1_656
O3 O3 Ga3 105.2(4) 2_554 1_656
Ga2 O3 Ga3 148.5(4) . 1_656
Ga3 O3 Ga3 69.15(17) 1_655 1_656
La O3 Ga3 89.7(3) 4_445 1_656
O2 O3 Ga3 129.3(3) 6 1_656
O3 O3 Ga3 18.22(16) 5 1_656
Ga3 O3 Ga3 39.95(13) 4_446 1_656
Ga2 O3 Ga3 125.1(2) 2_564 1_656
O3 O3 Ga3 90.7(3) 5_554 1_656
Ga1 O3 Ga3 116.09(19) 1_554 1_656
Nb O3 Ga3 116.09(19) 1_554 1_656
O2 O3 Ga3 164.9(4) 1_554 1_656
La O3 Ga3 49.13(14) 2 1_656
O1 O3 Ga3 88.2(3) . 1_656
Ga3 O3 Ga3 39.51(12) 2_565 1_656
La O3 Ga3 161.1(3) 1_554 1_656
O2 O3 Ga3 100.1(2) 3_564 1_656
O2 O3 Ga3 94.1(4) . 1_656
Ga2 O3 Ga3 94.0(2) 2_554 1_656
La O3 Ga3 80.09(16) 2_565 1_656
O2 O3 Ga3 50.27(18) 3_565 1_656
Ga2 O3 Ga3 80.2(2) 1_556 1_656
O2 O3 Ga3 52.8(2) 6_655 1_656
O1 O3 Ga3 138.6(3) 1_554 1_656
O1 O3 Ga3 64.3(2) 1_545 1_656
La O3 Ga3 46.51(9) 4 1_656
Ga3 O3 Ga3 145.6(2) . 1_656
Ga3 O3 O3 136.7(5) 4_445 1_556
Nb O3 O3 52.1(4) . 1_556
Ga1 O3 O3 52.1(4) . 1_556
La O3 O3 59.5(4) . 1_556
Ga3 O3 O3 121.0(3) 2_564 1_556
O3 O3 O3 22.4(7) 6 1_556
O3 O3 O3 90.0 3 1_556
O3 O3 O3 90.000(1) 4 1_556
O2 O3 O3 97.2(4) 2_565 1_556
O3 O3 O3 159.2(4) 6_554 1_556
O2 O3 O3 97.1(4) 5_445 1_556
O2 O3 O3 140.6(5) 4_444 1_556
O1 O3 O3 83.6(4) 2_455 1_556
O3 O3 O3 40.3(4) 2 1_556
O2 O3 O3 34.1(2) 4_445 1_556
O3 O3 O3 142.0(5) 2_554 1_556
Ga2 O3 O3 114.8(3) . 1_556
Ga3 O3 O3 111.3(2) 1_655 1_556
La O3 O3 71.1(2) 4_445 1_556
O2 O3 O3 95.2(3) 6 1_556
O3 O3 O3 51.6(4) 5 1_556
Ga3 O3 O3 18.38(15) 4_446 1_556
Ga2 O3 O3 107.42(19) 2_564 1_556
O3 O3 O3 130.8(3) 5_554 1_556
Ga1 O3 O3 157.95(13) 1_554 1_556
Nb O3 O3 157.95(13) 1_554 1_556
O2 O3 O3 122.7(2) 1_554 1_556
La O3 O3 73.43(18) 2 1_556
O1 O3 O3 61.3(3) . 1_556
Ga3 O3 O3 30.3(2) 2_565 1_556
La O3 O3 151.85(12) 1_554 1_556
O2 O3 O3 121.3(3) 3_564 1_556
O2 O3 O3 52.0(3) . 1_556
Ga2 O3 O3 105.2(2) 2_554 1_556
La O3 O3 75.0(2) 2_565 1_556
O2 O3 O3 53.5(3) 3_565 1_556
Ga2 O3 O3 40.85(13) 1_556 1_556
O2 O3 O3 94.2(2) 6_655 1_556
O1 O3 O3 128.2(2) 1_554 1_556
O1 O3 O3 64.7(2) 1_545 1_556
La O3 O3 75.69(18) 4 1_556
Ga3 O3 O3 105.61(17) . 1_556
Ga3 O3 O3 42.12(13) 1_656 1_556
Ga3 O3 O3 43.4(5) 4_445 1_554
Nb O3 O3 127.9(4) . 1_554
Ga1 O3 O3 127.9(4) . 1_554
La O3 O3 120.5(4) . 1_554
Ga3 O3 O3 59.0(3) 2_564 1_554
O3 O3 O3 157.6(7) 6 1_554
O3 O3 O3 90.0 3 1_554
O3 O3 O3 90.000(2) 4 1_554
O2 O3 O3 82.8(4) 2_565 1_554
O3 O3 O3 20.8(4) 6_554 1_554
O2 O3 O3 82.9(4) 5_445 1_554
O2 O3 O3 39.4(5) 4_444 1_554
O1 O3 O3 96.4(4) 2_455 1_554
O3 O3 O3 139.7(4) 2 1_554
O2 O3 O3 145.9(2) 4_445 1_554
O3 O3 O3 38.0(5) 2_554 1_554
Ga2 O3 O3 65.2(3) . 1_554
Ga3 O3 O3 68.7(2) 1_655 1_554
La O3 O3 108.9(2) 4_445 1_554
O2 O3 O3 84.8(3) 6 1_554
O3 O3 O3 128.4(4) 5 1_554
Ga3 O3 O3 161.62(15) 4_446 1_554
Ga2 O3 O3 72.58(19) 2_564 1_554
O3 O3 O3 49.2(3) 5_554 1_554
Ga1 O3 O3 22.05(13) 1_554 1_554
Nb O3 O3 22.05(13) 1_554 1_554
O2 O3 O3 57.3(2) 1_554 1_554
La O3 O3 106.58(18) 2 1_554
O1 O3 O3 118.7(3) . 1_554
Ga3 O3 O3 149.7(2) 2_565 1_554
La O3 O3 28.15(12) 1_554 1_554
O2 O3 O3 58.7(3) 3_564 1_554
O2 O3 O3 128.0(3) . 1_554
Ga2 O3 O3 74.8(2) 2_554 1_554
La O3 O3 105.0(2) 2_565 1_554
O2 O3 O3 126.5(3) 3_565 1_554
Ga2 O3 O3 139.15(13) 1_556 1_554
O2 O3 O3 85.8(2) 6_655 1_554
O1 O3 O3 51.8(2) 1_554 1_554
O1 O3 O3 115.3(2) 1_545 1_554
La O3 O3 104.31(18) 4 1_554
Ga3 O3 O3 74.39(17) . 1_554
Ga3 O3 O3 137.88(13) 1_656 1_554
O3 O3 O3 179.999(1) 1_556 1_554
Ga3 O3 O2 57.4(3) 4_445 3_454
Nb O3 O2 154.3(6) . 3_454
Ga1 O3 O2 154.3(6) . 3_454
La O3 O2 81.0(3) . 3_454
Ga3 O3 O2 115.9(5) 2_564 3_454
O3 O3 O2 131.2(6) 6 3_454
O3 O3 O2 118.8(5) 3 3_454
O3 O3 O2 153.4(3) 4 3_454
O2 O3 O2 109.8(4) 2_565 3_454
O3 O3 O2 79.1(4) 6_554 3_454
O2 O3 O2 61.4(3) 5_445 3_454
O2 O3 O2 26.2(2) 4_444 3_454
O1 O3 O2 34.5(4) 2_455 3_454
O3 O3 O2 118.6(2) 2 3_454
O2 O3 O2 83.3(3) 4_445 3_454
O3 O3 O2 77.3(4) 2_554 3_454
Ga2 O3 O2 9.7(2) . 3_454
Ga3 O3 O2 119.9(4) 1_655 3_454
La O3 O2 54.30(17) 4_445 3_454
O2 O3 O2 69.6(4) 6 3_454
O3 O3 O2 161.9(4) 5 3_454
Ga3 O3 O2 109.0(3) 4_446 3_454
Ga2 O3 O2 85.9(3) 2_564 3_454
O3 O3 O2 111.0(5) 5_554 3_454
Ga1 O3 O2 83.3(3) 1_554 3_454
Nb O3 O2 83.3(3) 1_554 3_454
O2 O3 O2 33.02(18) 1_554 3_454
La O3 O2 102.4(3) 2 3_454
O1 O3 O2 105.7(3) . 3_454
Ga3 O3 O2 141.1(4) 2_565 3_454
La O3 O2 52.89(18) 1_554 3_454
O2 O3 O2 115.1(4) 3_564 3_454
O2 O3 O2 73.47(14) . 3_454
Ga2 O3 O2 59.8(2) 2_554 3_454
La O3 O2 128.5(3) 2_565 3_454
O2 O3 O2 152.1(5) 3_565 3_454
Ga2 O3 O2 76.3(3) 1_556 3_454
O2 O3 O2 139.4(2) 6_655 3_454
O1 O3 O2 77.0(2) 1_554 3_454
O1 O3 O2 80.2(2) 1_545 3_454
La O3 O2 167.7(4) 4 3_454
Ga3 O3 O2 49.6(2) . 3_454
Ga3 O3 O2 143.7(4) 1_656 3_454
O3 O3 O2 116.5(3) 1_556 3_454
O3 O3 O2 63.5(3) 1_554 3_454
Ga3 O3 O2 49.0(3) 4_445 1_654
Nb O3 O2 68.8(3) . 1_654
Ga1 O3 O2 68.8(3) . 1_654
La O3 O2 172.5(4) . 1_654
Ga3 O3 O2 70.6(2) 2_564 1_654
O3 O3 O2 117.0(3) 6 1_654
O3 O3 O2 27.0(3) 3 1_654
O3 O3 O2 59.6(4) 4 1_654
O2 O3 O2 109.9(5) 2_565 1_654
O3 O3 O2 67.5(3) 6_554 1_654
O2 O3 O2 65.0(4) 5_445 1_654
O2 O3 O2 83.1(4) 4_444 1_654
O1 O3 O2 134.9(4) 2_455 1_654
O3 O3 O2 79.1(3) 2 1_654
O2 O3 O2 124.8(4) 4_445 1_654
O3 O3 O2 30.8(4) 2_554 1_654
Ga2 O3 O2 114.3(4) . 1_654
Ga3 O3 O2 14.92(19) 1_655 1_654
La O3 O2 103.8(3) 4_445 1_654
O2 O3 O2 144.2(4) 6 1_654
O3 O3 O2 73.6(3) 5 1_654
Ga3 O3 O2 105.9(3) 4_446 1_654
Ga2 O3 O2 120.5(4) 2_564 1_654
O3 O3 O2 33.36(19) 5_554 1_654
Ga1 O3 O2 44.1(2) 1_554 1_654
Nb O3 O2 44.1(2) 1_554 1_654
O2 O3 O2 118.8(5) 1_554 1_654
La O3 O2 52.80(16) 2 1_654
O1 O3 O2 143.6(3) . 1_654
Ga3 O3 O2 109.1(3) 2_565 1_654
La O3 O2 91.3(3) 1_554 1_654
O2 O3 O2 71.5(3) 3_564 1_654
O2 O3 O2 162.8(5) . 1_654
Ga2 O3 O2 60.0(2) 2_554 1_654
La O3 O2 111.6(3) 2_565 1_654
O2 O3 O2 100.81(17) 3_565 1_654
Ga2 O3 O2 140.5(4) 1_556 1_654
O2 O3 O2 33.1(4) 6_655 1_654
O1 O3 O2 104.6(4) 1_554 1_654
O1 O3 O2 80.4(2) 1_545 1_654
La O3 O2 66.7(2) 4 1_654
Ga3 O3 O2 137.7(4) . 1_654
Ga3 O3 O2 75.8(2) 1_656 1_654
O3 O3 O2 116.6(3) 1_556 1_654
O3 O3 O2 63.4(3) 1_554 1_654
O2 O3 O2 106.4(5) 3_454 1_654
Ga3 O3 La 26.3(2) 4_445 4_444
Nb O3 La 137.2(4) . 4_444
Ga1 O3 La 137.2(4) . 4_444
La O3 La 112.5(3) . 4_444
Ga3 O3 La 101.6(4) 2_564 4_444
O3 O3 La 158.7(8) 6 4_444
O3 O3 La 91.3(4) 3 4_444
O3 O3 La 126.70(15) 4 4_444
O2 O3 La 118.2(5) 2_565 4_444
O3 O3 La 63.0(4) 6_554 4_444
O2 O3 La 48.0(4) 5_445 4_444
O2 O3 La 11.7(3) 4_444 4_444
O1 O3 La 64.9(3) 2_455 4_444
O3 O3 La 115.7(3) 2 4_444
O2 O3 La 104.3(3) 4_445 4_444
O3 O3 La 45.5(3) 2_554 4_444
Ga2 O3 La 39.58(12) . 4_444
Ga3 O3 La 88.1(2) 1_655 4_444
La O3 La 66.22(15) 4_445 4_444
O2 O3 La 93.2(3) 6 4_444
O3 O3 La 145.1(2) 5 4_444
Ga3 O3 La 122.1(3) 4_446 4_444
Ga2 O3 La 98.6(3) 2_564 4_444
O3 O3 La 82.6(4) 5_554 4_444
Ga1 O3 La 56.82(14) 1_554 4_444
Nb O3 La 56.82(14) 1_554 4_444
O2 O3 La 52.4(2) 1_554 4_444
La O3 La 86.39(17) 2 4_444
O1 O3 La 133.8(3) . 4_444
Ga3 O3 La 167.6(4) 2_565 4_444
La O3 La 49.96(12) 1_554 4_444
O2 O3 La 101.3(4) 3_564 4_444
O2 O3 La 104.7(3) . 4_444
Ga2 O3 La 42.07(9) 2_554 4_444
La O3 La 142.3(4) 2_565 4_444
O2 O3 La 169.1(4) 3_565 4_444
Ga2 O3 La 102.9(2) 1_556 4_444
O2 O3 La 107.7(3) 6_655 4_444
O1 O3 La 81.4(3) 1_554 4_444
O1 O3 La 78.4(2) 1_545 4_444
La O3 La 139.0(2) 4 4_444
Ga3 O3 La 73.86(15) . 4_444
Ga3 O3 La 135.5(2) 1_656 4_444
O3 O3 La 137.34(18) 1_556 4_444
O3 O3 La 42.66(18) 1_554 4_444
O2 O3 La 31.8(2) 3_454 4_444
O2 O3 La 74.8(3) 1_654 4_444
Ga3 O3 O2 43.7(4) 4_445 2
Nb O3 O2 79.4(4) . 2
Ga1 O3 O2 79.4(4) . 2
La O3 O2 133.3(5) . 2
Ga3 O3 O2 121.3(3) 2_564 2
O3 O3 O2 111.8(6) 6 2
O3 O3 O2 43.5(5) 3 2
O3 O3 O2 103.4(4) 4 2
O2 O3 O2 161.1(6) 2_565 2
O3 O3 O2 103.2(4) 6_554 2
O2 O3 O2 17.8(5) 5_445 2
O2 O3 O2 71.8(4) 4_444 2
O1 O3 O2 90.1(3) 2_455 2
O3 O3 O2 57.6(3) 2 2
O2 O3 O2 79.8(3) 4_445 2
O3 O3 O2 52.4(4) 2_554 2
Ga2 O3 O2 88.2(2) . 2
Ga3 O3 O2 63.7(2) 1_655 2
La O3 O2 52.8(2) 4_445 2
O2 O3 O2 147.7(3) 6 2
O3 O3 O2 88.19(16) 5 2
Ga3 O3 O2 75.6(3) 4_446 2
Ga2 O3 O2 157.8(3) 2_564 2
O3 O3 O2 83.5(2) 5_554 2
Ga1 O3 O2 80.3(2) 1_554 2
Nb O3 O2 80.3(2) 1_554 2
O2 O3 O2 109.9(3) 1_554 2
La O3 O2 26.20(14) 2 2
O1 O3 O2 154.3(5) . 2
Ga3 O3 O2 112.5(3) 2_565 2
La O3 O2 107.4(2) 1_554 2
O2 O3 O2 122.1(3) 3_564 2
O2 O3 O2 113.2(4) . 2
Ga2 O3 O2 19.20(12) 2_554 2
La O3 O2 152.9(2) 2_565 2
O2 O3 O2 124.9(3) 3_565 2
Ga2 O3 O2 92.7(3) 1_556 2
O2 O3 O2 73.2(3) 6_655 2
O1 O3 O2 137.6(3) 1_554 2
O1 O3 O2 32.8(3) 1_545 2
La O3 O2 102.7(2) 4 2
Ga3 O3 O2 128.2(2) . 2
Ga3 O3 O2 75.3(2) 1_656 2
O3 O3 O2 93.8(2) 1_556 2
O3 O3 O2 86.2(2) 1_554 2
O2 O3 O2 78.6(3) 3_454 2
O2 O3 O2 51.17(17) 1_654 2
La O3 O2 60.22(17) 4_444 2
Ga3 O3 O2 128.7(7) 4_445 5_455
Nb O3 O2 106.2(4) . 5_455
Ga1 O3 O2 106.2(4) . 5_455
La O3 O2 51.0(3) . 5_455
Ga3 O3 O2 54.9(2) 2_564 5_455
O3 O3 O2 75.8(5) 6 5_455
O3 O3 O2 137.5(6) 3 5_455
O3 O3 O2 77.7(6) 4 5_455
O2 O3 O2 16.8(4) 2_565 5_455
O3 O3 O2 69.7(4) 6_554 5_455
O2 O3 O2 158.4(7) 5_445 5_455
O2 O3 O2 101.6(4) 4_444 5_455
O1 O3 O2 89.6(3) 2_455 5_455
O3 O3 O2 129.9(4) 2 5_455
O2 O3 O2 106.0(3) 4_445 5_455
O3 O3 O2 120.7(6) 2_554 5_455
Ga2 O3 O2 87.7(3) . 5_455
Ga3 O3 O2 114.3(4) 1_655 5_455
La O3 O2 129.4(3) 4_445 5_455
O2 O3 O2 30.0(2) 6 5_455
O3 O3 O2 97.3(2) 5 5_455
Ga3 O3 O2 111.8(3) 4_446 5_455
Ga2 O3 O2 14.8(2) 2_564 5_455
O3 O3 O2 92.4(2) 5_554 5_455
Ga1 O3 O2 93.0(3) 1_554 5_455
Nb O3 O2 93.0(3) 1_554 5_455
O2 O3 O2 64.8(4) 1_554 5_455
La O3 O2 160.0(3) 2 5_455
O1 O3 O2 32.9(3) . 5_455
Ga3 O3 O2 74.8(3) 2_565 5_455
La O3 O2 65.1(3) 1_554 5_455
O2 O3 O2 54.0(3) 3_564 5_455
O2 O3 O2 71.0(2) . 5_455
Ga2 O3 O2 154.8(3) 2_554 5_455
La O3 O2 31.9(2) 2_565 5_455
O2 O3 O2 61.1(2) 3_565 5_455
Ga2 O3 O2 92.32(19) 1_556 5_455
O2 O3 O2 107.2(4) 6_655 5_455
O1 O3 O2 34.8(3) 1_554 5_455
O1 O3 O2 153.1(3) 1_545 5_455
La O3 O2 80.2(3) 4 5_455
Ga3 O3 O2 48.2(2) . 5_455
Ga3 O3 O2 111.2(3) 1_656 5_455
O3 O3 O2 93.7(2) 1_556 5_455
O3 O3 O2 86.3(2) 1_554 5_455
O2 O3 O2 97.1(4) 3_454 5_455
O2 O3 O2 125.5(3) 1_654 5_455
La O3 O2 113.0(3) 4_444 5_455
O2 O3 O2 172.4(4) 2 5_455
Ga3 O3 O1 123.9(6) 4_445 2_565
Nb O3 O1 60.7(4) . 2_565
Ga1 O3 O1 60.7(4) . 2_565
La O3 O1 89.8(3) . 2_565
Ga3 O3 O1 34.8(2) 2_564 2_565
O3 O3 O1 64.8(6) 6 2_565
O3 O3 O1 85.3(4) 3 2_565
O3 O3 O1 25.5(4) 4 2_565
O2 O3 O1 37.4(3) 2_565 2_565
O3 O3 O1 73.8(5) 6_554 2_565
O2 O3 O1 146.2(5) 5_445 2_565
O2 O3 O1 131.6(7) 4_444 2_565
O1 O3 O1 140.4(3) 2_455 2_565
O3 O3 O1 96.1(2) 2 2_565
O2 O3 O1 119.2(4) 4_445 2_565
O3 O3 O1 101.5(2) 2_554 2_565
Ga2 O3 O1 137.5(4) . 2_565
Ga3 O3 O1 68.76(19) 1_655 2_565
La O3 O1 157.2(4) 4_445 2_565
O2 O3 O1 82.8(3) 6 2_565
O3 O3 O1 52.92(19) 5 2_565
Ga3 O3 O1 100.0(3) 4_446 2_565
Ga2 O3 O1 61.03(18) 2_564 2_565
O3 O3 O1 59.9(2) 5_554 2_565
Ga1 O3 O1 81.2(3) 1_554 2_565
Nb O3 O1 81.2(3) 1_554 2_565
O2 O3 O1 112.7(3) 1_554 2_565
La O3 O1 109.82(19) 2 2_565
O1 O3 O1 60.4(2) . 2_565
Ga3 O3 O1 56.0(2) 2_565 2_565
La O3 O1 94.2(3) 1_554 2_565
O2 O3 O1 35.2(3) 3_564 2_565
O2 O3 O1 106.8(3) . 2_565
Ga2 O3 O1 143.1(2) 2_554 2_565
La O3 O1 28.23(11) 2_565 2_565
O2 O3 O1 32.9(3) 3_565 2_565
Ga2 O3 O1 117.5(3) 1_556 2_565
O2 O3 O1 55.7(2) 6_655 2_565
O1 O3 O1 68.0(2) 1_554 2_565
O1 O3 O1 134.9(2) 1_545 2_565
La O3 O1 28.15(10) 4 2_565
Ga3 O3 O1 100.6(2) . 2_565
Ga3 O3 O1 70.98(18) 1_656 2_565
O3 O3 O1 86.3(2) 1_556 2_565
O3 O3 O1 93.7(2) 1_554 2_565
O2 O3 O1 145.0(4) 3_454 2_565
O2 O3 O1 83.4(2) 1_654 2_565
La O3 O1 136.3(4) 4_444 2_565
O2 O3 O1 128.8(2) 2 2_565
O2 O3 O1 52.9(2) 5_455 2_565
Ga3 O3 O1 13.3(4) 4_445 1_544
Nb O3 O1 109.6(4) . 1_544
Ga1 O3 O1 109.6(4) . 1_544
La O3 O1 132.9(3) . 1_544
Ga3 O3 O1 107.4(4) 2_564 1_544
O3 O3 O1 144.7(8) 6 1_544
O3 O3 O1 64.9(4) 3 1_544
O3 O3 O1 113.7(3) 4 1_544
O2 O3 O1 138.7(6) 2_565 1_544
O3 O3 O1 75.6(4) 6_554 1_544
O2 O3 O1 27.1(4) 5_445 1_544
O2 O3 O1 39.4(3) 4_444 1_544
O1 O3 O1 80.6(3) 2_455 1_544
O3 O3 O1 91.2(3) 2 1_544
O2 O3 O1 99.6(4) 4_445 1_544
O3 O3 O1 33.85(15) 2_554 1_544
Ga2 O3 O1 63.76(16) . 1_544
Ga3 O3 O1 69.36(15) 1_655 1_544
La O3 O1 61.54(19) 4_445 1_544
O2 O3 O1 120.9(3) 6 1_544
O3 O3 O1 117.77(17) 5 1_544
Ga3 O3 O1 105.9(3) 4_446 1_544
Ga2 O3 O1 124.2(4) 2_564 1_544
O3 O3 O1 75.3(3) 5_554 1_544
Ga1 O3 O1 58.30(19) 1_554 1_544
Nb O3 O1 58.30(19) 1_554 1_544
O2 O3 O1 80.1(3) 1_554 1_544
La O3 O1 59.38(18) 2 1_544
O1 O3 O1 160.1(2) . 1_544
Ga3 O3 O1 146.2(4) 2_565 1_544
La O3 O1 73.8(2) 1_554 1_544
O2 O3 O1 107.6(4) 3_564 1_544
O2 O3 O1 118.0(3) . 1_544
Ga2 O3 O1 19.01(16) 2_554 1_544
La O3 O1 159.1(4) 2_565 1_544
O2 O3 O1 153.4(3) 3_565 1_544
Ga2 O3 O1 106.0(3) 1_556 1_544
O2 O3 O1 86.9(2) 6_655 1_544
O1 O3 O1 104.7(4) 1_554 1_544
O1 O3 O1 59.46(13) 1_545 1_544
La O3 O1 120.92(17) 4 1_544
Ga3 O3 O1 101.2(2) . 1_544
Ga3 O3 O1 108.0(2) 1_656 1_544
O3 O3 O1 124.2(3) 1_556 1_544
O3 O3 O1 55.8(3) 1_554 1_544
O2 O3 O1 54.4(2) 3_454 1_544
O2 O3 O1 54.5(2) 1_654 1_544
La O3 O1 27.81(11) 4_444 1_544
O2 O3 O1 33.7(2) 2 1_544
O2 O3 O1 138.9(4) 5_455 1_544
O1 O3 O1 135.0(2) 2_565 1_544
Ga3 O3 O2 99.9(5) 4_445 3_455
Nb O3 O2 106.3(6) . 3_455
Ga1 O3 O2 106.3(6) . 3_455
La O3 O2 51.0(4) . 3_455
Ga3 O3 O2 154.8(4) 2_564 3_455
O3 O3 O2 75.9(6) 6 3_455
O3 O3 O2 117.4(5) 3 3_455
O3 O3 O2 148.7(2) 4 3_455
O2 O3 O2 116.2(3) 2_565 3_455
O3 O3 O2 134.7(3) 6_554 3_455
O2 O3 O2 70.1(3) 5_445 3_455
O2 O3 O2 82.7(3) 4_444 3_455
O1 O3 O2 26.8(3) 2_455 3_455
O3 O3 O2 74.7(3) 2 3_455
O2 O3 O2 26.49(19) 4_445 3_455
O3 O3 O2 122.3(2) 2_554 3_455
Ga2 O3 O2 56.9(2) . 3_455
Ga3 O3 O2 145.0(4) 1_655 3_455
La O3 O2 30.27(19) 4_445 3_455
O2 O3 O2 75.7(3) 6 3_455
O3 O3 O2 108.7(5) 5 3_455
Ga3 O3 O2 54.1(2) 4_446 3_455
Ga2 O3 O2 102.4(3) 2_564 3_455
O3 O3 O2 163.8(3) 5_554 3_455
Ga1 O3 O2 139.9(3) 1_554 3_455
Nb O3 O2 139.9(3) 1_554 3_455
O2 O3 O2 73.13(15) 1_554 3_455
La O3 O2 86.3(3) 2 3_455
O1 O3 O2 78.8(3) . 3_455
Ga3 O3 O2 85.9(3) 2_565 3_455
La O3 O2 104.9(2) 1_554 3_455
O2 O3 O2 153.8(5) 3_564 3_455
O2 O3 O2 31.4(2) . 3_455
Ga2 O3 O2 76.5(3) 2_554 3_455
La O3 O2 110.5(3) 2_565 3_455
O2 O3 O2 106.4(5) 3_565 3_455
Ga2 O3 O2 19.62(19) 1_556 3_455
O2 O3 O2 142.6(3) 6_655 3_455
O1 O3 O2 111.6(2) 1_554 3_455
O1 O3 O2 55.4(2) 1_545 3_455
La O3 O2 134.5(3) 4 3_455
Ga3 O3 O2 68.62(19) . 3_455
Ga3 O3 O2 94.0(3) 1_656 3_455
O3 O3 O2 58.8(2) 1_556 3_455
O3 O3 O2 121.2(2) 1_554 3_455
O2 O3 O2 57.75(17) 3_454 3_455
O2 O3 O2 133.9(4) 1_654 3_455
La O3 O2 83.3(2) 4_444 3_455
O2 O3 O2 82.7(4) 2 3_455
O2 O3 O2 100.3(3) 5_455 3_455
O1 O3 O2 136.1(3) 2_565 3_455
O1 O3 O2 88.6(3) 1_544 3_455
Ga3 O3 O2 93.6(4) 4_445 1_655
Nb O3 O2 21.9(3) . 1_655
Ga1 O3 O2 21.9(3) . 1_655
La O3 O2 117.8(5) . 1_655
Ga3 O3 O2 99.9(3) 2_564 1_655
O3 O3 O2 63.7(3) 6 1_655
O3 O3 O2 31.6(2) 3 1_655
O3 O3 O2 61.1(3) 4 1_655
O2 O3 O2 116.3(4) 2_565 1_655
O3 O3 O2 121.5(2) 6_554 1_655
O2 O3 O2 73.4(6) 5_445 1_655
O2 O3 O2 128.2(3) 4_444 1_655
O1 O3 O2 124.7(5) 2_455 1_655
O3 O3 O2 25.3(2) 2 1_655
O2 O3 O2 76.1(4) 4_445 1_655
O3 O3 O2 85.8(4) 2_554 1_655
Ga2 O3 O2 142.3(4) . 1_655
Ga3 O3 O2 54.62(18) 1_655 1_655
La O3 O2 85.5(3) 4_445 1_655
O2 O3 O2 149.4(3) 6 1_655
O3 O3 O2 30.75(19) 5 1_655
Ga3 O3 O2 50.3(2) 4_446 1_655
Ga2 O3 O2 140.2(3) 2_564 1_655
O3 O3 O2 79.7(3) 5_554 1_655
Ga1 O3 O2 101.1(2) 1_554 1_655
Nb O3 O2 101.1(2) 1_554 1_655
O2 O3 O2 166.9(4) 1_554 1_655
La O3 O2 31.96(17) 2 1_655
O1 O3 O2 108.3(3) . 1_655
Ga3 O3 O2 59.6(2) 2_565 1_655
La O3 O2 149.1(3) 1_554 1_655
O2 O3 O2 100.97(18) 3_564 1_655
O2 O3 O2 109.2(5) . 1_655
Ga2 O3 O2 76.7(2) 2_554 1_655
La O3 O2 96.1(2) 2_565 1_655
O2 O3 O2 67.4(2) 3_565 1_655
Ga2 O3 O2 91.1(3) 1_556 1_655
O2 O3 O2 43.1(3) 6_655 1_655
O1 O3 O2 145.8(3) 1_554 1_655
O1 O3 O2 55.6(2) 1_545 1_655
La O3 O2 52.28(17) 4 1_655
Ga3 O3 O2 164.2(3) . 1_655
Ga3 O3 O2 20.20(16) 1_656 1_655
O3 O3 O2 58.6(2) 1_556 1_655
O3 O3 O2 121.4(2) 1_554 1_655
O2 O3 O2 133.9(4) 3_454 1_655
O2 O3 O2 58.00(17) 1_654 1_655
La O3 O2 116.6(2) 4_444 1_655
O2 O3 O2 57.5(2) 2 1_655
O2 O3 O2 128.1(2) 5_455 1_655
O1 O3 O2 80.1(2) 2_565 1_655
O1 O3 O2 88.8(2) 1_544 1_655
O2 O3 O2 99.8(4) 3_455 1_655
Ga3 O3 Ga2 168.7(4) 4_445 2_565
Nb O3 Ga2 77.3(3) . 2_565
Ga1 O3 Ga2 77.3(3) . 2_565
La O3 Ga2 30.32(16) . 2_565
Ga3 O3 Ga2 92.0(3) 2_564 2_565
O3 O3 Ga2 30.9(2) 6 2_565
O3 O3 Ga2 124.2(2) 3 2_565
O3 O3 Ga2 85.3(4) 4 2_565
O2 O3 Ga2 56.3(4) 2_565 2_565
O3 O3 Ga2 118.9(5) 6_554 2_565
O2 O3 Ga2 136.2(5) 5_445 2_565
O2 O3 Ga2 133.4(3) 4_444 2_565
O1 O3 Ga2 81.0(3) 2_455 2_565
O3 O3 Ga2 83.5(4) 2 2_565
O2 O3 Ga2 61.9(3) 4_445 2_565
O3 O3 Ga2 166.5(3) 2_554 2_565
Ga2 O3 Ga2 103.17(19) . 2_565
Ga3 O3 Ga2 128.3(2) 1_655 2_565
La O3 Ga2 98.5(3) 4_445 2_565
O2 O3 Ga2 55.2(3) 6 2_565
O3 O3 Ga2 70.8(3) 5 2_565
Ga3 O3 Ga2 62.27(16) 4_446 2_565
Ga2 O3 Ga2 62.95(13) 2_564 2_565
O3 O3 Ga2 125.2(2) 5_554 2_565
Ga1 O3 Ga2 140.0(3) 1_554 2_565
Nb O3 Ga2 140.0(3) 1_554 2_565
O2 O3 Ga2 93.5(2) 1_554 2_565
La O3 Ga2 117.2(3) 2 2_565
O1 O3 Ga2 16.9(2) . 2_565
Ga3 O3 Ga2 35.69(8) 2_565 2_565
La O3 Ga2 110.8(2) 1_554 2_565
O2 O3 Ga2 91.7(3) 3_564 2_565
O2 O3 Ga2 42.0(2) . 2_565
Ga2 O3 Ga2 144.3(4) 2_554 2_565
La O3 Ga2 40.54(8) 2_565 2_565
O2 O3 Ga2 41.7(3) 3_565 2_565
Ga2 O3 Ga2 53.75(12) 1_556 2_565
O2 O3 Ga2 109.2(3) 6_655 2_565
O1 O3 Ga2 83.7(2) 1_554 2_565
O1 O3 Ga2 106.3(3) 1_545 2_565
La O3 Ga2 76.04(14) 4 2_565
Ga3 O3 Ga2 71.92(11) . 2_565
Ga3 O3 Ga2 74.34(16) 1_656 2_565
O3 O3 Ga2 44.46(17) 1_556 2_565
O3 O3 Ga2 135.54(17) 1_554 2_565
O2 O3 Ga2 111.3(3) 3_454 2_565
O2 O3 Ga2 142.3(3) 1_654 2_565
La O3 Ga2 142.74(18) 4_444 2_565
O2 O3 Ga2 137.8(4) 2 2_565
O2 O3 Ga2 49.54(18) 5_455 2_565
O1 O3 Ga2 65.40(18) 2_565 2_565
O1 O3 Ga2 159.5(3) 1_544 2_565
O2 O3 Ga2 70.9(3) 3_455 2_565
O2 O3 Ga2 94.5(3) 1_655 2_565
Ga3 O3 O3 63.9(5) 4_445 4_445
Nb O3 O3 122.7(6) . 4_445
Ga1 O3 O3 122.7(6) . 4_445
La O3 O3 81.10(18) . 4_445
Ga3 O3 O3 147.5(3) 2_564 4_445
O3 O3 O3 110.3(6) 6 4_445
O3 O3 O3 103.1(7) 3 4_445
O3 O3 O3 163.1(7) 4 4_445
O2 O3 O3 135.3(4) 2_565 4_445
O3 O3 O3 108.9(4) 6_554 4_445
O2 O3 O3 42.6(5) 5_445 4_445
O2 O3 O3 50.9(5) 4_444 4_445
O1 O3 O3 30.60(7) 2_455 4_445
O3 O3 O3 86.39(15) 2 4_445
O2 O3 O3 56.1(2) 4_445 4_445
O3 O3 O3 86.56(17) 2_554 4_445
Ga2 O3 O3 38.16(15) . 4_445
Ga3 O3 O3 120.4(4) 1_655 4_445
La O3 O3 21.88(17) 4_445 4_445
O2 O3 O3 89.2(2) 6 4_445
O3 O3 O3 129.6(4) 5 4_445
Ga3 O3 O3 78.3(2) 4_446 4_445
Ga2 O3 O3 112.4(2) 2_564 4_445
O3 O3 O3 128.0(2) 5_554 4_445
Ga1 O3 O3 104.87(19) 1_554 4_445
Nb O3 O3 104.87(19) 1_554 4_445
O2 O3 O3 62.68(17) 1_554 4_445
La O3 O3 77.0(3) 2 4_445
O1 O3 O3 110.52(16) . 4_445
Ga3 O3 O3 119.79(18) 2_565 4_445
La O3 O3 85.14(11) 1_554 4_445
O2 O3 O3 146.9(3) 3_564 4_445
O2 O3 O3 64.5(2) . 4_445
Ga2 O3 O3 46.1(3) 2_554 4_445
La O3 O3 142.6(2) 2_565 4_445
O2 O3 O3 142.0(3) 3_565 4_445
Ga2 O3 O3 55.50(11) 1_556 4_445
O2 O3 O3 133.0(4) 6_655 4_445
O1 O3 O3 108.31(16) 1_554 4_445
O1 O3 O3 49.5(2) 1_545 4_445
La O3 O3 157.1(3) 4 4_445
Ga3 O3 O3 72.38(11) . 4_445
Ga3 O3 O3 111.4(3) 1_656 4_445
O3 O3 O3 90.000(2) 1_556 4_445
O3 O3 O3 90.000(1) 1_554 4_445
O2 O3 O3 32.45(17) 3_454 4_445
O2 O3 O3 105.7(3) 1_654 4_445
La O3 O3 48.3(2) 4_444 4_445
O2 O3 O3 59.8(3) 2 4_445
O2 O3 O3 119.2(3) 5_455 4_445
O1 O3 O3 170.8(3) 2_565 4_445
O1 O3 O3 53.5(3) 1_544 4_445
O2 O3 O3 36.2(2) 3_455 4_445
O2 O3 O3 105.0(3) 1_655 4_445
Ga2 O3 O3 106.26(11) 2_565 4_445
Ga3 O3 O3 103.7(3) 4_445 3_455
Nb O3 O3 140.2(3) . 3_455
Ga1 O3 O3 140.2(3) . 3_455
La O3 O3 35.8(3) . 3_455
Ga3 O3 O3 106.9(4) 2_564 3_455
O3 O3 O3 92.13(4) 6 3_455
O3 O3 O3 163.1(7) 3 3_455
O3 O3 O3 136.9(7) 4 3_455
O2 O3 O3 75.9(4) 2_565 3_455
O3 O3 O3 91.98(5) 6_554 3_455
O2 O3 O3 102.0(5) 5_445 3_455
O2 O3 O3 68.2(3) 4_444 3_455
O1 O3 O3 30.61(7) 2_455 3_455
O3 O3 O3 121.7(2) 2 3_455
O2 O3 O3 70.9(2) 4_445 3_455
O3 O3 O3 120.0(3) 2_554 3_455
Ga2 O3 O3 38.16(15) . 3_455
Ga3 O3 O3 158.5(3) 1_655 3_455
La O3 O3 72.30(13) 4_445 3_455
O2 O3 O3 29.62(19) 6 3_455
O3 O3 O3 135.5(3) 5 3_455
Ga3 O3 O3 96.24(13) 4_446 3_455
Ga2 O3 O3 55.47(19) 2_564 3_455
O3 O3 O3 133.6(3) 5_554 3_455
Ga1 O3 O3 111.44(16) 1_554 3_455
Nb O3 O3 111.44(16) 1_554 3_455
O2 O3 O3 32.9(2) 1_554 3_455
La O3 O3 134.0(3) 2 3_455
O1 O3 O3 58.6(2) . 3_455
Ga3 O3 O3 99.88(18) 2_565 3_455
La O3 O3 63.63(13) 1_554 3_455
O2 O3 O3 105.9(4) 3_564 3_455
O2 O3 O3 38.1(3) . 3_455
Ga2 O3 O3 103.5(2) 2_554 3_455
La O3 O3 85.5(3) 2_565 3_455
O2 O3 O3 104.9(3) 3_565 3_455
Ga2 O3 O3 55.50(11) 1_556 3_455
O2 O3 O3 166.2(4) 6_655 3_455
O1 O3 O3 62.15(17) 1_554 3_455
O1 O3 O3 102.7(2) 1_545 3_455
La O3 O3 136.1(3) 4 3_455
Ga3 O3 O3 19.41(14) . 3_455
Ga3 O3 O3 132.05(13) 1_656 3_455
O3 O3 O3 90.0 1_556 3_455
O3 O3 O3 90.0 1_554 3_455
O2 O3 O3 47.2(3) 3_454 3_455
O2 O3 O3 150.8(3) 1_654 3_455
La O3 O3 77.43(13) 4_444 3_455
O2 O3 O3 119.7(3) 2 3_455
O2 O3 O3 59.3(3) 5_455 3_455
O1 O3 O3 111.6(3) 2_565 3_455
O1 O3 O3 101.57(18) 1_544 3_455
O2 O3 O3 49.50(15) 3_455 3_455
O2 O3 O3 146.5(2) 1_655 3_455
Ga2 O3 O3 65.41(19) 2_565 3_455
O3 O3 O3 60.0 4_445 3_455
Ga3 O3 O2 166.8(7) 4_445 2_566
Nb O3 O2 58.6(3) . 2_566
Ga1 O3 O2 58.6(3) . 2_566
La O3 O2 47.0(2) . 2_566
Ga3 O3 O2 94.7(3) 2_564 2_566
O3 O3 O2 12.0(3) 6 2_566
O3 O3 O2 105.2(2) 3 2_566
O3 O3 O2 75.8(3) 4 2_566
O2 O3 O2 66.5(3) 2_565 2_566
O3 O3 O2 129.4(6) 6_554 2_566
O2 O3 O2 127.7(6) 5_445 2_566
O2 O3 O2 150.8(4) 4_444 2_566
O1 O3 O2 92.4(4) 2_455 2_566
O3 O3 O2 66.1(4) 2 2_566
O2 O3 O2 58.0(4) 4_445 2_566
O3 O3 O2 156.6(3) 2_554 2_566
Ga2 O3 O2 119.1(3) . 2_566
Ga3 O3 O2 113.9(3) 1_655 2_566
La O3 O2 97.2(3) 4_445 2_566
O2 O3 O2 74.3(3) 6 2_566
O3 O3 O2 52.7(4) 5 2_566
Ga3 O3 O2 48.9(2) 4_446 2_566
Ga2 O3 O2 78.9(2) 2_564 2_566
O3 O3 O2 119.6(3) 5_554 2_566
Ga1 O3 O2 143.3(3) 1_554 2_566
Nb O3 O2 143.3(3) 1_554 2_566
O2 O3 O2 112.5(3) 1_554 2_566
La O3 O2 99.6(3) 2 2_566
O1 O3 O2 34.3(3) . 2_566
Ga3 O3 O2 17.10(11) 2_565 2_566
La O3 O2 128.7(3) 1_554 2_566
O2 O3 O2 94.7(5) 3_564 2_566
O2 O3 O2 52.6(2) . 2_566
Ga2 O3 O2 135.8(4) 2_554 2_566
La O3 O2 44.9(2) 2_565 2_566
O2 O3 O2 31.2(4) 3_565 2_566
Ga2 O3 O2 55.9(2) 1_556 2_566
O2 O3 O2 94.1(2) 6_655 2_566
O1 O3 O2 99.3(3) 1_554 2_566
O1 O3 O2 95.3(4) 1_545 2_566
La O3 O2 63.8(2) 4 2_566
Ga3 O3 O2 90.99(18) . 2_566
Ga3 O3 O2 55.15(17) 1_656 2_566
O3 O3 O2 30.6(3) 1_556 2_566
O3 O3 O2 149.4(2) 1_554 2_566
O2 O3 O2 125.9(3) 3_454 2_566
O2 O3 O2 126.1(4) 1_654 2_566
La O3 O2 157.3(3) 4_444 2_566
O2 O3 O2 123.1(4) 2 2_566
O2 O3 O2 64.48(14) 5_455 2_566
O1 O3 O2 62.1(3) 2_565 2_566
O1 O3 O2 154.8(4) 1_544 2_566
O2 O3 O2 75.4(2) 3_455 2_566
O2 O3 O2 75.3(3) 1_655 2_566
Ga2 O3 O2 19.19(12) 2_565 2_566
O3 O3 O2 111.4(2) 4_445 2_566
O3 O3 O2 82.8(2) 3_455 2_566
Ga3 O3 O2 106.2(6) 4_445 5_446
Nb O3 O2 58.6(5) . 5_446
Ga1 O3 O2 58.6(5) . 5_446
La O3 O2 78.1(4) . 5_446
Ga3 O3 O2 144.5(4) 2_564 5_446
O3 O3 O2 52.4(6) 6 5_446
O3 O3 O2 75.7(3) 3 5_446
O3 O3 O2 105.2(3) 4 5_446
O2 O3 O2 127.8(5) 2_565 5_446
O3 O3 O2 167.6(4) 6_554 5_446
O2 O3 O2 66.5(4) 5_445 5_446
O2 O3 O2 116.6(7) 4_444 5_446
O1 O3 O2 75.5(4) 2_455 5_446
O3 O3 O2 25.8(2) 2 5_446
O2 O3 O2 25.3(4) 4_445 5_446
O3 O3 O2 116.5(5) 2_554 5_446
Ga2 O3 O2 102.6(4) . 5_446
Ga3 O3 O2 103.7(3) 1_655 5_446
La O3 O2 46.2(3) 4_445 5_446
O2 O3 O2 114.4(4) 6 5_446
O3 O3 O2 63.3(4) 5 5_446
Ga3 O3 O2 12.67(16) 4_446 5_446
Ga2 O3 O2 134.5(3) 2_564 5_446
O3 O3 O2 130.1(3) 5_554 5_446
Ga1 O3 O2 143.2(3) 1_554 5_446
Nb O3 O2 143.2(3) 1_554 5_446
O2 O3 O2 122.2(4) 1_554 5_446
La O3 O2 49.5(2) 2 5_446
O1 O3 O2 89.7(3) . 5_446
Ga3 O3 O2 58.3(2) 2_565 5_446
La O3 O2 152.3(3) 1_554 5_446
O2 O3 O2 145.2(3) 3_564 5_446
O2 O3 O2 62.2(3) . 5_446
Ga2 O3 O2 74.6(3) 2_554 5_446
La O3 O2 105.4(3) 2_565 5_446
O2 O3 O2 80.8(3) 3_565 5_446
Ga2 O3 O2 41.1(2) 1_556 5_446
O2 O3 O2 94.1(3) 6_655 5_446
O1 O3 O2 153.7(3) 1_554 5_446
O1 O3 O2 34.1(3) 1_545 5_446
La O3 O2 91.9(3) 4 5_446
Ga3 O3 O2 115.4(3) . 5_446
Ga3 O3 O2 46.1(2) 1_656 5_446
O3 O3 O2 30.63(16) 1_556 5_446
O3 O3 O2 149.37(16) 1_554 5_446
O2 O3 O2 99.6(4) 3_454 5_446
O2 O3 O2 101.4(3) 1_654 5_446
La O3 O2 109.7(3) 4_444 5_446
O2 O3 O2 64.7(2) 2 5_446
O2 O3 O2 122.5(3) 5_455 5_446
O1 O3 O2 111.5(3) 2_565 5_446
O1 O3 O2 93.6(3) 1_544 5_446
O2 O3 O2 49.2(2) 3_455 5_446
O2 O3 O2 51.1(3) 1_655 5_446
Ga2 O3 O2 73.2(2) 2_565 5_446
O3 O3 O2 67.8(2) 4_445 5_446
O3 O3 O2 96.1(2) 3_455 5_446
O2 O3 O2 61.2(3) 2_566 5_446
Ga3 O3 O2 46.5(5) 4_445 6_545
Nb O3 O2 102.8(5) . 6_545
Ga1 O3 O2 102.8(5) . 6_545
La O3 O2 108.5(4) . 6_545
Ga3 O3 O2 140.6(4) 2_564 6_545
O3 O3 O2 116.0(8) 6 6_545
O3 O3 O2 73.4(5) 3 6_545
O3 O3 O2 133.3(5) 4 6_545
O2 O3 O2 161.9(4) 2_565 6_545
O3 O3 O2 107.0(5) 6_554 6_545
O2 O3 O2 12.8(5) 5_445 6_545
O2 O3 O2 55.6(5) 4_444 6_545
O1 O3 O2 60.5(2) 2_455 6_545
O3 O3 O2 71.1(2) 2 6_545
O2 O3 O2 66.3(3) 4_445 6_545
O3 O3 O2 66.1(2) 2_554 6_545
Ga2 O3 O2 61.1(2) . 6_545
Ga3 O3 O2 91.6(3) 1_655 6_545
La O3 O2 29.0(2) 4_445 6_545
O2 O3 O2 118.4(3) 6 6_545
O3 O3 O2 111.5(2) 5 6_545
Ga3 O3 O2 76.5(3) 4_446 6_545
Ga2 O3 O2 138.1(2) 2_564 6_545
O3 O3 O2 105.9(3) 5_554 6_545
Ga1 O3 O2 91.6(2) 1_554 6_545
Nb O3 O2 91.6(2) 1_554 6_545
O2 O3 O2 85.2(3) 1_554 6_545
La O3 O2 50.39(17) 2 6_545
O1 O3 O2 137.1(3) . 6_545
Ga3 O3 O2 122.0(4) 2_565 6_545
La O3 O2 95.7(2) 1_554 6_545
O2 O3 O2 140.9(3) 3_564 6_545
O2 O3 O2 89.6(4) . 6_545
Ga2 O3 O2 18.2(2) 2_554 6_545
La O3 O2 167.7(4) 2_565 6_545
O2 O3 O2 143.1(4) 3_565 6_545
Ga2 O3 O2 73.7(3) 1_556 6_545
O2 O3 O2 103.1(3) 6_655 6_545
O1 O3 O2 126.1(3) 1_554 6_545
O1 O3 O2 32.1(2) 1_545 6_545
La O3 O2 131.7(2) 4 6_545
Ga3 O3 O2 99.95(19) . 6_545
Ga3 O3 O2 94.9(3) 1_656 6_545
O3 O3 O2 93.7(2) 1_556 6_545
O3 O3 O2 86.3(2) 1_554 6_545
O2 O3 O2 52.2(3) 3_454 6_545
O2 O3 O2 77.6(2) 1_654 6_545
La O3 O2 46.48(17) 4_444 6_545
O2 O3 O2 29.93(15) 2 6_545
O2 O3 O2 148.1(2) 5_455 6_545
O1 O3 O2 158.7(2) 2_565 6_545
O1 O3 O2 33.3(3) 1_544 6_545
O2 O3 O2 58.3(4) 3_455 6_545
O2 O3 O2 81.7(2) 1_655 6_545
Ga2 O3 O2 127.3(3) 2_565 6_545
O3 O3 O2 29.9(3) 4_445 6_545
O3 O3 O2 89.7(2) 3_455 6_545
O2 O3 O2 123.2(5) 2_566 6_545
O2 O3 O2 63.8(2) 5_446 6_545
Ga3 O3 Ga2 107.7(6) 4_445 1_665
Nb O3 Ga2 74.1(4) . 1_665
Ga1 O3 Ga2 74.1(4) . 1_665
La O3 Ga2 99.2(3) . 1_665
Ga3 O3 Ga2 16.02(14) 2_564 1_665
O3 O3 Ga2 83.5(6) 6 1_665
O3 O3 Ga2 85.4(4) 3 1_665
O3 O3 Ga2 29.2(3) 4 1_665
O2 O3 Ga2 36.0(3) 2_565 1_665
O3 O3 Ga2 55.0(4) 6_554 1_665
O2 O3 Ga2 139.8(4) 5_445 1_665
O2 O3 Ga2 113.1(6) 4_444 1_665
O1 O3 Ga2 141.3(3) 2_455 1_665
O3 O3 Ga2 110.47(14) 2 1_665
O2 O3 Ga2 137.7(3) 4_445 1_665
O3 O3 Ga2 86.4(2) 2_554 1_665
Ga2 O3 Ga2 125.3(4) . 1_665
Ga3 O3 Ga2 62.1(2) 1_655 1_665
La O3 Ga2 175.3(3) 4_445 1_665
O2 O3 Ga2 81.3(3) 6 1_665
O3 O3 Ga2 67.5(2) 5 1_665
Ga3 O3 Ga2 118.3(2) 4_446 1_665
Ga2 O3 Ga2 55.57(18) 2_564 1_665
O3 O3 Ga2 45.86(11) 5_554 1_665
Ga1 O3 Ga2 63.4(2) 1_554 1_665
Nb O3 Ga2 63.4(2) 1_554 1_665
O2 O3 Ga2 101.4(3) 1_554 1_665
La O3 Ga2 114.85(18) 2 1_665
O1 O3 Ga2 71.2(2) . 1_665
Ga3 O3 Ga2 74.81(16) 2_565 1_665
La O3 Ga2 77.6(3) 1_554 1_665
O2 O3 Ga2 16.44(19) 3_564 1_665
O2 O3 Ga2 118.6(3) . 1_665
Ga2 O3 Ga2 133.6(2) 2_554 1_665
La O3 Ga2 39.77(11) 2_565 1_665
O2 O3 Ga2 51.7(2) 3_565 1_665
Ga2 O3 Ga2 133.8(2) 1_556 1_665
O2 O3 Ga2 55.4(2) 6_655 1_665
O1 O3 Ga2 55.76(17) 1_554 1_665
O1 O3 Ga2 145.2(2) 1_545 1_665
La O3 Ga2 39.37(10) 4 1_665
Ga3 O3 Ga2 95.2(2) . 1_665
Ga3 O3 Ga2 85.68(14) 1_656 1_665
O3 O3 Ga2 105.11(15) 1_556 1_665
O3 O3 Ga2 74.89(15) 1_554 1_665
O2 O3 Ga2 130.4(4) 3_454 1_665
O2 O3 Ga2 75.2(2) 1_654 1_665
La O3 Ga2 117.5(3) 4_444 1_665
O2 O3 Ga2 125.8(2) 2 1_665
O2 O3 Ga2 52.8(2) 5_455 1_665
O1 O3 Ga2 18.84(18) 2_565 1_665
O1 O3 Ga2 120.2(3) 1_544 1_665
O2 O3 Ga2 149.9(3) 3_455 1_665
O2 O3 Ga2 90.16(19) 1_655 1_665
Ga2 O3 Ga2 80.11(15) 2_565 1_665
O3 O3 Ga2 162.8(2) 4_445 1_665
O3 O3 Ga2 110.8(3) 3_455 1_665
O2 O3 Ga2 80.0(2) 2_566 1_665
O2 O3 Ga2 129.3(3) 5_446 1_665
O2 O3 Ga2 151.7(3) 6_545 1_665
Ga3 O3 La 97.9(4) 4_445 2_455
Nb O3 La 128.9(6) . 2_455
Ga1 O3 La 128.9(6) . 2_455
La O3 La 42.26(19) . 2_455
Ga3 O3 La 132.0(4) 2_564 2_455
O3 O3 La 88.3(4) 6 2_455
O3 O3 La 139.6(6) 3 2_455
O3 O3 La 155.4(5) 4 2_455
O2 O3 La 99.0(3) 2_565 2_455
O3 O3 La 111.3(2) 6_554 2_455
O2 O3 La 82.1(4) 5_445 2_455
O2 O3 La 69.2(3) 4_444 2_455
O1 O3 La 10.1(2) 2_455 2_455
O3 O3 La 100.0(3) 2 2_455
O2 O3 La 50.0(2) 4_445 2_455
O3 O3 La 119.6(2) 2_554 2_455
Ga2 O3 La 38.19(13) . 2_455
Ga3 O3 La 159.9(3) 1_655 2_455
La O3 La 47.82(11) 4_445 2_455
O2 O3 La 53.77(17) 6 2_455
O3 O3 La 128.9(5) 5 2_455
Ga3 O3 La 77.5(2) 4_446 2_455
Ga2 O3 La 80.25(14) 2_564 2_455
O3 O3 La 151.7(5) 5_554 2_455
Ga1 O3 La 124.3(2) 1_554 2_455
Nb O3 La 124.3(2) 1_554 2_455
O2 O3 La 48.74(17) 1_554 2_455
La O3 La 109.1(3) 2 2_455
O1 O3 La 71.34(13) . 2_455
Ga3 O3 La 98.1(2) 2_565 2_455
La O3 La 81.21(15) 1_554 2_455
O2 O3 La 130.9(3) 3_564 2_455
O2 O3 La 30.4(3) . 2_455
Ga2 O3 La 85.90(18) 2_554 2_455
La O3 La 102.84(15) 2_565 2_455
O2 O3 La 112.4(3) 3_565 2_455
Ga2 O3 La 37.19(8) 1_556 2_455
O2 O3 La 168.0(4) 6_655 2_455
O1 O3 La 86.63(15) 1_554 2_455
O1 O3 La 77.7(2) 1_545 2_455
La O3 La 146.6(2) 4 2_455
Ga3 O3 La 43.54(7) . 2_455
Ga3 O3 La 117.2(3) 1_656 2_455
O3 O3 La 77.43(15) 1_556 2_455
O3 O3 La 102.57(15) 1_554 2_455
O2 O3 La 43.1(3) 3_454 2_455
O2 O3 La 145.0(3) 1_654 2_455
La O3 La 74.31(12) 4_444 2_455
O2 O3 La 98.5(3) 2 2_455
O2 O3 La 82.1(2) 5_455 2_455
O1 O3 La 130.99(19) 2_565 2_455
O1 O3 La 90.70(16) 1_544 2_455
O2 O3 La 25.40(13) 3_455 2_455
O2 O3 La 125.2(3) 1_655 2_455
Ga2 O3 La 70.88(12) 2_565 2_455
O3 O3 La 39.85(11) 4_445 2_455
O3 O3 La 25.07(8) 3_455 2_455
O2 O3 La 83.03(19) 2_566 2_455
O2 O3 La 74.3(3) 5_446 2_455
O2 O3 La 69.3(2) 6_545 2_455
Ga2 O3 La 134.8(2) 1_665 2_455
Ga3 O3 La 18.8(2) 4_445 2_554
Nb O3 La 96.1(3) . 2_554
Ga1 O3 La 96.1(3) . 2_554
La O3 La 157.1(3) . 2_554
Ga3 O3 La 84.0(3) 2_564 2_554
O3 O3 La 143.6(3) 6 2_554
O3 O3 La 49.5(3) 3 2_554
O3 O3 La 87.6(3) 4 2_554
O2 O3 La 121.7(5) 2_565 2_554
O3 O3 La 61.1(3) 6_554 2_554
O2 O3 La 47.1(3) 5_445 2_554
O2 O3 La 53.6(2) 4_444 2_554
O1 O3 La 106.3(3) 2_455 2_554
O3 O3 La 93.3(3) 2 2_554
O2 O3 La 120.9(4) 4_445 2_554
O3 O3 La 10.2(3) 2_554 2_554
Ga2 O3 La 84.2(2) . 2_554
Ga3 O3 La 44.30(11) 1_655 2_554
La O3 La 86.18(18) 4_445 2_554
O2 O3 La 129.7(4) 6 2_554
O3 O3 La 102.3(3) 5 2_554
Ga3 O3 La 116.5(3) 4_446 2_554
Ga2 O3 La 118.5(3) 2_564 2_554
O3 O3 La 49.1(2) 5_554 2_554
Ga1 O3 La 38.17(8) 1_554 2_554
Nb O3 La 38.17(8) 1_554 2_554
O2 O3 La 92.8(3) 1_554 2_554
La O3 La 59.93(11) 2 2_554
O1 O3 La 163.3(5) . 2_554
Ga3 O3 La 137.7(2) 2_565 2_554
La O3 La 73.03(18) 1_554 2_554
O2 O3 La 84.5(4) 3_564 2_554
O2 O3 La 144.7(3) . 2_554
Ga2 O3 La 39.46(8) 2_554 2_554
La O3 La 134.6(3) 2_565 2_554
O2 O3 La 130.9(3) 3_565 2_554
Ga2 O3 La 130.8(3) 1_556 2_554
O2 O3 La 63.4(2) 6_655 2_554
O1 O3 La 98.0(3) 1_554 2_554
O1 O3 La 74.8(2) 1_545 2_554
La O3 La 96.56(16) 4 2_554
Ga3 O3 La 114.2(2) . 2_554
Ga3 O3 La 99.99(16) 1_656 2_554
O3 O3 La 133.36(16) 1_556 2_554
O3 O3 La 46.64(16) 1_554 2_554
O2 O3 La 76.1(3) 3_454 2_554
O2 O3 La 30.3(2) 1_654 2_554
La O3 La 44.62(8) 4_444 2_554
O2 O3 La 42.3(2) 2 2_554
O2 O3 La 130.8(3) 5_455 2_554
O1 O3 La 108.4(2) 2_565 2_554
O1 O3 La 26.69(9) 1_544 2_554
O2 O3 La 114.8(3) 3_455 2_554
O2 O3 La 79.99(19) 1_655 2_554
Ga2 O3 La 172.55(19) 2_565 2_554
O3 O3 La 80.2(3) 4_445 2_554
O3 O3 La 121.79(14) 3_455 2_554
O2 O3 La 154.7(2) 2_566 2_554
O2 O3 La 106.5(2) 5_446 2_554
O2 O3 La 57.2(2) 6_545 2_554
Ga2 O3 La 94.8(2) 1_665 2_554
La O3 La 116.39(17) 2_455 2_554
Ga3 O3 O1 47.9(3) 4_445 2_454
Nb O3 O1 158.3(4) . 2_454
Ga1 O3 O1 158.3(4) . 2_454
La O3 O1 96.6(3) . 2_454
Ga3 O3 O1 86.1(4) 2_564 2_454
O3 O3 O1 153.25(12) 6 2_454
O3 O3 O1 112.2(3) 3 2_454
O3 O3 O1 122.6(2) 4 2_454
O2 O3 O1 92.6(4) 2_565 2_454
O3 O3 O1 48.3(3) 6_554 2_454
O2 O3 O1 74.2(5) 5_445 2_454
O2 O3 O1 15.4(4) 4_444 2_454
O1 O3 O1 62.8(3) 2_455 2_454
O3 O3 O1 141.6(3) 2 2_454
O2 O3 O1 114.1(3) 4_445 2_454
O3 O3 O1 58.9(4) 2_554 2_454
Ga2 O3 O1 31.65(19) . 2_454
Ga3 O3 O1 99.0(3) 1_655 2_454
La O3 O1 82.90(19) 4_445 2_454
O2 O3 O1 69.0(3) 6 2_454
O3 O3 O1 161.6(5) 5 2_454
Ga3 O3 O1 139.5(3) 4_446 2_454
Ga2 O3 O1 72.0(2) 2_564 2_454
O3 O3 O1 82.7(4) 5_554 2_454
Ga1 O3 O1 54.99(17) 1_554 2_454
Nb O3 O1 54.99(17) 1_554 2_454
O2 O3 O1 30.1(2) 1_554 2_454
La O3 O1 112.81(19) 2 2_454
O1 O3 O1 110.2(3) . 2_454
Ga3 O3 O1 158.9(2) 2_565 2_454
La O3 O1 25.37(8) 1_554 2_454
O2 O3 O1 85.5(3) 3_564 2_454
O2 O3 O1 97.1(3) . 2_454
Ga2 O3 O1 68.60(14) 2_554 2_454
La O3 O1 116.4(3) 2_565 2_454
O2 O3 O1 146.0(4) 3_565 2_454
Ga2 O3 O1 105.59(19) 1_556 2_454
O2 O3 O1 117.8(3) 6_655 2_454
O1 O3 O1 55.70(18) 1_554 2_454
O1 O3 O1 102.6(3) 1_545 2_454
La O3 O1 136.9(3) 4 2_454
Ga3 O3 O1 51.54(13) . 2_454
Ga3 O3 O1 161.5(2) 1_656 2_454
O3 O3 O1 146.43(15) 1_556 2_454
O3 O3 O1 33.57(16) 1_554 2_454
O2 O3 O1 30.9(2) 3_454 2_454
O2 O3 O1 89.5(3) 1_654 2_454
La O3 O1 26.57(6) 4_444 2_454
O2 O3 O1 86.71(19) 2 2_454
O2 O3 O1 86.5(3) 5_455 2_454
O1 O3 O1 119.1(4) 2_565 2_454
O1 O3 O1 53.57(15) 1_544 2_454
O2 O3 O1 88.1(2) 3_455 2_454
O2 O3 O1 141.5(2) 1_655 2_454
Ga2 O3 O1 123.45(19) 2_565 2_454
O3 O3 O1 61.39(13) 4_445 2_454
O3 O3 O1 61.39(13) 3_455 2_454
O2 O3 O1 142.5(2) 2_566 2_454
O2 O3 O1 129.1(3) 5_446 2_454
O2 O3 O1 70.64(17) 6_545 2_454
Ga2 O3 O1 101.6(3) 1_665 2_454
La O3 O1 69.34(15) 2_455 2_454
La O3 O1 62.72(14) 2_554 2_454
Ga3 O3 O3 116.6(6) 4_445 3_556
Nb O3 O3 30.3(3) . 3_556
Ga1 O3 O3 30.3(3) . 3_556
La O3 O3 87.5(4) . 3_556
Ga3 O3 O3 115.7(3) 2_564 3_556
O3 O3 O3 38.7(4) 6 3_556
O3 O3 O3 61.93(13) 3 3_556
O3 O3 O3 76.39(6) 4 3_556
O2 O3 O3 110.5(4) 2_565 3_556
O3 O3 O3 149.0(4) 6_554 3_556
O2 O3 O3 83.3(6) 5_445 3_556
O2 O3 O3 141.2(7) 4_444 3_556
O1 O3 O3 102.8(5) 2_455 3_556
O3 O3 O3 16.0(3) 2 3_556
O2 O3 O3 49.8(3) 4_445 3_556
O3 O3 O3 114.9(6) 2_554 3_556
Ga2 O3 O3 131.5(5) . 3_556
Ga3 O3 O3 84.7(3) 1_655 3_556
La O3 O3 74.3(4) 4_445 3_556
O2 O3 O3 122.5(3) 6 3_556
O3 O3 O3 34.4(3) 5 3_556
Ga3 O3 O3 22.08(12) 4_446 3_556
Ga2 O3 O3 128.6(2) 2_564 3_556
O3 O3 O3 108.0(4) 5_554 3_556
Ga1 O3 O3 131.7(2) 1_554 3_556
Nb O3 O3 131.7(2) 1_554 3_556
O2 O3 O3 148.1(4) 1_554 3_556
La O3 O3 49.1(2) 2 3_556
O1 O3 O3 84.7(3) . 3_556
Ga3 O3 O3 39.27(8) 2_565 3_556
La O3 O3 178.7(4) 1_554 3_556
O2 O3 O3 116.5(3) 3_564 3_556
O2 O3 O3 78.8(4) . 3_556
Ga2 O3 O3 89.9(3) 2_554 3_556
La O3 O3 86.47(16) 2_565 3_556
O2 O3 O3 57.57(17) 3_565 3_556
Ga2 O3 O3 62.8(2) 1_556 3_556
O2 O3 O3 70.0(3) 6_655 3_556
O1 O3 O3 147.3(3) 1_554 3_556
O1 O3 O3 53.5(3) 1_545 3_556
La O3 O3 62.98(16) 4 3_556
Ga3 O3 O3 133.5(3) . 3_556
Ga3 O3 O3 17.92(11) 1_656 3_556
O3 O3 O3 28.07(13) 1_556 3_556
O3 O3 O3 151.93(13) 1_554 3_556
O2 O3 O3 128.4(4) 3_454 3_556
O2 O3 O3 88.6(3) 1_654 3_556
La O3 O3 131.2(4) 4_444 3_556
O2 O3 O3 73.5(3) 2 3_556
O2 O3 O3 113.9(3) 5_455 3_556
O1 O3 O3 84.5(2) 2_565 3_556
O1 O3 O3 107.2(4) 1_544 3_556
O2 O3 O3 76.1(3) 3_455 3_556
O2 O3 O3 30.7(2) 1_655 3_556
Ga2 O3 O3 68.57(12) 2_565 3_556
O3 O3 O3 96.1(3) 4_445 3_556
O3 O3 O3 116.77(17) 3_455 3_556
O2 O3 O3 50.53(16) 2_566 3_556
O2 O3 O3 28.9(2) 5_446 3_556
O2 O3 O3 85.5(3) 6_545 3_556
Ga2 O3 O3 101.1(2) 1_665 3_556
La O3 O3 99.6(3) 2_455 3_556
La O3 O3 107.5(3) 2_554 3_556
O1 O3 O3 155.9(4) 2_454 3_556
Ga3 O3 O3 140.2(6) 4_445 4_556
Nb O3 O3 30.3(3) . 4_556
Ga1 O3 O3 30.3(3) . 4_556
La O3 O3 74.8(3) . 4_556
Ga3 O3 O3 95.5(3) 2_564 4_556
O3 O3 O3 18.10(17) 6 4_556
O3 O3 O3 76.39(6) 3 4_556
O3 O3 O3 61.93(13) 4 4_556
O2 O3 O3 83.3(4) 2_565 4_556
O3 O3 O3 134.4(5) 6_554 4_556
O2 O3 O3 110.5(6) 5_445 4_556
O2 O3 O3 167.2(7) 4_444 4_556
O1 O3 O3 111.0(4) 2_455 4_556
O3 O3 O3 42.9(3) 2 4_556
O2 O3 O3 61.8(2) 4_445 4_556
O3 O3 O3 129.7(6) 2_554 4_556
Ga2 O3 O3 141.8(3) . 4_556
Ga3 O3 O3 89.2(3) 1_655 4_556
La O3 O3 96.1(3) 4_445 4_556
O2 O3 O3 102.8(4) 6 4_556
O3 O3 O3 26.2(4) 5 4_556
Ga3 O3 O3 38.80(6) 4_446 4_556
Ga2 O3 O3 102.2(3) 2_564 4_556
O3 O3 O3 103.8(4) 5_554 4_556
Ga1 O3 O3 131.7(2) 1_554 4_556
Nb O3 O3 131.7(2) 1_554 4_556
O2 O3 O3 141.3(3) 1_554 4_556
La O3 O3 73.9(3) 2 4_556
O1 O3 O3 61.9(2) . 4_556
Ga3 O3 O3 13.25(11) 2_565 4_556
La O3 O3 151.6(4) 1_554 4_556
O2 O3 O3 96.0(3) 3_564 4_556
O2 O3 O3 75.0(3) . 4_556
Ga2 O3 O3 116.9(4) 2_554 4_556
La O3 O3 59.3(2) 2_565 4_556
O2 O3 O3 30.9(2) 3_565 4_556
Ga2 O3 O3 68.42(12) 1_556 4_556
O2 O3 O3 70.0(3) 6_655 4_556
O1 O3 O3 120.1(3) 1_554 4_556
O1 O3 O3 80.2(3) 1_545 4_556
La O3 O3 47.6(2) 4 4_556
Ga3 O3 O3 119.9(2) . 4_556
Ga3 O3 O3 26.43(16) 1_656 4_556
O3 O3 O3 28.07(13) 1_556 4_556
O3 O3 O3 151.93(13) 1_554 4_556
O2 O3 O3 144.6(3) 3_454 4_556
O2 O3 O3 99.0(4) 1_654 4_556
La O3 O3 158.5(4) 4_444 4_556
O2 O3 O3 99.6(3) 2 4_556
O2 O3 O3 87.5(3) 5_455 4_556
O1 O3 O3 61.2(3) 2_565 4_556
O1 O3 O3 133.2(4) 1_544 4_556
O2 O3 O3 86.8(2) 3_455 4_556
O2 O3 O3 46.6(3) 1_655 4_556
Ga2 O3 O3 48.08(15) 2_565 4_556
O3 O3 O3 116.77(17) 4_445 4_556
O3 O3 O3 110.1(2) 3_455 4_556
O2 O3 O3 28.93(17) 2_566 4_556
O2 O3 O3 50.52(18) 5_446 4_556
O2 O3 O3 112.3(3) 6_545 4_556
Ga2 O3 O3 79.6(2) 1_665 4_556
La O3 O3 103.65(17) 2_455 4_556
La O3 O3 125.9(3) 2_554 4_556
O1 O3 O3 171.3(3) 2_454 4_556
O3 O3 O3 27.22(12) 3_556 4_556
Ga3 O3 O3 33.3(3) 4_445 3_554
Nb O3 O3 102.7(5) . 3_554
Ga1 O3 O3 102.7(5) . 3_554
La O3 O3 148.5(4) . 3_554
Ga3 O3 O3 61.6(3) 2_564 3_554
O3 O3 O3 148.3(5) 6 3_554
O3 O3 O3 61.93(13) 3 3_554
O3 O3 O3 76.39(6) 4 3_554
O2 O3 O3 97.5(5) 2_565 3_554
O3 O3 O3 37.6(3) 6_554 3_554
O2 O3 O3 70.4(4) 5_445 3_554
O2 O3 O3 54.2(3) 4_444 3_554
O1 O3 O3 114.7(4) 2_455 3_554
O3 O3 O3 112.6(4) 2 3_554
O2 O3 O3 144.7(4) 4_445 3_554
O3 O3 O3 14.1(3) 2_554 3_554
Ga2 O3 O3 85.5(2) . 3_554
Ga3 O3 O3 42.9(3) 1_655 3_554
La O3 O3 107.5(3) 4_445 3_554
O2 O3 O3 112.2(4) 6 3_554
O3 O3 O3 105.8(5) 5 3_554
Ga3 O3 O3 138.4(3) 4_446 3_554
Ga2 O3 O3 95.5(3) 2_564 3_554
O3 O3 O3 32.4(4) 5_554 3_554
Ga1 O3 O3 13.88(6) 1_554 3_554
Nb O3 O3 13.88(6) 1_554 3_554
O2 O3 O3 84.0(2) 1_554 3_554
La O3 O3 81.3(2) 2 3_554
O1 O3 O3 139.0(4) . 3_554
Ga3 O3 O3 138.5(3) 2_565 3_554
La O3 O3 56.20(10) 1_554 3_554
O2 O3 O3 61.9(4) 3_564 3_554
O2 O3 O3 153.1(4) . 3_554
Ga2 O3 O3 62.35(19) 2_554 3_554
La O3 O3 113.3(3) 2_565 3_554
O2 O3 O3 120.8(4) 3_565 3_554
Ga2 O3 O3 151.4(3) 1_556 3_554
O2 O3 O3 61.9(3) 6_655 3_554
O1 O3 O3 75.6(2) 1_554 3_554
O1 O3 O3 99.1(3) 1_545 3_554
La O3 O3 89.0(3) 4 3_554
Ga3 O3 O3 102.36(19) . 3_554
Ga3 O3 O3 110.9(2) 1_656 3_554
O3 O3 O3 151.93(13) 1_556 3_554
O3 O3 O3 28.07(13) 1_554 3_554
O2 O3 O3 80.4(3) 3_454 3_554
O2 O3 O3 35.4(3) 1_654 3_554
La O3 O3 50.32(15) 4_444 3_554
O2 O3 O3 66.5(3) 2 3_554
O2 O3 O3 106.8(3) 5_455 3_554
O1 O3 O3 91.1(3) 2_565 3_554
O1 O3 O3 45.93(19) 1_544 3_554
O2 O3 O3 132.4(3) 3_455 3_554
O2 O3 O3 93.4(3) 1_655 3_554
Ga2 O3 O3 153.4(4) 2_565 3_554
O3 O3 O3 96.1(3) 4_445 3_554
O3 O3 O3 116.77(17) 3_455 3_554
O2 O3 O3 152.0(4) 2_566 3_554
O2 O3 O3 130.0(3) 5_446 3_554
O2 O3 O3 79.0(3) 6_545 3_554
Ga2 O3 O3 74.5(3) 1_665 3_554
La O3 O3 123.4(2) 2_455 3_554
La O3 O3 24.29(12) 2_554 3_554
O1 O3 O3 56.13(16) 2_454 3_554
O3 O3 O3 123.9(3) 3_556 3_554
O3 O3 O3 131.9(2) 4_556 3_554
Ga3 O3 O3 59.0(4) 4_445 4_554
Nb O3 O3 102.7(4) . 4_554
Ga1 O3 O3 102.7(4) . 4_554
La O3 O3 129.3(6) . 4_554
Ga3 O3 O3 35.5(3) 2_564 4_554
O3 O3 O3 132.9(7) 6 4_554
O3 O3 O3 76.39(6) 3 4_554
O3 O3 O3 61.93(13) 4 4_554
O2 O3 O3 70.4(5) 2_565 4_554
O3 O3 O3 18.12(19) 6_554 4_554
O2 O3 O3 97.5(3) 5_445 4_554
O2 O3 O3 67.1(4) 4_444 4_554
O1 O3 O3 123.6(4) 2_455 4_554
O3 O3 O3 127.8(4) 2 4_554
O2 O3 O3 171.8(4) 4_445 4_554
O3 O3 O3 41.2(3) 2_554 4_554
Ga2 O3 O3 92.6(3) . 4_554
Ga3 O3 O3 49.09(19) 1_655 4_554
La O3 O3 132.7(2) 4_445 4_554
O2 O3 O3 93.6(4) 6 4_554
O3 O3 O3 101.5(5) 5 4_554
Ga3 O3 O3 153.5(3) 4_446 4_554
Ga2 O3 O3 71.6(4) 2_564 4_554
O3 O3 O3 24.0(3) 5_554 4_554
Ga1 O3 O3 13.88(6) 1_554 4_554
Nb O3 O3 13.88(6) 1_554 4_554
O2 O3 O3 80.0(3) 1_554 4_554
La O3 O3 103.0(2) 2 4_554
O1 O3 O3 112.0(5) . 4_554
Ga3 O3 O3 123.4(3) 2_565 4_554
La O3 O3 47.43(19) 1_554 4_554
O2 O3 O3 35.6(4) 3_564 4_554
O2 O3 O3 145.8(4) . 4_554
Ga2 O3 O3 89.43(17) 2_554 4_554
La O3 O3 86.9(4) 2_565 4_554
O2 O3 O3 101.0(4) 3_565 4_554
Ga2 O3 O3 165.3(3) 1_556 4_554
O2 O3 O3 61.9(2) 6_655 4_554
O1 O3 O3 54.0(3) 1_554 4_554
O1 O3 O3 125.7(3) 1_545 4_554
La O3 O3 76.2(2) 4 4_554
Ga3 O3 O3 91.4(3) . 4_554
Ga3 O3 O3 114.4(2) 1_656 4_554
O3 O3 O3 151.93(13) 1_556 4_554
O3 O3 O3 28.07(13) 1_554 4_554
O2 O3 O3 91.5(3) 3_454 4_554
O2 O3 O3 50.6(2) 1_654 4_554
La O3 O3 68.43(12) 4_444 4_554
O2 O3 O3 92.9(3) 2 4_554
O2 O3 O3 80.9(4) 5_455 4_554
O1 O3 O3 68.4(3) 2_565 4_554
O1 O3 O3 72.17(19) 1_544 4_554
O2 O3 O3 149.3(3) 3_455 4_554
O2 O3 O3 103.4(2) 1_655 4_554
Ga2 O3 O3 126.3(4) 2_565 4_554
O3 O3 O3 116.77(17) 4_445 4_554
O3 O3 O3 110.1(2) 3_455 4_554
O2 O3 O3 130.1(4) 2_566 4_554
O2 O3 O3 152.0(3) 5_446 4_554
O2 O3 O3 105.4(3) 6_545 4_554
Ga2 O3 O3 50.1(2) 1_665 4_554
La O3 O3 128.3(3) 2_455 4_554
La O3 O3 51.28(11) 2_554 4_554
O1 O3 O3 61.20(16) 2_454 4_554
O3 O3 O3 131.9(2) 3_556 4_554
O3 O3 O3 123.9(3) 4_556 4_554
O3 O3 O3 27.22(12) 3_554 4_554
Ga3 O3 O1 64.3(3) 4_445 2
Nb O3 O1 48.3(2) . 2
Ga1 O3 O1 48.3(2) . 2
La O3 O1 145.8(5) . 2
Ga3 O3 O1 95.2(2) 2_564 2
O3 O3 O1 93.7(3) 6 2
O3 O3 O1 7.8(3) 3 2
O3 O3 O1 67.1(4) 4 2
O2 O3 O1 128.3(3) 2_565 2
O3 O3 O1 99.6(2) 6_554 2
O2 O3 O1 54.9(4) 5_445 2
O2 O3 O1 100.2(3) 4_444 2
O1 O3 O1 125.3(4) 2_455 2
O3 O3 O1 47.3(3) 2 2
O2 O3 O1 93.8(4) 4_445 2
O3 O3 O1 56.4(4) 2_554 2
Ga2 O3 O1 124.0(3) . 2
Ga3 O3 O1 36.07(18) 1_655 2
La O3 O1 84.0(2) 4_445 2
O2 O3 O1 174.4(4) 6 2
O3 O3 O1 56.1(2) 5 2
Ga3 O3 O1 74.0(2) 4_446 2
Ga2 O3 O1 147.8(3) 2_564 2
O3 O3 O1 62.4(2) 5_554 2
Ga1 O3 O1 75.9(2) 1_554 2
Nb O3 O1 75.9(2) 1_554 2
O2 O3 O1 141.3(3) 1_554 2
La O3 O1 23.34(11) 2 2
O1 O3 O1 137.1(2) . 2
Ga3 O3 O1 89.1(2) 2_565 2
La O3 O1 121.5(3) 1_554 2
O2 O3 O1 96.3(3) 3_564 2
O2 O3 O1 131.6(4) . 2
Ga2 O3 O1 54.78(13) 2_554 2
La O3 O1 116.48(18) 2_565 2
O2 O3 O1 92.2(3) 3_565 2
Ga2 O3 O1 109.8(3) 1_556 2
O2 O3 O1 37.83(17) 6_655 2
O1 O3 O1 136.0(3) 1_554 2
O1 O3 O1 54.51(16) 1_545 2
La O3 O1 65.75(11) 4 2
Ga3 O3 O1 162.9(2) . 2
Ga3 O3 O1 50.06(17) 1_656 2
O3 O3 O1 86.6(2) 1_556 2
O3 O3 O1 93.4(2) 1_554 2
O2 O3 O1 114.3(3) 3_454 2
O2 O3 O1 32.1(2) 1_654 2
La O3 O1 89.03(19) 4_444 2
O2 O3 O1 37.04(15) 2 2
O2 O3 O1 144.8(3) 5_455 2
O1 O3 O1 92.07(13) 2_565 2
O1 O3 O1 61.7(2) 1_544 2
O2 O3 O1 109.6(3) 3_455 2
O2 O3 O1 30.0(2) 1_655 2
Ga2 O3 O1 124.4(3) 2_565 2
O3 O3 O1 96.1(3) 4_445 2
O3 O3 O1 155.8(3) 3_455 2
O2 O3 O1 105.2(3) 2_566 2
O2 O3 O1 69.5(2) 5_446 2
O2 O3 O1 66.69(19) 6_545 2
Ga2 O3 O1 93.12(15) 1_665 2
La O3 O1 131.8(3) 2_455 2
La O3 O1 50.04(18) 2_554 2
O1 O3 O1 112.0(2) 2_454 2
O3 O3 O1 58.7(2) 3_556 2
O3 O3 O1 76.3(3) 4_556 2
O3 O3 O1 65.6(3) 3_554 2
O3 O3 O1 82.5(2) 4_554 2
Ga3 O3 La 91.9(6) 4_445 2_564
Nb O3 La 108.0(5) . 2_564
Ga1 O3 La 108.0(5) . 2_564
La O3 La 93.3(4) . 2_564
Ga3 O3 La 21.91(18) 2_564 2_564
O3 O3 La 108.2(7) 6 2_564
O3 O3 La 106.2(3) 3 2_564
O3 O3 La 61.7(3) 4 2_564
O2 O3 La 34.3(4) 2_565 2_564
O3 O3 La 29.3(4) 6_554 2_564
O2 O3 La 132.0(5) 5_445 2_564
O2 O3 La 82.4(6) 4_444 2_564
O1 O3 La 113.3(4) 2_455 2_564
O3 O3 La 144.34(9) 2 2_564
O2 O3 La 149.4(3) 4_445 2_564
O3 O3 La 78.0(4) 2_554 2_564
Ga2 O3 La 91.4(3) . 2_564
Ga3 O3 La 77.7(3) 1_655 2_564
La O3 La 150.6(3) 4_445 2_564
O2 O3 La 61.2(3) 6 2_564
O3 O3 La 101.6(3) 5 2_564
Ga3 O3 La 147.8(2) 4_446 2_564
Ga2 O3 La 35.72(15) 2_564 2_564
O3 O3 La 51.84(16) 5_554 2_564
Ga1 O3 La 50.03(18) 1_554 2_564
Nb O3 La 50.03(18) 1_554 2_564
O2 O3 La 68.4(3) 1_554 2_564
La O3 La 136.8(2) 2 2_564
O1 O3 La 75.1(3) . 2_564
Ga3 O3 La 102.1(2) 2_565 2_564
La O3 La 44.01(15) 1_554 2_564
O2 O3 La 20.88(17) 3_564 2_564
O2 O3 La 112.4(3) . 2_564
Ga2 O3 La 123.8(3) 2_554 2_564
La O3 La 55.37(16) 2_565 2_564
O2 O3 La 79.8(2) 3_565 2_564
Ga2 O3 La 134.7(2) 1_556 2_564
O2 O3 La 80.8(2) 6_655 2_564
O1 O3 La 24.57(10) 1_554 2_564
O1 O3 La 163.0(3) 1_545 2_564
La O3 La 73.33(19) 4 2_564
Ga3 O3 La 67.61(19) . 2_564
Ga3 O3 La 119.7(2) 1_656 2_564
O3 O3 La 130.37(10) 1_556 2_564
O3 O3 La 49.63(10) 1_554 2_564
O2 O3 La 96.3(3) 3_454 2_564
O2 O3 La 84.8(3) 1_654 2_564
La O3 La 89.9(2) 4_444 2_564
O2 O3 La 130.3(3) 2 2_564
O2 O3 La 43.54(17) 5_455 2_564
O1 O3 La 50.2(2) 2_565 2_564
O1 O3 La 105.0(3) 1_544 2_564
O2 O3 La 135.9(2) 3_455 2_564
O2 O3 La 121.8(2) 1_655 2_564
Ga2 O3 La 90.49(18) 2_565 2_564
O3 O3 La 128.80(16) 4_445 2_564
O3 O3 La 86.4(2) 3_455 2_564
O2 O3 La 100.1(3) 2_566 2_564
O2 O3 La 160.4(2) 5_446 2_564
O2 O3 La 135.7(3) 6_545 2_564
Ga2 O3 La 34.07(10) 1_665 2_564
La O3 La 111.1(2) 2_455 2_564
La O3 La 88.2(2) 2_554 2_564
O1 O3 La 68.93(19) 2_454 2_564
O3 O3 La 134.7(3) 3_556 2_564
O3 O3 La 110.4(2) 4_556 2_564
O3 O3 La 63.90(17) 3_554 2_564
O3 O3 La 37.4(2) 4_554 2_564
O1 O3 La 113.8(2) 2 2_564
Ga3 O3 O2 153.2(5) 4_445 6_556
Nb O3 O2 83.8(4) . 6_556
Ga1 O3 O2 83.8(4) . 6_556
La O3 O2 21.6(2) . 6_556
Ga3 O3 O2 108.2(3) 2_564 6_556
O3 O3 O2 35.57(16) 6 6_556
O3 O3 O2 128.08(13) 3 6_556
O3 O3 O2 101.0(4) 4 6_556
O2 O3 O2 70.5(4) 2_565 6_556
O3 O3 O2 129.4(4) 6_554 6_556
O2 O3 O2 120.7(5) 5_445 6_556
O2 O3 O2 123.6(3) 4_444 6_556
O1 O3 O2 66.0(3) 2_455 6_556
O3 O3 O2 79.3(4) 2 6_556
O2 O3 O2 46.90(17) 4_445 6_556
O3 O3 O2 175.85(16) 2_554 6_556
Ga2 O3 O2 91.8(2) . 6_556
Ga3 O3 O2 141.2(3) 1_655 6_556
La O3 O2 81.8(3) 4_445 6_556
O2 O3 O2 56.1(3) 6 6_556
O3 O3 O2 79.1(4) 5 6_556
Ga3 O3 O2 54.20(18) 4_446 6_556
Ga2 O3 O2 71.54(16) 2_564 6_556
O3 O3 O2 142.2(2) 5_554 6_556
Ga1 O3 O2 153.4(3) 1_554 6_556
Nb O3 O2 153.4(3) 1_554 6_556
O2 O3 O2 88.3(3) 1_554 6_556
La O3 O2 111.4(3) 2 6_556
O1 O3 O2 28.7(2) . 6_556
Ga3 O3 O2 43.85(13) 2_565 6_556
La O3 O2 113.0(2) 1_554 6_556
O2 O3 O2 107.7(3) 3_564 6_556
O2 O3 O2 26.1(3) . 6_556
Ga2 O3 O2 128.3(3) 2_554 6_556
La O3 O2 57.27(14) 2_565 6_556
O2 O3 O2 56.4(2) 3_565 6_556
Ga2 O3 O2 37.05(13) 1_556 6_556
O2 O3 O2 121.5(3) 6_655 6_556
O1 O3 O2 91.5(2) 1_554 6_556
O1 O3 O2 93.4(3) 1_545 6_556
La O3 O2 90.36(17) 4 6_556
Ga3 O3 O2 68.21(14) . 6_556
Ga3 O3 O2 77.5(2) 1_656 6_556
O3 O3 O2 39.15(17) 1_556 6_556
O3 O3 O2 140.85(16) 1_554 6_556
O2 O3 O2 98.7(3) 3_454 6_556
O2 O3 O2 152.6(3) 1_654 6_556
La O3 O2 130.39(19) 4_444 6_556
O2 O3 O2 126.2(4) 2 6_556
O2 O3 O2 60.34(15) 5_455 6_556
O1 O3 O2 82.3(2) 2_565 6_556
O1 O3 O2 142.5(3) 1_544 6_556
O2 O3 O2 53.9(3) 3_455 6_556
O2 O3 O2 96.5(3) 1_655 6_556
Ga2 O3 O2 16.99(10) 2_565 6_556
O3 O3 O2 89.50(13) 4_445 6_556
O3 O3 O2 56.56(17) 3_455 6_556
O2 O3 O2 27.32(19) 2_566 6_556
O2 O3 O2 62.9(3) 5_446 6_556
O2 O3 O2 110.8(3) 6_545 6_556
Ga2 O3 O2 96.99(17) 1_665 6_556
La O3 O2 56.22(13) 2_455 6_556
La O3 O2 167.7(3) 2_554 6_556
O1 O3 O2 117.87(18) 2_454 6_556
O3 O3 O2 66.79(17) 3_556 6_556
O3 O3 O2 53.55(17) 4_556 6_556
O3 O3 O2 167.0(3) 3_554 6_556
O3 O3 O2 140.8(4) 4_554 6_556
O1 O3 O2 125.5(3) 2 6_556
La O3 O2 103.55(19) 2_564 6_556
Ga3 O3 La 137.5(5) 4_445 4_455
Nb O3 La 108.9(3) . 4_455
Ga1 O3 La 108.9(3) . 4_455
La O3 La 27.8(2) . 4_455
Ga3 O3 La 78.0(2) 2_564 4_455
O3 O3 La 66.2(3) 6 4_455
O3 O3 La 152.9(5) 3 4_455
O3 O3 La 95.2(5) 4 4_455
O2 O3 La 38.8(3) 2_565 4_455
O3 O3 La 89.0(3) 6_554 4_455
O2 O3 La 144.0(5) 5_445 4_455
O2 O3 La 102.5(3) 4_444 4_455
O1 O3 La 70.77(17) 2_455 4_455
O3 O3 La 118.6(5) 2 4_455
O2 O3 La 83.7(3) 4_445 4_455
O3 O3 La 139.2(6) 2_554 4_455
Ga2 O3 La 78.63(16) . 4_455
Ga3 O3 La 136.3(3) 1_655 4_455
La O3 La 107.2(2) 4_445 4_455
O2 O3 La 20.8(2) 6 4_455
O3 O3 La 100.8(2) 5 4_455
Ga3 O3 La 94.77(19) 4_446 4_455
Ga2 O3 La 31.22(8) 2_564 4_455
O3 O3 La 115.58(17) 5_554 4_455
Ga1 O3 La 113.4(3) 1_554 4_455
Nb O3 La 113.4(3) 1_554 4_455
O2 O3 La 61.4(2) 1_554 4_455
La O3 La 151.9(3) 2 4_455
O1 O3 La 20.49(18) . 4_455
Ga3 O3 La 69.20(12) 2_565 4_455
La O3 La 75.34(17) 1_554 4_455
O2 O3 La 77.1(3) 3_564 4_455
O2 O3 La 47.79(15) . 4_455
Ga2 O3 La 146.4(2) 2_554 4_455
La O3 La 42.64(8) 2_565 4_455
O2 O3 La 64.8(2) 3_565 4_455
Ga2 O3 La 69.33(11) 1_556 4_455
O2 O3 La 125.3(3) 6_655 4_455
O1 O3 La 50.89(17) 1_554 4_455
O1 O3 La 130.3(3) 1_545 4_455
La O3 La 93.31(16) 4 4_455
Ga3 O3 La 40.15(7) . 4_455
Ga3 O3 La 108.71(18) 1_656 4_455
O3 O3 La 78.51(15) 1_556 4_455
O3 O3 La 101.49(15) 1_554 4_455
O2 O3 La 88.3(3) 3_454 4_455
O2 O3 La 148.6(3) 1_654 4_455
La O3 La 113.86(19) 4_444 4_455
O2 O3 La 160.0(3) 2 4_455
O2 O3 La 23.22(12) 5_455 4_455
O1 O3 La 69.67(14) 2_565 4_455
O1 O3 La 141.4(2) 1_544 4_455
O2 O3 La 77.5(2) 3_455 4_455
O2 O3 La 128.8(3) 1_655 4_455
Ga2 O3 La 35.54(6) 2_565 4_455
O3 O3 La 101.37(17) 4_445 4_455
O3 O3 La 42.88(19) 3_455 4_455
O2 O3 La 54.25(16) 2_566 4_455
O2 O3 La 103.4(2) 5_446 4_455
O2 O3 La 131.2(2) 6_545 4_455
Ga2 O3 La 74.24(15) 1_665 4_455
La O3 La 61.93(9) 2_455 4_455
La O3 La 148.1(3) 2_554 4_455
O1 O3 La 89.72(17) 2_454 4_455
O3 O3 La 104.07(15) 3_556 4_455
O3 O3 La 82.3(2) 4_556 4_455
O3 O3 La 126.5(3) 3_554 4_455
O3 O3 La 102.6(4) 4_554 4_455
O1 O3 La 156.9(2) 2 4_455
La O3 La 65.76(14) 2_564 4_455
O2 O3 La 40.65(11) 6_556 4_455
Ga3 O3 O3 78.8(3) 4_445 5_445
Nb O3 O3 98.6(6) . 5_445
Ga1 O3 O3 98.6(6) . 5_445
La O3 O3 78.3(5) . 5_445
Ga3 O3 O3 172.4(5) 2_564 5_445
O3 O3 O3 88.4(9) 6 5_445
O3 O3 O3 92.7(4) 3 5_445
O3 O3 O3 144.8(4) 4 5_445
O2 O3 O3 143.6(4) 2_565 5_445
O3 O3 O3 133.4(5) 6_554 5_445
O2 O3 O3 43.6(2) 5_445 5_445
O2 O3 O3 75.4(5) 4_444 5_445
O1 O3 O3 42.2(3) 2_455 5_445
O3 O3 O3 62.3(2) 2 5_445
O2 O3 O3 34.6(3) 4_445 5_445
O3 O3 O3 99.16(13) 2_554 5_445
Ga2 O3 O3 62.0(2) . 5_445
Ga3 O3 O3 118.28(18) 1_655 5_445
La O3 O3 4.63(9) 4_445 5_445
O2 O3 O3 100.7(3) 6 5_445
O3 O3 O3 104.7(5) 5 5_445
Ga3 O3 O3 53.2(3) 4_446 5_445
Ga2 O3 O3 127.3(3) 2_564 5_445
O3 O3 O3 138.1(2) 5_554 5_445
Ga1 O3 O3 123.7(2) 1_554 5_445
Nb O3 O3 123.7(2) 1_554 5_445
O2 O3 O3 85.1(3) 1_554 5_445
La O3 O3 62.08(12) 2 5_445
O1 O3 O3 104.9(4) . 5_445
Ga3 O3 O3 96.9(4) 2_565 5_445
La O3 O3 110.5(3) 1_554 5_445
O2 O3 O3 172.0(5) 3_564 5_445
O2 O3 O3 58.3(3) . 5_445
Ga2 O3 O3 50.79(6) 2_554 5_445
La O3 O3 134.8(4) 2_565 5_445
O2 O3 O3 120.1(5) 3_565 5_445
Ga2 O3 O3 40.6(3) 1_556 5_445
O2 O3 O3 121.8(3) 6_655 5_445
O1 O3 O3 130.3(3) 1_554 5_445
O1 O3 O3 30.76(6) 1_545 5_445
La O3 O3 133.2(4) 4 5_445
Ga3 O3 O3 89.0(2) . 5_445
Ga3 O3 O3 86.7(3) 1_656 5_445
O3 O3 O3 66.6(3) 1_556 5_445
O3 O3 O3 113.4(3) 1_554 5_445
O2 O3 O3 57.6(2) 3_454 5_445
O2 O3 O3 106.51(16) 1_654 5_445
La O3 O3 70.75(16) 4_444 5_445
O2 O3 O3 55.3(2) 2 5_445
O2 O3 O3 127.4(3) 5_455 5_445
O1 O3 O3 152.8(4) 2_565 5_445
O1 O3 O3 65.93(16) 1_544 5_445
O2 O3 O3 27.4(3) 3_455 5_445
O2 O3 O3 83.9(3) 1_655 5_445
Ga2 O3 O3 94.2(4) 2_565 5_445
O3 O3 O3 25.4(2) 4_445 5_445
O3 O3 O3 71.9(2) 3_455 5_445
O2 O3 O3 92.6(4) 2_566 5_445
O2 O3 O3 42.4(3) 5_446 5_445
O2 O3 O3 33.1(2) 6_545 5_445
Ga2 O3 O3 171.5(4) 1_665 5_445
La O3 O3 47.0(2) 2_455 5_445
La O3 O3 90.20(12) 2_554 5_445
O1 O3 O3 86.8(2) 2_454 5_445
O3 O3 O3 70.8(4) 3_556 5_445
O3 O3 O3 91.9(3) 4_556 5_445
O3 O3 O3 111.9(2) 3_554 5_445
O3 O3 O3 137.3(2) 4_554 5_445
O1 O3 O3 84.82(13) 2 5_445
La O3 O3 153.4(3) 2_564 5_445
O2 O3 O3 77.7(3) 6_556 5_445
La O3 O3 104.8(3) 4_455 5_445
Ga3 O3 O3 135.0(5) 4_445 5_455
Nb O3 O3 110.6(5) . 5_455
Ga1 O3 O3 110.6(5) . 5_455
La O3 O3 7.27(17) . 5_455
Ga3 O3 O3 100.6(2) 2_564 5_455
O3 O3 O3 62.4(2) 6 5_455
O3 O3 O3 156.2(2) 3 5_455
O3 O3 O3 113.2(5) 4 5_455
O2 O3 O3 61.2(3) 2_565 5_455
O3 O3 O3 106.4(3) 6_554 5_455
O2 O3 O3 123.5(5) 5_445 5_455
O2 O3 O3 99.3(4) 4_444 5_455
O1 O3 O3 52.2(2) 2_455 5_455
O3 O3 O3 105.8(5) 2 5_455
O2 O3 O3 62.8(3) 4_445 5_455
O3 O3 O3 149.4(7) 2_554 5_455
Ga2 O3 O3 69.3(2) . 5_455
Ga3 O3 O3 157.4(3) 1_655 5_455
La O3 O3 85.0(2) 4_445 5_455
O2 O3 O3 29.6(2) 6 5_455
O3 O3 O3 104.7(5) 5 5_455
Ga3 O3 O3 79.3(3) 4_446 5_455
Ga2 O3 O3 51.50(6) 2_564 5_455
O3 O3 O3 138.0(2) 5_554 5_455
Ga1 O3 O3 130.7(4) 1_554 5_455
Nb O3 O3 130.7(4) 1_554 5_455
O2 O3 O3 60.8(2) 1_554 5_455
La O3 O3 134.5(4) 2 5_455
O1 O3 O3 29.26(8) . 5_455
Ga3 O3 O3 69.2(2) 2_565 5_455
La O3 O3 85.3(2) 1_554 5_455
O2 O3 O3 99.7(3) 3_564 5_455
O2 O3 O3 25.48(18) . 5_455
Ga2 O3 O3 128.1(2) 2_554 5_455
La O3 O3 60.48(7) 2_565 5_455
O2 O3 O3 74.2(3) 3_565 5_455
Ga2 O3 O3 47.56(17) 1_556 5_455
O2 O3 O3 141.5(3) 6_655 5_455
O1 O3 O3 68.55(19) 1_554 5_455
O1 O3 O3 108.1(3) 1_545 5_455
La O3 O3 107.50(19) 4 5_455
Ga3 O3 O3 40.16(13) . 5_455
Ga3 O3 O3 105.4(3) 1_656 5_455
O3 O3 O3 66.6(3) 1_556 5_455
O3 O3 O3 113.4(3) 1_554 5_455
O2 O3 O3 78.0(3) 3_454 5_455
O2 O3 O3 171.2(3) 1_654 5_455
La O3 O3 108.7(3) 4_444 5_455
O2 O3 O3 137.7(3) 2 5_455
O2 O3 O3 45.76(12) 5_455 5_455
O1 O3 O3 88.69(13) 2_565 5_455
O1 O3 O3 131.6(2) 1_544 5_455
O2 O3 O3 55.0(3) 3_455 5_455
O2 O3 O3 124.6(4) 1_655 5_455
Ga2 O3 O3 34.12(13) 2_565 5_455
O3 O3 O3 82.1(2) 4_445 5_455
O3 O3 O3 31.3(3) 3_455 5_455
O2 O3 O3 52.1(2) 2_566 5_455
O2 O3 O3 85.2(3) 5_446 5_455
O2 O3 O3 110.8(3) 6_545 5_455
Ga2 O3 O3 96.11(12) 1_665 5_455
La O3 O3 42.40(14) 2_455 5_455
La O3 O3 153.0(3) 2_554 5_455
O1 O3 O3 90.8(3) 2_454 5_455
O3 O3 O3 94.6(3) 3_556 5_455
O3 O3 O3 80.5(2) 4_556 5_455
O3 O3 O3 141.4(3) 3_554 5_455
O3 O3 O3 122.4(4) 4_554 5_455
O1 O3 O3 153.0(4) 2 5_455
La O3 O3 87.12(17) 2_564 5_455
O2 O3 O3 28.10(18) 6_556 5_455
La O3 O3 22.60(5) 4_455 5_455
O3 O3 O3 82.3(3) 5_445 5_455
Ga3 O3 O2 70.5(5) 4_445 2_564
Nb O3 O2 123.6(5) . 2_564
Ga1 O3 O2 123.6(5) . 2_564
La O3 O2 103.4(4) . 2_564
Ga3 O3 O2 38.4(3) 2_564 2_564
O3 O3 O2 131.1(7) 6 2_564
O3 O3 O2 103.7(2) 3 2_564
O3 O3 O2 77.2(3) 4 2_564
O2 O3 O2 55.6(4) 2_565 2_564
O3 O3 O2 10.3(2) 6_554 2_564
O2 O3 O2 110.1(5) 5_445 2_564
O2 O3 O2 60.0(6) 4_444 2_564
O1 O3 O2 102.8(4) 2_455 2_564
O3 O3 O2 154.7(3) 2 2_564
O2 O3 O2 154.3(4) 4_445 2_564
O3 O3 O2 60.9(5) 2_554 2_564
Ga2 O3 O2 74.9(3) . 2_564
Ga3 O3 O2 76.2(3) 1_655 2_564
La O3 O2 130.6(3) 4_445 2_564
O2 O3 O2 66.8(3) 6 2_564
O3 O3 O2 119.3(4) 5 2_564
Ga3 O3 O2 170.8(3) 4_446 2_564
Ga2 O3 O2 47.9(2) 2_564 2_564
O3 O3 O2 50.1(3) 5_554 2_564
Ga1 O3 O2 34.84(16) 1_554 2_564
Nb O3 O2 34.84(16) 1_554 2_564
O2 O3 O2 56.3(2) 1_554 2_564
La O3 O2 128.7(2) 2 2_564
O1 O3 O2 93.1(4) . 2_564
Ga3 O3 O2 125.2(3) 2_565 2_564
La O3 O2 25.27(16) 1_554 2_564
O2 O3 O2 37.7(3) 3_564 2_564
O2 O3 O2 118.5(3) . 2_564
Ga2 O3 O2 102.1(3) 2_554 2_564
La O3 O2 78.1(2) 2_565 2_564
O2 O3 O2 102.7(3) 3_565 2_564
Ga2 O3 O2 138.9(2) 1_556 2_564
O2 O3 O2 86.8(3) 6_655 2_564
O1 O3 O2 28.0(2) 1_554 2_564
O1 O3 O2 142.5(3) 1_545 2_564
La O3 O2 90.8(3) 4 2_564
Ga3 O3 O2 64.4(2) . 2_564
Ga3 O3 O2 136.0(2) 1_656 2_564
O3 O3 O2 152.75(14) 1_556 2_564
O3 O3 O2 27.25(14) 1_554 2_564
O2 O3 O2 77.6(3) 3_454 2_564
O2 O3 O2 77.5(3) 1_654 2_564
La O3 O2 66.8(2) 4_444 2_564
O2 O3 O2 112.5(3) 2 2_564
O2 O3 O2 60.3(2) 5_455 2_564
O1 O3 O2 71.8(3) 2_565 2_564
O1 O3 O2 83.1(3) 1_544 2_564
O2 O3 O2 129.4(2) 3_455 2_564
O2 O3 O2 129.6(3) 1_655 2_564
Ga2 O3 O2 109.7(2) 2_565 2_564
O3 O3 O2 109.15(14) 4_445 2_564
O3 O3 O2 83.54(17) 3_455 2_564
O2 O3 O2 122.1(4) 2_566 2_564
O2 O3 O2 176.5(2) 5_446 2_564
O2 O3 O2 112.7(3) 6_545 2_564
Ga2 O3 O2 53.84(19) 1_665 2_564
La O3 O2 104.7(2) 2_455 2_564
La O3 O2 70.81(19) 2_554 2_564
O1 O3 O2 47.78(19) 2_454 2_564
O3 O3 O2 153.6(3) 3_556 2_564
O3 O3 O2 132.9(3) 4_556 2_564
O3 O3 O2 47.69(12) 3_554 2_564
O3 O3 O2 27.31(18) 4_554 2_564
O1 O3 O2 109.6(3) 2 2_564
La O3 O2 23.09(13) 2_564 2_564
O2 O3 O2 119.4(2) 6_556 2_564
La O3 O2 78.8(2) 4_455 2_564
O3 O3 O2 134.6(3) 5_445 2_564
O3 O3 O2 96.2(3) 5_455 2_564
Ga3 O3 La 75.0(5) 4_445 4_554
Nb O3 La 81.3(4) . 4_554
Ga1 O3 La 81.3(4) . 4_554
La O3 La 129.6(5) . 4_554
Ga3 O3 La 24.30(14) 2_564 4_554
O3 O3 La 111.3(6) 6 4_554
O3 O3 La 66.2(3) 3 4_554
O3 O3 La 38.99(11) 4 4_554
O2 O3 La 64.1(4) 2_565 4_554
O3 O3 La 37.7(2) 6_554 4_554
O2 O3 La 107.8(4) 5_445 4_554
O2 O3 La 89.8(5) 4_444 4_554
O1 O3 La 145.7(5) 2_455 4_554
O3 O3 La 111.8(2) 2 4_554
O2 O3 La 161.2(3) 4_445 4_554
O3 O3 La 53.18(17) 2_554 4_554
Ga2 O3 La 115.3(4) . 4_554
Ga3 O3 La 37.72(17) 1_655 4_554
La O3 La 147.7(2) 4_445 4_554
O2 O3 La 101.1(4) 6 4_554
O3 O3 La 79.1(3) 5 4_554
Ga3 O3 La 133.5(2) 4_446 4_554
Ga2 O3 La 75.0(2) 2_564 4_554
O3 O3 La 13.54(10) 5_554 4_554
Ga1 O3 La 33.00(11) 1_554 4_554
Nb O3 La 33.00(11) 1_554 4_554
O2 O3 La 99.7(3) 1_554 4_554
La O3 La 96.94(16) 2 4_554
O1 O3 La 103.7(3) . 4_554
Ga3 O3 La 101.37(19) 2_565 4_554
La O3 La 67.7(2) 1_554 4_554
O2 O3 La 25.1(3) 3_564 4_554
O2 O3 La 149.8(3) . 4_554
Ga2 O3 La 100.75(19) 2_554 4_554
La O3 La 73.04(19) 2_565 4_554
O2 O3 La 80.2(3) 3_565 4_554
Ga2 O3 La 166.7(2) 1_556 4_554
O2 O3 La 43.48(17) 6_655 4_554
O1 O3 La 63.5(2) 1_554 4_554
O1 O3 La 126.70(18) 1_545 4_554
La O3 La 53.28(13) 4 4_554
Ga3 O3 La 106.0(3) . 4_554
Ga3 O3 La 93.52(14) 1_656 4_554
O3 O3 La 128.97(11) 1_556 4_554
O3 O3 La 51.03(11) 1_554 4_554
O2 O3 La 114.5(3) 3_454 4_554
O2 O3 La 46.54(16) 1_654 4_554
La O3 La 89.8(2) 4_444 4_554
O2 O3 La 97.0(2) 2 4_554
O2 O3 La 79.0(2) 5_455 4_554
O1 O3 La 49.19(19) 2_565 4_554
O1 O3 La 87.0(2) 1_544 4_554
O2 O3 La 172.2(3) 3_455 4_554
O2 O3 La 86.53(17) 1_655 4_554
Ga2 O3 La 113.4(2) 2_565 4_554
O3 O3 La 137.65(14) 4_445 4_554
O3 O3 La 125.3(2) 3_455 4_554
O2 O3 La 110.9(3) 2_566 4_554
O2 O3 La 137.6(3) 5_446 4_554
O2 O3 La 118.7(2) 6_545 4_554
Ga2 O3 La 33.29(9) 1_665 4_554
La O3 La 148.2(3) 2_455 4_554
La O3 La 61.56(13) 2_554 4_554
O1 O3 La 84.1(2) 2_454 4_554
O3 O3 La 111.4(2) 3_556 4_554
O3 O3 La 100.9(2) 4_556 4_554
O3 O3 La 41.88(19) 3_554 4_554
O3 O3 La 22.97(13) 4_554 4_554
O1 O3 La 73.75(15) 2 4_554
La O3 La 40.01(11) 2_564 4_554
O2 O3 La 130.3(2) 6_556 4_554
La O3 La 102.2(2) 4_455 4_554
O3 O3 La 151.4(2) 5_445 4_554
O3 O3 La 124.7(2) 5_455 4_554
O2 O3 La 43.56(15) 2_564 4_554
Ga3 O3 O2 16.7(4) 4_445 5_444
Nb O3 O2 123.5(4) . 5_444
Ga1 O3 O2 123.5(4) . 5_444
La O3 O2 131.2(4) . 5_444
Ga3 O3 O2 82.8(3) 2_564 5_444
O3 O3 O2 171.2(4) 6 5_444
O3 O3 O2 77.2(3) 3 5_444
O3 O3 O2 103.7(2) 4 5_444
O2 O3 O2 110.1(5) 2_565 5_444
O3 O3 O2 47.5(4) 6_554 5_444
O2 O3 O2 55.6(3) 5_445 5_444
O2 O3 O2 28.2(2) 4_444 5_444
O1 O3 O2 87.6(4) 2_455 5_444
O3 O3 O2 117.3(4) 2 5_444
O2 O3 O2 124.4(4) 4_445 5_444
O3 O3 O2 24.6(4) 2_554 5_444
Ga2 O3 O2 60.0(2) . 5_444
Ga3 O3 O2 67.0(3) 1_655 5_444
La O3 O2 85.15(19) 4_445 5_444
O2 O3 O2 102.7(5) 6 5_444
O3 O3 O2 129.0(4) 5 5_444
Ga3 O3 O2 134.5(3) 4_446 5_444
Ga2 O3 O2 97.6(3) 2_564 5_444
O3 O3 O2 59.6(4) 5_554 5_444
Ga1 O3 O2 34.83(14) 1_554 5_444
Nb O3 O2 34.83(14) 1_554 5_444
O2 O3 O2 65.2(2) 1_554 5_444
La O3 O2 83.7(2) 2 5_444
O1 O3 O2 142.5(4) . 5_444
Ga3 O3 O2 164.5(3) 2_565 5_444
La O3 O2 47.94(17) 1_554 5_444
O2 O3 O2 82.8(4) 3_564 5_444
O2 O3 O2 127.1(2) . 5_444
Ga2 O3 O2 47.58(16) 2_554 5_444
La O3 O2 132.0(3) 2_565 5_444
O2 O3 O2 147.7(4) 3_565 5_444
Ga2 O3 O2 125.5(2) 1_556 5_444
O2 O3 O2 86.8(2) 6_655 5_444
O1 O3 O2 77.2(3) 1_554 5_444
O1 O3 O2 88.0(3) 1_545 5_444
La O3 O2 116.1(3) 4 5_444
Ga3 O3 O2 86.5(2) . 5_444
Ga3 O3 O2 127.6(2) 1_656 5_444
O3 O3 O2 152.73(17) 1_556 5_444
O3 O3 O2 27.27(17) 1_554 5_444
O2 O3 O2 53.67(18) 3_454 5_444
O2 O3 O2 55.4(4) 1_654 5_444
La O3 O2 23.05(14) 4_444 5_444
O2 O3 O2 60.38(16) 2 5_444
O2 O3 O2 112.0(4) 5_455 5_444
O1 O3 O2 116.0(3) 2_565 5_444
O1 O3 O2 28.6(2) 1_544 5_444
O2 O3 O2 105.9(2) 3_455 5_444
O2 O3 O2 107.5(3) 1_655 5_444
Ga2 O3 O2 158.0(3) 2_565 5_444
O3 O3 O2 70.1(2) 4_445 5_444
O3 O3 O2 95.5(2) 3_455 5_444
O2 O3 O2 176.5(4) 2_566 5_444
O2 O3 O2 122.1(3) 5_446 5_444
O2 O3 O2 59.76(19) 6_545 5_444
Ga2 O3 O2 97.8(3) 1_665 5_444
La O3 O2 96.8(2) 2_455 5_444
La O3 O2 27.69(18) 2_554 5_444
O1 O3 O2 35.08(18) 2_454 5_444
O3 O3 O2 132.8(3) 3_556 5_444
O3 O3 O2 153.6(3) 4_556 5_444
O3 O3 O2 27.28(19) 3_554 5_444
O3 O3 O2 47.69(12) 4_554 5_444
O1 O3 O2 77.5(3) 2 5_444
La O3 O2 76.7(2) 2_564 5_444
O2 O3 O2 151.7(2) 6_556 5_444
La O3 O2 122.6(3) 4_455 5_444
O3 O3 O2 89.8(2) 5_445 5_444
O3 O3 O2 125.8(3) 5_455 5_444
O2 O3 O2 54.5(2) 2_564 5_444
La O3 O2 67.5(2) 4_554 5_444
Ga3 O3 La 84.3(3) 4_445 1_655
Nb O3 La 29.4(2) . 1_655
Ga1 O3 La 29.4(2) . 1_655
La O3 La 134.4(4) . 1_655
Ga3 O3 La 80.1(2) 2_564 1_655
O3 O3 La 77.75(11) 6 1_655
O3 O3 La 19.5(3) 3 1_655
O3 O3 La 45.1(3) 4 1_655
O2 O3 La 106.1(3) 2_565 1_655
O3 O3 La 98.90(18) 6_554 1_655
O2 O3 La 78.8(4) 5_445 1_655
O2 O3 La 120.5(3) 4_444 1_655
O1 O3 La 144.6(4) 2_455 1_655
O3 O3 La 47.9(2) 2 1_655
O2 O3 La 98.8(4) 4_445 1_655
O3 O3 La 70.1(3) 2_554 1_655
Ga2 O3 La 147.8(2) . 1_655
Ga3 O3 La 32.80(12) 1_655 1_655
La O3 La 102.8(3) 4_445 1_655
O2 O3 La 151.3(3) 6 1_655
O3 O3 La 35.3(2) 5 1_655
Ga3 O3 La 72.72(17) 4_446 1_655
Ga2 O3 La 128.7(3) 2_564 1_655
O3 O3 La 57.1(2) 5_554 1_655
Ga1 O3 La 79.90(14) 1_554 1_655
Nb O3 La 79.90(14) 1_554 1_655
O2 O3 La 158.3(3) 1_554 1_655
La O3 La 41.71(8) 2 1_655
O1 O3 La 115.3(2) . 1_655
Ga3 O3 La 70.69(14) 2_565 1_655
La O3 La 127.7(3) 1_554 1_655
O2 O3 La 81.1(2) 3_564 1_655
O2 O3 La 130.6(4) . 1_655
Ga2 O3 La 78.94(14) 2_554 1_655
La O3 La 92.32(15) 2_565 1_655
O2 O3 La 69.0(2) 3_565 1_655
Ga2 O3 La 113.7(3) 1_556 1_655
O2 O3 La 20.85(14) 6_655 1_655
O1 O3 La 126.1(3) 1_554 1_655
O1 O3 La 71.85(15) 1_545 1_655
La O3 La 41.77(7) 4 1_655
Ga3 O3 La 168.6(3) . 1_655
Ga3 O3 La 36.70(6) 1_656 1_655
O3 O3 La 78.69(14) 1_556 1_655
O3 O3 La 101.32(14) 1_554 1_655
O2 O3 La 138.2(3) 3_454 1_655
O2 O3 La 39.6(2) 1_654 1_655
La O3 La 110.38(15) 4_444 1_655
O2 O3 La 60.99(16) 2 1_655
O2 O3 La 121.7(3) 5_455 1_655
O1 O3 La 68.93(11) 2_565 1_655
O1 O3 La 84.36(13) 1_544 1_655
O2 O3 La 121.8(3) 3_455 1_655
O2 O3 La 22.68(12) 1_655 1_655
Ga2 O3 La 106.03(18) 2_565 1_655
O3 O3 La 118.5(3) 4_445 1_655
O3 O3 La 168.65(15) 3_455 1_655
O2 O3 La 87.77(19) 2_566 1_655
O2 O3 La 73.7(2) 5_446 1_655
O2 O3 La 90.2(2) 6_545 1_655
Ga2 O3 La 73.48(11) 1_665 1_655
La O3 La 147.1(3) 2_455 1_655
La O3 La 67.10(9) 2_554 1_655
O1 O3 La 129.0(2) 2_454 1_655
O3 O3 La 51.93(16) 3_556 1_655
O3 O3 La 59.7(2) 4_556 1_655
O3 O3 La 74.3(2) 3_554 1_655
O3 O3 La 80.86(17) 4_554 1_655
O1 O3 La 24.17(7) 2 1_655
La O3 La 101.48(18) 2_564 1_655
O2 O3 La 113.1(2) 6_556 1_655
La O3 La 133.54(17) 4_455 1_655
O3 O3 La 102.3(2) 5_445 1_655
O3 O3 La 139.9(3) 5_455 1_655
O2 O3 La 106.9(2) 2_564 1_655
La O3 La 64.15(10) 4_554 1_655
O2 O3 La 94.2(2) 5_444 1_655
Ga3 O3 O3 38.19(19) 4_445 5_444
Nb O3 O3 130.5(4) . 5_444
Ga1 O3 O3 130.5(4) . 5_444
La O3 O3 102.4(4) . 5_444
Ga3 O3 O3 123.8(5) 2_564 5_444
O3 O3 O3 136.7(9) 6 5_444
O3 O3 O3 92.6(4) 3 5_444
O3 O3 O3 143.7(3) 4 5_444
O2 O3 O3 133.7(5) 2_565 5_444
O3 O3 O3 85.0(5) 6_554 5_444
O2 O3 O3 35.4(4) 5_445 5_444
O2 O3 O3 28.3(4) 4_444 5_444
O1 O3 O3 50.3(3) 2_455 5_444
O3 O3 O3 99.50(16) 2 5_444
O2 O3 O3 82.3(4) 4_445 5_444
O3 O3 O3 60.8(3) 2_554 5_444
Ga2 O3 O3 36.3(2) . 5_444
Ga3 O3 O3 99.8(2) 1_655 5_444
La O3 O3 44.08(12) 4_445 5_444
O2 O3 O3 96.3(3) 6 5_444
O3 O3 O3 139.33(16) 5 5_444
Ga3 O3 O3 100.7(3) 4_446 5_444
Ga2 O3 O3 110.7(3) 2_564 5_444
O3 O3 O3 101.5(5) 5_554 5_444
Ga1 O3 O3 77.9(3) 1_554 5_444
Nb O3 O3 77.9(3) 1_554 5_444
O2 O3 O3 58.3(3) 1_554 5_444
La O3 O3 76.78(8) 2 5_444
O1 O3 O3 130.2(3) . 5_444
Ga3 O3 O3 145.5(5) 2_565 5_444
La O3 O3 67.9(2) 1_554 5_444
O2 O3 O3 123.5(5) 3_564 5_444
O2 O3 O3 89.1(3) . 5_444
Ga2 O3 O3 33.16(6) 2_554 5_444
La O3 O3 154.9(2) 2_565 5_444
O2 O3 O3 168.7(5) 3_565 5_444
Ga2 O3 O3 82.5(3) 1_556 5_444
O2 O3 O3 117.4(3) 6_655 5_444
O1 O3 O3 97.6(3) 1_554 5_444
O1 O3 O3 60.13(17) 1_545 5_444
La O3 O3 151.3(2) 4 5_444
Ga3 O3 O3 76.3(2) . 5_444
Ga3 O3 O3 123.3(3) 1_656 5_444
O3 O3 O3 115.2(3) 1_556 5_444
O3 O3 O3 64.8(3) 1_554 5_444
O2 O3 O3 26.7(2) 3_454 5_444
O2 O3 O3 85.0(3) 1_654 5_444
La O3 O3 22.17(12) 4_444 5_444
O2 O3 O3 52.08(11) 2 5_444
O2 O3 O3 123.1(3) 5_455 5_444
O1 O3 O3 158.5(5) 2_565 5_444
O1 O3 O3 30.54(11) 1_544 5_444
O2 O3 O3 63.1(3) 3_455 5_444
O2 O3 O3 108.7(2) 1_655 5_444
Ga2 O3 O3 131.0(3) 2_565 5_444
O3 O3 O3 27.1(3) 4_445 5_444
O3 O3 O3 72.2(3) 3_455 5_444
O2 O3 O3 138.4(4) 2_566 5_444
O2 O3 O3 88.6(3) 5_446 5_444
O2 O3 O3 28.53(13) 6_545 5_444
Ga2 O3 O3 139.7(4) 1_665 5_444
La O3 O3 60.4(2) 2_455 5_444
La O3 O3 56.10(16) 2_554 5_444
O1 O3 O3 42.56(17) 2_454 5_444
O3 O3 O3 113.4(4) 3_556 5_444
O3 O3 O3 139.0(4) 4_556 5_444
O3 O3 O3 69.3(2) 3_554 5_444
O3 O3 O3 90.2(2) 4_554 5_444
O1 O3 O3 87.71(11) 2 5_444
La O3 O3 110.6(3) 2_564 5_444
O2 O3 O3 115.1(3) 6_556 5_444
La O3 O3 114.5(2) 4_455 5_444
O3 O3 O3 48.60(10) 5_445 5_444
O3 O3 O3 101.1(3) 5_455 5_444
O2 O3 O3 88.0(3) 2_564 5_444
La O3 O3 110.6(3) 4_554 5_444
O2 O3 O3 43.1(2) 5_444 5_444
La O3 O3 111.78(11) 1_655 5_444
Ga3 O3 O3 95.9(6) 4_445 5_454
Nb O3 O3 148.2(3) . 5_454
Ga1 O3 O3 148.2(3) . 5_454
La O3 O3 55.72(17) . 5_454
Ga3 O3 O3 76.1(3) 2_564 5_454
O3 O3 O3 107.42(19) 6 5_454
O3 O3 O3 154.4(3) 3 5_454
O3 O3 O3 112.9(5) 4 5_454
O2 O3 O3 54.8(2) 2_565 5_454
O3 O3 O3 61.0(3) 6_554 5_454
O2 O3 O3 116.3(5) 5_445 5_454
O2 O3 O3 61.8(5) 4_444 5_454
O1 O3 O3 59.1(3) 2_455 5_454
O3 O3 O3 153.1(5) 2 5_454
O2 O3 O3 103.1(3) 4_445 5_454
O3 O3 O3 101.8(7) 2_554 5_454
Ga2 O3 O3 46.3(3) . 5_454
Ga3 O3 O3 127.9(5) 1_655 5_454
La O3 O3 100.2(2) 4_445 5_454
O2 O3 O3 21.3(3) 6 5_454
O3 O3 O3 139.33(16) 5 5_454
Ga3 O3 O3 126.4(3) 4_446 5_454
Ga2 O3 O3 30.85(5) 2_564 5_454
O3 O3 O3 101.5(5) 5_554 5_454
Ga1 O3 O3 83.4(4) 1_554 5_454
Nb O3 O3 83.4(4) 1_554 5_454
O2 O3 O3 22.7(2) 1_554 5_454
La O3 O3 157.6(2) 2 5_454
O1 O3 O3 62.09(18) . 5_454
Ga3 O3 O3 110.80(18) 2_565 5_454
La O3 O3 36.7(2) 1_554 5_454
O2 O3 O3 75.0(3) 3_564 5_454
O2 O3 O3 67.2(2) . 5_454
Ga2 O3 O3 113.3(3) 2_554 5_454
La O3 O3 74.08(6) 2_565 5_454
O2 O3 O3 102.6(2) 3_565 5_454
Ga2 O3 O3 87.3(2) 1_556 5_454
O2 O3 O3 135.4(4) 6_655 5_454
O1 O3 O3 30.06(11) 1_554 5_454
O1 O3 O3 131.0(2) 1_545 5_454
La O3 O3 119.9(2) 4 5_454
Ga3 O3 O3 13.22(8) . 5_454
Ga3 O3 O3 150.3(3) 1_656 5_454
O3 O3 O3 115.2(3) 1_556 5_454
O3 O3 O3 64.8(3) 1_554 5_454
O2 O3 O3 55.2(3) 3_454 5_454
O2 O3 O3 127.4(5) 1_654 5_454
La O3 O3 73.5(3) 4_444 5_454
O2 O3 O3 132.5(3) 2 5_454
O2 O3 O3 42.2(2) 5_455 5_454
O1 O3 O3 91.76(16) 2_565 5_454
O1 O3 O3 101.3(3) 1_544 5_454
O2 O3 O3 81.8(2) 3_455 5_454
O2 O3 O3 169.9(3) 1_655 5_454
Ga2 O3 O3 76.53(14) 2_565 5_454
O3 O3 O3 82.2(2) 4_445 5_454
O3 O3 O3 32.6(2) 3_455 5_454
O2 O3 O3 95.6(2) 2_566 5_454
O2 O3 O3 128.4(4) 5_446 5_454
O2 O3 O3 107.4(2) 6_545 5_454
Ga2 O3 O3 83.8(2) 1_665 5_454
La O3 O3 56.61(15) 2_455 5_454
La O3 O3 108.5(4) 2_554 5_454
O1 O3 O3 48.2(3) 2_454 5_454
O3 O3 O3 143.1(3) 3_556 5_454
O3 O3 O3 124.0(2) 4_556 5_454
O3 O3 O3 92.8(3) 3_554 5_454
O3 O3 O3 78.9(4) 4_554 5_454
O1 O3 O3 158.1(4) 2 5_454
La O3 O3 54.63(18) 2_564 5_454
O2 O3 O3 76.4(2) 6_556 5_454
La O3 O3 41.62(11) 4_455 5_454
O3 O3 O3 101.1(3) 5_445 5_454
O3 O3 O3 48.60(10) 5_455 5_454
O2 O3 O3 51.7(3) 2_564 5_454
La O3 O3 92.7(3) 4_554 5_454
O2 O3 O3 81.4(3) 5_444 5_454
La O3 O3 156.1(3) 1_655 5_454
O3 O3 O3 80.9(3) 5_444 5_454
Ga2 O2 Ga3 119.7(8) 1_556 1_556
Ga2 O2 La 105.5(5) 1_556 .
Ga3 O2 La 120.0(6) 1_556 .
Ga2 O2 O2 39.9(3) 1_556 3_455
Ga3 O2 O2 129.5(8) 1_556 3_455
La O2 O2 110.4(3) . 3_455
Ga2 O2 O2 39.9(3) 1_556 4_445
Ga3 O2 O2 143.8(9) 1_556 4_445
La O2 O2 65.7(6) . 4_445
O2 O2 O2 60.0 3_455 4_445
Ga2 O2 O3 117.1(6) 1_556 2_455
Ga3 O2 O3 62.6(5) 1_556 2_455
La O2 O3 127.5(7) . 2_455
O2 O2 O3 86.9(8) 3_455 2_455
O2 O2 O3 146.2(8) 4_445 2_455
Ga2 O2 O2 101.6(8) 1_556 6_556
Ga3 O2 O2 39.7(6) 1_556 6_556
La O2 O2 97.4(5) . 6_556
O2 O2 O2 136.5(4) 3_455 6_556
O2 O2 O2 106.5(4) 4_445 6_556
O3 O2 O2 102.3(4) 2_455 6_556
Ga2 O2 O3 159.0(7) 1_556 5_455
Ga3 O2 O3 39.3(4) 1_556 5_455
La O2 O3 91.4(4) . 5_455
O2 O2 O3 144.2(10) 3_455 5_455
O2 O2 O3 154.2(9) 4_445 5_455
O3 O2 O3 57.4(5) 2_455 5_455
O2 O2 O3 63.2(5) 6_556 5_455
Ga2 O2 La 90.6(6) 1_556 2_455
Ga3 O2 La 112.6(7) 1_556 2_455
La O2 La 103.4(6) . 2_455
O2 O2 La 50.8(4) 3_455 2_455
O2 O2 La 98.9(4) 4_445 2_455
O3 O2 La 50.1(4) 2_455 2_455
O2 O2 La 152.1(2) 6_556 2_455
O3 O2 La 97.7(6) 5_455 2_455
Ga2 O2 O1 84.0(4) 1_556 2_455
Ga3 O2 O1 154.0(9) 1_556 2_455
La O2 O1 55.9(3) . 2_455
O2 O2 O1 61.4(3) 3_455 2_455
O2 O2 O1 61.4(3) 4_445 2_455
O3 O2 O1 98.3(6) 2_455 2_455
O2 O2 O1 153.0(5) 6_556 2_455
O3 O2 O1 116.3(6) 5_455 2_455
La O2 O1 52.3(3) 2_455 2_455
Ga2 O2 O3 89.0(5) 1_556 3_456
Ga3 O2 O3 35.6(3) 1_556 3_456
La O2 O3 154.0(7) . 3_456
O2 O2 O3 94.6(6) 3_455 3_456
O2 O2 O3 125.8(3) 4_445 3_456
O3 O2 O3 58.5(6) 2_455 3_456
O2 O2 O3 58.0(6) 6_556 3_456
O3 O2 O3 70.8(5) 5_455 3_456
La O2 O3 97.7(6) 2_455 3_456
O1 O2 O3 148.9(7) 2_455 3_456
Ga2 O2 O1 31.0(3) 1_556 2_456
Ga3 O2 O1 89.2(6) 1_556 2_456
La O2 O1 122.3(6) . 2_456
O2 O2 O1 63.1(2) 3_455 2_456
O2 O2 O1 63.1(2) 4_445 2_456
O3 O2 O1 109.9(4) 2_455 2_456
O2 O2 O1 73.8(6) 6_556 2_456
O3 O2 O1 128.4(6) 5_455 2_456
La O2 O1 109.0(4) 2_455 2_456
O1 O2 O1 115.0(3) 2_455 2_456
O3 O2 O1 62.7(4) 3_456 2_456
Ga2 O2 O3 133.2(8) 1_556 3_455
Ga3 O2 O3 94.4(6) 1_556 3_455
La O2 O3 79.3(5) . 3_455
O2 O2 O3 94.1(5) 3_455 3_455
O2 O2 O3 121.1(3) 4_445 3_455
O3 O2 O3 49.5(5) 2_455 3_455
O2 O2 O3 124.3(4) 6_556 3_455
O3 O2 O3 61.4(5) 5_455 3_455
La O2 O3 44.5(3) 2_455 3_455
O1 O2 O3 59.8(4) 2_455 3_455
O3 O2 O3 106.5(6) 3_456 3_455
O1 O2 O3 152.1(6) 2_456 3_455
Ga2 O2 O1 127.7(8) 1_556 .
Ga3 O2 O1 75.4(4) 1_556 .
La O2 O1 45.3(3) . .
O2 O2 O1 154.3(6) 3_455 .
O2 O2 O1 96.6(7) 4_445 .
O3 O2 O1 114.0(4) 2_455 .
O2 O2 O1 56.3(4) 6_556 .
O3 O2 O1 57.7(3) 5_455 .
La O2 O1 132.3(5) 2_455 .
O1 O2 O1 99.3(3) 2_455 .
O3 O2 O1 108.8(5) 3_456 .
O1 O2 O1 118.3(6) 2_456 .
O3 O2 O1 89.3(4) 3_455 .
Ga2 O2 Nb 149.6(8) 1_556 1_455
Ga3 O2 Nb 61.5(4) 1_556 1_455
La O2 Nb 97.4(4) . 1_455
O2 O2 Nb 113.1(8) 3_455 1_455
O2 O2 Nb 153.8(3) 4_445 1_455
O3 O2 Nb 33.3(3) 2_455 1_455
O2 O2 Nb 95.0(3) 6_556 1_455
O3 O2 Nb 33.3(3) 5_455 1_455
La O2 Nb 64.3(4) 2_455 1_455
O1 O2 Nb 92.7(5) 2_455 1_455
O3 O2 Nb 78.2(4) 3_456 1_455
O1 O2 Nb 139.5(4) 2_456 1_455
O3 O2 Nb 32.9(2) 3_455 1_455
O1 O2 Nb 82.8(2) . 1_455
Ga2 O2 Ga1 149.6(8) 1_556 1_455
Ga3 O2 Ga1 61.5(4) 1_556 1_455
La O2 Ga1 97.4(4) . 1_455
O2 O2 Ga1 113.1(8) 3_455 1_455
O2 O2 Ga1 153.8(3) 4_445 1_455
O3 O2 Ga1 33.3(3) 2_455 1_455
O2 O2 Ga1 95.0(3) 6_556 1_455
O3 O2 Ga1 33.3(3) 5_455 1_455
La O2 Ga1 64.3(4) 2_455 1_455
O1 O2 Ga1 92.7(5) 2_455 1_455
O3 O2 Ga1 78.2(4) 3_456 1_455
O1 O2 Ga1 139.5(4) 2_456 1_455
O3 O2 Ga1 32.9(2) 3_455 1_455
O1 O2 Ga1 82.8(2) . 1_455
Nb O2 Ga1 0.0 1_455 1_455
Ga2 O2 Ga2 111.6(8) 1_556 2_565
Ga3 O2 Ga2 59.8(5) 1_556 2_565
La O2 Ga2 68.5(4) . 2_565
O2 O2 Ga2 151.3(7) 3_455 2_565
O2 O2 Ga2 96.5(7) 4_445 2_565
O3 O2 Ga2 117.2(3) 2_455 2_565
O2 O2 Ga2 29.1(2) 6_556 2_565
O3 O2 Ga2 62.7(3) 5_455 2_565
La O2 Ga2 157.6(5) 2_455 2_565
O1 O2 Ga2 124.4(4) 2_455 2_565
O3 O2 Ga2 86.3(5) 3_456 2_565
O1 O2 Ga2 92.5(5) 2_456 2_565
O3 O2 Ga2 113.2(3) 3_455 2_565
O1 O2 Ga2 28.7(3) . 2_565
Nb O2 Ga2 95.2(2) 1_455 2_565
Ga1 O2 Ga2 95.2(2) 1_455 2_565
Ga2 O2 O2 141.0(5) 1_556 6
Ga3 O2 O2 97.3(4) 1_556 6
La O2 O2 39.0(4) . 6
O2 O2 O2 123.2(5) 3_455 6
O2 O2 O2 102.42(19) 4_445 6
O3 O2 O2 89.6(4) 2_455 6
O2 O2 O2 99.5(6) 6_556 6
O3 O2 O2 59.4(4) 5_455 6
La O2 O2 85.7(6) 2_455 6
O1 O2 O2 63.2(5) 2_455 6
O3 O2 O2 130.0(3) 3_456 6
O1 O2 O2 160.2(5) 2_456 6
O3 O2 O2 46.2(3) 3_455 6
O1 O2 O2 46.9(4) . 6
Nb O2 O2 58.40(17) 1_455 6
Ga1 O2 O2 58.40(17) 1_455 6
Ga2 O2 O2 75.1(4) 2_565 6
Ga2 O2 O3 80.6(5) 1_556 6
Ga3 O2 O3 114.0(8) 1_556 6
La O2 O3 36.5(4) . 6
O2 O2 O3 106.5(5) 3_455 6
O2 O2 O3 46.7(6) 4_445 6
O3 O2 O3 161.8(5) 2_455 6
O2 O2 O3 76.7(3) 6_556 6
O3 O2 O3 107.8(5) 5_455 6
La O2 O3 130.5(4) 2_455 6
O1 O2 O3 78.2(3) 2_455 6
O3 O2 O3 130.4(7) 3_456 6
O1 O2 O3 87.5(5) 2_456 6
O3 O2 O3 115.8(4) 3_455 6
O1 O2 O3 50.0(3) . 6
Nb O2 O3 128.5(4) 1_455 6
Ga1 O2 O3 128.5(4) 1_455 6
Ga2 O2 O3 54.5(3) 2_565 6
O2 O2 O3 72.8(3) 6 6
Ga2 O2 La 64.5(6) 1_556 1_556
Ga3 O2 La 68.4(6) 1_556 1_556
La O2 La 102.7(6) . 1_556
O2 O2 La 102.3(2) 3_455 1_556
O2 O2 La 75.4(3) 4_445 1_556
O3 O2 La 122.1(4) 2_455 1_556
O2 O2 La 37.2(3) 6_556 1_556
O3 O2 La 100.0(5) 5_455 1_556
La O2 La 147.9(3) 2_455 1_556
O1 O2 La 136.5(5) 2_455 1_556
O3 O2 La 63.8(5) 3_456 1_556
O1 O2 La 39.9(3) 2_456 1_556
O3 O2 La 161.4(4) 3_455 1_556
O1 O2 La 79.7(4) . 1_556
Nb O2 La 129.6(3) 1_455 1_556
Ga1 O2 La 129.6(3) 1_455 1_556
Ga2 O2 La 52.6(3) 2_565 1_556
O2 O2 La 126.4(6) 6 1_556
O3 O2 La 68.0(4) 6 1_556
Ga2 O2 Ga3 107.8(4) 1_556 4_346
Ga3 O2 Ga3 48.9(4) 1_556 4_346
La O2 Ga3 144.8(5) . 4_346
O2 O2 Ga3 88.8(7) 3_455 4_346
O2 O2 Ga3 146.2(6) 4_445 4_346
O3 O2 Ga3 20.7(3) 2_455 4_346
O2 O2 Ga3 86.8(3) 6_556 4_346
O3 O2 Ga3 59.4(3) 5_455 4_346
La O2 Ga3 65.5(3) 2_455 4_346
O1 O2 Ga3 116.9(6) 2_455 4_346
O3 O2 Ga3 37.7(4) 3_456 4_346
O1 O2 Ga3 92.5(3) 2_456 4_346
O3 O2 Ga3 69.8(3) 3_455 4_346
O1 O2 Ga3 116.2(2) . 4_346
Nb O2 Ga3 47.43(17) 1_455 4_346
Ga1 O2 Ga3 47.43(17) 1_455 4_346
Ga2 O2 Ga3 108.3(2) 2_565 4_346
O2 O2 Ga3 105.83(18) 6 4_346
O3 O2 Ga3 162.8(4) 6 4_346
La O2 Ga3 101.5(3) 1_556 4_346
Ga2 O2 Ga3 44.0(4) 1_556 4_446
Ga3 O2 Ga3 124.9(9) 1_556 4_446
La O2 Ga3 66.6(3) . 4_446
O2 O2 Ga3 75.1(4) 3_455 4_446
O2 O2 Ga3 19.7(3) 4_445 4_446
O3 O2 Ga3 160.9(4) 2_455 4_446
O2 O2 Ga3 86.8(3) 6_556 4_446
O3 O2 Ga3 140.7(6) 5_455 4_446
La O2 Ga3 118.4(3) 2_455 4_446
O1 O2 Ga3 79.0(3) 2_455 4_446
O3 O2 Ga3 115.7(6) 3_456 4_446
O1 O2 Ga3 56.2(3) 2_456 4_446
O3 O2 Ga3 136.9(4) 3_455 4_446
O1 O2 Ga3 85.0(3) . 4_446
Nb O2 Ga3 164.0(3) 1_455 4_446
Ga1 O2 Ga3 164.0(3) 1_455 4_446
Ga2 O2 Ga3 78.6(4) 2_565 4_446
O2 O2 Ga3 105.57(15) 6 4_446
O3 O2 Ga3 36.6(2) 6 4_446
La O2 Ga3 57.5(3) 1_556 4_446
Ga3 O2 Ga3 148.6(3) 4_346 4_446
Ga2 O2 O3 52.7(6) 1_556 1_556
Ga3 O2 O3 100.1(8) 1_556 1_556
La O2 O3 76.9(5) . 1_556
O2 O2 O3 91.3(4) 3_455 1_556
O2 O2 O3 44.2(3) 4_445 1_556
O3 O2 O3 154.4(5) 2_455 1_556
O2 O2 O3 62.5(3) 6_556 1_556
O3 O2 O3 122.0(6) 5_455 1_556
La O2 O3 140.4(3) 2_455 1_556
O1 O2 O3 103.3(3) 2_455 1_556
O3 O2 O3 96.3(7) 3_456 1_556
O1 O2 O3 47.9(4) 2_456 1_556
O3 O2 O3 156.0(4) 3_455 1_556
O1 O2 O3 76.1(4) . 1_556
Nb O2 O3 155.2(4) 1_455 1_556
Ga1 O2 O3 155.2(4) 1_455 1_556
Ga2 O2 O3 60.1(3) 2_565 1_556
O2 O2 O3 112.4(3) 6 1_556
O3 O2 O3 40.5(5) 6 1_556
La O2 O3 33.8(2) 1_556 1_556
Ga3 O2 O3 133.7(4) 4_346 1_556
Ga3 O2 O3 24.81(15) 4_446 1_556
Ga2 O2 La 56.8(3) 1_556 2_456
Ga3 O2 La 68.2(3) 1_556 2_456
La O2 La 158.8(6) . 2_456
O2 O2 La 64.9(4) 3_455 2_456
O2 O2 La 96.0(2) 4_445 2_456
O3 O2 La 73.6(4) 2_455 2_456
O2 O2 La 77.0(5) 6_556 2_456
O3 O2 La 103.8(4) 5_455 2_456
La O2 La 89.3(3) 2_455 2_456
O1 O2 La 126.0(4) 2_455 2_456
O3 O2 La 33.3(2) 3_456 2_456
O1 O2 La 36.57(15) 2_456 2_456
O3 O2 La 120.9(5) 3_455 2_456
O1 O2 La 133.4(5) . 2_456
Nb O2 La 103.4(3) 1_455 2_456
Ga1 O2 La 103.4(3) 1_455 2_456
Ga2 O2 La 105.2(4) 2_565 2_456
O2 O2 La 161.46(15) 6 2_456
O3 O2 La 123.0(5) 6 2_456
La O2 La 60.6(2) 1_556 2_456
Ga3 O2 La 56.07(14) 4_346 2_456
Ga3 O2 La 92.5(3) 4_446 2_456
O3 O2 La 82.5(4) 1_556 2_456
Ga2 O2 La 49.3(3) 1_556 4_445
Ga3 O2 La 168.5(5) 1_556 4_445
La O2 La 70.0(2) . 4_445
O2 O2 La 41.0(4) 3_455 4_445
O2 O2 La 31.9(2) 4_445 4_445
O3 O2 La 117.0(5) 2_455 4_445
O2 O2 La 138.4(4) 6_556 4_445
O3 O2 La 151.4(6) 5_455 4_445
La O2 La 67.5(2) 2_455 4_445
O1 O2 La 35.3(2) 2_455 4_445
O3 O2 La 133.3(3) 3_456 4_445
O1 O2 La 80.1(2) 2_456 4_445
O3 O2 La 93.1(4) 3_455 4_445
O1 O2 La 113.5(3) . 4_445
Nb O2 La 125.3(5) 1_455 4_445
Ga1 O2 La 125.3(5) 1_455 4_445
Ga2 O2 La 124.5(4) 2_565 4_445
O2 O2 La 94.2(5) 6 4_445
O3 O2 La 70.2(2) 6 4_445
La O2 La 105.0(3) 1_556 4_445
Ga3 O2 La 126.7(4) 4_346 4_445
Ga3 O2 La 51.63(12) 4_446 4_445
O3 O2 La 76.0(2) 1_556 4_445
La O2 La 100.4(2) 2_456 4_445
Ga2 O2 Ga3 138.0(6) 1_556 .
Ga3 O2 Ga3 100.7(5) 1_556 .
La O2 Ga3 57.5(3) . .
O2 O2 Ga3 105.5(3) 3_455 .
O2 O2 Ga3 109.83(18) 4_445 .
O3 O2 Ga3 70.3(4) 2_455 .
O2 O2 Ga3 117.7(5) 6_556 .
O3 O2 Ga3 62.0(4) 5_455 .
La O2 Ga3 61.7(3) 2_455 .
O1 O2 Ga3 54.2(3) 2_455 .
O3 O2 Ga3 123.4(5) 3_456 .
O1 O2 Ga3 168.4(5) 2_456 .
O3 O2 Ga3 22.4(2) 3_455 .
O1 O2 Ga3 70.6(3) . .
Nb O2 Ga3 45.2(2) 1_455 .
Ga1 O2 Ga3 45.2(2) 1_455 .
Ga2 O2 Ga3 97.7(2) 2_565 .
O2 O2 Ga3 24.6(2) 6 .
O3 O2 Ga3 93.8(3) 6 .
La O2 Ga3 150.2(4) 1_556 .
Ga3 O2 Ga3 89.6(3) 4_346 .
Ga3 O2 Ga3 120.4(2) 4_446 .
O3 O2 Ga3 134.3(3) 1_556 .
La O2 Ga3 143.2(5) 2_456 .
La O2 Ga3 89.4(3) 4_445 .
Ga2 O2 O3 120.3(6) 1_556 4_456
Ga3 O2 O3 1.5(3) 1_556 4_456
La O2 O3 118.6(4) . 4_456
O2 O2 O3 131.0(6) 3_455 4_456
O2 O2 O3 143.3(6) 4_445 4_456
O3 O2 O3 63.7(4) 2_455 4_456
O2 O2 O3 38.6(3) 6_556 4_456
O3 O2 O3 38.7(5) 5_455 4_456
La O2 O3 113.8(4) 2_455 4_456
O1 O2 O3 154.0(6) 2_455 4_456
O3 O2 O3 36.9(3) 3_456 4_456
O1 O2 O3 89.7(4) 2_456 4_456
O3 O2 O3 94.6(3) 3_455 4_456
O1 O2 O3 73.9(3) . 4_456
Nb O2 O3 61.75(19) 1_455 4_456
Ga1 O2 O3 61.75(19) 1_455 4_456
Ga2 O2 O3 58.4(2) 2_565 4_456
O2 O2 O3 96.4(4) 6 4_456
O3 O2 O3 112.6(5) 6 4_456
La O2 O3 68.1(3) 1_556 4_456
Ga3 O2 O3 50.25(17) 4_346 4_456
Ga3 O2 O3 124.2(5) 4_446 4_456
O3 O2 O3 99.4(5) 1_556 4_456
La O2 O3 69.4(2) 2_456 4_456
La O2 O3 169.5(4) 4_445 4_456
Ga3 O2 O3 100.4(3) . 4_456
Ga2 O2 Ga3 37.3(4) 1_556 2_455
Ga3 O2 Ga3 116.0(4) 1_556 2_455
La O2 Ga3 123.8(3) . 2_455
O2 O2 Ga3 14.3(4) 3_455 2_455
O2 O2 Ga3 67.2(4) 4_445 2_455
O3 O2 Ga3 82.2(4) 2_455 2_455
O2 O2 Ga3 124.3(6) 6_556 2_455
O3 O2 Ga3 138.5(5) 5_455 2_455
La O2 Ga3 56.4(2) 2_455 2_455
O1 O2 Ga3 75.5(3) 2_455 2_455
O3 O2 Ga3 80.7(3) 3_456 2_455
O1 O2 Ga3 53.44(18) 2_456 2_455
O3 O2 Ga3 100.9(5) 3_455 2_455
O1 O2 Ga3 163.7(4) . 2_455
Nb O2 Ga3 112.6(4) 1_455 2_455
Ga1 O2 Ga3 112.6(4) 1_455 2_455
Ga2 O2 Ga3 145.8(5) 2_565 2_455
O2 O2 Ga3 136.2(7) 6 2_455
O3 O2 Ga3 113.7(3) 6 2_455
La O2 Ga3 93.3(3) 1_556 2_455
Ga3 O2 Ga3 79.6(2) 4_346 2_455
Ga3 O2 Ga3 78.83(17) 4_446 2_455
O3 O2 Ga3 89.9(3) 1_556 2_455
La O2 Ga3 50.61(12) 2_456 2_455
La O2 Ga3 53.80(12) 4_445 2_455
Ga3 O2 Ga3 115.9(4) . 2_455
O3 O2 Ga3 117.4(3) 4_456 2_455
Ga2 O2 O3 87.3(4) 1_556 .
Ga3 O2 O3 139.0(6) 1_556 .
La O2 O3 20.0(2) . .
O2 O2 O3 91.2(4) 3_455 .
O2 O2 O3 47.8(5) 4_445 .
O3 O2 O3 134.8(5) 2_455 .
O2 O2 O3 109.5(3) 6_556 .
O3 O2 O3 110.9(4) 5_455 .
La O2 O3 96.0(4) 2_455 .
O1 O2 O3 43.9(2) 2_455 .
O3 O2 O3 165.9(8) 3_456 .
O1 O2 O3 109.2(4) 2_456 .
O3 O2 O3 85.8(4) 3_455 .
O1 O2 O3 63.6(3) . .
Nb O2 O3 111.1(4) 1_455 .
Ga1 O2 O3 111.1(4) 1_455 .
Ga2 O2 O3 82.4(3) 2_565 .
O2 O2 O3 54.7(4) 6 .
O3 O2 O3 35.5(3) 6 .
La O2 O3 102.4(4) 1_556 .
Ga3 O2 O3 155.5(5) 4_346 .
Ga3 O2 O3 53.7(2) 4_446 .
O3 O2 O3 70.7(2) 1_556 .
La O2 O3 143.8(4) 2_456 .
La O2 O3 50.41(19) 4_445 .
Ga3 O2 O3 66.8(3) . .
O3 O2 O3 137.5(4) 4_456 .
Ga3 O2 O3 104.2(3) 2_455 .
Ga2 O2 O2 51.4(3) 1_556 2_456
Ga3 O2 O2 92.5(5) 1_556 2_456
La O2 O2 147.5(5) . 2_456
O2 O2 O2 37.1(5) 3_455 2_456
O2 O2 O2 88.2(4) 4_445 2_456
O3 O2 O2 65.9(3) 2_455 2_456
O2 O2 O2 108.9(7) 6_556 2_456
O3 O2 O2 117.3(5) 5_455 2_456
La O2 O2 60.1(2) 2_455 2_456
O1 O2 O2 95.3(4) 2_455 2_456
O3 O2 O2 57.7(3) 3_456 2_456
O1 O2 O2 51.9(3) 2_456 2_456
O3 O2 O2 100.2(5) 3_455 2_456
O1 O2 O2 165.2(6) . 2_456
Nb O2 O2 99.1(4) 1_455 2_456
Ga1 O2 O2 99.1(4) 1_455 2_456
Ga2 O2 O2 136.9(6) 2_565 2_456
O2 O2 O2 145.5(8) 6 2_456
O3 O2 O2 132.0(5) 6 2_456
La O2 O2 88.0(4) 1_556 2_456
Ga3 O2 O2 58.1(2) 4_346 2_456
Ga3 O2 O2 95.4(3) 4_446 2_456
O3 O2 O2 98.2(5) 1_556 2_456
La O2 O2 31.9(2) 2_456 2_456
La O2 O2 77.6(2) 4_445 2_456
Ga3 O2 O2 120.9(6) . 2_456
O3 O2 O2 93.9(4) 4_456 2_456
Ga3 O2 O2 23.81(13) 2_455 2_456
O3 O2 O2 128.0(4) . 2_456
Ga2 O2 O2 89.5(9) 1_556 2_566
Ga3 O2 O2 75.2(7) 1_556 2_566
La O2 O2 67.6(3) . 2_566
O2 O2 O2 128.7(8) 3_455 2_566
O2 O2 O2 75.4(7) 4_445 2_566
O3 O2 O2 137.1(5) 2_455 2_566
O2 O2 O2 36.4(2) 6_556 2_566
O3 O2 O2 85.4(4) 5_455 2_566
La O2 O2 170.7(5) 2_455 2_566
O1 O2 O2 118.5(4) 2_455 2_566
O3 O2 O2 91.6(7) 3_456 2_566
O1 O2 O2 75.3(7) 2_456 2_566
O3 O2 O2 132.3(4) 3_455 2_566
O1 O2 O2 43.0(3) . 2_566
Nb O2 O2 118.1(3) 1_455 2_566
Ga1 O2 O2 118.1(3) 1_455 2_566
Ga2 O2 O2 22.83(9) 2_565 2_566
O2 O2 O2 88.3(3) 6 2_566
O3 O2 O2 40.5(2) 6 2_566
La O2 O2 38.5(4) 1_556 2_566
Ga3 O2 O2 123.2(4) 4_346 2_566
Ga3 O2 O2 56.6(4) 4_446 2_566
O3 O2 O2 37.3(4) 1_556 2_566
La O2 O2 98.5(6) 2_456 2_566
La O2 O2 105.9(4) 4_445 2_566
Ga3 O2 O2 112.9(3) . 2_566
O3 O2 O2 74.0(4) 4_456 2_566
Ga3 O2 O2 125.8(6) 2_455 2_566
O3 O2 O2 74.8(3) . 2_566
O2 O2 O2 126.2(8) 2_456 2_566
Ga2 O2 Ga2 96.7(5) 1_556 .
Ga3 O2 Ga2 142.0(7) 1_556 .
La O2 Ga2 51.8(3) . .
O2 O2 Ga2 72.01(11) 3_455 .
O2 O2 Ga2 72.01(11) 4_445 .
O3 O2 Ga2 92.5(5) 2_455 .
O2 O2 Ga2 147.7(5) 6_556 .
O3 O2 Ga2 103.7(5) 5_455 .
La O2 Ga2 52.2(3) 2_455 .
O1 O2 Ga2 12.7(2) 2_455 .
O3 O2 Ga2 149.2(7) 3_456 .
O1 O2 Ga2 127.7(3) 2_456 .
O3 O2 Ga2 49.2(3) 3_455 .
O1 O2 Ga2 91.5(3) . .
Nb O2 Ga2 81.8(4) 1_455 .
Ga1 O2 Ga2 81.8(4) 1_455 .
Ga2 O2 Ga2 118.9(3) 2_565 .
O2 O2 Ga2 51.6(5) 6 .
O3 O2 Ga2 80.4(3) 6 .
La O2 Ga2 145.0(3) 1_556 .
Ga3 O2 Ga2 112.6(5) 4_346 .
Ga3 O2 Ga2 88.18(18) 4_446 .
O3 O2 Ga2 111.3(3) 1_556 .
La O2 Ga2 135.0(4) 2_456 .
La O2 Ga2 47.81(14) 4_445 .
Ga3 O2 Ga2 41.62(15) . .
O3 O2 Ga2 141.8(4) 4_456 .
Ga3 O2 Ga2 85.7(3) 2_455 .
O3 O2 Ga2 44.87(19) . .
O2 O2 Ga2 103.3(4) 2_456 .
O2 O2 Ga2 118.6(3) 2_566 .
Ga2 O2 La 161.0(9) 1_556 4_455
Ga3 O2 La 59.6(3) 1_556 4_455
La O2 La 64.9(2) . 4_455
O2 O2 La 157.2(5) 3_455 4_455
O2 O2 La 127.9(7) 4_445 4_455
O3 O2 La 80.3(3) 2_455 4_455
O2 O2 La 65.4(4) 6_556 4_455
O3 O2 La 26.9(3) 5_455 4_455
La O2 La 107.3(4) 2_455 4_455
O1 O2 La 101.7(4) 2_455 4_455
O3 O2 La 94.6(3) 3_456 4_455
O1 O2 La 139.2(5) 2_456 4_455
O3 O2 La 63.3(3) 3_455 4_455
O1 O2 La 33.93(12) . 4_455
Nb O2 La 49.02(12) 1_455 4_455
Ga1 O2 La 49.02(12) 1_455 4_455
Ga2 O2 La 50.32(13) 2_565 4_455
O2 O2 La 38.7(3) 6 4_455
O3 O2 La 82.9(3) 6 4_455
La O2 La 100.5(3) 1_556 4_455
Ga3 O2 La 85.88(19) 4_346 4_455
Ga3 O2 La 118.8(3) 4_446 4_455
O3 O2 La 108.3(4) 1_556 4_455
La O2 La 127.8(2) 2_456 4_455
La O2 La 131.8(3) 4_445 4_455
Ga3 O2 La 52.34(14) . 4_455
O3 O2 La 58.53(18) 4_456 4_455
Ga3 O2 La 161.6(5) 2_455 4_455
O3 O2 La 84.7(3) . 4_455
O2 O2 La 143.9(4) 2_456 4_455
O2 O2 La 71.81(17) 2_566 4_455
Ga2 O2 La 89.6(2) . 4_455
Ga2 O2 O3 167.8(9) 1_556 4_455
Ga3 O2 O3 68.2(4) 1_556 4_455
La O2 O3 75.4(4) . 4_455
O2 O2 O3 128.1(6) 3_455 4_455
O2 O2 O3 139.0(4) 4_445 4_455
O3 O2 O3 56.5(4) 2_455 4_455
O2 O2 O3 90.3(4) 6_556 4_455
O3 O2 O3 29.6(5) 5_455 4_455
La O2 O3 77.5(4) 2_455 4_455
O1 O2 O3 86.7(5) 2_455 4_455
O3 O2 O3 94.9(3) 3_456 4_455
O1 O2 O3 157.0(4) 2_456 4_455
O3 O2 O3 34.6(3) 3_455 4_455
O1 O2 O3 61.7(2) . 4_455
Nb O2 O3 23.23(16) 1_455 4_455
Ga1 O2 O3 23.23(16) 1_455 4_455
Ga2 O2 O3 80.2(2) 2_565 4_455
O2 O2 O3 37.0(3) 6 4_455
O3 O2 O3 105.3(3) 6 4_455
La O2 O3 127.4(4) 1_556 4_455
Ga3 O2 O3 69.6(3) 4_346 4_455
Ga3 O2 O3 141.2(3) 4_446 4_455
O3 O2 O3 137.8(4) 1_556 4_455
La O2 O3 124.5(3) 2_456 4_455
La O2 O3 122.0(5) 4_445 4_455
Ga3 O2 O3 32.6(2) . 4_455
O3 O2 O3 67.8(2) 4_456 4_455
Ga3 O2 O3 132.1(5) 2_455 4_455
O3 O2 O3 91.5(5) . 4_455
O2 O2 O3 122.0(5) 2_456 4_455
O2 O2 O3 101.9(3) 2_566 4_455
Ga2 O2 O3 74.2(3) . 4_455
La O2 O3 30.06(12) 4_455 4_455
Ga2 O2 O2 84.7(3) 1_556 5_346
Ga3 O2 O2 62.3(4) 1_556 5_346
La O2 O2 163.7(10) . 5_346
O2 O2 O2 69.3(6) 3_455 5_346
O2 O2 O2 123.3(4) 4_445 5_346
O3 O2 O2 37.1(4) 2_455 5_346
O2 O2 O2 92.8(6) 6_556 5_346
O3 O2 O2 81.9(4) 5_455 5_346
La O2 O2 63.1(4) 2_455 5_346
O1 O2 O2 114.1(7) 2_455 5_346
O3 O2 O2 35.0(3) 3_456 5_346
O1 O2 O2 72.8(3) 2_456 5_346
O3 O2 O2 84.5(6) 3_455 5_346
O1 O2 O2 136.43(19) . 5_346
Nb O2 O2 69.0(4) 1_455 5_346
Ga1 O2 O2 69.0(4) 1_455 5_346
Ga2 O2 O2 120.1(4) 2_565 5_346
O2 O2 O2 126.7(5) 6 5_346
O3 O2 O2 159.7(7) 6 5_346
La O2 O2 93.1(5) 1_556 5_346
Ga3 O2 O2 23.19(19) 4_346 5_346
Ga3 O2 O2 126.9(4) 4_446 5_346
O3 O2 O2 119.2(6) 1_556 5_346
La O2 O2 36.8(2) 2_456 5_346
La O2 O2 109.9(3) 4_445 5_346
Ga3 O2 O2 106.5(6) . 5_346
O3 O2 O2 63.8(2) 4_456 5_346
Ga3 O2 O2 58.09(14) 2_455 5_346
O3 O2 O2 157.4(5) . 5_346
O2 O2 O2 35.4(2) 2_456 5_346
O2 O2 O2 126.1(7) 2_566 5_346
Ga2 O2 O2 115.3(6) . 5_346
La O2 O2 108.7(2) 4_455 5_346
O3 O2 O2 91.9(4) 4_455 5_346
Ga2 O2 Ga1 99.0(5) 1_556 1_456
Ga3 O2 Ga1 23.3(2) 1_556 1_456
La O2 Ga1 141.9(5) . 1_456
O2 O2 Ga1 107.2(5) 3_455 1_456
O2 O2 Ga1 132.48(17) 4_445 1_456
O3 O2 Ga1 60.2(3) 2_455 1_456
O2 O2 Ga1 48.6(3) 6_556 1_456
O3 O2 Ga1 60.2(4) 5_455 1_456
La O2 Ga1 105.1(3) 2_455 1_456
O1 O2 Ga1 157.4(6) 2_455 1_456
O3 O2 Ga1 12.5(2) 3_456 1_456
O1 O2 Ga1 70.4(3) 2_456 1_456
O3 O2 Ga1 104.5(3) 3_455 1_456
O1 O2 Ga1 96.5(3) . 1_456
Nb O2 Ga1 73.27(16) 1_455 1_456
Ga1 O2 Ga1 73.27(16) 1_455 1_456
Ga2 O2 Ga1 75.5(2) 2_565 1_456
O2 O2 Ga1 119.5(3) 6 1_456
O3 O2 Ga1 124.4(5) 6 1_456
La O2 Ga1 62.5(2) 1_556 1_456
Ga3 O2 Ga1 40.72(9) 4_346 1_456
Ga3 O2 Ga1 118.6(4) 4_446 1_456
O3 O2 Ga1 96.2(4) 1_556 1_456
La O2 Ga1 45.03(11) 2_456 1_456
La O2 Ga1 145.4(3) 4_445 1_456
Ga3 O2 Ga1 117.6(3) . 1_456
O3 O2 Ga1 24.53(17) 4_456 1_456
Ga3 O2 Ga1 93.23(19) 2_455 1_456
O3 O2 Ga1 157.9(5) . 1_456
O2 O2 Ga1 70.2(3) 2_456 1_456
O2 O2 Ga1 84.1(4) 2_566 1_456
Ga2 O2 Ga1 152.5(4) . 1_456
La O2 Ga1 82.75(15) 4_455 1_456
O3 O2 Ga1 86.6(3) 4_455 1_456
O2 O2 Ga1 44.6(2) 5_346 1_456
Ga2 O2 Nb 99.0(5) 1_556 1_456
Ga3 O2 Nb 23.3(2) 1_556 1_456
La O2 Nb 141.9(5) . 1_456
O2 O2 Nb 107.2(5) 3_455 1_456
O2 O2 Nb 132.48(17) 4_445 1_456
O3 O2 Nb 60.2(3) 2_455 1_456
O2 O2 Nb 48.6(3) 6_556 1_456
O3 O2 Nb 60.2(4) 5_455 1_456
La O2 Nb 105.1(3) 2_455 1_456
O1 O2 Nb 157.4(6) 2_455 1_456
O3 O2 Nb 12.5(2) 3_456 1_456
O1 O2 Nb 70.4(3) 2_456 1_456
O3 O2 Nb 104.5(3) 3_455 1_456
O1 O2 Nb 96.5(3) . 1_456
Nb O2 Nb 73.27(16) 1_455 1_456
Ga1 O2 Nb 73.27(16) 1_455 1_456
Ga2 O2 Nb 75.5(2) 2_565 1_456
O2 O2 Nb 119.5(3) 6 1_456
O3 O2 Nb 124.4(5) 6 1_456
La O2 Nb 62.5(2) 1_556 1_456
Ga3 O2 Nb 40.72(9) 4_346 1_456
Ga3 O2 Nb 118.6(4) 4_446 1_456
O3 O2 Nb 96.2(4) 1_556 1_456
La O2 Nb 45.03(11) 2_456 1_456
La O2 Nb 145.4(3) 4_445 1_456
Ga3 O2 Nb 117.6(3) . 1_456
O3 O2 Nb 24.53(17) 4_456 1_456
Ga3 O2 Nb 93.23(19) 2_455 1_456
O3 O2 Nb 157.9(5) . 1_456
O2 O2 Nb 70.2(3) 2_456 1_456
O2 O2 Nb 84.1(4) 2_566 1_456
Ga2 O2 Nb 152.5(4) . 1_456
La O2 Nb 82.75(15) 4_455 1_456
O3 O2 Nb 86.6(3) 4_455 1_456
O2 O2 Nb 44.6(2) 5_346 1_456
Ga1 O2 Nb 0.0 1_456 1_456
Ga2 O2 O1 82.8(5) 1_556 1_445
Ga3 O2 O1 95.4(6) 1_556 1_445
La O2 O1 129.2(6) . 1_445
O2 O2 O1 47.9(5) 3_455 1_445
O2 O2 O1 107.1(6) 4_445 1_445
O3 O2 O1 39.2(3) 2_455 1_445
O2 O2 O1 130.7(4) 6_556 1_445
O3 O2 O1 96.3(5) 5_455 1_445
La O2 O1 25.7(2) 2_455 1_445
O1 O2 O1 76.0(4) 2_455 1_445
O3 O2 O1 73.1(5) 3_456 1_445
O1 O2 O1 90.7(3) 2_456 1_445
O3 O2 O1 61.5(4) 3_455 1_445
O1 O2 O1 149.0(5) . 1_445
Nb O2 O1 67.1(3) 1_455 1_445
Ga1 O2 O1 67.1(3) 1_455 1_445
Ga2 O2 O1 154.9(3) 2_565 1_445
O2 O2 O1 107.2(5) 6 1_445
O3 O2 O1 150.6(3) 6 1_445
La O2 O1 124.9(3) 1_556 1_445
Ga3 O2 O1 46.6(2) 4_346 1_445
Ga3 O2 O1 122.9(2) 4_446 1_445
O3 O2 O1 134.9(3) 1_556 1_445
La O2 O1 64.6(3) 2_456 1_445
La O2 O1 80.5(3) 4_445 1_445
Ga3 O2 O1 82.6(4) . 1_445
O3 O2 O1 96.8(3) 4_456 1_445
Ga3 O2 O1 45.59(18) 2_455 1_445
O3 O2 O1 119.8(4) . 1_445
O2 O2 O1 38.7(3) 2_456 1_445
O2 O2 O1 162.9(6) 2_566 1_445
Ga2 O2 O1 77.6(3) . 1_445
La O2 O1 116.0(4) 4_455 1_445
O3 O2 O1 87.3(4) 4_455 1_445
O2 O2 O1 38.2(4) 5_346 1_445
Ga1 O2 O1 82.1(2) 1_456 1_445
Nb O2 O1 82.1(2) 1_456 1_445
Ga2 O2 O3 139.9(5) 1_556 6_455
Ga3 O2 O3 41.8(5) 1_556 6_455
La O2 O3 114.1(4) . 6_455
O2 O2 O3 115.8(8) 3_455 6_455
O2 O2 O3 174.1(6) 4_445 6_455
O3 O2 O3 28.9(3) 2_455 6_455
O2 O2 O3 79.4(2) 6_556 6_455
O3 O2 O3 29.0(3) 5_455 6_455
La O2 O3 75.3(3) 2_455 6_455
O1 O2 O3 113.3(6) 2_455 6_455
O3 O2 O3 57.1(5) 3_456 6_455
O1 O2 O3 119.5(4) 2_456 6_455
O3 O2 O3 53.8(4) 3_455 6_455
O1 O2 O3 86.6(2) . 6_455
Nb O2 O3 21.71(19) 1_455 6_455
Ga1 O2 O3 21.71(19) 1_455 6_455
Ga2 O2 O3 88.8(2) 2_565 6_455
O2 O2 O3 76.2(3) 6 6_455
O3 O2 O3 136.7(4) 6 6_455
La O2 O3 110.1(3) 1_556 6_455
Ga3 O2 O3 32.2(2) 4_346 6_455
Ga3 O2 O3 166.2(5) 4_446 6_455
O3 O2 O3 141.6(4) 1_556 6_455
La O2 O3 85.2(3) 2_456 6_455
La O2 O3 142.2(5) 4_445 6_455
Ga3 O2 O3 66.6(3) . 6_455
O3 O2 O3 42.4(3) 4_456 6_455
Ga3 O2 O3 109.7(4) 2_455 6_455
O3 O2 O3 130.8(3) . 6_455
O2 O2 O3 89.9(4) 2_456 6_455
O2 O2 O3 110.2(3) 2_566 6_455
Ga2 O2 O3 103.1(4) . 6_455
La O2 O3 54.2(2) 4_455 6_455
O3 O2 O3 39.3(4) 4_455 6_455
O2 O2 O3 55.4(3) 5_346 6_455
Ga1 O2 O3 51.6(2) 1_456 6_455
Nb O2 O3 51.6(2) 1_456 6_455
O1 O2 O3 68.2(3) 1_445 6_455
Ga2 O2 Ga2 72.9(4) 1_556 2_455
Ga3 O2 Ga2 84.1(4) 1_556 2_455
La O2 Ga2 149.5(6) . 2_455
O2 O2 Ga2 48.7(6) 3_455 2_455
O2 O2 Ga2 106.8(5) 4_445 2_455
O3 O2 Ga2 44.2(3) 2_455 2_455
O2 O2 Ga2 112.9(4) 6_556 2_455
O3 O2 Ga2 98.9(4) 5_455 2_455
La O2 Ga2 46.89(19) 2_455 2_455
O1 O2 Ga2 94.0(4) 2_455 2_455
O3 O2 Ga2 55.1(3) 3_456 2_455
O1 O2 Ga2 72.3(2) 2_456 2_455
O3 O2 Ga2 80.6(4) 3_455 2_455
O1 O2 Ga2 156.4(3) . 2_455
Nb O2 Ga2 77.2(3) 1_455 2_455
Ga1 O2 Ga2 77.2(3) 1_455 2_455
Ga2 O2 Ga2 141.4(3) 2_565 2_455
O2 O2 Ga2 126.8(5) 6 2_455
O3 O2 Ga2 153.0(3) 6 2_455
La O2 Ga2 103.7(2) 1_556 2_455
Ga3 O2 Ga2 40.28(13) 4_346 2_455
Ga3 O2 Ga2 116.8(2) 4_446 2_455
O3 O2 Ga2 119.7(4) 1_556 2_455
La O2 Ga2 43.16(12) 2_456 2_455
La O2 Ga2 88.5(2) 4_445 2_455
Ga3 O2 Ga2 102.6(4) . 2_455
O3 O2 Ga2 85.6(2) 4_456 2_455
Ga3 O2 Ga2 39.62(11) 2_455 2_455
O3 O2 Ga2 135.8(4) . 2_455
O2 O2 Ga2 22.02(16) 2_456 2_455
O2 O2 Ga2 141.5(6) 2_566 2_455
Ga2 O2 Ga2 97.7(4) . 2_455
La O2 Ga2 124.1(3) 4_455 2_455
O3 O2 Ga2 100.0(4) 4_455 2_455
O2 O2 Ga2 21.92(17) 5_346 2_455
Ga1 O2 Ga2 65.96(14) 1_456 2_455
Nb O2 Ga2 65.96(14) 1_456 2_455
O1 O2 Ga2 21.5(2) 1_445 2_455
O3 O2 Ga2 70.2(3) 6_455 2_455
Ga2 O2 Ga3 136.8(5) 1_556 2_465
Ga3 O2 Ga3 21.5(4) 1_556 2_465
La O2 Ga3 114.1(3) . 2_465
O2 O2 Ga3 129.8(7) 3_455 2_465
O2 O2 Ga3 164.3(6) 4_445 2_465
O3 O2 Ga3 47.4(3) 2_455 2_465
O2 O2 Ga3 57.8(2) 6_556 2_465
O3 O2 Ga3 23.2(3) 5_455 2_465
La O2 Ga3 96.3(4) 2_455 2_465
O1 O2 Ga3 132.6(6) 2_455 2_465
O3 O2 Ga3 47.8(2) 3_456 2_465
O1 O2 Ga3 108.3(3) 2_456 2_465
O3 O2 Ga3 72.9(3) 3_455 2_465
O1 O2 Ga3 75.45(17) . 2_465
Nb O2 Ga3 40.05(9) 1_455 2_465
Ga1 O2 Ga3 40.05(9) 1_455 2_465
Ga2 O2 Ga3 70.04(16) 2_565 2_465
O2 O2 Ga3 82.2(3) 6 2_465
O3 O2 Ga3 123.0(4) 6 2_465
La O2 Ga3 89.7(3) 1_556 2_465
Ga3 O2 Ga3 41.06(10) 4_346 2_465
Ga3 O2 Ga3 144.6(5) 4_446 2_465
O3 O2 Ga3 120.1(4) 1_556 2_465
La O2 Ga3 80.60(16) 2_456 2_465
La O2 Ga3 163.7(5) 4_445 2_465
Ga3 O2 Ga3 80.7(2) . 2_465
O3 O2 Ga3 21.70(15) 4_456 2_465
Ga3 O2 Ga3 119.6(3) 2_455 2_465
O3 O2 Ga3 133.9(3) . 2_465
O2 O2 Ga3 96.4(3) 2_456 2_465
O2 O2 Ga3 89.9(3) 2_566 2_465
Ga2 O2 Ga3 121.0(4) . 2_465
La O2 Ga3 49.21(9) 4_455 2_465
O3 O2 Ga3 48.7(2) 4_455 2_465
O2 O2 Ga3 61.48(15) 5_346 2_465
Ga1 O2 Ga3 38.08(7) 1_456 2_465
Nb O2 Ga3 38.08(7) 1_456 2_465
O1 O2 Ga3 85.4(2) 1_445 2_465
O3 O2 Ga3 21.56(13) 6_455 2_465
Ga2 O2 Ga3 81.19(19) 2_455 2_465
Ga2 O2 Ga3 81.4(6) 1_556 2_565
Ga3 O2 Ga3 96.8(7) 1_556 2_565
La O2 Ga3 51.7(4) . 2_565
O2 O2 Ga3 115.6(6) 3_455 2_565
O2 O2 Ga3 56.9(6) 4_445 2_565
O3 O2 Ga3 156.9(4) 2_455 2_565
O2 O2 Ga3 58.24(14) 6_556 2_565
O3 O2 Ga3 100.2(5) 5_455 2_565
La O2 Ga3 149.4(3) 2_455 2_565
O1 O2 Ga3 97.3(3) 2_455 2_565
O3 O2 Ga3 111.6(7) 3_456 2_565
O1 O2 Ga3 78.4(4) 2_456 2_565
O3 O2 Ga3 128.3(3) 3_455 2_565
O1 O2 Ga3 46.3(2) . 2_565
Nb O2 Ga3 128.9(3) 1_455 2_565
Ga1 O2 Ga3 128.9(3) 1_455 2_565
Ga2 O2 Ga3 39.76(19) 2_565 2_565
O2 O2 Ga3 82.3(2) 6 2_565
O3 O2 Ga3 19.1(2) 6 2_565
La O2 Ga3 51.0(2) 1_556 2_565
Ga3 O2 Ga3 145.0(4) 4_346 2_565
Ga3 O2 Ga3 40.50(16) 4_446 2_565
O3 O2 Ga3 31.1(2) 1_556 2_565
La O2 Ga3 110.1(4) 2_456 2_565
La O2 Ga3 85.3(2) 4_445 2_565
Ga3 O2 Ga3 106.0(2) . 2_565
O3 O2 Ga3 95.5(4) 4_456 2_565
Ga3 O2 Ga3 118.3(3) 2_455 2_565
O3 O2 Ga3 54.4(2) . 2_565
O2 O2 Ga3 129.3(5) 2_456 2_565
O2 O2 Ga3 21.86(14) 2_566 2_565
Ga2 O2 Ga3 99.2(2) . 2_565
La O2 Ga3 79.9(2) 4_455 2_565
O3 O2 Ga3 107.6(3) 4_455 2_565
O2 O2 Ga3 144.0(6) 5_346 2_565
Ga1 O2 Ga3 105.3(4) 1_456 2_565
Nb O2 Ga3 105.3(4) 1_456 2_565
O1 O2 Ga3 163.4(2) 1_445 2_565
O3 O2 Ga3 128.1(3) 6_455 2_565
Ga2 O2 Ga3 150.6(3) 2_455 2_565
Ga3 O2 Ga3 109.7(3) 2_465 2_565
Ga2 O2 O2 62.4(5) 1_556 1_556
Ga3 O2 O2 58.3(5) 1_556 1_556
La O2 O2 130.4(5) . 1_556
O2 O2 O2 90.001(1) 3_455 1_556
O2 O2 O2 90.000(1) 4_445 1_556
O3 O2 O2 97.2(4) 2_455 1_556
O2 O2 O2 46.9(4) 6_556 1_556
O3 O2 O2 97.1(4) 5_455 1_556
La O2 O2 123.4(2) 2_455 1_556
O1 O2 O2 146.4(3) 2_455 1_556
O3 O2 O2 39.4(5) 3_456 1_556
O1 O2 O2 31.4(3) 2_456 1_556
O3 O2 O2 145.9(2) 3_455 1_556
O1 O2 O2 101.3(4) . 1_556
Nb O2 O2 115.9(2) 1_455 1_556
Ga1 O2 O2 115.9(2) 1_455 1_556
Ga2 O2 O2 72.6(2) 2_565 1_556
O2 O2 O2 146.5(5) 6 1_556
O3 O2 O2 95.2(3) 6 1_556
La O2 O2 27.70(17) 1_556 1_556
Ga3 O2 O2 76.5(3) 4_346 1_556
Ga3 O2 O2 76.7(2) 4_446 1_556
O3 O2 O2 57.3(2) 1_556 1_556
La O2 O2 34.1(3) 2_456 1_556
La O2 O2 111.4(2) 4_445 1_556
Ga3 O2 O2 159.05(12) . 1_556
O3 O2 O2 58.7(3) 4_456 1_556
Ga3 O2 O2 77.3(2) 2_455 1_556
O3 O2 O2 128.0(3) . 1_556
O2 O2 O2 64.6(4) 2_456 1_556
O2 O2 O2 64.6(4) 2_566 1_556
Ga2 O2 O2 159.11(13) . 1_556
La O2 O2 110.2(2) 4_455 1_556
O3 O2 O2 126.5(3) 4_455 1_556
O2 O2 O2 65.5(5) 5_346 1_556
Ga1 O2 O2 42.6(2) 1_456 1_556
Nb O2 O2 42.6(2) 1_456 1_556
O1 O2 O2 98.4(3) 1_445 1_556
O3 O2 O2 94.2(2) 6_455 1_556
Ga2 O2 O2 76.9(2) 2_455 1_556
Ga3 O2 O2 78.6(2) 2_465 1_556
Ga3 O2 O2 78.71(17) 2_565 1_556
Ga2 O2 O2 117.6(5) 1_556 1_554
Ga3 O2 O2 121.7(5) 1_556 1_554
La O2 O2 49.6(5) . 1_554
O2 O2 O2 90.000(1) 3_455 1_554
O2 O2 O2 90.0 4_445 1_554
O3 O2 O2 82.8(4) 2_455 1_554
O2 O2 O2 133.1(4) 6_556 1_554
O3 O2 O2 82.9(4) 5_455 1_554
La O2 O2 56.6(2) 2_455 1_554
O1 O2 O2 33.6(3) 2_455 1_554
O3 O2 O2 140.6(5) 3_456 1_554
O1 O2 O2 148.6(3) 2_456 1_554
O3 O2 O2 34.1(2) 3_455 1_554
O1 O2 O2 78.7(4) . 1_554
Nb O2 O2 64.1(2) 1_455 1_554
Ga1 O2 O2 64.1(2) 1_455 1_554
Ga2 O2 O2 107.4(2) 2_565 1_554
O2 O2 O2 33.5(5) 6 1_554
O3 O2 O2 84.8(3) 6 1_554
La O2 O2 152.30(17) 1_556 1_554
Ga3 O2 O2 103.5(3) 4_346 1_554
Ga3 O2 O2 103.3(2) 4_446 1_554
O3 O2 O2 122.7(2) 1_556 1_554
La O2 O2 145.9(3) 2_456 1_554
La O2 O2 68.6(2) 4_445 1_554
Ga3 O2 O2 20.95(12) . 1_554
O3 O2 O2 121.3(3) 4_456 1_554
Ga3 O2 O2 102.7(2) 2_455 1_554
O3 O2 O2 52.0(3) . 1_554
O2 O2 O2 115.4(4) 2_456 1_554
O2 O2 O2 115.4(4) 2_566 1_554
Ga2 O2 O2 20.89(13) . 1_554
La O2 O2 69.8(2) 4_455 1_554
O3 O2 O2 53.5(3) 4_455 1_554
O2 O2 O2 114.5(5) 5_346 1_554
Ga1 O2 O2 137.4(2) 1_456 1_554
Nb O2 O2 137.4(2) 1_456 1_554
O1 O2 O2 81.6(3) 1_445 1_554
O3 O2 O2 85.8(2) 6_455 1_554
Ga2 O2 O2 103.1(2) 2_455 1_554
Ga3 O2 O2 101.4(2) 2_465 1_554
Ga3 O2 O2 101.29(17) 2_565 1_554
O2 O2 O2 179.999(4) 1_556 1_554
Ga2 O2 O2 84.8(4) 1_556 2_455
Ga3 O2 O2 123.8(7) 1_556 2_455
La O2 O2 95.8(7) . 2_455
O2 O2 O2 45.5(2) 3_455 2_455
O2 O2 O2 88.4(4) 4_445 2_455
O3 O2 O2 61.2(4) 2_455 2_455
O2 O2 O2 163.2(2) 6_556 2_455
O3 O2 O2 106.2(7) 5_455 2_455
La O2 O2 11.16(5) 2_455 2_455
O1 O2 O2 42.3(4) 2_455 2_455
O3 O2 O2 107.1(4) 3_456 2_455
O1 O2 O2 107.5(3) 2_456 2_455
O3 O2 O2 48.6(5) 3_455 2_455
O1 O2 O2 131.0(6) . 2_455
Nb O2 O2 73.0(5) 1_455 2_455
Ga1 O2 O2 73.0(5) 1_455 2_455
Ga2 O2 O2 159.5(5) 2_565 2_455
O2 O2 O2 84.4(8) 6 2_455
O3 O2 O2 119.9(4) 6 2_455
La O2 O2 147.3(4) 1_556 2_455
Ga3 O2 O2 76.5(2) 4_346 2_455
Ga3 O2 O2 108.0(3) 4_446 2_455
O3 O2 O2 131.2(3) 1_556 2_455
La O2 O2 94.05(16) 2_456 2_455
La O2 O2 56.7(2) 4_445 2_455
Ga3 O2 O2 62.0(5) . 2_455
O3 O2 O2 124.9(4) 4_456 2_455
Ga3 O2 O2 54.04(11) 2_455 2_455
O3 O2 O2 86.2(4) . 2_455
O2 O2 O2 62.95(8) 2_456 2_455
O2 O2 O2 160.3(4) 2_566 2_455
Ga2 O2 O2 44.0(4) . 2_455
La O2 O2 111.7(6) 4_455 2_455
O3 O2 O2 83.1(5) 4_455 2_455
O2 O2 O2 72.1(3) 5_346 2_455
Ga1 O2 O2 115.4(2) 1_456 2_455
Nb O2 O2 115.4(2) 1_456 2_455
O1 O2 O2 33.96(19) 1_445 2_455
O3 O2 O2 85.8(4) 6_455 2_455
Ga2 O2 O2 53.73(8) 2_455 2_455
Ga3 O2 O2 107.1(4) 2_465 2_455
Ga3 O2 O2 138.5(3) 2_565 2_455
O2 O2 O2 127.5(3) 1_556 2_455
O2 O2 O2 52.5(3) 1_554 2_455
Ga2 O2 O2 116.7(6) 1_556 2_565
Ga3 O2 O2 107.1(4) 1_556 2_565
La O2 O2 13.16(17) . 2_565
O2 O2 O2 123.3(5) 3_455 2_565
O2 O2 O2 77.2(7) 4_445 2_565
O3 O2 O2 121.4(6) 2_455 2_565
O2 O2 O2 88.1(3) 6_556 2_565
O3 O2 O2 78.9(3) 5_455 2_565
La O2 O2 108.9(5) 2_455 2_565
O1 O2 O2 66.2(3) 2_455 2_565
O3 O2 O2 141.9(4) 3_456 2_565
O1 O2 O2 128.2(6) 2_456 2_565
O3 O2 O2 77.0(4) 3_455 2_565
O1 O2 O2 33.3(2) . 2_565
Nb O2 O2 89.0(3) 1_455 2_565
Ga1 O2 O2 89.0(3) 1_455 2_565
Ga2 O2 O2 59.02(11) 2_565 2_565
O2 O2 O2 32.1(2) 6 2_565
O3 O2 O2 40.8(3) 6 2_565
La O2 O2 100.7(4) 1_556 2_565
Ga3 O2 O2 135.3(4) 4_346 2_565
Ga3 O2 O2 75.1(3) 4_446 2_565
O3 O2 O2 80.5(3) 1_556 2_565
La O2 O2 161.2(6) 2_456 2_565
La O2 O2 83.1(3) 4_445 2_565
Ga3 O2 O2 54.6(2) . 2_565
O3 O2 O2 105.7(2) 4_456 2_565
Ga3 O2 O2 136.9(3) 2_455 2_565
O3 O2 O2 33.1(3) . 2_565
O2 O2 O2 160.3(4) 2_456 2_565
O2 O2 O2 62.95(8) 2_566 2_565
Ga2 O2 O2 59.9(2) . 2_565
La O2 O2 52.09(15) 4_455 2_565
O3 O2 O2 66.1(3) 4_455 2_565
O2 O2 O2 158.0(6) 5_346 2_565
Ga1 O2 O2 129.4(3) 1_456 2_565
Nb O2 O2 129.4(3) 1_456 2_565
O1 O2 O2 134.1(5) 1_445 2_565
O3 O2 O2 103.4(4) 6_455 2_565
Ga2 O2 O2 155.5(5) 2_455 2_565
Ga3 O2 O2 101.2(2) 2_465 2_565
Ga3 O2 O2 51.53(19) 2_565 2_565
O2 O2 O2 127.5(3) 1_556 2_565
O2 O2 O2 52.5(3) 1_554 2_565
O2 O2 O2 103.1(5) 2_455 2_565
Ga2 O2 O3 18.6(3) 1_556 4_446
Ga3 O2 O3 114.1(5) 1_556 4_446
La O2 O3 120.1(3) . 4_446
O2 O2 O3 27.9(2) 3_455 4_446
O2 O2 O3 55.7(4) 4_445 4_446
O3 O2 O3 98.5(4) 2_455 4_446
O2 O2 O3 108.8(6) 6_556 4_446
O3 O2 O3 148.5(4) 5_455 4_446
La O2 O3 76.4(3) 2_455 4_446
O1 O2 O3 84.8(3) 2_455 4_446
O3 O2 O3 79.4(4) 3_456 4_446
O1 O2 O3 35.2(2) 2_456 4_446
O3 O2 O3 120.8(5) 3_455 4_446
O1 O2 O3 146.0(5) . 4_446
Nb O2 O3 131.0(4) 1_455 4_446
Ga1 O2 O3 131.0(4) 1_455 4_446
Ga2 O2 O3 126.0(5) 2_565 4_446
O2 O2 O3 147.9(6) 6 4_446
O3 O2 O3 99.0(4) 6 4_446
La O2 O3 74.6(3) 1_556 4_446
Ga3 O2 O3 90.8(3) 4_346 4_446
Ga3 O2 O3 62.5(2) 4_446 4_446
O3 O2 O3 70.1(3) 1_556 4_446
La O2 O3 46.1(2) 2_456 4_446
La O2 O3 54.5(2) 4_445 4_446
Ga3 O2 O3 133.4(4) . 4_446
O3 O2 O3 115.1(4) 4_456 4_446
Ga3 O2 O3 20.23(11) 2_455 4_446
O3 O2 O3 100.52(17) . 4_446
O2 O2 O3 33.2(2) 2_456 4_446
O2 O2 O3 105.5(6) 2_566 4_446
Ga2 O2 O3 96.9(3) . 4_446
La O2 O3 173.4(4) 4_455 4_446
O3 O2 O3 152.1(5) 4_455 4_446
O2 O2 O3 67.7(2) 5_346 4_446
Ga1 O2 O3 91.1(3) 1_456 4_446
Nb O2 O3 91.1(3) 1_456 4_446
O1 O2 O3 64.9(2) 1_445 4_446
O3 O2 O3 122.9(3) 6_455 4_446
Ga2 O2 O3 54.32(17) 2_455 4_446
Ga3 O2 O3 125.6(3) 2_465 4_446
Ga3 O2 O3 99.8(3) 2_565 4_446
O2 O2 O3 63.5(3) 1_556 4_446
O2 O2 O3 116.5(3) 1_554 4_446
O2 O2 O3 72.9(2) 2_455 4_446
O2 O2 O3 132.5(4) 2_565 4_446
Ga2 O2 O3 109.9(4) 1_556 1_456
Ga3 O2 O3 30.5(4) 1_556 1_456
La O2 O3 143.5(4) . 1_456
O2 O2 O3 102.3(7) 3_455 1_456
O2 O2 O3 149.1(3) 4_445 1_456
O3 O2 O3 37.6(4) 2_455 1_456
O2 O2 O3 67.5(3) 6_556 1_456
O3 O2 O3 52.1(5) 5_455 1_456
La O2 O3 84.8(3) 2_455 1_456
O1 O2 O3 135.7(6) 2_455 1_456
O3 O2 O3 24.5(2) 3_456 1_456
O1 O2 O3 86.6(3) 2_456 1_456
O3 O2 O3 82.8(3) 3_455 1_456
O1 O2 O3 103.3(3) . 1_456
Nb O2 O3 53.8(2) 1_455 1_456
Ga1 O2 O3 53.8(2) 1_455 1_456
Ga2 O2 O3 90.3(2) 2_565 1_456
O2 O2 O3 108.4(2) 6 1_456
O3 O2 O3 144.0(4) 6 1_456
La O2 O3 85.2(3) 1_556 1_456
Ga3 O2 O3 19.29(12) 4_346 1_456
Ga3 O2 O3 140.0(4) 4_446 1_456
O3 O2 O3 118.8(5) 1_556 1_456
La O2 O3 53.3(2) 2_456 1_456
La O2 O3 142.9(4) 4_445 1_456
Ga3 O2 O3 99.0(3) . 1_456
O3 O2 O3 31.97(18) 4_456 1_456
Ga3 O2 O3 90.6(3) 2_455 1_456
O3 O2 O3 162.8(5) . 1_456
O2 O2 O3 67.1(3) 2_456 1_456
O2 O2 O3 103.9(4) 2_566 1_456
Ga2 O2 O3 129.8(5) . 1_456
La O2 O3 78.7(2) 4_455 1_456
O3 O2 O3 71.78(16) 4_455 1_456
O2 O2 O3 33.10(19) 5_346 1_456
Ga1 O2 O3 22.79(15) 1_456 1_456
Nb O2 O3 22.79(15) 1_456 1_456
O1 O2 O3 65.0(2) 1_445 1_456
O3 O2 O3 32.9(4) 6_455 1_456
Ga2 O2 O3 54.45(19) 2_455 1_456
Ga3 O2 O3 29.56(18) 2_465 1_456
Ga3 O2 O3 125.7(4) 2_565 1_456
O2 O2 O3 63.4(3) 1_556 1_456
O2 O2 O3 116.6(3) 1_554 1_456
O2 O2 O3 95.8(3) 2_455 1_456
O2 O2 O3 130.8(3) 2_565 1_456
O3 O2 O3 96.4(4) 4_446 1_456
Ga2 O2 O2 25.1(2) 1_556 5_446
Ga3 O2 O2 124.5(9) 1_556 5_446
La O2 O2 83.6(4) . 5_446
O2 O2 O2 59.6(2) 3_455 5_446
O2 O2 O2 22.0(3) 4_445 5_446
O3 O2 O2 142.2(4) 2_455 5_446
O2 O2 O2 92.5(5) 6_556 5_446
O3 O2 O2 154.4(8) 5_455 5_446
La O2 O2 107.9(3) 2_455 5_446
O1 O2 O2 81.4(2) 2_455 5_446
O3 O2 O2 104.2(6) 3_456 5_446
O1 O2 O2 41.6(2) 2_456 5_446
O3 O2 O2 140.9(5) 3_455 5_446
O1 O2 O2 103.2(5) . 5_446
Nb O2 O2 172.3(6) 1_455 5_446
Ga1 O2 O2 172.3(6) 1_455 5_446
Ga2 O2 O2 92.3(5) 2_565 5_446
O2 O2 O2 122.2(3) 6 5_446
O3 O2 O2 55.5(3) 6 5_446
La O2 O2 57.2(4) 1_556 5_446
Ga3 O2 O2 131.3(3) 4_346 5_446
Ga3 O2 O2 18.88(16) 4_446 5_446
O3 O2 O2 32.5(3) 1_556 5_446
La O2 O2 76.3(3) 2_456 5_446
La O2 O2 47.89(10) 4_445 5_446
Ga3 O2 O2 131.8(3) . 5_446
O3 O2 O2 124.4(6) 4_456 5_446
Ga3 O2 O2 61.04(12) 2_455 5_446
O3 O2 O2 68.0(3) . 5_446
O2 O2 O2 76.5(3) 2_456 5_446
O2 O2 O2 69.5(6) 2_566 5_446
Ga2 O2 O2 92.9(2) . 5_446
La O2 O2 137.1(5) 4_455 5_446
O3 O2 O2 159.1(4) 4_455 5_446
O2 O2 O2 108.6(3) 5_346 5_446
Ga1 O2 O2 110.6(5) 1_456 5_446
Nb O2 O2 110.6(5) 1_456 5_446
O1 O2 O2 106.3(3) 1_445 5_446
O3 O2 O2 161.1(4) 6_455 5_446
Ga2 O2 O2 98.0(2) 2_455 5_446
Ga3 O2 O2 146.0(5) 2_465 5_446
Ga3 O2 O2 57.4(3) 2_565 5_446
O2 O2 O2 68.2(3) 1_556 5_446
O2 O2 O2 111.8(3) 1_554 5_446
O2 O2 O2 99.2(2) 2_455 5_446
O2 O2 O2 93.3(4) 2_565 5_446
O3 O2 O2 43.71(16) 4_446 5_446
O3 O2 O2 128.2(5) 1_456 5_446
Ga2 O2 O2 116.6(10) 1_556 5_456
Ga3 O2 O2 47.7(3) 1_556 5_456
La O2 O2 78.5(4) . 5_456
O2 O2 O2 155.7(6) 3_455 5_456
O2 O2 O2 107.5(9) 4_445 5_456
O3 O2 O2 105.8(3) 2_455 5_456
O2 O2 O2 21.6(2) 6_556 5_456
O3 O2 O2 53.8(2) 5_455 5_456
La O2 O2 151.5(5) 2_455 5_456
O1 O2 O2 134.1(4) 2_455 5_456
O3 O2 O2 75.7(4) 3_456 5_456
O1 O2 O2 92.8(6) 2_456 5_456
O3 O2 O2 110.0(3) 3_455 5_456
O1 O2 O2 35.1(3) . 5_456
Nb O2 O2 87.12(15) 1_455 5_456
Ga1 O2 O2 87.12(15) 1_455 5_456
Ga2 O2 O2 12.17(15) 2_565 5_456
O2 O2 O2 78.3(3) 6 5_456
O3 O2 O2 66.7(4) 6 5_456
La O2 O2 53.4(4) 1_556 5_456
Ga3 O2 O2 96.2(2) 4_346 5_456
Ga3 O2 O2 88.9(5) 4_446 5_456
O3 O2 O2 68.1(5) 1_556 5_456
La O2 O2 98.4(4) 2_456 5_456
La O2 O2 136.5(5) 4_445 5_456
Ga3 O2 O2 98.3(2) . 5_456
O3 O2 O2 46.21(16) 4_456 5_456
Ga3 O2 O2 145.3(6) 2_455 5_456
O3 O2 O2 93.8(4) . 5_456
O2 O2 O2 130.1(6) 2_456 5_456
O2 O2 O2 32.3(3) 2_566 5_456
Ga2 O2 O2 126.6(3) . 5_456
La O2 O2 47.14(11) 4_455 5_456
O3 O2 O2 75.54(19) 4_455 5_456
O2 O2 O2 108.6(3) 5_346 5_456
Ga1 O2 O2 64.4(2) 1_456 5_456
Nb O2 O2 64.4(2) 1_456 5_456
O1 O2 O2 142.8(3) 1_445 5_456
O3 O2 O2 78.01(19) 6_455 5_456
Ga2 O2 O2 130.3(3) 2_455 5_456
Ga3 O2 O2 58.43(11) 2_465 5_456
Ga3 O2 O2 51.4(3) 2_565 5_456
O2 O2 O2 68.2(3) 1_556 5_456
O2 O2 O2 111.8(3) 1_554 5_456
O2 O2 O2 158.6(7) 2_455 5_456
O2 O2 O2 67.83(15) 2_565 5_456
O3 O2 O2 127.9(6) 4_446 5_456
O3 O2 O2 78.2(2) 1_456 5_456
O2 O2 O2 100.6(7) 5_446 5_456
Ga2 O2 Ga2 134.3(4) 1_556 2_564
Ga3 O2 Ga2 98.9(3) 1_556 2_564
La O2 Ga2 29.02(18) . 2_564
O2 O2 Ga2 127.40(14) 3_455 2_564
O2 O2 Ga2 94.5(5) 4_445 2_564
O3 O2 Ga2 101.4(4) 2_455 2_564
O2 O2 Ga2 92.8(4) 6_556 2_564
O3 O2 Ga2 64.1(3) 5_455 2_564
La O2 Ga2 96.5(4) 2_455 2_564
O1 O2 Ga2 66.0(3) 2_455 2_564
O3 O2 Ga2 134.0(3) 3_456 2_564
O1 O2 Ga2 147.8(5) 2_456 2_564
O3 O2 Ga2 58.7(2) 3_455 2_564
O1 O2 Ga2 37.3(3) . 2_564
Nb O2 Ga2 69.21(19) 1_455 2_564
Ga1 O2 Ga2 69.21(19) 1_455 2_564
Ga2 O2 Ga2 66.02(16) 2_565 2_564
O2 O2 Ga2 12.50(13) 6 2_564
O3 O2 Ga2 60.7(3) 6 2_564
La O2 Ga2 115.3(4) 1_556 2_564
Ga3 O2 Ga2 116.2(3) 4_346 2_564
Ga3 O2 Ga2 94.8(2) 4_446 2_564
O3 O2 Ga2 99.9(3) 1_556 2_564
La O2 Ga2 167.1(2) 2_456 2_564
La O2 Ga2 92.4(2) 4_445 2_564
Ga3 O2 Ga2 36.72(9) . 2_564
O3 O2 Ga2 97.7(2) 4_456 2_564
Ga3 O2 Ga2 141.5(3) 2_455 2_564
O3 O2 Ga2 47.1(2) . 2_564
O2 O2 Ga2 156.5(6) 2_456 2_564
O2 O2 Ga2 76.9(2) 2_566 2_564
Ga2 O2 Ga2 55.94(14) . 2_564
La O2 Ga2 39.41(9) 4_455 2_564
O3 O2 Ga2 46.6(2) 4_455 2_564
O2 O2 Ga2 138.2(5) 5_346 2_564
Ga1 O2 Ga2 122.12(18) 1_456 2_564
Nb O2 Ga2 122.12(18) 1_456 2_564
O1 O2 Ga2 119.2(4) 1_445 2_564
O3 O2 Ga2 85.1(3) 6_455 2_564
Ga2 O2 Ga2 139.2(4) 2_455 2_564
Ga3 O2 Ga2 87.32(15) 2_465 2_564
Ga3 O2 Ga2 69.82(17) 2_565 2_564
O2 O2 Ga2 138.6(2) 1_556 2_564
O2 O2 Ga2 41.4(2) 1_554 2_564
O2 O2 Ga2 93.8(5) 2_455 2_564
O2 O2 Ga2 20.02(16) 2_565 2_564
O3 O2 Ga2 146.6(3) 4_446 2_564
O3 O2 Ga2 115.6(3) 1_456 2_564
O2 O2 Ga2 112.5(3) 5_446 2_564
O2 O2 Ga2 71.2(2) 5_456 2_564
Ga2 O2 La 14.5(4) 1_556 4_446
Ga3 O2 La 106.8(6) 1_556 4_446
La O2 La 110.0(4) . 4_446
O2 O2 La 52.45(17) 3_455 4_446
O2 O2 La 46.8(2) 4_445 4_446
O3 O2 La 119.0(4) 2_455 4_446
O2 O2 La 87.2(5) 6_556 4_446
O3 O2 La 145.8(5) 5_455 4_446
La O2 La 102.5(2) 2_455 4_446
O1 O2 La 97.9(3) 2_455 4_446
O3 O2 La 79.4(4) 3_456 4_446
O1 O2 La 17.63(17) 2_456 4_446
O3 O2 La 146.5(4) 3_455 4_446
O1 O2 La 120.6(5) . 4_446
Nb O2 La 152.0(3) 1_455 4_446
Ga1 O2 La 152.0(3) 1_455 4_446
Ga2 O2 La 99.9(4) 2_565 4_446
O2 O2 La 148.70(13) 6 4_446
O3 O2 La 79.2(3) 6 4_446
La O2 La 50.48(17) 1_556 4_446
Ga3 O2 La 105.0(2) 4_346 4_446
Ga3 O2 La 43.91(14) 4_446 4_446
O3 O2 La 44.6(3) 1_556 4_446
La O2 La 49.83(14) 2_456 4_446
La O2 La 62.75(14) 4_445 4_446
Ga3 O2 La 152.1(3) . 4_446
O3 O2 La 107.3(4) 4_456 4_446
Ga3 O2 La 46.68(11) 2_455 4_446
O3 O2 La 94.2(3) . 4_446
O2 O2 La 54.3(3) 2_456 4_446
O2 O2 La 79.1(5) 2_566 4_446
Ga2 O2 La 110.51(17) . 4_446
La O2 La 150.1(5) 4_455 4_446
O3 O2 La 174.2(3) 4_455 4_446
O2 O2 La 83.0(3) 5_346 4_446
Ga1 O2 La 87.8(2) 1_456 4_446
Nb O2 La 87.8(2) 1_456 4_446
O1 O2 La 90.4(2) 1_445 4_446
O3 O2 La 135.0(3) 6_455 4_446
Ga2 O2 La 76.27(14) 2_455 4_446
Ga3 O2 La 125.8(3) 2_465 4_446
Ga3 O2 La 75.4(2) 2_565 4_446
O2 O2 La 48.69(14) 1_556 4_446
O2 O2 La 131.31(14) 1_554 4_446
O2 O2 La 98.0(2) 2_455 4_446
O2 O2 La 119.0(4) 2_565 4_446
O3 O2 La 26.45(13) 4_446 4_446
O3 O2 La 102.4(3) 1_456 4_446
O2 O2 La 26.49(15) 5_446 4_446
O2 O2 La 103.4(5) 5_456 4_446
Ga2 O2 La 138.7(3) 2_564 4_446
Ga2 O2 Nb 76.9(4) 1_556 .
Ga3 O2 Nb 130.0(7) 1_556 .
La O2 Nb 30.4(2) . .
O2 O2 Nb 94.4(5) 3_455 .
O2 O2 Nb 38.1(5) 4_445 .
O3 O2 Nb 155.8(5) 2_455 .
O2 O2 Nb 93.3(2) 6_556 .
O3 O2 Nb 116.5(4) 5_455 .
La O2 Nb 114.0(3) 2_455 .
O1 O2 Nb 61.9(2) 2_455 .
O3 O2 Nb 145.1(7) 3_456 .
O1 O2 Nb 92.1(3) 2_456 .
O3 O2 Nb 106.3(3) 3_455 .
O1 O2 Nb 60.3(2) . .
Nb O2 Nb 127.8(3) 1_455 .
Ga1 O2 Nb 127.8(3) 1_455 .
Ga2 O2 Nb 70.2(2) 2_565 .
O2 O2 Nb 69.41(15) 6 .
O3 O2 Nb 16.60(16) 6 .
La O2 Nb 81.3(3) 1_556 .
Ga3 O2 Nb 175.2(3) 4_346 .
Ga3 O2 Nb 36.17(10) 4_446 .
O3 O2 Nb 49.9(2) 1_556 .
La O2 Nb 128.6(4) 2_456 .
La O2 Nb 55.44(12) 4_445 .
Ga3 O2 Nb 86.08(18) . .
O3 O2 Nb 128.6(4) 4_456 .
Ga3 O2 Nb 104.26(17) 2_455 .
O3 O2 Nb 21.11(18) . .
O2 O2 Nb 126.2(3) 2_456 .
O2 O2 Nb 57.1(2) 2_566 .
Ga2 O2 Nb 65.17(13) . .
La O2 Nb 89.8(2) 4_455 .
O3 O2 Nb 105.6(3) 4_455 .
O2 O2 Nb 161.4(2) 5_346 .
Ga1 O2 Nb 140.7(4) 1_456 .
Nb O2 Nb 140.7(4) 1_456 .
O1 O2 Nb 134.6(3) 1_445 .
O3 O2 Nb 143.2(3) 6_455 .
Ga2 O2 Nb 143.1(2) 2_455 .
Ga3 O2 Nb 135.7(3) 2_465 .
Ga3 O2 Nb 35.43(10) 2_565 .
O2 O2 Nb 107.0(2) 1_556 .
O2 O2 Nb 73.0(2) 1_554 .
O2 O2 Nb 103.3(3) 2_455 .
O2 O2 Nb 39.94(19) 2_565 .
O3 O2 Nb 93.7(2) 4_446 .
O3 O2 Nb 160.4(4) 1_456 .
O2 O2 Nb 53.5(2) 5_446 .
O2 O2 Nb 82.4(4) 5_456 .
Ga2 O2 Nb 58.98(12) 2_564 .
La O2 Nb 79.8(2) 4_446 .
Ga2 O2 Ga1 76.9(4) 1_556 .
Ga3 O2 Ga1 130.0(7) 1_556 .
La O2 Ga1 30.4(2) . .
O2 O2 Ga1 94.4(5) 3_455 .
O2 O2 Ga1 38.1(5) 4_445 .
O3 O2 Ga1 155.8(5) 2_455 .
O2 O2 Ga1 93.3(2) 6_556 .
O3 O2 Ga1 116.5(4) 5_455 .
La O2 Ga1 114.0(3) 2_455 .
O1 O2 Ga1 61.9(2) 2_455 .
O3 O2 Ga1 145.1(7) 3_456 .
O1 O2 Ga1 92.1(3) 2_456 .
O3 O2 Ga1 106.3(3) 3_455 .
O1 O2 Ga1 60.3(2) . .
Nb O2 Ga1 127.8(3) 1_455 .
Ga1 O2 Ga1 127.8(3) 1_455 .
Ga2 O2 Ga1 70.2(2) 2_565 .
O2 O2 Ga1 69.41(15) 6 .
O3 O2 Ga1 16.60(16) 6 .
La O2 Ga1 81.3(3) 1_556 .
Ga3 O2 Ga1 175.2(3) 4_346 .
Ga3 O2 Ga1 36.17(10) 4_446 .
O3 O2 Ga1 49.9(2) 1_556 .
La O2 Ga1 128.6(4) 2_456 .
La O2 Ga1 55.44(12) 4_445 .
Ga3 O2 Ga1 86.08(18) . .
O3 O2 Ga1 128.6(4) 4_456 .
Ga3 O2 Ga1 104.26(17) 2_455 .
O3 O2 Ga1 21.11(18) . .
O2 O2 Ga1 126.2(3) 2_456 .
O2 O2 Ga1 57.1(2) 2_566 .
Ga2 O2 Ga1 65.17(13) . .
La O2 Ga1 89.8(2) 4_455 .
O3 O2 Ga1 105.6(3) 4_455 .
O2 O2 Ga1 161.4(2) 5_346 .
Ga1 O2 Ga1 140.7(4) 1_456 .
Nb O2 Ga1 140.7(4) 1_456 .
O1 O2 Ga1 134.6(3) 1_445 .
O3 O2 Ga1 143.2(3) 6_455 .
Ga2 O2 Ga1 143.1(2) 2_455 .
Ga3 O2 Ga1 135.7(3) 2_465 .
Ga3 O2 Ga1 35.43(10) 2_565 .
O2 O2 Ga1 107.0(2) 1_556 .
O2 O2 Ga1 73.0(2) 1_554 .
O2 O2 Ga1 103.3(3) 2_455 .
O2 O2 Ga1 39.94(19) 2_565 .
O3 O2 Ga1 93.7(2) 4_446 .
O3 O2 Ga1 160.4(4) 1_456 .
O2 O2 Ga1 53.5(2) 5_446 .
O2 O2 Ga1 82.4(4) 5_456 .
Ga2 O2 Ga1 58.98(12) 2_564 .
La O2 Ga1 79.8(2) 4_446 .
Nb O2 Ga1 0.0 . .
Ga2 O2 O3 55.5(4) 1_556 2
Ga3 O2 O3 136.1(8) 1_556 2
La O2 O3 51.1(3) . 2
O2 O2 O3 77.6(5) 3_455 2
O2 O2 O3 18.0(5) 4_445 2
O3 O2 O3 161.1(6) 2_455 2
O2 O2 O3 96.5(2) 6_556 2
O3 O2 O3 136.3(4) 5_455 2
La O2 O3 111.0(3) 2_455 2
O1 O2 O3 64.7(3) 2_455 2
O3 O2 O3 133.0(6) 3_456 2
O1 O2 O3 72.8(3) 2_456 2
O3 O2 O3 120.2(3) 3_455 2
O1 O2 O3 78.7(3) . 2
Nb O2 O3 147.6(3) 1_455 2
Ga1 O2 O3 147.6(3) 1_455 2
Ga2 O2 O3 80.8(3) 2_565 2
O2 O2 O3 89.8(2) 6 2
O3 O2 O3 28.9(3) 6 2
La O2 O3 72.6(3) 1_556 2
Ga3 O2 O3 163.3(3) 4_346 2
Ga3 O2 O3 17.30(17) 4_446 2
O3 O2 O3 38.8(3) 1_556 2
La O2 O3 108.6(3) 2_456 2
La O2 O3 44.26(19) 4_445 2
Ga3 O2 O3 103.1(2) . 2
O3 O2 O3 135.1(5) 4_456 2
Ga3 O2 O3 85.20(19) 2_455 2
O3 O2 O3 36.5(4) . 2
O2 O2 O3 105.7(3) 2_456 2
O2 O2 O3 61.7(3) 2_566 2
Ga2 O2 O3 72.5(2) . 2
La O2 O3 110.3(3) 4_455 2
O3 O2 O3 126.5(3) 4_455 2
O2 O2 O3 140.2(3) 5_346 2
Ga1 O2 O3 134.9(4) 1_456 2
Nb O2 O3 134.9(4) 1_456 2
O1 O2 O3 123.7(2) 1_445 2
O3 O2 O3 164.4(3) 6_455 2
Ga2 O2 O3 124.8(2) 2_455 2
Ga3 O2 O3 150.9(4) 2_465 2
Ga3 O2 O3 41.20(15) 2_565 2
O2 O2 O3 93.8(2) 1_556 2
O2 O2 O3 86.2(2) 1_554 2
O2 O2 O3 99.9(3) 2_455 2
O2 O2 O3 61.3(3) 2_565 2
O3 O2 O3 72.7(3) 4_446 2
O3 O2 O3 157.1(4) 1_456 2
O2 O2 O3 32.5(2) 5_446 2
O2 O2 O3 92.6(5) 5_456 2
Ga2 O2 O3 80.0(2) 2_564 2
La O2 O3 59.0(2) 4_446 2
Nb O2 O3 21.35(13) . 2
Ga1 O2 O3 21.35(13) . 2
Ga2 O2 O2 111.3(6) 1_556 5_345
Ga3 O2 O2 95.3(6) 1_556 5_345
La O2 O2 103.1(6) . 5_345
O2 O2 O2 71.7(5) 3_455 5_345
O2 O2 O2 119.0(4) 4_445 5_345
O3 O2 O2 34.4(3) 2_455 5_345
O2 O2 O2 134.35(6) 6_556 5_345
O3 O2 O2 75.9(5) 5_455 5_345
La O2 O2 21.8(2) 2_455 5_345
O1 O2 O2 63.9(4) 2_455 5_345
O3 O2 O2 91.0(6) 3_456 5_345
O1 O2 O2 123.9(4) 2_456 5_345
O3 O2 O2 28.2(3) 3_455 5_345
O1 O2 O2 116.9(4) . 5_345
Nb O2 O2 42.6(3) 1_455 5_345
Ga1 O2 O2 42.6(3) 1_455 5_345
Ga2 O2 O2 137.0(3) 2_565 5_345
O2 O2 O2 74.2(5) 6 5_345
O3 O2 O2 138.0(5) 6 5_345
La O2 O2 153.9(4) 1_556 5_345
Ga3 O2 O2 53.9(2) 4_346 5_345
Ga3 O2 O2 138.8(3) 4_446 5_345
O3 O2 O2 162.1(2) 1_556 5_345
La O2 O2 95.0(3) 2_456 5_345
La O2 O2 87.1(3) 4_445 5_345
Ga3 O2 O2 49.8(3) . 5_345
O3 O2 O2 96.2(3) 4_456 5_345
Ga3 O2 O2 75.1(3) 2_455 5_345
O3 O2 O2 103.1(4) . 5_345
O2 O2 O2 72.0(3) 2_456 5_345
O2 O2 O2 159.1(4) 2_566 5_345
Ga2 O2 O2 58.8(3) . 5_345
La O2 O2 87.3(3) 4_455 5_345
O3 O2 O2 57.2(3) 4_455 5_345
O2 O2 O2 60.9(4) 5_346 5_345
Ga1 O2 O2 94.4(3) 1_456 5_345
Nb O2 O2 94.4(3) 1_456 5_345
O1 O2 O2 33.3(2) 1_445 5_345
O3 O2 O2 55.1(2) 6_455 5_345
Ga2 O2 O2 52.8(2) 2_455 5_345
Ga3 O2 O2 76.6(2) 2_465 5_345
Ga3 O2 O2 154.8(4) 2_565 5_345
O2 O2 O2 126.4(2) 1_556 5_345
O2 O2 O2 53.6(2) 1_554 5_345
O2 O2 O2 31.1(3) 2_455 5_345
O2 O2 O2 103.6(5) 2_565 5_345
O3 O2 O2 95.3(3) 4_446 5_345
O3 O2 O2 71.9(3) 1_456 5_345
O2 O2 O2 129.7(4) 5_446 5_345
O2 O2 O2 129.7(4) 5_456 5_345
Ga2 O2 O2 86.5(3) 2_564 5_345
La O2 O2 121.7(2) 4_446 5_345
Nb O2 O2 123.9(4) . 5_345
Ga1 O2 O2 123.9(4) . 5_345
O3 O2 O2 128.1(3) 2 5_345
Ga2 O2 O3 33.9(4) 1_556 5_445
Ga3 O2 O3 143.5(5) 1_556 5_445
La O2 O3 95.7(3) . 5_445
O2 O2 O3 16.9(4) 3_455 5_445
O2 O2 O3 43.6(4) 4_445 5_445
O3 O2 O3 102.8(4) 2_455 5_445
O2 O2 O3 135.4(5) 6_556 5_445
O3 O2 O3 158.4(7) 5_455 5_445
La O2 O3 60.9(2) 2_455 5_445
O1 O2 O3 53.8(3) 2_455 5_445
O3 O2 O3 107.9(3) 3_456 5_445
O1 O2 O3 63.2(3) 2_456 5_445
O3 O2 O3 99.9(4) 3_455 5_445
O1 O2 O3 137.7(3) . 5_445
Nb O2 O3 125.2(5) 1_455 5_445
Ga1 O2 O3 125.2(5) 1_455 5_445
Ga2 O2 O3 138.7(4) 2_565 5_445
O2 O2 O3 116.8(6) 6 5_445
O3 O2 O3 89.6(2) 6 5_445
La O2 O3 98.3(3) 1_556 5_445
Ga3 O2 O3 105.7(3) 4_346 5_445
Ga3 O2 O3 60.18(16) 4_446 5_445
O3 O2 O3 79.5(3) 1_556 5_445
La O2 O3 75.6(2) 2_456 5_445
La O2 O3 25.73(16) 4_445 5_445
Ga3 O2 O3 105.2(3) . 5_445
O3 O2 O3 144.8(3) 4_456 5_445
Ga3 O2 O3 28.26(16) 2_455 5_445
O3 O2 O3 75.9(3) . 5_445
O2 O2 O3 52.1(2) 2_456 5_445
O2 O2 O3 116.1(5) 2_566 5_445
Ga2 O2 O3 66.0(2) . 5_445
La O2 O3 155.4(3) 4_455 5_445
O3 O2 O3 134.3(5) 4_455 5_445
O2 O2 O3 85.8(2) 5_346 5_445
Ga1 O2 O3 120.2(3) 1_456 5_445
Nb O2 O3 120.2(3) 1_456 5_445
O1 O2 O3 63.6(2) 1_445 5_445
O3 O2 O3 131.8(4) 6_455 5_445
Ga2 O2 O3 65.6(2) 2_455 5_445
Ga3 O2 O3 146.7(4) 2_465 5_445
Ga3 O2 O3 100.1(2) 2_565 5_445
O2 O2 O3 93.7(2) 1_556 5_445
O2 O2 O3 86.3(2) 1_554 5_445
O2 O2 O3 52.82(18) 2_455 5_445
O2 O2 O3 108.8(3) 2_565 5_445
O3 O2 O3 31.1(4) 4_446 5_445
O3 O2 O3 118.7(3) 1_456 5_445
O2 O2 O3 47.06(17) 5_446 5_445
O2 O2 O3 147.7(6) 5_456 5_445
Ga2 O2 O3 117.3(3) 2_564 5_445
La O2 O3 48.35(17) 4_446 5_445
Nb O2 O3 77.53(18) . 5_445
Ga1 O2 O3 77.53(18) . 5_445
O3 O2 O3 60.9(2) 2 5_445
O2 O2 O3 82.7(2) 5_345 5_445
Ga2 O2 O3 62.1(5) 1_556 4_445
Ga3 O2 O3 152.4(7) 1_556 4_445
La O2 O3 82.4(4) . 4_445
O2 O2 O3 32.4(3) 3_455 4_445
O2 O2 O3 57.4(3) 4_445 4_445
O3 O2 O3 91.4(5) 2_455 4_445
O2 O2 O3 162.6(4) 6_556 4_445
O3 O2 O3 134.2(6) 5_455 4_445
La O2 O3 41.74(19) 2_455 4_445
O1 O2 O3 29.1(2) 2_455 4_445
O3 O2 O3 123.6(4) 3_456 4_445
O1 O2 O3 91.5(3) 2_456 4_445
O3 O2 O3 72.9(4) 3_455 4_445
O1 O2 O3 127.4(4) . 4_445
Nb O2 O3 102.4(5) 1_455 4_445
Ga1 O2 O3 102.4(5) 1_455 4_445
Ga2 O2 O3 147.6(3) 2_565 4_445
O2 O2 O3 91.2(6) 6 4_445
O3 O2 O3 93.6(3) 6 4_445
La O2 O3 125.6(3) 1_556 4_445
Ga3 O2 O3 103.6(4) 4_346 4_445
Ga3 O2 O3 77.03(18) 4_446 4_445
O3 O2 O3 100.74(18) 1_556 4_445
La O2 O3 96.9(3) 2_456 4_445
La O2 O3 25.75(15) 4_445 4_445
Ga3 O2 O3 76.9(3) . 4_445
O3 O2 O3 153.8(5) 4_456 4_445
Ga3 O2 O3 46.42(19) 2_455 4_445
O3 O2 O3 66.0(2) . 4_445
O2 O2 O3 66.8(3) 2_456 4_445
O2 O2 O3 131.5(4) 2_566 4_445
Ga2 O2 O3 39.7(2) . 4_445
La O2 O3 128.6(4) 4_455 4_445
O3 O2 O3 106.4(5) 4_455 4_445
O2 O2 O3 91.7(4) 5_346 4_445
Ga1 O2 O3 135.5(3) 1_456 4_445
Nb O2 O3 135.5(3) 1_456 4_445
O1 O2 O3 57.0(2) 1_445 4_445
O3 O2 O3 116.8(4) 6_455 4_445
Ga2 O2 O3 69.9(2) 2_455 4_445
Ga3 O2 O3 138.0(4) 2_465 4_445
Ga3 O2 O3 110.3(2) 2_565 4_445
O2 O2 O3 121.2(2) 1_556 4_445
O2 O2 O3 58.8(2) 1_554 4_445
O2 O2 O3 31.01(18) 2_455 4_445
O2 O2 O3 94.0(3) 2_565 4_445
O3 O2 O3 57.76(17) 4_446 4_445
O3 O2 O3 122.0(4) 1_456 4_445
O2 O2 O3 70.1(2) 5_446 4_445
O2 O2 O3 159.6(4) 5_456 4_445
Ga2 O2 O3 95.1(3) 2_564 4_445
La O2 O3 76.60(16) 4_446 4_445
Nb O2 O3 77.56(19) . 4_445
Ga1 O2 O3 77.56(19) . 4_445
O3 O2 O3 69.72(19) 2 4_445
O2 O2 O3 61.8(2) 5_345 4_445
O3 O2 O3 28.4(3) 5_445 4_445
Ga2 O2 O3 139.9(7) 1_556 1_455
Ga3 O2 O3 71.1(5) 1_556 1_455
La O2 O3 98.8(5) . 1_455
O2 O2 O3 101.8(6) 3_455 1_455
O2 O2 O3 145.1(4) 4_445 1_455
O3 O2 O3 28.9(4) 2_455 1_455
O2 O2 O3 106.4(3) 6_556 1_455
O3 O2 O3 45.2(4) 5_455 1_455
La O2 O3 52.5(3) 2_455 1_455
O1 O2 O3 83.9(5) 2_455 1_455
O3 O2 O3 82.2(4) 3_456 1_455
O1 O2 O3 138.8(4) 2_456 1_455
O3 O2 O3 25.0(2) 3_455 1_455
O1 O2 O3 92.0(3) . 1_455
Nb O2 O3 11.87(16) 1_455 1_455
Ga1 O2 O3 11.87(16) 1_455 1_455
Ga2 O2 O3 106.8(2) 2_565 1_455
O2 O2 O3 60.7(2) 6 1_455
O3 O2 O3 133.4(3) 6 1_455
La O2 O3 139.5(3) 1_556 1_455
Ga3 O2 O3 47.2(2) 4_346 1_455
Ga3 O2 O3 161.9(4) 4_446 1_455
O3 O2 O3 166.9(4) 1_556 1_455
La O2 O3 102.4(3) 2_456 1_455
La O2 O3 114.5(4) 4_445 1_455
Ga3 O2 O3 42.5(2) . 1_455
O3 O2 O3 71.50(18) 4_456 1_455
Ga3 O2 O3 102.6(4) 2_455 1_455
O3 O2 O3 109.2(5) . 1_455
O2 O2 O3 92.0(4) 2_456 1_455
O2 O2 O3 129.5(3) 2_566 1_455
Ga2 O2 O3 74.0(3) . 1_455
La O2 O3 59.0(2) 4_455 1_455
O3 O2 O3 30.4(2) 4_455 1_455
O2 O2 O3 66.0(4) 5_346 1_455
Ga1 O2 O3 79.5(2) 1_456 1_455
Nb O2 O3 79.5(2) 1_456 1_455
O1 O2 O3 57.2(3) 1_445 1_455
O3 O2 O3 29.4(3) 6_455 1_455
Ga2 O2 O3 70.0(3) 2_455 1_455
Ga3 O2 O3 49.98(16) 2_465 1_455
Ga3 O2 O3 138.0(3) 2_565 1_455
O2 O2 O3 121.4(2) 1_556 1_455
O2 O2 O3 58.6(2) 1_554 1_455
O2 O2 O3 61.2(4) 2_455 1_455
O2 O2 O3 92.6(4) 2_565 1_455
O3 O2 O3 122.0(4) 4_446 1_455
O3 O2 O3 58.00(17) 1_456 1_455
O2 O2 O3 160.4(5) 5_446 1_455
O2 O2 O3 99.0(3) 5_456 1_455
Ga2 O2 O3 72.6(3) 2_564 1_455
La O2 O3 146.3(3) 4_446 1_455
Nb O2 O3 128.5(3) . 1_455
Ga1 O2 O3 128.5(3) . 1_455
O3 O2 O3 144.9(3) 2 1_455
O2 O2 O3 30.74(19) 5_345 1_455
O3 O2 O3 113.4(4) 5_445 1_455
O3 O2 O3 90.8(4) 4_445 1_455
Ga2 O2 O3 78.8(4) 1_556 2_456
Ga3 O2 O3 43.8(3) 1_556 2_456
La O2 O3 155.7(6) . 2_456
O2 O2 O3 88.4(4) 3_455 2_456
O2 O2 O3 115.25(19) 4_445 2_456
O3 O2 O3 66.5(3) 2_455 2_456
O2 O2 O3 58.5(4) 6_556 2_456
O3 O2 O3 80.7(3) 5_455 2_456
La O2 O3 100.4(3) 2_455 2_456
O1 O2 O3 147.6(4) 2_455 2_456
O3 O2 O3 10.6(4) 3_456 2_456
O1 O2 O3 52.1(2) 2_456 2_456
O3 O2 O3 115.6(4) 3_455 2_456
O1 O2 O3 113.0(4) . 2_456
Nb O2 O3 88.6(3) 1_455 2_456
Ga1 O2 O3 88.6(3) 1_455 2_456
Ga2 O2 O3 87.6(3) 2_565 2_456
O2 O2 O3 140.1(4) 6 2_456
O3 O2 O3 124.8(5) 6 2_456
La O2 O3 56.9(2) 1_556 2_456
Ga3 O2 O3 45.9(2) 4_346 2_456
Ga3 O2 O3 105.8(4) 4_446 2_456
O3 O2 O3 87.9(3) 1_556 2_456
La O2 O3 24.45(11) 2_456 2_456
La O2 O3 124.8(2) 4_445 2_456
Ga3 O2 O3 133.7(3) . 2_456
O3 O2 O3 44.9(3) 4_456 2_456
Ga3 O2 O3 74.18(18) 2_455 2_456
O3 O2 O3 158.6(5) . 2_456
O2 O2 O3 52.6(3) 2_456 2_456
O2 O2 O3 88.8(5) 2_566 2_456
Ga2 O2 O3 152.4(4) . 2_456
La O2 O3 103.4(2) 4_455 2_456
O3 O2 O3 105.5(4) 4_455 2_456
O2 O2 O3 37.5(3) 5_346 2_456
Ga1 O2 O3 20.77(11) 1_456 2_456
Nb O2 O3 20.77(11) 1_456 2_456
O1 O2 O3 74.8(3) 1_445 2_456
O3 O2 O3 67.57(16) 6_455 2_456
Ga2 O2 O3 54.80(18) 2_455 2_456
Ga3 O2 O3 57.98(17) 2_465 2_456
Ga3 O2 O3 106.9(4) 2_565 2_456
O2 O2 O3 30.6(3) 1_556 2_456
O2 O2 O3 149.4(3) 1_554 2_456
O2 O2 O3 108.4(2) 2_455 2_456
O2 O2 O3 146.1(3) 2_565 2_456
O3 O2 O3 70.3(2) 4_446 2_456
O3 O2 O3 34.8(3) 1_456 2_456
O2 O2 O3 93.6(4) 5_446 2_456
O2 O2 O3 78.3(3) 5_456 2_456
Ga2 O2 O3 142.7(2) 2_564 2_456
La O2 O3 68.8(2) 4_446 2_456
Nb O2 O3 137.6(4) . 2_456
Ga1 O2 O3 137.6(4) . 2_456
O3 O2 O3 123.1(4) 2 2_456
O2 O2 O3 97.2(3) 5_345 2_456
O3 O2 O3 100.0(2) 5_445 2_456
O3 O2 O3 119.5(3) 4_445 2_456
O3 O2 O3 91.8(3) 1_455 2_456
Ga2 O2 O3 92.9(5) 1_556 5_456
Ga3 O2 O3 28.0(4) 1_556 5_456
La O2 O3 127.7(6) . 5_456
O2 O2 O3 114.6(3) 3_455 5_456
O2 O2 O3 117.5(3) 4_445 5_456
O3 O2 O3 80.7(4) 2_455 5_456
O2 O2 O3 30.4(4) 6_556 5_456
O3 O2 O3 66.5(4) 5_455 5_456
La O2 O3 125.3(3) 2_455 5_456
O1 O2 O3 176.0(4) 2_455 5_456
O3 O2 O3 27.9(4) 3_456 5_456
O1 O2 O3 62.0(3) 2_456 5_456
O3 O2 O3 121.3(4) 3_455 5_456
O1 O2 O3 84.7(4) . 5_456
Nb O2 O3 88.6(2) 1_455 5_456
Ga1 O2 O3 88.6(2) 1_455 5_456
Ga2 O2 O3 59.2(2) 2_565 5_456
O2 O2 O3 120.6(5) 6 5_456
O3 O2 O3 103.9(5) 6 5_456
La O2 O3 43.19(18) 1_556 5_456
Ga3 O2 O3 61.47(17) 4_346 5_456
Ga3 O2 O3 100.6(4) 4_446 5_456
O3 O2 O3 76.8(4) 1_556 5_456
La O2 O3 49.98(17) 2_456 5_456
La O2 O3 142.1(3) 4_445 5_456
Ga3 O2 O3 128.5(2) . 5_456
O3 O2 O3 28.2(3) 4_456 5_456
Ga3 O2 O3 100.5(2) 2_455 5_456
O3 O2 O3 138.8(5) . 5_456
O2 O2 O3 80.7(3) 2_456 5_456
O2 O2 O3 64.0(4) 2_566 5_456
Ga2 O2 O3 170.0(3) . 5_456
La O2 O3 82.0(2) 4_455 5_456
O3 O2 O3 95.9(3) 4_455 5_456
O2 O2 O3 62.9(3) 5_346 5_456
Ga1 O2 O3 20.76(12) 1_456 5_456
Nb O2 O3 20.76(12) 1_456 5_456
O1 O2 O3 101.1(3) 1_445 5_456
O3 O2 O3 67.56(19) 6_455 5_456
Ga2 O2 O3 82.56(19) 2_455 5_456
Ga3 O2 O3 49.08(15) 2_465 5_456
Ga3 O2 O3 84.8(3) 2_565 5_456
O2 O2 O3 30.63(16) 1_556 5_456
O2 O2 O3 149.37(16) 1_554 5_456
O2 O2 O3 135.0(3) 2_455 5_456
O2 O2 O3 117.6(3) 2_565 5_456
O3 O2 O3 91.4(3) 4_446 5_456
O3 O2 O3 43.1(2) 1_456 5_456
O2 O2 O3 96.9(5) 5_446 5_456
O2 O2 O3 49.8(3) 5_456 5_456
Ga2 O2 O3 118.0(2) 2_564 5_456
La O2 O3 79.3(2) 4_446 5_456
Nb O2 O3 120.0(4) . 5_456
Ga1 O2 O3 120.0(4) . 5_456
O3 O2 O3 115.6(4) 2 5_456
O2 O2 O3 115.0(3) 5_345 5_456
O3 O2 O3 122.5(3) 5_445 5_456
O3 O2 O3 146.9(3) 4_445 5_456
O3 O2 O3 96.8(2) 1_455 5_456
O3 O2 O3 28.54(19) 2_456 5_456
Ga2 O2 O3 51.4(5) 1_556 6_445
Ga3 O2 O3 122.2(5) 1_556 6_445
La O2 O3 116.3(4) . 6_445
O2 O2 O3 12.9(5) 3_455 6_445
O2 O2 O3 72.4(5) 4_445 6_445
O3 O2 O3 74.2(4) 2_455 6_445
O2 O2 O3 140.3(6) 6_556 6_445
O3 O2 O3 131.3(5) 5_455 6_445
La O2 O3 39.77(19) 2_455 6_445
O1 O2 O3 62.6(3) 2_455 6_445
O3 O2 O3 89.6(4) 3_456 6_445
O1 O2 O3 70.7(3) 2_456 6_445
O3 O2 O3 84.1(4) 3_455 6_445
O1 O2 O3 161.6(4) . 6_445
Nb O2 O3 100.4(4) 1_455 6_445
Ga1 O2 O3 100.4(4) 1_455 6_445
Ga2 O2 O3 162.7(4) 2_565 6_445
O2 O2 O3 119.7(7) 6 6_445
O3 O2 O3 118.4(3) 6 6_445
La O2 O3 110.7(3) 1_556 6_445
Ga3 O2 O3 77.6(3) 4_346 6_445
Ga3 O2 O3 88.04(18) 4_446 6_445
O3 O2 O3 103.7(2) 1_556 6_445
La O2 O3 63.9(2) 2_456 6_445
La O2 O3 50.00(17) 4_445 6_445
Ga3 O2 O3 98.6(4) . 6_445
O3 O2 O3 123.7(3) 4_456 6_445
Ga3 O2 O3 17.33(19) 2_455 6_445
O3 O2 O3 98.7(3) . 6_445
O2 O2 O3 32.8(3) 2_456 6_445
O2 O2 O3 140.9(5) 2_566 6_445
Ga2 O2 O3 71.2(3) . 6_445
La O2 O3 147.0(4) 4_455 6_445
O3 O2 O3 117.0(4) 4_455 6_445
O2 O2 O3 60.1(2) 5_346 6_445
Ga1 O2 O3 101.8(2) 1_456 6_445
Nb O2 O3 101.8(2) 1_456 6_445
O1 O2 O3 35.01(13) 1_445 6_445
O3 O2 O3 103.1(3) 6_455 6_445
Ga2 O2 O3 38.47(16) 2_455 6_445
Ga3 O2 O3 118.5(3) 2_465 6_445
Ga3 O2 O3 128.5(2) 2_565 6_445
O2 O2 O3 93.7(2) 1_556 6_445
O2 O2 O3 86.3(2) 1_554 6_445
O2 O2 O3 36.7(2) 2_455 6_445
O2 O2 O3 128.2(3) 2_565 6_445
O3 O2 O3 36.7(3) 4_446 6_445
O3 O2 O3 92.9(3) 1_456 6_445
O2 O2 O3 72.4(2) 5_446 6_445
O2 O2 O3 161.9(5) 5_456 6_445
Ga2 O2 O3 126.9(3) 2_564 6_445
La O2 O3 62.77(17) 4_446 6_445
Nb O2 O3 105.12(18) . 6_445
Ga1 O2 O3 105.12(18) . 6_445
O3 O2 O3 89.76(16) 2 6_445
O2 O2 O3 59.8(2) 5_345 6_445
O3 O2 O3 28.9(2) 5_445 6_445
O3 O2 O3 34.2(3) 4_445 6_445
O3 O2 O3 89.3(3) 1_455 6_445
O3 O2 O3 85.4(2) 2_456 6_445
O3 O2 O3 113.5(3) 5_456 6_445
Ga2 O2 La 110.6(7) 1_556 4_456
Ga3 O2 La 26.0(5) 1_556 4_456
La O2 La 104.3(4) . 4_456
O2 O2 La 139.31(18) 3_455 4_456
O2 O2 La 120.4(6) 4_445 4_456
O3 O2 La 88.6(3) 2_455 4_456
O2 O2 La 13.95(17) 6_556 4_456
O3 O2 La 51.7(4) 5_455 4_456
La O2 La 138.6(3) 2_455 4_456
O1 O2 La 158.9(4) 2_455 4_456
O3 O2 La 49.9(3) 3_456 4_456
O1 O2 La 80.7(4) 2_456 4_456
O3 O2 La 113.0(3) 3_455 4_456
O1 O2 La 59.8(3) . 4_456
Nb O2 La 82.07(17) 1_455 4_456
Ga1 O2 La 82.07(17) 1_455 4_456
Ga2 O2 La 36.87(13) 2_565 4_456
O2 O2 La 97.1(5) 6 4_456
O3 O2 La 89.0(4) 6 4_456
La O2 La 48.42(17) 1_556 4_456
Ga3 O2 La 74.10(16) 4_346 4_456
Ga3 O2 La 100.7(4) 4_446 4_456
O3 O2 La 76.2(3) 1_556 4_456
La O2 La 75.1(2) 2_456 4_456
La O2 La 152.2(5) 4_445 4_456
Ga3 O2 La 110.85(18) . 4_456
O3 O2 La 24.84(16) 4_456 4_456
Ga3 O2 La 125.4(3) 2_455 4_456
O3 O2 La 119.3(4) . 4_456
O2 O2 La 105.7(4) 2_456 4_456
O2 O2 La 49.3(3) 2_566 4_456
Ga2 O2 La 148.6(2) . 4_456
La O2 La 59.64(14) 4_455 4_456
O3 O2 La 80.5(2) 4_455 4_456
O2 O2 La 83.3(3) 5_346 4_456
Ga1 O2 La 38.71(11) 1_456 4_456
Nb O2 La 38.71(11) 1_456 4_456
O1 O2 La 119.7(2) 1_445 4_456
O3 O2 La 65.54(17) 6_455 4_456
Ga2 O2 La 104.66(18) 2_455 4_456
Ga3 O2 La 43.98(10) 2_465 4_456
Ga3 O2 La 71.1(2) 2_565 4_456
O2 O2 La 50.54(13) 1_556 4_456
O2 O2 La 129.45(13) 1_554 4_456
O2 O2 La 149.8(3) 2_455 4_456
O2 O2 La 93.1(2) 2_565 4_456
O3 O2 La 114.0(4) 4_446 4_456
O3 O2 La 55.00(16) 1_456 4_456
O2 O2 La 105.2(5) 5_446 4_456
O2 O2 La 25.81(14) 5_456 4_456
Ga2 O2 La 93.11(18) 2_564 4_456
La O2 La 96.1(3) 4_446 4_456
Nb O2 La 105.5(3) . 4_456
Ga1 O2 La 105.5(3) . 4_456
O3 O2 La 110.3(4) 2 4_456
O2 O2 La 120.4(2) 5_345 4_456
O3 O2 La 143.9(3) 5_445 4_456
O3 O2 La 171.6(3) 4_445 4_456
O3 O2 La 93.15(17) 1_455 4_456
O3 O2 La 53.11(16) 2_456 4_456
O3 O2 La 25.13(12) 5_456 4_456
O3 O2 La 138.5(3) 6_445 4_456
Ga2 O2 O1 88.3(7) 1_556 1_556
Ga3 O2 O1 50.4(6) 1_556 1_556
La O2 O1 98.0(5) . 1_556
O2 O2 O1 125.1(2) 3_455 1_556
O2 O2 O1 94.2(5) 4_445 1_556
O3 O2 O1 111.8(4) 2_455 1_556
O2 O2 O1 13.7(2) 6_556 1_556
O3 O2 O1 76.8(4) 5_455 1_556
La O2 O1 158.1(3) 2_455 1_556
O1 O2 O1 149.0(5) 2_455 1_556
O3 O2 O1 60.4(5) 3_456 1_556
O1 O2 O1 61.9(3) 2_456 1_556
O3 O2 O1 137.9(3) 3_455 1_556
O1 O2 O1 62.6(3) . 1_556
Nb O2 O1 108.4(2) 1_455 1_556
Ga1 O2 O1 108.4(2) 1_455 1_556
Ga2 O2 O1 33.9(2) 2_565 1_556
O2 O2 O1 108.6(5) 6 1_556
O3 O2 O1 70.9(3) 6 1_556
La O2 O1 23.77(12) 1_556 1_556
Ga3 O2 O1 94.0(2) 4_346 1_556
Ga3 O2 O1 74.7(3) 4_446 1_556
O3 O2 O1 50.0(3) 1_556 1_556
La O2 O1 71.8(3) 2_456 1_556
La O2 O1 125.8(4) 4_445 1_556
Ga3 O2 O1 129.3(3) . 1_556
O3 O2 O1 49.6(2) 4_456 1_556
Ga3 O2 O1 114.4(3) 2_455 1_556
O3 O2 O1 105.9(4) . 1_556
O2 O2 O1 103.1(4) 2_456 1_556
O2 O2 O1 31.3(3) 2_566 1_556
Ga2 O2 O1 149.6(3) . 1_556
La O2 O1 77.5(2) 4_455 1_556
O3 O2 O1 103.7(3) 4_455 1_556
O2 O2 O1 94.9(4) 5_346 1_556
Ga1 O2 O1 53.57(18) 1_456 1_556
Nb O2 O1 53.57(18) 1_456 1_556
O1 O2 O1 132.7(3) 1_445 1_556
O3 O2 O1 91.6(2) 6_455 1_556
Ga2 O2 O1 112.3(2) 2_455 1_556
Ga3 O2 O1 70.15(18) 2_465 1_556
Ga3 O2 O1 51.8(2) 2_565 1_556
O2 O2 O1 38.69(14) 1_556 1_556
O2 O2 O1 141.31(14) 1_554 1_556
O2 O2 O1 165.8(3) 2_455 1_556
O2 O2 O1 91.1(3) 2_565 1_556
O3 O2 O1 97.1(3) 4_446 1_556
O3 O2 O1 75.0(2) 1_456 1_556
O2 O2 O1 79.0(4) 5_446 1_556
O2 O2 O1 31.0(3) 5_456 1_556
Ga2 O2 O1 99.9(3) 2_564 1_556
La O2 O1 74.1(3) 4_446 1_556
Nb O2 O1 87.1(3) . 1_556
Ga1 O2 O1 87.1(3) . 1_556
O3 O2 O1 86.2(3) 2 1_556
O2 O2 O1 145.7(2) 5_345 1_556
O3 O2 O1 122.0(3) 5_445 1_556
O3 O2 O1 148.9(3) 4_445 1_556
O3 O2 O1 119.6(2) 1_455 1_556
O3 O2 O1 57.9(2) 2_456 1_556
O3 O2 O1 33.02(16) 5_456 1_556
O3 O2 O1 131.5(3) 6_445 1_556
La O2 O1 26.41(9) 4_456 1_556
Ga2 O2 O2 112.7(7) 1_556 4_345
Ga3 O2 O2 58.9(4) 1_556 4_345
La O2 O2 134.5(4) . 4_345
O2 O2 O2 85.9(9) 3_455 4_345
O2 O2 O2 145.9(9) 4_445 4_345
O3 O2 O2 7.2(4) 2_455 4_345
O2 O2 O2 98.18(19) 6_556 4_345
O3 O2 O2 59.2(2) 5_455 4_345
La O2 O2 53.9(3) 2_455 4_345
O1 O2 O2 104.0(5) 2_455 4_345
O3 O2 O2 51.5(5) 3_456 4_345
O1 O2 O2 103.1(4) 2_456 4_345
O3 O2 O2 56.7(2) 3_455 4_345
O1 O2 O2 116.8(2) . 4_345
Nb O2 O2 38.82(13) 1_455 4_345
Ga1 O2 O2 38.82(13) 1_455 4_345
Ga2 O2 O2 116.0(2) 2_565 4_345
O2 O2 O2 96.18(8) 6 4_345
O3 O2 O2 166.6(4) 6 4_345
La O2 O2 115.32(14) 1_556 4_345
Ga3 O2 O2 13.8(2) 4_346 4_345
Ga3 O2 O2 156.6(3) 4_446 4_345
O3 O2 O2 147.2(2) 1_556 4_345
La O2 O2 66.7(3) 2_456 4_345
La O2 O2 119.2(5) 4_445 4_345
Ga3 O2 O2 77.45(13) . 4_345
O3 O2 O2 60.10(16) 4_456 4_345
Ga3 O2 O2 79.5(4) 2_455 4_345
O3 O2 O2 141.9(3) . 4_345
O2 O2 O2 61.3(4) 2_456 4_345
O2 O2 O2 134.1(3) 2_566 4_345
Ga2 O2 O2 98.9(3) . 4_345
La O2 O2 83.68(13) 4_455 4_345
O3 O2 O2 62.01(19) 4_455 4_345
O2 O2 O2 30.5(5) 5_346 4_345
Ga1 O2 O2 54.10(16) 1_456 4_345
Nb O2 O2 54.10(16) 1_456 4_345
O1 O2 O2 39.3(3) 1_445 4_345
O3 O2 O2 30.25(19) 6_455 4_345
Ga2 O2 O2 40.4(3) 2_455 4_345
Ga3 O2 O2 46.06(7) 2_465 4_345
Ga3 O2 O2 155.4(3) 2_565 4_345
O2 O2 O2 90.0 1_556 4_345
O2 O2 O2 90.0 1_554 4_345
O2 O2 O2 65.1(3) 2_455 4_345
O2 O2 O2 127.7(3) 2_565 4_345
O3 O2 O2 94.4(4) 4_446 4_345
O3 O2 O2 31.77(19) 1_456 4_345
O2 O2 O2 137.7(4) 5_446 4_345
O2 O2 O2 104.18(12) 5_456 4_345
Ga2 O2 O2 107.69(12) 2_564 4_345
La O2 O2 113.2(3) 4_446 4_345
Nb O2 O2 162.9(2) . 4_345
Ga1 O2 O2 162.9(2) . 4_345
O3 O2 O2 163.0(4) 2 4_345
O2 O2 O2 40.3(2) 5_345 4_345
O3 O2 O2 102.4(5) 5_445 4_345
O3 O2 O2 94.2(4) 4_445 4_345
O3 O2 O2 35.7(2) 1_455 4_345
O3 O2 O2 59.4(2) 2_456 4_345
O3 O2 O2 74.77(15) 5_456 4_345
O3 O2 O2 73.5(4) 6_445 4_345
La O2 O2 84.80(11) 4_456 4_345
O1 O2 O2 106.70(12) 1_556 4_345
Ga2 O2 O2 152.1(4) 1_556 3_465
Ga3 O2 O2 32.5(4) 1_556 3_465
La O2 O2 95.3(3) . 3_465
O2 O2 O2 145.9(9) 3_455 3_465
O2 O2 O2 154.1(9) 4_445 3_465
O3 O2 O2 59.2(2) 2_455 3_465
O2 O2 O2 56.7(3) 6_556 3_465
O3 O2 O2 7.2(4) 5_455 3_465
La O2 O2 102.6(3) 2_455 3_465
O1 O2 O2 123.5(3) 2_455 3_465
O3 O2 O2 65.2(3) 3_456 3_465
O1 O2 O2 121.3(3) 2_456 3_465
O3 O2 O2 68.2(2) 3_455 3_465
O1 O2 O2 58.1(2) . 3_465
Nb O2 O2 38.82(13) 1_455 3_465
Ga1 O2 O2 38.82(13) 1_455 3_465
Ga2 O2 O2 59.0(2) 2_565 3_465
O2 O2 O2 65.4(5) 6 3_465
O3 O2 O2 107.5(4) 6 3_465
La O2 O2 93.2(2) 1_556 3_465
Ga3 O2 O2 58.14(16) 4_346 3_465
Ga3 O2 O2 137.7(5) 4_446 3_465
O3 O2 O2 116.9(4) 1_556 3_465
La O2 O2 98.42(17) 2_456 3_465
La O2 O2 158.5(2) 4_445 3_465
Ga3 O2 O2 69.23(12) . 3_465
O3 O2 O2 31.8(3) 4_456 3_465
Ga3 O2 O2 137.6(4) 2_455 3_465
O3 O2 O2 115.1(3) . 3_465
O2 O2 O2 115.0(4) 2_456 3_465
O2 O2 O2 81.3(3) 2_566 3_465
Ga2 O2 O2 110.83(14) . 3_465
La O2 O2 30.42(19) 4_455 3_465
O3 O2 O2 36.9(3) 4_455 3_465
O2 O2 O2 79.8(3) 5_346 3_465
Ga1 O2 O2 54.10(16) 1_456 3_465
Nb O2 O2 54.10(16) 1_456 3_465
O1 O2 O2 98.5(3) 1_445 3_465
O3 O2 O2 30.28(16) 6_455 3_465
Ga2 O2 O2 98.3(3) 2_455 3_465
Ga3 O2 O2 18.83(15) 2_465 3_465
Ga3 O2 O2 97.8(3) 2_565 3_465
O2 O2 O2 90.0 1_556 3_465
O2 O2 O2 90.0 1_554 3_465
O2 O2 O2 111.8(4) 2_455 3_465
O2 O2 O2 82.4(3) 2_565 3_465
O3 O2 O2 144.1(3) 4_446 3_465
O3 O2 O2 48.4(3) 1_456 3_465
O2 O2 O2 148.9(5) 5_446 3_465
O2 O2 O2 49.21(17) 5_456 3_465
Ga2 O2 O2 69.1(2) 2_564 3_465
La O2 O2 138.66(15) 4_446 3_465
Nb O2 O2 118.1(3) . 3_465
Ga1 O2 O2 118.1(3) . 3_465
O3 O2 O2 136.4(4) 2 3_465
O2 O2 O2 81.0(2) 5_345 3_465
O3 O2 O2 162.0(5) 5_445 3_465
O3 O2 O2 140.8(3) 4_445 3_465
O3 O2 O2 50.62(14) 1_455 3_465
O3 O2 O2 74.77(18) 2_456 3_465
O3 O2 O2 59.38(16) 5_456 3_465
O3 O2 O2 133.3(4) 6_445 3_465
La O2 O2 44.82(14) 4_456 3_465
O1 O2 O2 70.30(16) 1_556 3_465
O2 O2 O2 60.000(1) 4_345 3_465
Ga2 O2 O2 65.6(2) 1_556 5_445
Ga3 O2 O2 166.9(7) 1_556 5_445
La O2 O2 48.0(3) . 5_445
O2 O2 O2 62.7(3) 3_455 5_445
O2 O2 O2 32.9(3) 4_445 5_445
O3 O2 O2 127.3(7) 2_455 5_445
O2 O2 O2 129.7(4) 6_556 5_445
O3 O2 O2 135.0(5) 5_455 5_445
La O2 O2 78.2(4) 2_455 5_445
O1 O2 O2 30.07(17) 2_455 5_445
O3 O2 O2 154.1(4) 3_456 5_445
O1 O2 O2 94.1(3) 2_456 5_445
O3 O2 O2 88.6(5) 3_455 5_445
O1 O2 O2 92.0(3) . 5_445
Nb O2 O2 120.9(6) 1_455 5_445
Ga1 O2 O2 120.9(6) 1_455 5_445
Ga2 O2 O2 107.4(4) 2_565 5_445
O2 O2 O2 75.6(5) 6 5_445
O3 O2 O2 53.7(3) 6 5_445
La O2 O2 106.6(5) 1_556 5_445
Ga3 O2 O2 143.3(6) 4_346 5_445
Ga3 O2 O2 49.1(2) 4_446 5_445
O3 O2 O2 73.2(3) 1_556 5_445
La O2 O2 120.77(19) 2_456 5_445
La O2 O2 21.96(5) 4_445 5_445
Ga3 O2 O2 77.5(4) . 5_445
O3 O2 O2 165.4(5) 4_456 5_445
Ga3 O2 O2 75.76(11) 2_455 5_445
O3 O2 O2 28.5(2) . 5_445
O2 O2 O2 99.5(2) 2_456 5_445
O2 O2 O2 93.4(4) 2_566 5_445
Ga2 O2 O2 39.4(2) . 5_445
La O2 O2 111.1(3) 4_455 5_445
O3 O2 O2 108.9(5) 4_455 5_445
O2 O2 O2 130.8(4) 5_346 5_445
Ga1 O2 O2 164.4(4) 1_456 5_445
Nb O2 O2 164.4(4) 1_456 5_445
O1 O2 O2 97.2(4) 1_445 5_445
O3 O2 O2 142.4(6) 6_455 5_445
Ga2 O2 O2 108.9(3) 2_455 5_445
Ga3 O2 O2 157.5(4) 2_465 5_445
Ga3 O2 O2 71.5(3) 2_565 5_445
O2 O2 O2 122.8(3) 1_556 5_445
O2 O2 O2 57.2(3) 1_554 5_445
O2 O2 O2 67.1(4) 2_455 5_445
O2 O2 O2 61.2(3) 2_565 5_445
O3 O2 O2 74.8(2) 4_446 5_445
O3 O2 O2 162.3(5) 1_456 5_445
O2 O2 O2 54.54(15) 5_446 5_445
O2 O2 O2 119.4(5) 5_456 5_445
Ga2 O2 O2 71.8(2) 2_564 5_445
La O2 O2 76.6(2) 4_446 5_445
Nb O2 O2 37.3(2) . 5_445
Ga1 O2 O2 37.3(2) . 5_445
O3 O2 O2 34.8(3) 2 5_445
O2 O2 O2 93.3(5) 5_345 5_445
O3 O2 O2 47.64(15) 5_445 5_445
O3 O2 O2 40.3(2) 4_445 5_445
O3 O2 O2 113.3(5) 1_455 5_445
O3 O2 O2 144.3(3) 2_456 5_445
O3 O2 O2 149.7(6) 5_456 5_445
O3 O2 O2 70.7(2) 6_445 5_445
La O2 O2 142.6(5) 4_456 5_445
O1 O2 O2 120.8(5) 1_556 5_445
O2 O2 O2 132.1(6) 4_345 5_445
O2 O2 O2 140.8(2) 3_465 5_445
Ga2 O2 O2 144.3(7) 1_556 5_455
Ga3 O2 O2 81.4(2) 1_556 5_455
La O2 O2 41.5(3) . 5_455
O2 O2 O2 145.6(2) 3_455 5_455
O2 O2 O2 105.8(7) 4_445 5_455
O3 O2 O2 97.9(4) 2_455 5_455
O2 O2 O2 75.9(4) 6_556 5_455
O3 O2 O2 50.0(3) 5_455 5_455
La O2 O2 108.2(6) 2_455 5_455
O1 O2 O2 84.2(4) 2_455 5_455
O3 O2 O2 117.0(3) 3_456 5_455
O1 O2 O2 142.4(7) 2_456 5_455
O3 O2 O2 65.3(4) 3_455 5_455
O1 O2 O2 24.2(3) . 5_455
Nb O2 O2 64.6(2) 1_455 5_455
Ga1 O2 O2 64.6(2) 1_455 5_455
Ga2 O2 O2 51.5(2) 2_565 5_455
O2 O2 O2 23.8(2) 6 5_455
O3 O2 O2 64.0(4) 6 5_455
La O2 O2 103.7(5) 1_556 5_455
Ga3 O2 O2 107.6(3) 4_346 5_455
Ga3 O2 O2 100.6(4) 4_446 5_455
O3 O2 O2 97.9(5) 1_556 5_455
La O2 O2 149.1(3) 2_456 5_455
La O2 O2 109.7(3) 4_445 5_455
Ga3 O2 O2 46.5(2) . 5_455
O3 O2 O2 80.19(18) 4_456 5_455
Ga3 O2 O2 159.5(5) 2_455 5_455
O3 O2 O2 61.4(3) . 5_455
O2 O2 O2 163.6(7) 2_456 5_455
O2 O2 O2 67.12(16) 2_566 5_455
Ga2 O2 O2 73.7(3) . 5_455
La O2 O2 23.33(6) 4_455 5_455
O3 O2 O2 41.6(2) 4_455 5_455
O2 O2 O2 130.8(4) 5_346 5_455
Ga1 O2 O2 104.72(15) 1_456 5_455
Nb O2 O2 104.72(15) 1_456 5_455
O1 O2 O2 126.3(6) 1_445 5_455
O3 O2 O2 75.4(3) 6_455 5_455
Ga2 O2 O2 141.6(5) 2_455 5_455
Ga3 O2 O2 72.54(8) 2_465 5_455
Ga3 O2 O2 66.8(3) 2_565 5_455
O2 O2 O2 122.8(3) 1_556 5_455
O2 O2 O2 57.2(3) 1_554 5_455
O2 O2 O2 108.0(7) 2_455 5_455
O2 O2 O2 28.89(19) 2_565 5_455
O3 O2 O2 161.4(4) 4_446 5_455
O3 O2 O2 102.0(2) 1_456 5_455
O2 O2 O2 119.4(5) 5_446 5_455
O2 O2 O2 54.54(15) 5_456 5_455
Ga2 O2 O2 18.24(15) 2_564 5_455
La O2 O2 142.1(5) 4_446 5_455
Nb O2 O2 67.8(3) . 5_455
Ga1 O2 O2 67.8(3) . 5_455
O3 O2 O2 89.0(3) 2 5_455
O2 O2 O2 93.3(5) 5_345 5_455
O3 O2 O2 135.0(3) 5_445 5_455
O3 O2 O2 113.2(4) 4_445 5_455
O3 O2 O2 71.6(4) 1_455 5_455
O3 O2 O2 124.8(2) 2_456 5_455
O3 O2 O2 99.8(3) 5_456 5_455
O3 O2 O2 143.5(5) 6_445 5_455
La O2 O2 75.1(2) 4_456 5_455
O1 O2 O2 84.8(4) 1_556 5_455
O2 O2 O2 102.82(14) 4_345 5_455
O2 O2 O2 53.75(15) 3_465 5_455
O2 O2 O2 88.3(3) 5_445 5_455
Ga2 O2 Ga3 129.0(7) 1_556 4_345
Ga3 O2 Ga3 89.4(6) 1_556 4_345
La O2 Ga3 91.0(5) . 4_345
O2 O2 Ga3 89.1(5) 3_455 4_345
O2 O2 Ga3 126.8(3) 4_445 4_345
O3 O2 Ga3 38.4(4) 2_455 4_345
O2 O2 Ga3 124.1(3) 6_556 4_345
O3 O2 Ga3 61.5(4) 5_455 4_345
La O2 Ga3 38.4(2) 2_455 4_345
O1 O2 Ga3 65.9(4) 2_455 4_345
O3 O2 Ga3 96.4(5) 3_456 4_345
O1 O2 Ga3 141.6(4) 2_456 4_345
O3 O2 Ga3 11.8(2) 3_455 4_345
O1 O2 Ga3 98.4(3) . 4_345
Nb O2 Ga3 29.21(18) 1_455 4_345
Ga1 O2 Ga3 29.21(18) 1_455 4_345
Ga2 O2 Ga3 119.4(2) 2_565 4_345
O2 O2 Ga3 57.5(3) 6 4_345
O3 O2 Ga3 127.5(4) 6 4_345
La O2 Ga3 157.6(2) 1_556 4_345
Ga3 O2 Ga3 59.0(2) 4_346 4_345
Ga3 O2 Ga3 144.9(3) 4_446 4_345
O3 O2 Ga3 167.3(3) 1_556 4_345
La O2 Ga3 109.1(3) 2_456 4_345
La O2 Ga3 96.3(3) 4_445 4_345
Ga3 O2 Ga3 34.12(16) . 4_345
O3 O2 Ga3 89.8(3) 4_456 4_345
Ga3 O2 Ga3 93.6(3) 2_455 4_345
O3 O2 Ga3 96.5(3) . 4_345
O2 O2 Ga3 89.8(4) 2_456 4_345
O2 O2 Ga3 140.6(4) 2_566 4_345
Ga2 O2 Ga3 56.9(2) . 4_345
La O2 Ga3 69.1(2) 4_455 4_345
O3 O2 Ga3 39.2(2) 4_455 4_345
O2 O2 Ga3 72.7(5) 5_346 4_345
Ga1 O2 Ga3 95.9(2) 1_456 4_345
Nb O2 Ga3 95.9(2) 1_456 4_345
O1 O2 Ga3 51.4(2) 1_445 4_345
O3 O2 Ga3 47.6(2) 6_455 4_345
Ga2 O2 Ga3 69.4(2) 2_455 4_345
Ga3 O2 Ga3 68.3(2) 2_465 4_345
Ga3 O2 Ga3 139.8(2) 2_565 4_345
O2 O2 Ga3 135.47(10) 1_556 4_345
O2 O2 Ga3 44.53(10) 1_554 4_345
O2 O2 Ga3 45.1(3) 2_455 4_345
O2 O2 Ga3 88.6(4) 2_565 4_345
O3 O2 Ga3 113.8(4) 4_446 4_345
O3 O2 Ga3 73.4(3) 1_456 4_345
O2 O2 Ga3 143.4(4) 5_446 4_345
O2 O2 Ga3 113.8(3) 5_456 4_345
Ga2 O2 Ga3 69.9(2) 2_564 4_345
La O2 Ga3 140.3(3) 4_446 4_345
Nb O2 Ga3 117.4(3) . 4_345
Ga1 O2 Ga3 117.4(3) . 4_345
O3 O2 Ga3 129.3(3) 2 4_345
O2 O2 Ga3 18.63(14) 5_345 4_345
O3 O2 Ga3 97.9(3) 5_445 4_345
O3 O2 Ga3 73.3(3) 4_445 4_345
O3 O2 Ga3 18.36(13) 1_455 4_345
O3 O2 Ga3 104.9(3) 2_456 4_345
O3 O2 Ga3 114.5(2) 5_456 4_345
O3 O2 Ga3 77.8(3) 6_445 4_345
La O2 Ga3 111.26(18) 4_456 4_345
O1 O2 Ga3 137.58(17) 1_556 4_345
O2 O2 Ga3 45.54(10) 4_345 4_345
O2 O2 Ga3 67.62(11) 3_465 4_345
O2 O2 Ga3 95.8(5) 5_445 4_345
O2 O2 Ga3 75.0(4) 5_455 4_345
Ga2 O2 O2 39.1(4) 1_556 3_456
Ga3 O2 O2 81.2(3) 1_556 3_456
La O2 O2 137.4(7) . 3_456
O2 O2 O2 61.14(13) 3_455 3_456
O2 O2 O2 76.04(6) 4_445 3_456
O3 O2 O2 94.8(4) 2_455 3_456
O2 O2 O2 75.6(4) 6_556 3_456
O3 O2 O2 120.0(4) 5_455 3_456
La O2 O2 100.2(3) 2_455 3_456
O1 O2 O2 119.9(4) 2_455 3_456
O3 O2 O2 50.4(3) 3_456 3_456
O1 O2 O2 15.15(11) 2_456 3_456
O3 O2 O2 139.5(5) 3_455 3_456
O1 O2 O2 127.3(5) . 3_456
Nb O2 O2 124.9(4) 1_455 3_456
Ga1 O2 O2 124.9(4) 1_455 3_456
Ga2 O2 O2 99.3(3) 2_565 3_456
O2 O2 O2 174.1(6) 6 3_456
O3 O2 O2 102.5(5) 6 3_456
La O2 O2 47.72(9) 1_556 3_456
Ga3 O2 O2 77.6(2) 4_346 3_456
Ga3 O2 O2 71.0(3) 4_446 3_456
O3 O2 O2 62.5(4) 1_556 3_456
La O2 O2 21.51(13) 2_456 3_456
La O2 O2 87.5(3) 4_445 3_456
Ga3 O2 O2 161.3(5) . 3_456
O3 O2 O2 82.0(2) 4_456 3_456
Ga3 O2 O2 48.7(2) 2_455 3_456
O3 O2 O2 123.3(5) . 3_456
O2 O2 O2 40.4(3) 2_456 3_456
O2 O2 O2 85.7(5) 2_566 3_456
Ga2 O2 O2 132.0(2) . 3_456
La O2 O2 138.3(2) 4_455 3_456
O3 O2 O2 144.9(4) 4_455 3_456
O2 O2 O2 57.7(3) 5_346 3_456
Ga1 O2 O2 59.87(17) 1_456 3_456
Nb O2 O2 59.87(17) 1_456 3_456
O1 O2 O2 78.7(3) 1_445 3_456
O3 O2 O2 105.9(4) 6_455 3_456
Ga2 O2 O2 58.9(2) 2_455 3_456
Ga3 O2 O2 97.8(2) 2_465 3_456
Ga3 O2 O2 92.1(3) 2_565 3_456
O2 O2 O2 28.86(13) 1_556 3_456
O2 O2 O2 151.14(13) 1_554 3_456
O2 O2 O2 101.3(3) 2_455 3_456
O2 O2 O2 143.0(5) 2_565 3_456
O3 O2 O2 35.2(3) 4_446 3_456
O3 O2 O2 73.2(3) 1_456 3_456
O2 O2 O2 55.3(3) 5_446 3_456
O2 O2 O2 96.6(4) 5_456 3_456
Ga2 O2 O2 161.9(5) 2_564 3_456
La O2 O2 29.3(2) 4_446 3_456
Nb O2 O2 107.1(4) . 3_456
Ga1 O2 O2 107.1(4) . 3_456
O3 O2 O2 87.4(4) 2 3_456
O2 O2 O2 111.6(3) 5_345 3_456
O3 O2 O2 66.1(3) 5_445 3_456
O3 O2 O2 92.7(3) 4_445 3_456
O3 O2 O2 123.7(4) 1_455 3_456
O3 O2 O2 39.9(2) 2_456 3_456
O3 O2 O2 56.45(17) 5_456 3_456
O3 O2 O2 65.5(3) 6_445 3_456
La O2 O2 79.01(13) 4_456 3_456
O1 O2 O2 66.02(15) 1_556 3_456
O2 O2 O2 88.0(4) 4_345 3_456
O2 O2 O2 113.5(3) 3_465 3_456
O2 O2 O2 104.7(4) 5_445 3_456
O2 O2 O2 150.7(5) 5_455 3_456
Ga3 O2 O2 128.1(4) 4_345 3_456
Ga2 O2 O2 39.1(4) 1_556 4_446
Ga3 O2 O2 86.0(6) 1_556 4_446
La O2 O2 111.6(6) . 4_446
O2 O2 O2 76.04(6) 3_455 4_446
O2 O2 O2 61.14(13) 4_445 4_446
O3 O2 O2 120.7(4) 2_455 4_446
O2 O2 O2 62.6(4) 6_556 4_446
O3 O2 O2 122.9(6) 5_455 4_446
La O2 O2 123.9(3) 2_455 4_446
O1 O2 O2 119.9(4) 2_455 4_446
O3 O2 O2 66.8(4) 3_456 4_446
O1 O2 O2 15.15(11) 2_456 4_446
O3 O2 O2 167.2(5) 3_455 4_446
O1 O2 O2 103.1(6) . 4_446
Nb O2 O2 144.6(3) 1_455 4_446
Ga1 O2 O2 144.6(3) 1_455 4_446
Ga2 O2 O2 78.0(5) 2_565 4_446
O2 O2 O2 146.5(5) 6 4_446
O3 O2 O2 75.5(4) 6 4_446
La O2 O2 26.25(19) 1_556 4_446
Ga3 O2 O2 101.33(19) 4_346 4_446
Ga3 O2 O2 49.0(3) 4_446 4_446
O3 O2 O2 35.0(4) 1_556 4_446
La O2 O2 47.55(9) 2_456 4_446
La O2 O2 84.9(2) 4_445 4_446
Ga3 O2 O2 169.0(4) . 4_446
O3 O2 O2 86.1(3) 4_456 4_446
Ga3 O2 O2 67.73(17) 2_455 4_446
O3 O2 O2 102.4(4) . 4_446
O2 O2 O2 66.9(3) 2_456 4_446
O2 O2 O2 60.1(6) 2_566 4_446
Ga2 O2 O2 132.0(2) . 4_446
La O2 O2 126.8(5) 4_455 4_446
O3 O2 O2 152.2(5) 4_455 4_446
O2 O2 O2 84.3(3) 5_346 4_446
Ga1 O2 O2 71.43(19) 1_456 4_446
Nb O2 O2 71.43(19) 1_456 4_446
O1 O2 O2 105.7(3) 1_445 4_446
O3 O2 O2 123.0(3) 6_455 4_446
Ga2 O2 O2 86.68(18) 2_455 4_446
Ga3 O2 O2 106.9(3) 2_465 4_446
Ga3 O2 O2 64.2(4) 2_565 4_446
O2 O2 O2 28.86(13) 1_556 4_446
O2 O2 O2 151.14(13) 1_554 4_446
O2 O2 O2 121.3(3) 2_455 4_446
O2 O2 O2 115.2(5) 2_565 4_446
O3 O2 O2 48.43(19) 4_446 4_446
O3 O2 O2 91.2(3) 1_456 4_446
O2 O2 O2 39.4(3) 5_446 4_446
O2 O2 O2 79.6(6) 5_456 4_446
Ga2 O2 O2 134.0(5) 2_564 4_446
La O2 O2 24.66(12) 4_446 4_446
Nb O2 O2 82.9(3) . 4_446
Ga1 O2 O2 82.9(3) . 4_446
O3 O2 O2 66.3(3) 2 4_446
O2 O2 O2 138.9(4) 5_345 4_446
O3 O2 O2 73.0(2) 5_445 4_446
O3 O2 O2 101.2(2) 4_445 4_446
O3 O2 O2 148.4(3) 1_455 4_446
O3 O2 O2 56.78(18) 2_456 4_446
O3 O2 O2 58.0(2) 5_456 4_446
O3 O2 O2 84.9(3) 6_445 4_446
La O2 O2 71.8(3) 4_456 4_446
O1 O2 O2 49.6(3) 1_556 4_446
O2 O2 O2 113.5(3) 4_345 4_446
O2 O2 O2 115.7(2) 3_465 4_446
O2 O2 O2 94.0(4) 5_445 4_446
O2 O2 O2 127.3(7) 5_455 4_446
Ga3 O2 O2 156.0(3) 4_345 4_446
O2 O2 O2 27.93(12) 3_456 4_446
Ga2 O2 O2 92.0(5) 1_556 3_454
Ga3 O2 O2 140.1(9) 1_556 3_454
La O2 O2 66.5(3) . 3_454
O2 O2 O2 61.14(13) 3_455 3_454
O2 O2 O2 76.04(6) 4_445 3_454
O3 O2 O2 82.2(6) 2_455 3_454
O2 O2 O2 161.4(5) 6_556 3_454
O3 O2 O2 106.4(6) 5_455 3_454
La O2 O2 38.0(3) 2_455 3_454
O1 O2 O2 16.08(15) 2_455 3_454
O3 O2 O2 135.7(7) 3_456 3_454
O1 O2 O2 122.0(3) 2_456 3_454
O3 O2 O2 46.3(3) 3_455 3_454
O1 O2 O2 105.3(3) . 3_454
Nb O2 O2 78.9(4) 1_455 3_454
Ga1 O2 O2 78.9(4) 1_455 3_454
Ga2 O2 O2 133.2(3) 2_565 3_454
O2 O2 O2 62.3(5) 6 3_454
O3 O2 O2 93.3(3) 6 3_454
La O2 O2 151.4(4) 1_556 3_454
Ga3 O2 O2 101.2(5) 4_346 3_454
Ga3 O2 O2 94.4(2) 4_446 3_454
O3 O2 O2 119.0(3) 1_556 3_454
La O2 O2 121.3(4) 2_456 3_454
La O2 O2 46.80(16) 4_445 3_454
Ga3 O2 O2 46.5(2) . 3_454
O3 O2 O2 140.5(5) 4_456 3_454
Ga3 O2 O2 74.0(3) 2_455 3_454
O3 O2 O2 58.09(18) . 3_454
O2 O2 O2 89.5(5) 2_456 3_454
O2 O2 O2 132.7(3) 2_566 3_454
Ga2 O2 O2 14.70(7) . 3_454
La O2 O2 98.2(3) 4_455 3_454
O3 O2 O2 77.1(4) 4_455 3_454
O2 O2 O2 101.1(7) 5_346 3_454
Ga1 O2 O2 141.9(5) 1_456 3_454
Nb O2 O2 141.9(5) 1_456 3_454
O1 O2 O2 63.1(4) 1_445 3_454
O3 O2 O2 98.4(5) 6_455 3_454
Ga2 O2 O2 83.0(4) 2_455 3_454
Ga3 O2 O2 118.9(5) 2_465 3_454
Ga3 O2 O2 112.3(2) 2_565 3_454
O2 O2 O2 151.14(13) 1_556 3_454
O2 O2 O2 28.86(13) 1_554 3_454
O2 O2 O2 29.4(4) 2_455 3_454
O2 O2 O2 74.4(2) 2_565 3_454
O3 O2 O2 88.0(3) 4_446 3_454
O3 O2 O2 119.7(5) 1_456 3_454
O2 O2 O2 94.6(3) 5_446 3_454
O2 O2 O2 139.9(3) 5_456 3_454
Ga2 O2 O2 68.65(14) 2_564 3_454
La O2 O2 106.5(2) 4_446 3_454
Nb O2 O2 77.33(16) . 3_454
Ga1 O2 O2 77.33(16) . 3_454
O3 O2 O2 80.7(3) 2 3_454
O2 O2 O2 47.9(3) 5_345 3_454
O3 O2 O2 58.7(2) 5_445 3_454
O3 O2 O2 30.5(2) 4_445 3_454
O3 O2 O2 69.1(4) 1_455 3_454
O3 O2 O2 137.8(4) 2_456 3_454
O3 O2 O2 162.7(5) 5_456 3_454
O3 O2 O2 58.2(3) 6_445 3_454
La O2 O2 157.3(3) 4_456 3_454
O1 O2 O2 163.9(4) 1_556 3_454
O2 O2 O2 88.0(4) 4_345 3_454
O2 O2 O2 113.5(3) 3_465 3_454
O2 O2 O2 45.9(2) 5_445 3_454
O2 O2 O2 85.6(3) 5_455 3_454
Ga3 O2 O2 50.8(3) 4_345 3_454
O2 O2 O2 122.3(3) 3_456 3_454
O2 O2 O2 130.6(2) 4_446 3_454
Ga2 O2 Ga3 83.2(3) 1_556 4_445
Ga3 O2 Ga3 151.1(4) 1_556 4_445
La O2 Ga3 31.24(19) . 4_445
O2 O2 Ga3 79.2(3) 3_455 4_445
O2 O2 Ga3 46.8(3) 4_445 4_445
O3 O2 Ga3 125.3(5) 2_455 4_445
O2 O2 Ga3 123.8(3) 6_556 4_445
O3 O2 Ga3 117.0(4) 5_455 4_445
La O2 Ga3 82.2(3) 2_455 4_445
O1 O2 Ga3 29.89(16) 2_455 4_445
O3 O2 Ga3 172.2(4) 3_456 4_445
O1 O2 Ga3 109.9(3) 2_456 4_445
O3 O2 Ga3 78.9(3) 3_455 4_445
O1 O2 Ga3 76.5(2) . 4_445
Nb O2 Ga3 108.5(3) 1_455 4_445
Ga1 O2 Ga3 108.5(3) 1_455 4_445
Ga2 O2 Ga3 96.8(2) 2_565 4_445
O2 O2 Ga3 57.8(3) 6 4_445
O3 O2 Ga3 48.5(2) 6 4_445
La O2 Ga3 112.5(3) 1_556 4_445
Ga3 O2 Ga3 145.5(5) 4_346 4_445
Ga3 O2 Ga3 58.27(12) 4_446 4_445
O3 O2 Ga3 79.2(2) 1_556 4_445
La O2 Ga3 139.1(2) 2_456 4_445
La O2 Ga3 39.60(9) 4_445 4_445
Ga3 O2 Ga3 63.37(15) . 4_445
O3 O2 Ga3 149.7(3) 4_456 4_445
Ga3 O2 Ga3 92.92(18) 2_455 4_445
O3 O2 Ga3 14.41(14) . 4_445
O2 O2 Ga3 116.3(3) 2_456 4_445
O2 O2 Ga3 88.6(2) 2_566 4_445
Ga2 O2 Ga3 32.90(7) . 4_445
La O2 Ga3 92.81(18) 4_455 4_445
O3 O2 Ga3 92.7(3) 4_455 4_445
O2 O2 Ga3 143.0(5) 5_346 4_445
Ga1 O2 Ga3 172.3(4) 1_456 4_445
Nb O2 Ga3 172.3(4) 1_456 4_445
O1 O2 Ga3 105.5(3) 1_445 4_445
O3 O2 Ga3 129.9(4) 6_455 4_445
Ga2 O2 Ga3 121.7(3) 2_455 4_445
Ga3 O2 Ga3 140.0(2) 2_465 4_445
Ga3 O2 Ga3 67.57(14) 2_565 4_445
O2 O2 Ga3 134.98(18) 1_556 4_445
O2 O2 Ga3 45.02(18) 1_554 4_445
O2 O2 Ga3 72.1(3) 2_455 4_445
O2 O2 Ga3 44.05(19) 2_565 4_445
O3 O2 Ga3 93.1(2) 4_446 4_445
O3 O2 Ga3 161.6(4) 1_456 4_445
O2 O2 Ga3 68.66(19) 5_446 4_445
O2 O2 Ga3 108.0(3) 5_456 4_445
Ga2 O2 Ga3 53.49(10) 2_564 4_445
La O2 Ga3 93.06(15) 4_446 4_445
Nb O2 Ga3 32.54(6) . 4_445
Ga1 O2 Ga3 32.54(6) . 4_445
O3 O2 Ga3 41.29(18) 2 4_445
O2 O2 Ga3 91.6(3) 5_345 4_445
O3 O2 Ga3 65.26(18) 5_445 4_445
O3 O2 Ga3 51.96(19) 4_445 4_445
O3 O2 Ga3 103.7(3) 1_455 4_445
O3 O2 Ga3 161.8(3) 2_456 4_445
O3 O2 Ga3 152.4(4) 5_456 4_445
O3 O2 Ga3 85.4(2) 6_445 4_445
La O2 Ga3 133.6(3) 4_456 4_445
O1 O2 Ga3 119.4(3) 1_556 4_445
O2 O2 Ga3 131.8(3) 4_345 4_445
O2 O2 Ga3 122.51(19) 3_465 4_445
O2 O2 Ga3 18.34(14) 5_445 4_445
O2 O2 Ga3 70.1(2) 5_455 4_445
Ga3 O2 Ga3 88.4(2) 4_345 4_445
O2 O2 Ga3 121.9(3) 3_456 4_445
O2 O2 Ga3 106.8(3) 4_446 4_445
O2 O2 Ga3 44.84(12) 3_454 4_445
Ga2 O2 O2 92.0(5) 1_556 4_444
Ga3 O2 O2 148.2(4) 1_556 4_444
La O2 O2 40.0(2) . 4_444
O2 O2 O2 76.03(6) 3_455 4_444
O2 O2 O2 61.14(13) 4_445 4_444
O3 O2 O2 107.0(5) 2_455 4_444
O2 O2 O2 137.3(4) 6_556 4_444
O3 O2 O2 109.0(4) 5_455 4_444
La O2 O2 66.0(3) 2_455 4_444
O1 O2 O2 16.08(15) 2_455 4_444
O3 O2 O2 163.6(7) 3_456 4_444
O1 O2 O2 122.0(3) 2_456 4_444
O3 O2 O2 61.6(2) 3_455 4_444
O1 O2 O2 83.4(3) . 4_444
Nb O2 O2 92.9(2) 1_455 4_444
Ga1 O2 O2 92.9(2) 1_455 4_444
Ga2 O2 O2 108.4(3) 2_565 4_444
O2 O2 O2 51.2(2) 6 4_444
O3 O2 O2 65.8(3) 6 4_444
La O2 O2 130.8(3) 1_556 4_444
Ga3 O2 O2 127.3(4) 4_346 4_444
Ga3 O2 O2 75.3(2) 4_446 4_444
O3 O2 O2 97.3(3) 1_556 4_444
La O2 O2 140.9(4) 2_456 4_444
La O2 O2 43.1(3) 4_445 4_444
Ga3 O2 O2 49.14(11) . 4_444
O3 O2 O2 147.4(3) 4_456 4_444
Ga3 O2 O2 90.3(4) 2_455 4_444
O3 O2 O2 30.3(2) . 4_444
O2 O2 O2 111.1(5) 2_456 4_444
O2 O2 O2 104.7(3) 2_566 4_444
Ga2 O2 O2 14.70(7) . 4_444
La O2 O2 89.7(2) 4_455 4_444
O3 O2 O2 81.0(3) 4_455 4_444
O2 O2 O2 128.9(7) 5_346 4_444
Ga1 O2 O2 166.0(3) 1_456 4_444
Nb O2 O2 166.0(3) 1_456 4_444
O1 O2 O2 90.8(4) 1_445 4_444
O3 O2 O2 114.6(3) 6_455 4_444
Ga2 O2 O2 109.7(4) 2_455 4_444
Ga3 O2 O2 129.7(2) 2_465 4_444
Ga3 O2 O2 84.7(2) 2_565 4_444
O2 O2 O2 151.14(13) 1_556 4_444
O2 O2 O2 28.86(13) 1_554 4_444
O2 O2 O2 56.8(4) 2_455 4_444
O2 O2 O2 50.2(3) 2_565 4_444
O3 O2 O2 96.8(4) 4_446 4_444
O3 O2 O2 143.8(4) 1_456 4_444
O2 O2 O2 82.9(3) 5_446 4_444
O2 O2 O2 118.0(4) 5_456 4_444
Ga2 O2 O2 51.71(18) 2_564 4_444
La O2 O2 104.3(2) 4_446 4_444
Nb O2 O2 50.48(17) . 4_444
Ga1 O2 O2 50.48(17) . 4_444
O3 O2 O2 58.9(2) 2 4_444
O2 O2 O2 73.4(3) 5_345 4_444
O3 O2 O2 66.0(3) 5_445 4_444
O3 O2 O2 44.4(3) 4_445 4_444
O3 O2 O2 86.6(2) 1_455 4_444
O3 O2 O2 163.7(4) 2_456 4_444
O3 O2 O2 167.6(5) 5_456 4_444
O3 O2 O2 78.4(4) 6_445 4_444
La O2 O2 143.2(4) 4_456 4_444
O1 O2 O2 136.0(4) 1_556 4_444
O2 O2 O2 113.5(3) 4_345 4_444
O2 O2 O2 115.7(2) 3_465 4_444
O2 O2 O2 28.4(4) 5_445 4_444
O2 O2 O2 69.9(3) 5_455 4_444
Ga3 O2 O2 70.42(15) 4_345 4_444
O2 O2 O2 130.6(2) 3_456 4_444
O2 O2 O2 122.3(3) 4_446 4_444
O2 O2 O2 27.93(12) 3_454 4_444
Ga3 O2 O2 18.32(13) 4_445 4_444
Ga2 O2 La 118.4(6) 1_556 2_565
Ga3 O2 La 87.5(4) 1_556 2_565
La O2 La 34.4(3) . 2_565
O2 O2 La 141.6(6) 3_455 2_565
O2 O2 La 84.6(6) 4_445 2_565
O3 O2 La 124.4(3) 2_455 2_565
O2 O2 La 64.0(3) 6_556 2_565
O3 O2 La 69.6(3) 5_455 2_565
La O2 La 130.9(4) 2_455 2_565
O1 O2 La 90.0(3) 2_455 2_565
O3 O2 La 119.7(5) 3_456 2_565
O1 O2 La 115.7(5) 2_456 2_565
O3 O2 La 92.1(3) 3_455 2_565
O1 O2 La 12.69(12) . 2_565
Nb O2 La 91.75(19) 1_455 2_565
Ga1 O2 La 91.75(19) 1_455 2_565
Ga2 O2 La 34.97(11) 2_565 2_565
O2 O2 La 46.4(3) 6 2_565
O3 O2 La 38.6(2) 6 2_565
La O2 La 80.6(3) 1_556 2_565
Ga3 O2 La 128.62(19) 4_346 2_565
Ga3 O2 La 74.7(2) 4_446 2_565
O3 O2 La 69.7(3) 1_556 2_565
La O2 La 139.3(4) 2_456 2_565
La O2 La 101.0(2) 4_445 2_565
Ga3 O2 La 71.05(14) . 2_565
O3 O2 La 86.0(2) 4_456 2_565
Ga3 O2 La 151.8(3) 2_455 2_565
O3 O2 La 51.52(19) . 2_565
O2 O2 La 167.7(6) 2_456 2_565
O2 O2 La 42.1(2) 2_566 2_565
Ga2 O2 La 83.93(16) . 2_565
La O2 La 44.36(11) 4_455 2_565
O3 O2 La 69.33(18) 4_455 2_565
O2 O2 La 149.09(14) 5_346 2_565
Ga1 O2 La 107.8(3) 1_456 2_565
Nb O2 La 107.8(3) 1_456 2_565
O1 O2 La 153.5(4) 1_445 2_565
O3 O2 La 98.2(2) 6_455 2_565
Ga2 O2 La 168.4(2) 2_455 2_565
Ga3 O2 La 88.10(16) 2_465 2_565
Ga3 O2 La 38.68(11) 2_565 2_565
O2 O2 La 105.39(18) 1_556 2_565
O2 O2 La 74.61(18) 1_554 2_565
O2 O2 La 126.6(5) 2_455 2_565
O2 O2 La 24.05(10) 2_565 2_565
O3 O2 La 137.1(3) 4_446 2_565
O3 O2 La 116.0(2) 1_456 2_565
O2 O2 La 93.3(4) 5_446 2_565
O2 O2 La 44.19(19) 5_456 2_565
Ga2 O2 La 34.75(8) 2_564 2_565
La O2 La 114.0(3) 4_446 2_565
Nb O2 La 47.71(11) . 2_565
Ga1 O2 La 47.71(11) . 2_565
O3 O2 La 66.67(18) 2 2_565
O2 O2 La 120.3(3) 5_345 2_565
O3 O2 La 125.0(2) 5_445 2_565
O3 O2 La 116.7(2) 4_445 2_565
O3 O2 La 99.6(2) 1_455 2_565
O3 O2 La 122.4(3) 2_456 2_565
O3 O2 La 93.8(3) 5_456 2_565
O3 O2 La 150.2(2) 6_445 2_565
La O2 La 69.87(18) 4_456 2_565
O1 O2 La 67.6(2) 1_556 2_565
O2 O2 La 128.0(2) 4_345 2_565
O2 O2 La 70.5(3) 3_465 2_565
O2 O2 La 79.6(2) 5_445 2_565
O2 O2 La 28.1(2) 5_455 2_565
Ga3 O2 La 102.49(19) 4_345 2_565
O2 O2 La 127.7(4) 3_456 2_565
O2 O2 La 100.8(4) 4_446 2_565
O2 O2 La 98.40(16) 3_454 2_565
Ga3 O2 La 64.91(12) 4_445 2_565
O2 O2 La 73.9(2) 4_444 2_565
Ga2 O2 O2 96.0(7) 1_556 3_565
Ga3 O2 O2 94.1(4) 1_556 3_565
La O2 O2 41.3(5) . 3_565
O2 O2 O2 126.8(8) 3_455 3_565
O2 O2 O2 66.8(8) 4_445 3_565
O3 O2 O2 145.7(4) 2_455 3_565
O2 O2 O2 59.6(3) 6_556 3_565
O3 O2 O2 88.4(3) 5_455 3_565
La O2 O2 144.6(2) 2_455 3_565
O1 O2 O2 93.7(4) 2_455 3_565
O3 O2 O2 117.1(5) 3_456 3_565
O1 O2 O2 93.5(4) 2_456 3_565
O3 O2 O2 113.7(2) 3_455 3_565
O1 O2 O2 31.87(12) . 3_565
Nb O2 O2 114.43(19) 1_455 3_565
Ga1 O2 O2 114.43(19) 1_455 3_565
Ga2 O2 O2 34.27(10) 2_565 3_565
O2 O2 O2 67.5(3) 6 3_565
O3 O2 O2 20.9(3) 6 3_565
La O2 O2 62.71(19) 1_556 3_565
Ga3 O2 O2 142.3(2) 4_346 3_565
Ga3 O2 O2 53.3(3) 4_446 3_565
O3 O2 O2 46.6(3) 1_556 3_565
La O2 O2 123.2(3) 2_456 3_565
La O2 O2 90.9(4) 4_445 3_565
Ga3 O2 O2 91.71(17) . 3_565
O3 O2 O2 92.62(19) 4_456 3_565
Ga3 O2 O2 132.1(4) 2_455 3_565
O3 O2 O2 49.9(3) . 3_565
O2 O2 O2 144.8(5) 2_456 3_565
O2 O2 O2 26.3(4) 2_566 3_565
Ga2 O2 O2 92.4(3) . 3_565
La O2 O2 65.80(11) 4_455 3_565
O3 O2 O2 92.47(17) 4_455 3_565
O2 O2 O2 152.0(4) 5_346 3_565
Ga1 O2 O2 108.14(16) 1_456 3_565
Nb O2 O2 108.14(16) 1_456 3_565
O1 O2 O2 169.7(2) 1_445 3_565
O3 O2 O2 117.3(2) 6_455 3_565
Ga2 O2 O2 165.7(3) 2_455 3_565
Ga3 O2 O2 102.19(15) 2_465 3_565
Ga3 O2 O2 15.46(13) 2_565 3_565
O2 O2 O2 90.000(1) 1_556 3_565
O2 O2 O2 90.0 1_554 3_565
O2 O2 O2 135.8(2) 2_455 3_565
O2 O2 O2 38.1(3) 2_565 3_565
O3 O2 O2 114.6(4) 4_446 3_565
O3 O2 O2 124.6(2) 1_456 3_565
O2 O2 O2 71.3(4) 5_446 3_565
O2 O2 O2 46.41(16) 5_456 3_565
Ga2 O2 O2 55.08(16) 2_564 3_565
La O2 O2 90.8(3) 4_446 3_565
Nb O2 O2 35.9(3) . 3_565
Ga1 O2 O2 35.9(3) . 3_565
O3 O2 O2 49.3(3) 2 3_565
O2 O2 O2 141.4(2) 5_345 3_565
O3 O2 O2 110.2(4) 5_445 3_565
O3 O2 O2 113.4(3) 4_445 3_565
O3 O2 O2 122.8(2) 1_455 3_565
O3 O2 O2 115.1(2) 2_456 3_565
O3 O2 O2 89.19(15) 5_456 3_565
O3 O2 O2 139.0(3) 6_445 3_565
La O2 O2 70.30(9) 4_456 3_565
O1 O2 O2 57.23(12) 1_556 3_565
O2 O2 O2 147.4(2) 4_345 3_565
O2 O2 O2 87.4(2) 3_465 3_565
O2 O2 O2 73.1(5) 5_445 3_565
O2 O2 O2 51.4(3) 5_455 3_565
Ga3 O2 O2 124.81(12) 4_345 3_565
O2 O2 O2 106.8(3) 3_456 3_565
O2 O2 O2 79.0(4) 4_446 3_565
O2 O2 O2 106.8(3) 3_454 3_565
Ga3 O2 O2 64.2(3) 4_445 3_565
O2 O2 O2 79.0(4) 4_444 3_565
La O2 O2 23.26(9) 2_565 3_565
Ga2 O2 O2 144.5(7) 1_556 4_455
Ga3 O2 O2 45.7(3) 1_556 4_455
La O2 O2 74.6(3) . 4_455
O2 O2 O2 173.2(8) 3_455 4_455
O2 O2 O2 126.8(8) 4_445 4_455
O3 O2 O2 86.3(3) 2_455 4_455
O2 O2 O2 44.8(4) 6_556 4_455
O3 O2 O2 29.2(3) 5_455 4_455
La O2 O2 124.3(3) 2_455 4_455
O1 O2 O2 120.5(3) 2_455 4_455
O3 O2 O2 81.1(3) 3_456 4_455
O1 O2 O2 118.6(3) 2_456 4_455
O3 O2 O2 82.2(3) 3_455 4_455
O1 O2 O2 31.87(12) . 4_455
Nb O2 O2 61.0(2) 1_455 4_455
Ga1 O2 O2 61.0(2) 1_455 4_455
Ga2 O2 O2 34.26(10) 2_565 4_455
O2 O2 O2 57.6(5) 6 4_455
O3 O2 O2 80.3(3) 6 4_455
La O2 O2 80.65(15) 1_556 4_455
Ga3 O2 O2 84.6(2) 4_346 4_455
Ga3 O2 O2 111.5(3) 4_446 4_455
O3 O2 O2 94.4(3) 1_556 4_455
La O2 O2 112.26(17) 2_456 4_455
La O2 O2 144.5(3) 4_445 4_455
Ga3 O2 O2 72.92(17) . 4_455
O3 O2 O2 44.3(2) 4_456 4_455
Ga3 O2 O2 161.6(2) 2_455 4_455
O3 O2 O2 94.1(3) . 4_455
O2 O2 O2 137.9(3) 2_456 4_455
O2 O2 O2 57.08(15) 2_566 4_455
Ga2 O2 O2 109.13(12) . 4_455
La O2 O2 20.6(2) 4_455 4_455
O3 O2 O2 47.6(2) 4_455 4_455
O2 O2 O2 104.65(15) 5_346 4_455
Ga1 O2 O2 68.58(16) 1_456 4_455
Nb O2 O2 68.58(16) 1_456 4_455
O1 O2 O2 125.5(3) 1_445 4_455
O3 O2 O2 57.5(2) 6_455 4_455
Ga2 O2 O2 124.9(3) 2_455 4_455
Ga3 O2 O2 43.67(15) 2_465 4_455
Ga3 O2 O2 71.02(17) 2_565 4_455
O2 O2 O2 90.0 1_556 4_455
O2 O2 O2 90.0 1_554 4_455
O2 O2 O2 130.7(4) 2_455 4_455
O2 O2 O2 61.48(14) 2_565 4_455
O3 O2 O2 153.4(3) 4_446 4_455
O3 O2 O2 71.7(2) 1_456 4_455
O2 O2 O2 126.5(5) 5_446 4_455
O2 O2 O2 27.9(3) 5_456 4_455
Ga2 O2 O2 55.08(17) 2_564 4_455
La O2 O2 131.1(3) 4_446 4_455
Nb O2 O2 92.0(2) . 4_455
Ga1 O2 O2 92.0(2) . 4_455
O3 O2 O2 109.1(3) 2 4_455
O2 O2 O2 102.93(16) 5_345 4_455
O3 O2 O2 169.5(4) 5_445 4_455
O3 O2 O2 148.70(19) 4_445 4_455
O3 O2 O2 72.5(2) 1_455 4_455
O3 O2 O2 88.13(18) 2_456 4_455
O3 O2 O2 63.38(15) 5_456 4_455
O3 O2 O2 160.5(3) 6_445 4_455
La O2 O2 39.63(13) 4_456 4_455
O1 O2 O2 57.23(12) 1_556 4_455
O2 O2 O2 87.4(2) 4_345 4_455
O2 O2 O2 27.4(2) 3_465 4_455
O2 O2 O2 122.6(3) 5_445 4_455
O2 O2 O2 36.9(3) 5_455 4_455
Ga3 O2 O2 86.14(17) 4_345 4_455
O2 O2 O2 118.64(15) 3_456 4_455
O2 O2 O2 106.8(3) 4_446 4_455
O2 O2 O2 118.64(15) 3_454 4_455
Ga3 O2 O2 105.42(18) 4_445 4_455
O2 O2 O2 106.8(3) 4_444 4_455
La O2 O2 44.56(13) 2_565 4_455
O2 O2 O2 60.000(1) 3_565 4_455
Ga2 O2 O3 60.7(6) 1_556 6_556
Ga3 O2 O3 79.6(7) 1_556 6_556
La O2 O3 91.7(6) . 6_556
O2 O2 O3 100.3(3) 3_455 6_556
O2 O2 O3 64.3(3) 4_445 6_556
O3 O2 O3 134.9(5) 2_455 6_556
O2 O2 O3 44.4(3) 6_556 6_556
O3 O2 O3 107.3(5) 5_455 6_556
La O2 O3 150.5(3) 2_455 6_556
O1 O2 O3 124.4(4) 2_455 6_556
O3 O2 O3 76.5(5) 3_456 6_556
O1 O2 O3 42.4(3) 2_456 6_556
O3 O2 O3 165.0(4) 3_455 6_556
O1 O2 O3 75.9(4) . 6_556
Nb O2 O3 139.3(3) 1_455 6_556
Ga1 O2 O3 139.3(3) 1_455 6_556
Ga2 O2 O3 51.9(3) 2_565 6_556
O2 O2 O3 120.4(5) 6 6_556
O3 O2 O3 56.1(3) 6 6_556
La O2 O3 12.84(14) 1_556 6_556
Ga3 O2 O3 114.3(3) 4_346 6_556
Ga3 O2 O3 45.5(2) 4_446 6_556
O3 O2 O3 21.2(2) 1_556 6_556
La O2 O3 69.8(3) 2_456 6_556
La O2 O3 95.1(3) 4_445 6_556
Ga3 O2 O3 145.1(3) . 6_556
O3 O2 O3 79.1(3) 4_456 6_556
Ga3 O2 O3 94.1(3) 2_455 6_556
O3 O2 O3 89.8(4) . 6_556
O2 O2 O3 93.8(4) 2_456 6_556
O2 O2 O3 32.9(4) 2_566 6_556
Ga2 O2 O3 132.2(3) . 6_556
La O2 O3 102.1(4) 4_455 6_556
O3 O2 O3 131.4(4) 4_455 6_556
O2 O2 O3 104.4(5) 5_346 6_556
Ga1 O2 O3 75.2(3) 1_456 6_556
Nb O2 O3 75.2(3) 1_456 6_556
O1 O2 O3 132.4(3) 1_445 6_556
O3 O2 O3 121.5(3) 6_455 6_556
Ga2 O2 O3 112.1(3) 2_455 6_556
Ga3 O2 O3 100.4(3) 2_465 6_556
Ga3 O2 O3 40.3(2) 2_565 6_556
O2 O2 O3 39.15(17) 1_556 6_556
O2 O2 O3 140.85(17) 1_554 6_556
O2 O2 O3 145.4(3) 2_455 6_556
O2 O2 O3 91.6(4) 2_565 6_556
O3 O2 O3 74.1(3) 4_446 6_556
O3 O2 O3 98.0(3) 1_456 6_556
O2 O2 O3 48.1(3) 5_446 6_556
O2 O2 O3 56.0(4) 5_456 6_556
Ga2 O2 O3 108.4(3) 2_564 6_556
La O2 O3 48.06(19) 4_446 6_556
Nb O2 O3 68.7(3) . 6_556
Ga1 O2 O3 68.7(3) . 6_556
O3 O2 O3 60.0(2) 2 6_556
O2 O2 O3 164.8(3) 5_345 6_556
O3 O2 O3 92.9(2) 5_445 6_556
O3 O2 O3 118.2(3) 4_445 6_556
O3 O2 O3 150.3(2) 1_455 6_556
O3 O2 O3 69.2(3) 2_456 6_556
O3 O2 O3 55.6(3) 5_456 6_556
O3 O2 O3 110.8(3) 6_445 6_556
La O2 O3 57.3(2) 4_456 6_556
O1 O2 O3 30.94(15) 1_556 6_556
O2 O2 O3 128.07(14) 4_345 6_556
O2 O2 O3 101.0(2) 3_465 6_556
O2 O2 O3 94.3(4) 5_445 6_556
O2 O2 O3 100.0(5) 5_455 6_556
Ga3 O2 O3 168.5(2) 4_345 6_556
O2 O2 O3 53.7(2) 3_456 6_556
O2 O2 O3 27.3(3) 4_446 6_556
O2 O2 O3 140.0(3) 3_454 6_556
Ga3 O2 O3 99.7(3) 4_445 6_556
O2 O2 O3 118.0(3) 4_444 6_556
La O2 O3 74.1(3) 2_565 6_556
O2 O2 O3 53.7(2) 3_565 6_556
O2 O2 O3 83.9(2) 4_455 6_556
Ga2 O2 O3 126.5(7) 1_556 2_454
Ga3 O2 O3 103.0(6) 1_556 2_454
La O2 O3 75.1(4) . 2_454
O2 O2 O3 88.6(4) 3_455 2_454
O2 O2 O3 112.56(17) 4_445 2_454
O3 O2 O3 55.6(4) 2_455 2_454
O2 O2 O3 131.8(4) 6_556 2_454
O3 O2 O3 69.4(5) 5_455 2_454
La O2 O3 41.0(2) 2_455 2_454
O1 O2 O3 51.2(4) 2_455 2_454
O3 O2 O3 113.7(6) 3_456 2_454
O1 O2 O3 150.1(5) 2_456 2_454
O3 O2 O3 8.6(2) 3_455 2_454
O1 O2 O3 91.4(4) . 2_454
Nb O2 O3 41.5(2) 1_455 2_454
Ga1 O2 O3 41.5(2) 1_455 2_454
Ga2 O2 O3 117.4(3) 2_565 2_454
O2 O2 O3 45.9(3) 6 2_454
O3 O2 O3 111.3(3) 6 2_454
La O2 O3 168.9(2) 1_556 2_454
Ga3 O2 O3 76.3(3) 4_346 2_454
Ga3 O2 O3 128.9(3) 4_446 2_454
O3 O2 O3 150.0(3) 1_556 2_454
La O2 O3 124.0(4) 2_456 2_454
La O2 O3 84.6(3) 4_445 2_454
Ga3 O2 O3 21.24(16) . 2_454
O3 O2 O3 103.2(3) 4_456 2_454
Ga3 O2 O3 96.9(3) 2_455 2_454
O3 O2 O3 79.3(3) . 2_454
O2 O2 O3 99.7(4) 2_456 2_454
O2 O2 O3 134.1(4) 2_566 2_454
Ga2 O2 O3 40.83(18) . 2_454
La O2 O3 68.6(2) 4_455 2_454
O3 O2 O3 41.5(3) 4_455 2_454
O2 O2 O3 88.7(5) 5_346 2_454
Ga1 O2 O3 112.5(3) 1_456 2_454
Nb O2 O3 112.5(3) 1_456 2_454
O1 O2 O3 61.4(3) 1_445 2_454
O3 O2 O3 62.3(3) 6_455 2_454
Ga2 O2 O3 81.8(3) 2_455 2_454
Ga3 O2 O3 81.5(3) 2_465 2_454
Ga3 O2 O3 126.0(2) 2_565 2_454
O2 O2 O3 152.75(14) 1_556 2_454
O2 O2 O3 27.25(14) 1_554 2_454
O2 O2 O3 43.2(4) 2_455 2_454
O2 O2 O3 74.6(3) 2_565 2_454
O3 O2 O3 116.1(4) 4_446 2_454
O3 O2 O3 90.4(3) 1_456 2_454
O2 O2 O3 132.3(4) 5_446 2_454
O2 O2 O3 115.7(3) 5_456 2_454
Ga2 O2 O3 57.80(19) 2_564 2_454
La O2 O3 140.6(3) 4_446 2_454
Nb O2 O3 100.2(2) . 2_454
Ga1 O2 O3 100.2(2) . 2_454
O3 O2 O3 112.5(3) 2 2_454
O2 O2 O3 29.1(2) 5_345 2_454
O3 O2 O3 92.8(3) 5_445 2_454
O3 O2 O3 65.2(2) 4_445 2_454
O3 O2 O3 33.2(2) 1_455 2_454
O3 O2 O3 122.1(4) 2_456 2_454
O3 O2 O3 129.9(3) 5_456 2_454
O3 O2 O3 79.7(3) 6_445 2_454
La O2 O3 121.1(2) 4_456 2_454
O1 O2 O3 145.2(2) 1_556 2_454
O2 O2 O3 62.75(14) 4_345 2_454
O2 O2 O3 76.34(13) 3_465 2_454
O2 O2 O3 80.2(4) 5_445 2_454
O2 O2 O3 67.3(4) 5_455 2_454
Ga3 O2 O3 17.31(11) 4_345 2_454
O2 O2 O3 140.1(4) 3_456 2_454
O2 O2 O3 164.5(4) 4_446 2_454
O2 O2 O3 37.8(2) 3_454 2_454
Ga3 O2 O3 71.3(2) 4_445 2_454
O2 O2 O3 53.60(13) 4_444 2_454
La O2 O3 92.3(2) 2_565 2_454
O2 O2 O3 112.40(14) 3_565 2_454
O2 O2 O3 88.31(16) 4_455 2_454
O3 O2 O3 166.1(3) 6_556 2_454
Ga2 O2 O3 144.7(6) 1_556 5_454
Ga3 O2 O3 94.6(5) 1_556 5_454
La O2 O3 58.2(3) . 5_454
O2 O2 O3 112.0(3) 3_455 5_454
O2 O2 O3 114.6(2) 4_445 5_454
O3 O2 O3 69.4(4) 2_455 5_454
O2 O2 O3 111.0(5) 6_556 5_454
O3 O2 O3 55.6(3) 5_455 5_454
La O2 O3 66.6(3) 2_455 5_454
O1 O2 O3 60.8(3) 2_455 5_454
O3 O2 O3 119.4(6) 3_456 5_454
O1 O2 O3 175.1(5) 2_456 5_454
O3 O2 O3 24.5(2) 3_455 5_454
O1 O2 O3 65.8(3) . 5_454
Nb O2 O3 41.5(2) 1_455 5_454
Ga1 O2 O3 41.5(2) 1_455 5_454
Ga2 O2 O3 92.1(2) 2_565 5_454
O2 O2 O3 21.8(2) 6 5_454
O3 O2 O3 93.7(4) 6 5_454
La O2 O3 144.7(3) 1_556 5_454
Ga3 O2 O3 87.7(3) 4_346 5_454
Ga3 O2 O3 123.3(2) 4_446 5_454
O3 O2 O3 134.0(3) 1_556 5_454
La O2 O3 143.0(4) 2_456 5_454
La O2 O3 95.8(3) 4_445 5_454
Ga3 O2 O3 6.82(15) . 5_454
O3 O2 O3 94.1(3) 4_456 5_454
Ga3 O2 O3 121.9(4) 2_455 5_454
O3 O2 O3 69.7(2) . 5_454
O2 O2 O3 124.7(5) 2_456 5_454
O2 O2 O3 108.7(3) 2_566 5_454
Ga2 O2 O3 48.1(2) . 5_454
La O2 O3 45.68(19) 4_455 5_454
O3 O2 O3 26.4(4) 4_455 5_454
O2 O2 O3 106.3(6) 5_346 5_454
Ga1 O2 O3 112.5(3) 1_456 5_454
Nb O2 O3 112.5(3) 1_456 5_454
O1 O2 O3 85.9(4) 1_445 5_454
O3 O2 O3 62.3(2) 6_455 5_454
Ga2 O2 O3 105.0(4) 2_455 5_454
Ga3 O2 O3 75.0(2) 2_465 5_454
Ga3 O2 O3 104.2(2) 2_565 5_454
O2 O2 O3 152.73(17) 1_556 5_454
O2 O2 O3 27.27(17) 1_554 5_454
O2 O2 O3 67.8(5) 2_455 5_454
O2 O2 O3 53.4(3) 2_565 5_454
O3 O2 O3 139.9(4) 4_446 5_454
O3 O2 O3 95.1(4) 1_456 5_454
O2 O2 O3 136.4(3) 5_446 5_454
O2 O2 O3 92.0(3) 5_456 5_454
Ga2 O2 O3 34.35(12) 2_564 5_454
La O2 O3 158.6(3) 4_446 5_454
Nb O2 O3 87.83(19) . 5_454
Ga1 O2 O3 87.83(19) . 5_454
O3 O2 O3 106.2(3) 2 5_454
O2 O2 O3 52.7(3) 5_345 5_454
O3 O2 O3 112.0(4) 5_445 5_454
O3 O2 O3 83.7(3) 4_445 5_454
O3 O2 O3 40.7(3) 1_455 5_454
O3 O2 O3 129.9(3) 2_456 5_454
O3 O2 O3 122.1(3) 5_456 5_454
O3 O2 O3 104.6(4) 6_445 5_454
La O2 O3 104.0(2) 4_456 5_454
O1 O2 O3 122.9(2) 1_556 5_454
O2 O2 O3 76.33(13) 4_345 5_454
O2 O2 O3 62.73(17) 3_465 5_454
O2 O2 O3 82.9(4) 5_445 5_454
O2 O2 O3 41.6(3) 5_455 5_454
Ga3 O2 O3 35.61(15) 4_345 5_454
O2 O2 O3 163.6(4) 3_456 5_454
O2 O2 O3 168.3(5) 4_446 5_454
O2 O2 O3 53.3(2) 3_454 5_454
Ga3 O2 O3 67.78(19) 4_445 5_454
O2 O2 O3 54.71(19) 4_444 5_454
La O2 O3 67.58(14) 2_565 5_454
O2 O2 O3 89.27(14) 3_565 5_454
O2 O2 O3 66.23(17) 4_455 5_454
O3 O2 O3 141.4(3) 6_556 5_454
O3 O2 O3 25.62(18) 2_454 5_454
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.382(9) 6
La O3 2.382(9) .
La O2 2.404(11) .
La O2 2.405(11) 6
La O1 2.528(6) .
La O1 2.528(6) 2_455
La O2 2.83(2) 4_445
La O2 2.83(2) 2_565
La Ga2 3.3755(17) 1_556
La Ga2 3.3755(17) 2_564
La Ga1 3.4626(9) .
La Nb 3.4626(9) .
Ga1 O3 1.969(11) 2
Ga1 O3 1.969(11) .
Ga1 O3 1.969(11) 3
Ga1 O3 1.969(11) 5
Ga1 O3 1.969(11) 6
Ga1 O3 1.969(11) 4
Ga1 La 3.4626(9) 2
Ga1 La 3.4626(9) 4
Ga1 O2 3.568(15) 1_655
Ga1 O2 3.568(15) 5_445
Ga1 O2 3.568(15) 4_445
Ga2 O1 1.787(17) 2_455
Ga2 O2 1.812(11) 3_454
Ga2 O2 1.812(11) 4_444
Ga2 O2 1.812(11) 1_554
Ga2 O1 3.259(17) 2_454
Ga2 La 3.3755(17) 4_444
Ga2 La 3.3755(17) 2_454
Ga2 La 3.3755(17) 1_554
Ga2 O3 3.434(10) 4_445
Ga2 O3 3.434(10) .
Ga2 O3 3.434(10) 3_455
Ga2 La 3.5589(18) 4_445
Ga3 O3 1.807(10) 3_455
Ga3 O3 1.807(10) 5_454
Ga3 O2 1.837(10) 1_554
Ga3 O2 1.837(10) 6
Ga3 O3 2.547(16) 2_454
Ga3 O3 2.547(16) 4_455
Ga3 Nb 3.1380(11) 1_455
Ga3 Nb 3.1380(11) 1_454
Ga3 O1 3.563(8) 1_554
Ga3 O1 3.563(8) 2_455
Ga3 O3 3.621(9) 1_455
Ga3 O3 3.621(9) 6_454
Nb O3 1.969(11) 2
Nb O3 1.969(11) .
Nb O3 1.969(11) 3
Nb O3 1.969(11) 5
Nb O3 1.969(11) 6
Nb O3 1.969(11) 4
Nb Ga3 3.1380(11) 1_656
Nb Ga3 3.1380(11) 4_446
Nb Ga3 3.1380(11) 4_445
Nb Ga3 3.1380(11) 1_655
Nb Ga3 3.1380(11) 2_565
Nb Ga3 3.1380(11) 2_564
O1 Ga2 1.787(17) 2_565
O1 La 2.528(6) 2_565
O1 La 2.528(6) 4_455
O1 O2 2.90(2) 2_565
O1 O2 2.90(2) 6
O1 O2 2.90(2) 5_455
O1 O2 3.08(2) 2_566
O1 O2 3.08(2) 6_556
O1 O2 3.08(2) 5_456
O1 O3 3.137(10) 6
O1 O3 3.137(10) 5_455
O1 O3 3.137(10) 2_565
O1 Ga2 3.259(17) 2_564
O1 O2 3.552(13) 3_565
O1 O2 3.552(13) .
O1 O2 3.552(13) 4_455
O1 Ga3 3.563(8) 2_565
O1 Ga3 3.563(8) 1_556
O1 Ga3 3.563(8) 4_456
O1 O3 4.316(12) .
O1 O3 4.316(12) 4_455
O1 O3 4.316(12) 3_565
O1 Ga3 4.625(12) 2_564
O1 Ga3 4.625(12) 4_455
O1 Nb 4.706(3) 1_455
O1 Ga1 4.706(3) 1_455
O1 Ga1 4.706(3) 1_565
O1 Nb 4.706(3) 1_565
O1 O2 4.758(18) 4_445
O1 O2 4.758(18) 1_665
O1 O2 4.758(18) 3_465
O1 O3 4.82(2) 1_556
O1 O3 4.82(2) 3_566
O1 O3 4.82(2) 4_456
O1 La 4.812(14) 1_556
O1 La 4.812(14) 2_566
O1 La 4.812(14) 4_456
O1 O3 4.847(18) 4
O1 O3 4.847(18) 3_455
O1 O3 4.847(18) 1_565
O1 Ga2 4.875(5) 1_566
O1 Ga2 4.875(5) 1_556
O1 Ga2 4.875(5) 1_666
O1 O1 4.938(12) 2_465
O1 O1 4.938(12) 2_455
O1 O1 4.938(12) 2_565
O1 O1 5.0460 1_554
O1 O1 5.0460 1_556
O1 Ga3 5.258(5) 4_446
O1 Ga3 5.258(5) 1_666
O1 Ga3 5.258(5) 2_465
O1 O3 5.344(12) 5
O1 O3 5.344(12) 2_455
O1 O3 5.344(12) 6_565
O1 O3 5.297(13) 4_556
O1 O3 5.297(13) 3_456
O1 O3 5.297(13) 1_566
O1 O2 5.57(2) 1_554
O1 O2 5.57(2) 3_564
O1 O2 5.57(2) 4_454
O1 O3 5.639(18) 6_554
O1 O3 5.639(18) 5_454
O1 O3 5.639(18) 2_564
O1 O1 5.696(19) 2_466
O1 O1 5.696(19) 2_456
O1 O1 5.696(19) 2_566
O1 O3 5.782(10) 2
O1 O3 5.782(10) 6_455
O1 O3 5.782(10) 5_565
O1 La 5.843(2) 2_455
O1 La 5.843(2) 4
O1 La 5.843(2) 1_565
O1 O2 6.177(9) 3_455
O1 O2 6.177(9) 4
O1 O2 6.177(9) 1_565
O1 O3 6.23(2) 6_556
O3 Ga3 1.807(10) 4_445
O3 Ga3 2.547(16) 2_564
O3 O3 2.62(3) 6
O3 O3 2.691(15) 3
O3 O3 2.691(15) 4
O3 O2 2.80(2) 2_565
O3 O3 2.81(3) 6_554
O3 O2 2.803(15) 5_445
O3 O2 2.949(16) 4_444
O3 O1 3.137(10) 2_455
O3 O3 3.17(3) 2
O3 O2 3.34(3) 4_445
O3 O3 3.33(2) 2_554
O3 Ga3 3.621(9) 1_655
O3 La 3.737(15) 4_445
O3 O2 3.840(18) 6
O3 O3 3.89(2) 5
O3 Ga3 3.933(17) 4_446
O3 Ga2 3.968(14) 2_564
O3 O3 4.02(3) 5_554
O3 Ga1 4.139(15) 1_554
O3 Nb 4.139(15) 1_554
O3 O2 4.21(2) 1_554
O3 La 4.239(13) 2
O3 Ga3 4.323(12) 2_565
O3 La 4.351(15) 1_554
O3 O2 4.38(2) 3_564
O3 O2 4.496(15) .
O3 Ga2 4.541(11) 2_554
O3 La 4.672(11) 2_565
O3 O2 4.655(16) 3_565
O3 Ga2 4.767(15) 1_556
O3 O2 4.776(14) 6_655
O3 O1 4.82(2) 1_554
O3 O1 4.847(18) 1_545
O3 La 4.894(10) 4
O3 Ga3 5.032(13) 1_656
O3 O3 5.0460 1_556
O3 O3 5.0460 1_554
O3 O2 5.102(13) 3_454
O3 O2 5.081(13) 1_654
O3 La 5.217(11) 4_444
O3 O2 5.313(18) 2
O3 O2 5.341(16) 5_455
O3 O1 5.344(12) 2_565
O3 O1 5.297(13) 1_544
O3 O2 5.34(2) 3_455
O3 O2 5.32(2) 1_655
O3 Ga2 5.406(10) 2_565
O3 O3 5.400(17) 4_445
O3 O3 5.400(17) 3_455
O3 O2 5.458(16) 2_566
O3 O2 5.46(2) 5_446
O3 O2 5.443(19) 6_545
O3 Ga2 5.524(14) 1_665
O3 La 5.555(10) 2_455
O3 La 5.588(10) 2_554
O3 O1 5.639(18) 2_454
O3 O3 5.719(7) 3_556
O3 O3 5.719(7) 4_556
O3 O3 5.719(7) 3_554
O3 O3 5.719(7) 4_554
O3 O1 5.782(10) 2
O3 La 5.923(17) 2_564
O3 O2 6.06(2) 6_556
O3 La 6.070(10) 4_455
O3 O3 6.088(19) 5_445
O3 O3 6.088(18) 5_455
O3 O2 6.07(2) 2_564
O3 La 6.100(14) 4_554
O3 O2 6.069(18) 5_444
O3 La 6.163(9) 1_655
O3 O3 6.174(16) 5_444
O3 O3 6.174(16) 5_454
O2 Ga2 1.812(11) 1_556
O2 Ga3 1.837(10) 1_556
O2 O2 2.781(15) 3_455
O2 O2 2.781(15) 4_445
O2 O3 2.80(2) 2_455
O2 O2 2.83(4) 6_556
O2 O3 2.803(15) 5_455
O2 La 2.83(2) 2_455
O2 O1 2.90(2) 2_455
O2 O3 2.948(16) 3_456
O2 O1 3.08(2) 2_456
O2 O3 3.34(3) 3_455
O2 Nb 3.568(15) 1_455
O2 Ga1 3.568(15) 1_455
O2 Ga2 3.650(17) 2_565
O2 O2 3.74(2) 6
O2 O3 3.840(18) 6
O2 La 3.94(2) 1_556
O2 Ga3 4.129(13) 4_346
O2 Ga3 4.197(15) 4_446
O2 O3 4.21(2) 1_556
O2 La 4.212(11) 2_456
O2 La 4.263(10) 4_445
O2 O3 4.38(2) 4_456
O2 Ga3 4.399(11) 2_455
O2 O2 4.494(16) 2_456
O2 O2 4.494(15) 2_566
O2 La 4.515(9) 4_455
O2 O3 4.655(16) 4_455
O2 O2 4.65(2) 5_346
O2 Ga1 4.740(11) 1_456
O2 Nb 4.740(11) 1_456
O2 O1 4.758(18) 1_445
O2 O3 4.776(14) 6_455
O2 Ga2 4.831(14) 2_455
O2 Ga3 4.870(9) 2_465
O2 Ga3 4.928(18) 2_565
O2 O2 5.0460 1_556
O2 O2 5.0460 1_554
O2 O2 5.117(19) 2_455
O2 O2 5.117(19) 2_565
O2 O3 5.102(13) 4_446
O2 O3 5.081(13) 1_456
O2 O2 5.21(3) 5_446
O2 O2 5.21(3) 5_456
O2 Ga2 5.270(11) 2_564
O2 La 5.284(13) 4_446
O2 O3 5.313(18) 2
O2 O2 5.25(4) 5_345
O2 O3 5.341(16) 5_445
O2 O3 5.34(2) 4_445
O2 O3 5.32(2) 1_455
O2 O3 5.458(16) 2_456
O2 O3 5.46(2) 5_456
O2 O3 5.443(19) 6_445
O2 La 5.489(15) 4_456
O2 O1 5.57(2) 1_556
O2 O2 5.56(2) 4_345
O2 O2 5.56(2) 3_465
O2 O2 5.754(15) 5_445
O2 O2 5.754(15) 5_455
O2 Ga3 5.72(2) 4_345
O2 O2 5.762(7) 3_456
O2 O2 5.762(7) 4_446
O2 O2 5.762(7) 3_454
O2 Ga3 5.774(10) 4_445
O2 O2 5.762(7) 4_444
O2 La 5.870(13) 2_565
O2 O2 6.03(3) 3_565
O2 O2 6.03(3) 4_455
O2 O3 6.06(2) 6_556
O2 O3 6.07(2) 2_454
O2 O3 6.069(18) 5_454
